# cif

formula: Al1.459 Mg1.001 Fe.538 O4
compound: <missing>
formula_title: <missing>
a: 8.1706
b: 8.1706
c: 8.1706
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.459
crystal_density: 3.842
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA+OgPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA+OgPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA+OgPAA==
atoms_occupancy: 4DgoAAC4CwCACAkAoKglACCbCABAxQ4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 0 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: (Al1.461 Mg1.001 Fe.538) O4
compound: <missing>
formula_title: <missing>
a: 8.1699
b: 8.1699
c: 8.1699
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.319
crystal_density: 3.844
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcASOkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcASOkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcASOkPAA==
atoms_occupancy: gEgoAAC4CwCACAkAoKglACCbCABAxQ4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 60 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEAAgAABAAgAACABAAAQAIAACAEAACACAAAAEAAIAQAAgCAAEAQABAEAAgCAAACAA==


formula: (Al1.461 Mg1.001 Fe.538) O4
compound: <missing>
formula_title: <missing>
a: 8.1696
b: 8.1696
c: 8.1696
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.258
crystal_density: 3.844
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0OgPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0OgPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0OgPAA==
atoms_occupancy: gEgoAEDXCwBA6QgAIGolACCbCADAAw8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 360 min


formula: (Al1.461 Mg1.001 Fe.538) O4
compound: <missing>
formula_title: <missing>
a: 8.1690
b: 8.1690
c: 8.1690
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.138
crystal_density: 3.845
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_occupancy: YHcoAID2CwAgmwgAoCslAGA9CAAAoA8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 960 min


formula: (Al1.461 Mg1.001 Fe.538) O4
compound: <missing>
formula_title: <missing>
a: 8.1685
b: 8.1685
c: 8.1685
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.038
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAmOkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAmOkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAmOkPAA==
atoms_occupancy: oJYoAID2CwDgewgAoCslAOD+BwCA3g8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 2460 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAAAgAEAAAEAAgAABAAgAACABAAAQAIAACAEAACACAAAAEAAEAQAAgCAAEAQABAEAAgCAAACAA==


formula: (Al1.459 Mg1.002 Fe.539) O4
compound: <missing>
formula_title: <missing>
a: 8.1684
b: 8.1684
c: 8.1684
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.018
crystal_density: 3.847
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAcOkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAcOkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAcOkPAA==
atoms_occupancy: oJYoAMAVDACgXAgAwPwkAKDfBwCgLBAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 5340 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAAAgAEAAAEAAgAABAAgAACABAAAQAIAACAEAACACAAAAEAAEAQAAgCAAEAQABAEAAgCAAACAA==


formula: (Al1.46 Mg1.001 Fe.539) O4
compound: <missing>
formula_title: <missing>
a: 8.1687
b: 8.1687
c: 8.1687
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.078
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAUOsPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAUOsPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAUOsPAA==
atoms_occupancy: YPQoAEDXCwBgPQgAIGolAMAzBwAgaxAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 11,100 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAAAgAEAAAEAAgAABAAgAACABAAAQAIAACAEAACACAAAAEAAEAQAAgCAAEAQABAEAAgCAAACAA==


formula: (Al1.46 Mg1.001 Fe.539) O4
compound: <missing>
formula_title: <missing>
a: 8.1693
b: 8.1693
c: 8.1693
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.198
crystal_density: 3.845
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAOO8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAOO8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAOO8PAA==
atoms_occupancy: AIEpAAA7CwAATQgAoKImAIAaBgDgSxAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 22,620 min


formula: Al1.46 Mg1.002 Fe.537 O4
compound: <missing>
formula_title: <missing>
a: 8.1698
b: 8.1698
c: 8.1698
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.298
crystal_density: 3.843
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAePAPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAePAPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAePAPAA==
atoms_occupancy: 4K8pACAMCwAATQgAABAnAMC8BQCgLBAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 35,340 min


formula: Al1.461 Mg1.001 Fe.54 O4
compound: <missing>
formula_title: <missing>
a: 8.1701
b: 8.1701
c: 8.1701
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.359
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPEPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPEPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPEPAA==
atoms_occupancy: wN4pAKDNCgBAbAgAYH0nAKBuBQAAHRAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 52,620 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAABAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAQABAIAAgCAAACAA==


formula: Al1.461 Mg1.001 Fe.537 O4
compound: <missing>
formula_title: <missing>
a: 8.1705
b: 8.1705
c: 8.1705
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.439
crystal_density: 3.842
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPEPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPEPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkPEPAA==
atoms_occupancy: wN4pAKDNCgCgXAgAYH0nAKBuBQBgDRAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 67,020 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAQABAIAAgEAAACAA==


formula: Al1.459 Mg1.003 Fe.537 O4
compound: <missing>
formula_title: <missing>
a: 8.1707
b: 8.1707
c: 8.1707
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.479
crystal_density: 3.841
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACPIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACPIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACPIPAA==
atoms_occupancy: wN4pAKDNCgCgXAgAoJwnAGBPBQBgDRAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 97,260 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACACAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: Al1.46 Mg1.002 Fe.54 O4
compound: <missing>
formula_title: <missing>
a: 8.1706
b: 8.1706
c: 8.1706
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.459
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACPIPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACPIPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACPIPAA==
atoms_occupancy: wN4pAAC+CgDgewgAQKwnAABfBQDA/Q8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 550 C
 Annealing time = 339,180 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: Al1.459 Mg1.003 Fe.54 O4
compound: <missing>
formula_title: <missing>
a: 8.1709
b: 8.1709
c: 8.1709
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.519
crystal_density: 3.845
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOcPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOcPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOcPAA==
atoms_occupancy: YPonAID2CwDAJwkA4EolACAYCQAApg4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 0 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACACAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: Al1.46 Mg1.001 Fe.537 O4
compound: <missing>
formula_title: <missing>
a: 8.1703
b: 8.1703
c: 8.1703
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.398
crystal_density: 3.841
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWOgPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWOgPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWOgPAA==
atoms_occupancy: oBkoAKDHCwAgGAkAYIklAEDpCABglg4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 3 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAABAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAQABAIAAgCAAACAA==


formula: (Al1.46 Mg1.001 Fe.539) O4
compound: <missing>
formula_title: <missing>
a: 8.1700
b: 8.1700
c: 8.1700
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.339
crystal_density: 3.844
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_occupancy: gEgoAKDHCwDg+AgAYIklAICLCAAg9A4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 9 min


formula: (Al1.458 Mg1.001 Fe.541) O4
compound: <missing>
formula_title: <missing>
a: 8.1697
b: 8.1697
c: 8.1697
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.278
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAcOkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAcOkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAcOkPAA==
atoms_occupancy: IFgoAKDHCwBA6QgAYIklAABNCACgMg8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 21 min


formula: (Al1.461 Mg.999 Fe.54) O4
compound: <missing>
formula_title: <missing>
a: 8.1694
b: 8.1694
c: 8.1694
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.218
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgOgPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgOgPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgOgPAA==
atoms_occupancy: 4DgoAEDXCwDg+AgA4EolAGC6CADAAw8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 45 min


formula: Al1.462 Mg Fe.537 O4
compound: <missing>
formula_title: <missing>
a: 8.1690
b: 8.1690
c: 8.1690
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.138
crystal_density: 3.844
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA6OkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA6OkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA6OkPAA==
atoms_occupancy: AIcoAAC4CwAAyggAAJklAMAtCACgMg8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 93 min


formula: Al1.46 Mg1.001 Fe.538 O4
compound: <missing>
formula_title: <missing>
a: 8.1700
b: 8.1700
c: 8.1700
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.339
crystal_density: 3.843
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAkOwPAA==
atoms_occupancy: YPQoAOBpCwDAqggA4EQmAMAzBwDAgA8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 189 min


formula: Al1.459 Mg1.003 Fe.54 O4
compound: <missing>
formula_title: <missing>
a: 8.1705
b: 8.1705
c: 8.1705
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.439
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0O0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0O0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA0O0PAA==
atoms_occupancy: oBMpAAA7CwAAyggA4MEmAKDlBgCAYQ8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 381 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAQABAIAAgEAAACAA==


formula: Al1.457 Mg1.001 Fe.544 O4
compound: <missing>
formula_title: <missing>
a: 8.1708
b: 8.1708
c: 8.1708
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.499
crystal_density: 3.848
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAsO8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAsO8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAsO8PAA==
atoms_occupancy: IFIpAODsCgCg2QgA4D4nAGBJBgDAgA8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 765 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACACAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: Al1.457 Mg Fe.541 O4
compound: <missing>
formula_title: <missing>
a: 8.1712
b: 8.1712
c: 8.1712
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.579
crystal_density: 3.843
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2O8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2O8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2O8PAA==
atoms_occupancy: wGEpAODsCgDAqggAQC8nACAqBgCgrw8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 1533 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACACAAAQAIAACAEAACAEAAAAIAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: (Al1.461 Mg1.001 Fe.538) O4
compound: <missing>
formula_title: <missing>
a: 8.1710
b: 8.1710
c: 8.1710
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.539
crystal_density: 3.842
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAEO8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAEO8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAEO8PAA==
atoms_occupancy: wGEpACAMCwAgmwgAYAAnAKBoBgAAoA8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 3069 min


formula: (Al1.46 Mg1.001 Fe.539) O4
compound: <missing>
formula_title: <missing>
a: 8.1712
b: 8.1712
c: 8.1712
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.579
crystal_density: 3.843
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAiO8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAiO8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAiO8PAA==
atoms_occupancy: IFIpAEDdCgCg2QgAIF4nAEB4BgCgMg8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 6141 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACACAAAQAIAACAEAACAEAAAAIAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: (Al1.46 Mg1.001 Fe.539) O4
compound: <missing>
formula_title: <missing>
a: 8.1708
b: 8.1708
c: 8.1708
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.499
crystal_density: 3.843
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2O8PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2O8PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA2O8PAA==
atoms_occupancy: YHEpAODsCgDAqggA4D4nAMA5BgBgkA8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 650 C
 Annealing time = 46,161 min


formula: Al1.457 Mg1.002 Fe.539 O4
compound: <missing>
formula_title: <missing>
a: 8.1708
b: 8.1708
c: 8.1708
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.499
crystal_density: 3.842
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMOgPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMOgPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMOgPAA==
atoms_occupancy: AAooAEDXCwAgGAkAwHklAKDZCACgtQ4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 0 min


formula: (Al1.461 Mg Fe.539) O4
compound: <missing>
formula_title: <missing>
a: 8.1699
b: 8.1699
c: 8.1699
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.319
crystal_density: 3.845
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIOkPAA==
atoms_occupancy: gEgoAAC4CwCACAkAAJklACCbCADg1A4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 1 min


formula: Al1.46 Mg Fe.538 O4
compound: <missing>
formula_title: <missing>
a: 8.1701
b: 8.1701
c: 8.1701
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.359
crystal_density: 3.842
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAOOoPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAOOoPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAOOoPAA==
atoms_occupancy: AIcoAGCoCwAAyggAQLglAIAOCABAQg8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 3 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAABAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAQABAIAAgCAAACAA==


formula: (Al1.463 Mg1.002 Fe.535) O4
compound: <missing>
formula_title: <missing>
a: 8.1704
b: 8.1704
c: 8.1704
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.419
crystal_density: 3.841
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAGOwPAA==
atoms_occupancy: gMUoAKBKCwDg+AgAAJMmAGDABwCgtQ4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 6 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAQABAIAAgEAAACAA==


formula: Al1.459 Mg1.001 Fe.539 O4
compound: <missing>
formula_title: <missing>
a: 8.1704
b: 8.1704
c: 8.1704
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.419
crystal_density: 3.843
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaOwPAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaOwPAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAaOwPAA==
atoms_occupancy: INUoAEBaCwCg2QgAIGQmAKBiBwCgMg8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 9 min


formula: Al1.462 Mg1.001 Fe.538 O4
compound: <missing>
formula_title: <missing>
a: 8.1706
b: 8.1706
c: 8.1706
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.459
crystal_density: 3.844
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWO0PAA==
atoms_occupancy: AAQpAGArCwBA6QgA4MEmAMAzBwDAAw8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 15 min

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAAEAAAAAAAAIAAABAAAAAABAAACAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAACABAAAQAIAACAEAACAEAAAAEAAIAQAAgCAAEAgABAIAAgEAAACAA==


formula: Al1.468 Mg1.004 Fe.53 O4
compound: <missing>
formula_title: <missing>
a: 8.1709
b: 8.1709
c: 8.1709
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.519
crystal_density: 3.838
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA+O0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA+O0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcA+O0PAA==
atoms_occupancy: IFIpAGArCwAgmwgAwPAmAED1BgAAIw8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 30 min


formula: Al1.463 Mg1.002 Fe.537 O4
compound: <missing>
formula_title: <missing>
a: 8.1706
b: 8.1706
c: 8.1706
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.459
crystal_density: 3.843
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAgO0PAA==
atoms_occupancy: AAQpAMAbCwDg+AgAwPAmAGBDBwDg1A4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 60 min


formula: Al1.463 Mg1.003 Fe.538 O4
compound: <missing>
formula_title: <missing>
a: 8.1708
b: 8.1708
c: 8.1708
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.499
crystal_density: 3.845
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMO0PAA==
atoms_occupancy: AAQpAAA7CwBA6QgA4MEmAGBDBwDAAw8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 120 min


formula: Al1.46 Mg1.001 Fe.541 O4
compound: <missing>
formula_title: <missing>
a: 8.1708
b: 8.1708
c: 8.1708
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.499
crystal_density: 3.846
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIO4PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIO4PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAIO4PAA==
atoms_occupancy: QCMpAMAbCwCg2QgAIOEmAADWBgDgUQ8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 240 min


formula: (Al1.45 Mg Fe.55) O4
compound: <missing>
formula_title: <missing>
a: 8.1706
b: 8.1706
c: 8.1706
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.459
crystal_density: 3.851
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAWO0PAA==
atoms_occupancy: gMUoAAA7CwCACAkAAJMmAED1BgDAgA8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 1680 min


formula: (Al1.455 Mg Fe.545) O4
compound: <missing>
formula_title: <missing>
a: 8.1706
b: 8.1706
c: 8.1706
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.459
crystal_density: 3.848
atoms_sites: ["AlM", "MgM", "Fe3+M", "MgT", "AlT", "Fe3+T", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcACO0PAA==
atoms_occupancy: INUoAAA7CwDg+AgAAJMmACAkBwDgUQ8AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kinetics of cation ordering in synthetic Mg(Al,Fe3+)2O4 spinels
 Note Sample F54, disordered at 1000 C for 24 h, then ordered at 750 C
 Annealing time = 17,520 min


formula: (Mg1.23 Fe1.08 Ca.69) (Al1.98 Cr.02) Si3 O12
compound: inclusion in diamond, Jericho kimberlite, Slave Craton, Canada
formula_title: <missing>
a: 11.5826
b: 11.5825
c: 11.5826
alpha: 90
beta: 90
gamma: 90
cell_volume: 1553.869
crystal_density: 3.835
atoms_sites: ["Mg", "Fe", "Ca", "Al", "Cr", "Si", "O"]
atoms_x: IKEHACChBwAgoQcAAAAAAAAAAABg4xYAoBwCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQPQCAA==
atoms_z: QEIPAEBCDwBAQg8AAAAAAAAAAABAQg8AcNYnAA==
atoms_occupancy: QAYZAAD5FQDACQ4AwGw8AECcAAAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 In situ analysis of garnet inclusion in diamond using
 single-crystal X-ray diffraction and X-ray micro-tomography
 Note: uncorrected for pressure inside the diamond

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAEAAAAAAABAAQAAAEAIAIAQAAEAQAAACAQCAAICAgQECAAAQIEECCBABBABBBCACCEEIQQBAEIQhAEIACEQiEQCEQCABERAIAIgACJARABAABAAAAQAAAAAAAAJAAAAAAAAAAAAAAAAAAA==


formula: (Mg1.23 Fe1.08 Ca.69) (Al1.98 Cr.02) Si3 O12
compound: inclusion in diamond, Jericho kimberlite, Slave Craton, Canada
formula_title: <missing>
a: 11.6044
b: 11.6044
c: 11.6044
alpha: 90
beta: 90
gamma: 90
cell_volume: 1562.673
crystal_density: 3.813
atoms_sites: ["Mg", "Fe", "Ca", "Al", "Cr", "Si", "O"]
atoms_x: IKEHACChBwAgoQcAAAAAAAAAAABg4xYAoBwCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA4OoCAA==
atoms_z: QEIPAEBCDwBAQg8AAAAAAAAAAABAQg8AcNYnAA==
atoms_occupancy: QAYZAAD5FQDACQ4AwGw8AECcAAAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 In situ analysis of garnet inclusion in diamond using
 single-crystal X-ray diffraction and X-ray micro-tomography
 Note: Parameters transformed to room conditions from pressure effect of diamond

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAEAAAAAAABAAQAAAIAIAQAgAAIAgAAACAgEAAQEBAgIEAAAgQIIEECACCACCCCAEIIQQhACAIQhCAIgAEQhEIgEIgIAEIiAgASAAIiAiAEAACAAABAAAAAAAAASAAAAAAAAAAAAAAAAAAA==


formula: Ca Zn2 Si2 O8 H2
compound: Christmas Mine, Gila County, Arizona, USA
pub_title: Redetermination of junitoite, CaZn2Si2O7*H2O
formula_title: <missing>
a: 12.5302
b: 6.3056
c: 8.5617
alpha: 90
beta: 90
gamma: 90
cell_volume: 676.464
crystal_density: 3.506
atoms_sites: ["Ca", "Zn", "Si", "O1", "O2", "O3", "O4", "OW5", "H"]
atoms_x: AAAAAABkDwD4NwcAmIMHAHjGBwAgkgwAAAAAAAAAAAAwIwIA
atoms_y: gIQeAMjsDgDQKgAA2EISABhsDQCwtP//AAAAAICEHgC4XhsA
atoms_z: kKofAHA8CAAwDRgAuJwAAMASHgB4eA8A2IgSAIheDwD4NwwA
atoms_occupancy: 0
atoms_u_iso: eIwAAEB+AAAYYAAA+KcAALCaAABYnQAA+H8AAEBGAQDA1AEA
atoms_aniso_label: ["Ca", "Zn", "Si", "O1", "O2", "O3", "O4", "OW5"]
atoms_aniso_u11: 8KUAAPh1AAD4VwAAaIMAACiHAABIwQAASGIAANioAQA=
atoms_aniso_u22: gHoAAHhzAABYawAA2K4AAHiqAACwfAAAKK8AAACzAQA=
atoms_aniso_u33: 0IQAAHiRAAAgXQAAWMUAAJieAAA4mgAAUG4AAOh2AAA=
atoms_aniso_u12: +AIAAIj1//+Q/P//2PD//7AdAAA4////AAAAAMibAAA=
atoms_aniso_u13: AAAAAPAKAAD4AgAAOOH//5jW//8ARgAAAAAAAAAAAAA=
atoms_aniso_u23: AAAAAMD0//94BQAAuEcAAKDJ//84BAAAAAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAAACAAAAAQAEAEAACAAEUQAAQAIAWQCEACUIgQCoYwBAQiSQUkA4kXpUAp6KIKZAFsKHgfyYb6SFpJxdWZCHJ4uuw6uniZMqlx+XBT0wVfElV9t9NdzXfjj/XadrpQ/StsaTdHLWKJljLVGllzVI7bcW1==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 9.3272
b: 13.5660
c: 6.5903
alpha: 90
beta: 106.433
gamma: 90
cell_volume: 799.826
crystal_density: 3.554
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: 2GYHAIDeGQDIlxMACGkCAPAJFQBIFA0AKJcOACiBBgA=
atoms_y: ELr+/8B9CADQuQcAkNQJAFCh//8wlf7/SM0NANDNDAA=
atoms_z: MJwuABhFNACQ3QoAwJsrAGDPKgAQFgcAsBQnAGApAwA=
atoms_occupancy: 0
atoms_u_iso: 0KEBAOisAQBYpgEAGNIBAJDDAQAwugEAgOcBAIAAAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 0 GPa

qdat:
AAAAAAAAAAACAAgEAAIIAACISAgEkABAEwgxkAbCMQgEDeLFS4JTxAPYdiXpmRd4lj+hky3/6cy5P33+/y+b7esU7PdreO7439//r/6e+L/f+/f9Xev9+/36//6337/av9u8fn1dr/tv57/a7nf6Z/7X//vP/+z/u/xr/X==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 9.164
b: 13.227
c: 6.470
alpha: 90
beta: 106.56
gamma: 90
cell_volume: 751.714
crystal_density: 3.781
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: EC8HALAXGgAAuhMAUDoCAGDvFAAw3AwAQEgOALCPBgA=
atoms_y: QI/+/5BnCAAQxQcAYOYJAHBo//+gZv7/4PMNAKAlDQA=
atoms_z: AHwuABA0NAAAIgsAwFUrAIBVKgDwRAcAsGUmABAuAwA=
atoms_occupancy: 0
atoms_u_iso: wIkBAKCGAQCghgEAMLoBAAD0AQBAlgEAYOQBAKADAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 0.89 GPa

qdat:
AAAAAAAAAAAAgAIBAACBAAARCQEASQACALCBGIBaCIggIG8XIycMp4gFqdonaaoLdF9OoMsPr1K6Xp9bo/un979/V43btWsf/od98/uu1O/K99//n+t3z//+/ed7+P9ev9M///x/n2737+/z03x+2fZZzbv37vm3v2Xe2d==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 9.065
b: 13.030
c: 6.375
alpha: 90
beta: 106.77
gamma: 90
cell_volume: 720.971
crystal_density: 3.943
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: 0PYGACAvGgAA0xMAIBACAIDyFACg8wwAwJ8OAFBtBgA=
atoms_y: QHb+//hjCACgxgcAUPEJAGBB//8gWv7/IPoNABAkDQA=
atoms_z: 0FEuAFAhNABgRAsA8BsrAOBFKgAwfQcAsGUmADBKAwA=
atoms_occupancy: 0
atoms_u_iso: ABMBAHAqAQDgDwEAACwBAMBXAQDgKAEAgFEBALBJAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 1.55 GPa

qdat:
AAAAAAAAAAAAgAEAgAAgQAAEQkAgCiAAQBYIUhAHYQiGAgL44ilwxThAbUrRL0tIL9Fte4EmPv7lZVo3vWfLtb6vT38Pe261lrtOvdr/1y57/He7/Wv9z/l7/+985b+/8+2873f/7/fuf637N97f8blvnLV7Vfv/Yr85p1==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 9.003
b: 12.919
c: 6.318
alpha: 90
beta: 106.87
gamma: 90
cell_volume: 703.221
crystal_density: 4.042
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: 0N0GADA9GgAg7xMAcPIBAADNFADQuQwAwG0OAECRBgA=
atoms_y: MGj+/4BZCACAwwcAkPcJAMAY//8wT/7/0P4NAJBJDQA=
atoms_z: wEMuANAUNAAQYgsAgAQrAHAVKgDggQcAUPglAEBxAwA=
atoms_occupancy: 0
atoms_u_iso: sDABADAkAQAwJAEAYE4BABBTAQDAVwEAUIsBABAIAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 2.14 GPa

qdat:
AAAAAAAAAAAAQACAQAAQIAACISAQBRAAEAqEFIQBOEIhgICtHIVaCMcQDak6JejohPkdbrgSxt7+VjTh+9t8eV63fOv4+ttnfb3fbt/33b26/uLv/+fPvVWr33+76/v33er/eV7/69X/7Xdf//b+/+P9e9yr/d/b/vPbnN==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 8.876
b: 12.887
c: 6.272
alpha: 90
beta: 106.85
gamma: 90
cell_volume: 686.622
crystal_density: 4.140
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: QMMGAFBZGgCw8BMAkPUBANDUFACQzAwA0JQOANCSBgA=
atoms_y: YGD+/5BOCACgxgcAIPkJAJAH///AN/7/wAkOANBPDQA=
atoms_z: QDcuADAeNACgfAsAEO0qAMD3KQCwogcAwCgmANByAwA=
atoms_occupancy: 0
atoms_u_iso: EDoBAFBAAQBwKgEAMD0BAPA2AQBgTgEAkF8BAEB9AQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 2.82 GPa

qdat:
AAAAAAAAAAAAIABAIAAQIAABCEgIAkgAEALhBhEAdhEIYAg2xIpLgkriAWY8hTyzEm+JWf2GLJ//sxUdH059rWv37v3Yz+/63fP+8dtP/q3/r70rebt3b+/6z7d9/v//un/23OxL618NU+8ff/Kb3W/mrh3+Yff38/Rs9z==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 8.873
b: 12.789
c: 6.251
alpha: 90
beta: 107.00
gamma: 90
cell_volume: 678.349
crystal_density: 4.190
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: cKIGAOBzGgDgARQAwNQBAJDnFABwyQwAMIUOACB1BgA=
atoms_y: gEr+/1BICACgxgcAsPoJAPD3/v9QOf7/ICwOACBkDQA=
atoms_z: kDIuAAAmNABgjwsAoLwqAPAIKgBAvQcAoPMlACCHAwA=
atoms_occupancy: 0
atoms_u_iso: gAYBAGAcAQAQIQEAsBcBAADhAADQfgEAIC8BAIBqAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 3.53 GPa

qdat:
AAAAAAAAAAAAIABAIAAIEAAAiEgEASQACAFwgwiAOwRCEAQN4ciUwZJwgGmb4X8rRFvRZr9gyxuv6ulLR9tq2dde77mrce23Xbzfvjf3/9vute9pfv/1zvermf7X/r9/t9v1f75Zu//y/z+Tvf+r9Xb+rdO/0xv/O3/mm9==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 8.827
b: 12.683
c: 6.213
alpha: 90
beta: 106.95
gamma: 90
cell_volume: 665.347
crystal_density: 4.272
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: cIkGABCFGgBACxQA4L4BACDQFADw1QwAYJYOAHCJBgA=
atoms_y: oDT+/+BJCABQywcAgAIKALDx/v8QGv7/EB4OAGCDDQA=
atoms_z: QB4uAOAiNAAguwsAILAqAEDSKQCgrQcAAOQlAHCbAwA=
atoms_occupancy: 0
atoms_u_iso: oCIBAJAtAQAQCAEAYDUBAOAoAQBAGQEA4CgBAMBXAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 3.97 GPa

qdat:
AAAAAAAAAAAAIABAEAAECAAARCQCAJIAAgCoQUQgCsIxDAIDeOIpMGKcIBZStEvJ0Q36KWe4OmPv/lcp6f3lny7XffeU7R+7br2Wu+befflnu17zF+9XeX65vbe+77tnvXu/S777z37vn+v+t+399+9vuP6q50j99etvvn==


formula: As S
compound: Baia Sprie mine, Romania
formula_title: <missing>
a: 8.719
b: 12.634
c: 6.149
alpha: 90
beta: 107.1
gamma: 90
cell_volume: 647.405
crystal_density: 4.391
atoms_sites: ["As1", "As2", "As3", "As4", "S1", "S2", "S3", "S4"]
atoms_x: YGIGAECWGgBwHBQAcKcBANDtFAAw3AwAkMAOALBdBgA=
atoms_y: GCH+/xBCCACQ0QcAkBAKABDJ/v8gD/7/MCEOAACTDQA=
atoms_z: ABguAMAfNADgzQsAAJQqAFCVKQDgFwgAsM8lABCSAwA=
atoms_occupancy: 0
atoms_u_iso: MMAAACDLAADgqwAAUMMAAGDRAAAgywAA8AQBAPC5AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure properties and the molecular nature of
 hydrostatically compressed realgar
 Note: P = 5.40 GPa

qdat:
AAAAAAAAAAAAEAAgEAACBAAAIQkBACSAAQAvCCGIAahMIQAg2a4olgSWxAKsaYp8swpXSSz6g45PfanJR0fTlUnt7t7p9Zn3d83+v7uc1vt+6d5/86rf5/7fXXbO9/v6/9/dP6946Xvt/s38+ser/zPfvPr/4d7xH309v/==


formula: Zr2.5 Ti Ca O8
compound: Rocca Castellaccio, Val Malenco, Sondrio, Italy
pub_title: The crystal structure of orthorhombic calzirtite from Val Malenco (Italy) Note: crystal n.2
formula_title: <missing>
a: 15.207
b: 15.207
c: 10.114
alpha: 90
beta: 90
gamma: 90
cell_volume: 2338.891
crystal_density: 5.044
atoms_sites: ["ZrM1", "TiM2", "CaM3", "ZrM4", "O1", "O2", "O3", "O4", "O5"]
atoms_x: YNEAAHA/CgAQRRQAIOAJAOCQEQAgxyIAANgOACDyBgAAAQQA
atoms_y: oBMQALCBGQBQhyMAYFgQAAAAAAAAAAAA4AEUAMBJFAAAHhQA
atoms_z: IKEHACChBwAgoQcA0AAWAEBCDwBAQg8A0IcMAGDw//+QLh4A
atoms_occupancy: gIQeAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: MKcAAJCXAADQnQAAwHYAAIC7AABAnAAA4KsAACDLAABAnAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAABAAAAEEAABAAABEAAxAAACBgAEhBIQWAZIIICASQghiNEEiQCRCKDGAno6aiByRCDpEadBij5kI+G6MNcMAMPCMcIwxgDQGGIQwBCIYgCEIBgIAiEABAAgIAAACAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Nd C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: <missing>
a: 7.2333
b: 4.9640
c: 8.4908
alpha: 90
beta: 90
gamma: 90
cell_volume: 304.872
crystal_density: 4.820
atoms_sites: ["Nd", "C", "O-H1", "O2", "O3"]
atoms_x: yLMVACCREgDAOAIAgOsRABDNJwA=
atoms_y: QEIPAEBCDwBAQg8AwL3w/7B0/v8=
atoms_z: KKooAGCREwCw1SQAIH4qAJBoJQA=
atoms_occupancy: 0
atoms_u_iso: QHkAAGBtAAAQ1gAAUMMAABCkAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAgAAAAGAAAKgAEAAAFABgCAAUEAwIgBJg8CAQEBxgQBjB4FKuASmC7CNiNUCZsSMQAuZP/Jc4qGMsSO6nrIFps4u29/J9RW7+FuaeW9699Y3uzu/v0/3d579h6VO079f7b7Vd9d3s/6WuTu7Tv71==


formula: Sm C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: <missing>
a: 7.1388
b: 4.9151
c: 8.4717
alpha: 90
beta: 90
gamma: 90
cell_volume: 297.254
crystal_density: 5.081
atoms_sites: ["Sm", "C", "O-H1", "O2", "O3"]
atoms_x: 2N8VABBqEgAQZgIA0P8RAIDkJwA=
atoms_y: QEIPAEBCDwBAQg8AwL3w/3CH/v8=
atoms_z: 4JcoAMCzEwAAAyUAoIoqADBGJQA=
atoms_occupancy: 0
atoms_u_iso: oIcAAMCPAABQ3AAAcN8AAHCtAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAQAAAACAAACIABAAABIAIBAADBASCIAMEPAQBBAMKAgIEGAYywEMoGGFcLHIHHKEUABWprvxcokHqNSn17pgRWcqufLfMfT7z2+5uPk/P21/O9tY//bv/DtV/p/x/ew9z5fX7vnu321fUz/XR1/1==


formula: Eu C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Eu(CO3)OH
a: 7.1002
b: 4.8932
c: 8.4530
alpha: 90
beta: 90
gamma: 90
cell_volume: 293.680
crystal_density: 5.179
atoms_sites: ["Eu", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: oI4IAFAwDABAhToAkGgMAHBDMwCAGTQA
atoms_y: 4BoPAFAFDwCwWQ8AoJEtACCOHwAgMTsA
atoms_z: QCkFAJD7GQCAZDQA4BwDADBeCACw5wgA
atoms_occupancy: 0
atoms_u_iso: YHwAAHB7AADgxAAAAMgAAHCUAADAqAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAABAAABEAAAAABEAEAAABAkIAgAECCgEAgiCEgAGBBgEM0ABKDhApLChBxjBFAAKc5VQOpoptiGZPe5cEayqbiuq7jUaMfW9losnb9WO07t3H97af4vzt8r/E/+HaNvffs2fry7/+Tt+TP7/==


formula: Gd C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Gd(CO3)OH
a: 7.0755
b: 4.8739
c: 8.4471
alpha: 90
beta: 90
gamma: 90
cell_volume: 291.301
crystal_density: 5.342
atoms_sites: ["Gd", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: MIYIAKArDAAggjoAEFwMAMCiMwBwwDMA
atoms_y: gAIPAPD7DgBQUA8AUH0tAIB+HwAQIzsA
atoms_z: CC8FACDkGQDAajQA8BEDAJBnCABg7AgA
atoms_occupancy: 0
atoms_u_iso: iIEAAFCRAAAAyAAAYNEAALCaAABQwwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAABAAABCAAAAAAiACAAAAgSEAQAGBBQCAQhDCQADAgwCEKAAjAwQYVBQhQwgTAAFnUZsDqSKTxDEzdKSFGoqk4iSrM1O3FllVcEpz91iuEZ+4+9U3+JY8vvPVfpg7j9y7uH51K2u3xY3Ts2P==


formula: Tb C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Tb(CO3)OH
a: 7.0256
b: 4.8577
c: 8.4657
alpha: 90
beta: 90
gamma: 90
cell_volume: 288.920
crystal_density: 5.424
atoms_sites: ["Tb", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: AFwIAKBEDACAWToAEEMMALBJMwAw7DMA
atoms_y: QO0OABAYDwCwWQ8AQFYtAIBMHwAgGDsA
atoms_z: AEEFAMDaGQAAozQA8PgCALBqCAAALgkA
atoms_occupancy: 0
atoms_u_iso: CH8AAHB7AAAw2QAA8NIAANCdAABQwwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAABhAAAAAAhADAAAAQJEAIAGATYBAEhBhCACgIUCDcgARQoESKhGGOokFAABzyvMH4hDs0TDE9tRZJle0ey8bz1XO0/vRdIz8/zTPd+7x3eue68ffqfr+/eunTV/f9j//7d73fH73Pfr==


formula: Dy C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Dy(CO3)OH
a: 6.9813
b: 4.8336
c: 8.4449
alpha: 90
beta: 90
gamma: 90
cell_volume: 284.972
crystal_density: 5.583
atoms_sites: ["Dy", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: SFAIAEA7DABgVjoAADUMAOBBMwBg5DMA
atoms_y: GNkOAPAUDwBgXg8AgCotANAuHwCQFjsA
atoms_z: 4EIFAADIGQCwpzQAIPECALBqCADQNQkA
atoms_occupancy: 0
atoms_u_iso: AIcAAKCMAAAgywAAoNcAABCkAAAgywAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAABAAAAwgAAAAAQgAgAAAIEUAEACgNWAQBQQwggBIDFhA9EAISaBojIBhjzJBwAAm8lty7EMKlkw0z+kKqUr0jssyvcW6e9s2GmCvl9i5e+tuPf/5T3xf2pbtz5+2ztL/drPf+/1v08v/d2v==


formula: Y C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Y(CO3)OH
a: 6.9591
b: 4.8141
c: 8.4722
alpha: 90
beta: 90
gamma: 90
cell_volume: 283.834
crystal_density: 3.883
atoms_sites: ["Y", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: sC4IAJBPDACwODoAkB0MAPAEMwAQNDQA
atoms_y: GI4OAPD7DgCAYQ8A8N0sALDgHgAQvzoA
atoms_z: cEQFAMCoGQCA4TQAkL0CAMBfCACwfQkA
atoms_occupancy: 0
atoms_u_iso: 8G4AAGBtAABguAAAMMAAAHCtAADgqwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAAwQAAAAAQQAwAAAECUACAEgGVAIBQRIQQBIBixAsSAIFpA4KkhKdpIQ4AAj9h2syzGXNTQhK62KoBzXD6lNdVF6PL7dNNBv2/497v7e3lvly3/v9b853f/7lM7/++d/33d/Xrm9387==


formula: Ho C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Ho(CO3)OH
a: 6.9583
b: 4.8121
c: 8.4558
alpha: 90
beta: 90
gamma: 90
cell_volume: 283.134
crystal_density: 5.676
atoms_sites: ["Ho", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: ADkIAMBHDABAOjoAQCIMAHARMwCgNTQA
atoms_y: qJQOAIDkDgCQbw8AEOEsAHDaHgDwuzoA
atoms_z: 6EQFAKClGQCQvTQAEMoCADBeCADQgAkA
atoms_occupancy: 0
atoms_u_iso: yIIAAICJAABg0QAAIMsAABCkAACwzAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAABAAAAwQAAAAAQQAwAAAECSACAEgHMgIBQQkQQBIAiQguSAEFVAoLiQpa4kQ4AASvx6eSTGPLawxZ6+GsFrPj7VMvbFeFrvtjNA7tfo/lnL7R3v3Z7/X/te9WurWzkVv/uft7nc+7XlTz8X==


formula: Er C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Er(CO3)OH
a: 6.9386
b: 4.7963
c: 8.4863
alpha: 90
beta: 90
gamma: 90
cell_volume: 282.421
crystal_density: 5.745
atoms_sites: ["Er", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: EBoIAHBlDABAIToAwBUMAIDUMgAAWDQA
atoms_y: 2F8OAGDhDgBQaQ8AsIwsAKCgHgDQbToA
atoms_z: MEgFAHCUGQCw2TQAMJsCAOBJCACQrAkA
atoms_occupancy: 0
atoms_u_iso: qH8AAICJAAAAyAAAAMgAAHCtAABwrQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAAoQAAAAAQQAoAAACCMABAIQHMQEAgJEQIBEAQYg0KAEC0w0GRgmEioJYAAhZQtfwtTjmvQiV+NQ8BuVSukTX0o8j63n4bRbff9dy5nX3Wq46z/1+1fs8/m7ZY+9/333O93r55c1Ovu==


formula: Tm C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Tm(CO3)OH
a: 6.9028
b: 4.7833
c: 8.5086
alpha: 90
beta: 90
gamma: 90
cell_volume: 280.938
crystal_density: 5.815
atoms_sites: ["Tm", "C", "O-H1", "O2", "O3", "O4"]
atoms_x: qPUHAABnDAAgBToAsO4LACCyMgAAcTQA
atoms_y: OFAOAGDhDgCgfQ8AgHssAHBdHgAQWzoA
atoms_z: sE8FAECDGQBADTUA0JECANBUCACQxQkA
atoms_occupancy: 0
atoms_u_iso: oH0AAJCXAABwxgAA0LYAAHCUAABguAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAAoIAAAAAIIAoAAABBEAAgQQFkICAwJCQCBEAMHAlEgECsZJNFgVDhYDGABCU8eUoLnolTRkH37gsg5F2l4KZ9S9G9+c8i6T761dc66e9biddm5/3e0v3v9eU6Pbv5/2w1v738rfP1b==


formula: Tm C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Tm(CO3)OH
a: 9.3951
b: 9.3951
c: 7.7546
alpha: 90
beta: 90
gamma: 90
cell_volume: 684.482
crystal_density: 4.773
atoms_sites: ["Tm", "C", "O-H1", "O2", "O3"]
atoms_x: GO4cAGBPHgBAQg8AwMIdABA7HgA=
atoms_y: 6BogAEBCDwDAUh8AQEIPAKCJJgA=
atoms_z: QEIPAAAOBgCANAoAcBsQAHDr/v8=
atoms_occupancy: 0
atoms_u_iso: UHgAAOB5AACQ4gAAsP4AAHCtAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAABAEAAAAIAAAAgIAAMAAAogAAAAEoAKAANABAAUAkALoEAAMEgEgBAHQsB6EAMgANwIicolghFZwLAkRCXxBciLQCfUmiEwx+EnqXAL5G4lInxW9xwlkpiCSXkrZSUVJySpoWhAVPVqYEYJWAVCFAJVS==


formula: Yb C (O4 H)
compound: Synthetic
pub_title: Crystal chemistry of RE(CO3)OH
formula_title: Yb(CO3)OH
a: 9.3771
b: 9.3771
c: 7.7117
alpha: 90
beta: 90
gamma: 90
cell_volume: 678.090
crystal_density: 4.899
atoms_sites: ["Yb", "C", "O-H1", "O2", "O3"]
atoms_x: WOAcAABfHgBAQg8AILMdANA0HgA=
atoms_y: qCggAEBCDwBwVx8AQEIPANCBJgA=
atoms_z: QEIPALASBgCgNwoAMC4QAJDV/v8=
atoms_occupancy: 0
atoms_u_iso: wF0AAIBwAACQ+wAA8OsAAOCrAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAABAEAAAAIAAAAQEAAKAAAYQAAAACMAGAAJgAgAKAKAFsCAAGBQBQAgDYOArBACQAD4EEssFoIJZYCgRIJH4QPJBUAdOGxBGZfiF3NgB9UuRsC8Su6eD1S4gibZSusF/U8pSsCcECbX4zAjBlwBIIUBnD==


formula: Cr O2 H
compound: synthetic at 4.0 GPa and 600 deg C for 24 hours
formula_title: <missing>
a: 4.8623
b: 4.2972
c: 2.9567
alpha: 90
beta: 90
gamma: 90
cell_volume: 61.778
crystal_density: 4.570
atoms_sites: ["Cr", "O1", "O2", "H"]
atoms_x: AAAAAIA3FgDgtSgAMDIgAA==
atoms_y: AKAPACCgHADgLgAA4OAMAA==
atoms_z: AAAAAAAAAAAAAAAAAAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Pressure-induced hydrogen bond symmetrisation in guyanaite, B-CrOOH:
 evidence from spectroscopy and ab initio simulations
 Sample: Run LT9

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAAAEAgAAAAiEAAAAAAAAAAAAAAggAAAABAASAgACAAAABAhA4AIEAAAAAAQEAgABABAAkAIAEUAoQAgABAEDQIIACAiQiEAKBAAAQABCECIBQI0dQIkIBRBAgoABMSER==


formula: Cr O2 H2
compound: synthetic at 4.0 GPa and 600 deg C for 24 hours
formula_title: <missing>
a: 4.8623
b: 4.2972
c: 2.9567
alpha: 90
beta: 90
gamma: 90
cell_volume: 61.778
crystal_density: 4.624
atoms_sites: ["Cr", "O", "H"]
atoms_x: AAAAACBNFQDAnR8A
atoms_y: AAAAAOBXDgBg6gAA
atoms_z: AAAAAAAAAAAAAAAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Pressure-induced hydrogen bond symmetrisation in guyanaite, B-CrOOH:
 evidence from spectroscopy and ab initio simulations
 Sample: Run LT9

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAEAgAAAAiEAAAIAAAAAABAAAggAAAgBAACQAQCgAAQBAhA4AKEAAgAAAYGBhAAABgQkAIgMUIoQAgwVAECYJKADAiwyUAKhAyBQgACEAIZQJ0dUImIBxFEkhBDOSkR==


formula: Cr O2 H2
compound: synthetic at 4.0 GPa and 600 deg C for 24 hours
formula_title: <missing>
a: 4.8691
b: 4.3184
c: 2.9594
alpha: 90
beta: 90
gamma: 90
cell_volume: 62.226
crystal_density: 4.590
atoms_sites: ["Cr", "O", "H"]
atoms_x: AAAAAKCLFQCw2h8A
atoms_y: AAAAAODUDgBwiAIA
atoms_z: AAAAAAAAAAAAAAAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Pressure-induced hydrogen bond symmetrisation in guyanaite, B-CrOOH:
 evidence from spectroscopy and ab initio simulations
 Sample: Run #630

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAIBgAAAAkIAAAAAAAAAACAABBAAAAgBAAFABAFAACgBCEBoAQIACAAAAwoBIAAAFBEQIIgQpCQgBEgyAwGgQYAMESjEoAsMCoLBAAFoAh0BTSTQqNgHjEESQEVToTT==


formula: As Sb O3
compound: Tsumeb, Namibia
pub_title: Crystal structure and bonding in the new mineral AsSbO3
formula_title: <missing>
a: 4.5757
b: 13.1288
c: 5.4216
alpha: 90
beta: 95.039
gamma: 90
cell_volume: 324.435
crystal_density: 5.009
atoms_sites: ["As", "Sb", "O1", "O2", "O3"]
atoms_x: YBECAMjXHgBArCcAQJgiAPCuBgA=
atoms_y: SNoFAADjCADQygUA4KkRAPCJCAA=
atoms_z: eKAPAOiPMgBwJgoAELI4AJBOOgA=
atoms_occupancy: 0
atoms_u_iso: cK0AAKC+AACgCQEA4CgBAKAJAQA=
atoms_aniso_label: ["As", "Sb", "O1", "O2", "O3"]
atoms_aniso_u11: cK0AAMDBAABAnAAA4KUBAGDqAAA=
atoms_aniso_u22: ILIAACDkAABAlgEAIMsAAECWAQA=
atoms_aniso_u33: MKcAAOiZAAAgywAAAPoAAECcAAA=
atoms_aniso_u12: IAMAAGgBAABw5f//AAAAAAAAAAA=
atoms_aniso_u13: 4Pz//4AlAABQ+///AAAAAOAVAAA=
atoms_aniso_u23: cBcAAHgAAAAgTgAAABkAAIA+AAA=
qdat:
AAAAAAAAAAAAAAAAgAAAAgAgIQAAgABBIQAQAIBMAAgAKEjFCISDkRACiQCQNGDRjgKhiodRJiKrgmrTTU5/oaZUqEDQsNovF4XdVH1XtuFGc8L5paZ9qtOdniLo/P6nl7ysTNZJu5pt+/N3cx+LPj8toM2sxut/fnuT3L==


formula: As2 O3
compound: Jachymov, Erzgebirge, Czech Republic
pub_title: Crystal structure and bonding in the new mineral AsSbO3
formula_title: <missing>
a: 4.5460
b: 13.0012
c: 5.3420
alpha: 90
beta: 94.329
gamma: 90
cell_volume: 314.830
crystal_density: 4.174
atoms_sites: ["As1", "As2", "O1", "O2", "O3"]
atoms_x: cH4CANBNAABgPAQA0JkJAEBsCAA=
atoms_y: EDAGAPBeFQCwTA0AwEoYALCcCAA=
atoms_z: 0MUPAFDCFQCQRhoAcAgoAKBDOgA=
atoms_occupancy: 0
atoms_u_iso: cBEBACAWAQCghgEAYGcBAKCGAQA=
atoms_aniso_label: ["As1", "As2", "O1", "O2", "O3"]
atoms_aniso_u11: kPsAAFD1AAAA9AEAYOoAAAD6AAA=
atoms_aniso_u22: gB8BAOBaAQCAOAEAwNQBAKCAAgA=
atoms_aniso_u33: UA4BAIDtAADAVwEAYGcBAEAZAQA=
atoms_aniso_u12: YAkAAFD7//8AAAAAoA8AAAAAAAA=
atoms_aniso_u13: 4Mr//+D8//8g0f//INH//2Dw//8=
atoms_aniso_u23: 0CAAAEAGAADgsf//YHP//4A+AAA=
qdat:
AAAAAAAAAAAAAAAAQAAAAQAQEEAAQAAQUEAIACAKQAEABgVhIhBQQkgAIiAGB4pKFEB8GJCWFNCUUIipcsejkyksougMNNWO2bDHJSc1sFwmqnKJnPcVqVzi4zbxr/9kthfYYVdpqpPmVP5Ot1TRvOpAtBi28cr1On/HlX==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.595
b: 3.595
c: 3.595
alpha: 90
beta: 90
gamma: 90
cell_volume: 46.462
crystal_density: 7.984
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 6.81 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAABAAAAAAAAAAAAAAAEAAAAAAAAAAgAAIAAAAAAAAAAACAAAAAAAAIAAAAAAAAAAAABA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.583
b: 3.583
c: 3.583
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.998
crystal_density: 8.064
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 8.36 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAEAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAgAAAQAAAAAAAAAAAAAAAgAAAAAAAAAIAACAAAAAAAAAAAAQAAAAAAABAAAAAAAAAAAAAI==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.569
b: 3.569
c: 3.569
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.461
crystal_density: 8.160
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 10.08 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAIAAACAAAAAAAAAAAAAAAIAAAAAAAAABAAAQAAAAAAAAAAACAAAAAAAAEAAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.557
b: 3.557
c: 3.557
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.004
crystal_density: 8.242
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 11.66 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAABAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAgAAAAAAAAAAAAAABAAAAAAAAAAIAACAAAAAAAAAAAAIAAAAAAAAgAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.551
b: 3.551
c: 3.551
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.777
crystal_density: 8.284
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 12.71 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAABAAAAQAAAAAAAAAAAAAAAgAAAAAAAAAEAABAAAAAAAAAAAAEAAAAAAAAIAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.545
b: 3.545
c: 3.545
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.550
crystal_density: 8.326
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 13.63 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAgAAAIAAAAAAAAAAAAAAAQAAAAAAAAABAAAQAAAAAAAAAAACAAAAAAAAEAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.539
b: 3.539
c: 3.539
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.324
crystal_density: 8.369
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 14.45 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAQAAAEAAAAAAAAAAAAAAAIAAAAAAAAAAgAAIAAAAAAAAAAAAgAAAAAAABAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.533
b: 3.533
c: 3.533
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.099
crystal_density: 8.412
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 15.58 GPa, T = 1273 K


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.527
b: 3.527
c: 3.527
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.875
crystal_density: 8.455
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 16.63 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAEAAABAAAAAAAAAAAAAAACAAAAAAAAAAEAABAAAAAAAAAAAAEAAAAAAAAIAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.521
b: 3.521
c: 3.521
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.651
crystal_density: 8.498
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 17.59 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAEAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAACAAAAgAAAAAAAAAAAAAAAgAAAAAAAAACAAAgAAAAAAAAAAACAAAAAAAAEAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.514
b: 3.514
c: 3.514
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.392
crystal_density: 8.549
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 18.69 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAABAAAAIAAAAAAAAAAAAAAAQAAAAAAAAABAAAIAAAAAAAAAAAAgAAAAAAABAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.509
b: 3.509
c: 3.509
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.207
crystal_density: 8.585
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 19.70 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAgAAAIAAAAAAAAAAAAAAAIAAAAAAAAAAgAAEAAAAAAAAAAAAQAAAAAAAAgAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.504
b: 3.504
c: 3.504
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.022
crystal_density: 8.622
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 20.64 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAABAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAQAAAEAAAAAAAAAAAAAAAEAAAAAAAAAAIAACAAAAAAAAAAAAIAAAAAAAAIAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.498
b: 3.498
c: 3.498
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.802
crystal_density: 8.667
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 21.57 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAABAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAIAAACAAAAAAAAAAAAAAACAAAAAAAAAAEAABAAAAAAAAAAAACAAAAAAAACAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.494
b: 3.494
c: 3.494
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.655
crystal_density: 8.696
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 22.44 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAIAAABAAAAAAAAAAAAAAABAAAAAAAAAACAAAgAAAAAAAAAAABAAAAAAAACAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.490
b: 3.490
c: 3.490
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.509
crystal_density: 8.726
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 23.17 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAEAAAAgAAAAAAAAAAAAAAAgAAAAAAAAABAAAQAAAAAAAAAAAAgAAAAAAABAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.485
b: 3.485
c: 3.485
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.326
crystal_density: 8.764
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 24.19 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAACAAAAQAAAAAAAAAAAAAAAQAAAAAAAAAAgAAIAAAAAAAAAAAAIAAAAAAAAQAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.480
b: 3.480
c: 3.480
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.144
crystal_density: 8.802
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 25.01 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAABAAAAQAAAAAAAAAAAAAAAIAAAAAAAAAAQAACAAAAAAAAAAAAIAAAAAAAAIAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.477
b: 3.477
c: 3.477
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.035
crystal_density: 8.825
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 25.72 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAABAAAAIAAAAAAAAAAAAAAAEAAAAAAAAAAQAACAAAAAAAAAAAAEAAAAAAAAEAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.473
b: 3.473
c: 3.473
alpha: 90
beta: 90
gamma: 90
cell_volume: 41.890
crystal_density: 8.855
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 26.55 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAgAAAEAAAAAAAAAAAAAAACAAAAAAAAAAEAABAAAAAAAAAAAACAAAAAAAACAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.468
b: 3.468
c: 3.468
alpha: 90
beta: 90
gamma: 90
cell_volume: 41.710
crystal_density: 8.893
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M605, P = 27.44 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAQAAACAAAAAAAAAAAAAAABAAAAAAAAAACAAAgAAAAAAAAAAABAAAAAAAABAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.595
b: 3.595
c: 3.595
alpha: 90
beta: 90
gamma: 90
cell_volume: 46.462
crystal_density: 7.984
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 6.81 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAABAAAAAAAAAAAAAAAEAAAAAAAAAAgAAIAAAAAAAAAAACAAAAAAAAIAAAAAAAAAAAABA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.583
b: 3.583
c: 3.583
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.998
crystal_density: 8.064
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 8.36 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAEAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAgAAAQAAAAAAAAAAAAAAAgAAAAAAAAAIAACAAAAAAAAAAAAQAAAAAAABAAAAAAAAAAAAAI==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.569
b: 3.569
c: 3.569
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.461
crystal_density: 8.160
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 10.08 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAIAAACAAAAAAAAAAAAAAAIAAAAAAAAABAAAQAAAAAAAAAAACAAAAAAAAEAAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.557
b: 3.557
c: 3.557
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.004
crystal_density: 8.242
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 11.66 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAABAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAgAAAAAAAAAAAAAABAAAAAAAAAAIAACAAAAAAAAAAAAIAAAAAAAAgAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.551
b: 3.551
c: 3.551
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.777
crystal_density: 8.284
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 12.71 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAABAAAAQAAAAAAAAAAAAAAAgAAAAAAAAAEAABAAAAAAAAAAAAEAAAAAAAAIAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.545
b: 3.545
c: 3.545
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.550
crystal_density: 8.326
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 13.63 GPa, T = 1273 K


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.539
b: 3.539
c: 3.539
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.324
crystal_density: 8.369
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 14.45 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAQAAAEAAAAAAAAAAAAAAAIAAAAAAAAAAgAAIAAAAAAAAAAAAgAAAAAAABAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.533
b: 3.533
c: 3.533
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.099
crystal_density: 8.412
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 15.58 GPa, T = 1273 K


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.527
b: 3.527
c: 3.527
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.875
crystal_density: 8.455
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 16.63 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAEAAABAAAAAAAAAAAAAAACAAAAAAAAAAEAABAAAAAAAAAAAAEAAAAAAAAIAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.521
b: 3.521
c: 3.521
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.651
crystal_density: 8.498
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 17.59 GPa, T = 1273 K


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.514
b: 3.514
c: 3.514
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.392
crystal_density: 8.549
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 18.69 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAABAAAAIAAAAAAAAAAAAAAAQAAAAAAAAABAAAIAAAAAAAAAAAAgAAAAAAABAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.509
b: 3.509
c: 3.509
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.207
crystal_density: 8.585
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 19.70 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAgAAAIAAAAAAAAAAAAAAAIAAAAAAAAAAgAAEAAAAAAAAAAAAQAAAAAAAAgAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.504
b: 3.504
c: 3.504
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.022
crystal_density: 8.622
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 20.64 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAABAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAQAAAEAAAAAAAAAAAAAAAEAAAAAAAAAAIAACAAAAAAAAAAAAIAAAAAAAAIAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.498
b: 3.498
c: 3.498
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.802
crystal_density: 8.667
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 21.57 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAABAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAIAAACAAAAAAAAAAAAAAACAAAAAAAAAAEAABAAAAAAAAAAAACAAAAAAAACAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.494
b: 3.494
c: 3.494
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.655
crystal_density: 8.696
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 22.44 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAIAAABAAAAAAAAAAAAAAABAAAAAAAAAACAAAgAAAAAAAAAAABAAAAAAAACAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.490
b: 3.490
c: 3.490
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.509
crystal_density: 8.726
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 23.17 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAEAAAAgAAAAAAAAAAAAAAAgAAAAAAAAABAAAQAAAAAAAAAAAAgAAAAAAABAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.485
b: 3.485
c: 3.485
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.326
crystal_density: 8.764
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 24.19 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAACAAAAQAAAAAAAAAAAAAAAQAAAAAAAAAAgAAIAAAAAAAAAAAAIAAAAAAAAQAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.480
b: 3.480
c: 3.480
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.144
crystal_density: 8.802
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 25.01 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAABAAAAQAAAAAAAAAAAAAAAIAAAAAAAAAAQAACAAAAAAAAAAAAIAAAAAAAAIAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.477
b: 3.477
c: 3.477
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.035
crystal_density: 8.825
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 25.72 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAABAAAAIAAAAAAAAAAAAAAAEAAAAAAAAAAQAACAAAAAAAAAAAAEAAAAAAAAEAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.473
b: 3.473
c: 3.473
alpha: 90
beta: 90
gamma: 90
cell_volume: 41.890
crystal_density: 8.855
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 26.55 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAgAAAEAAAAAAAAAAAAAAACAAAAAAAAAAEAABAAAAAAAAAAAACAAAAAAAACAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.468
b: 3.468
c: 3.468
alpha: 90
beta: 90
gamma: 90
cell_volume: 41.710
crystal_density: 8.893
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M620, P = 27.44 GPa, T = 1273 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAQAAACAAAAAAAAAAAAAAABAAAAAAAAAACAAAgAAAAAAAAAAABAAAAAAAABAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.595
b: 3.595
c: 3.595
alpha: 90
beta: 90
gamma: 90
cell_volume: 46.462
crystal_density: 7.984
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 4.73 GPa, T = 1073 K


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.581
b: 3.581
c: 3.581
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.921
crystal_density: 8.078
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 6.41 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAEAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAgAAAIAAAAAAAAAAAAAAAgAAAAAAAAAEAABAAAAAAAAAAAAQAAAAAAAAgAAAAAAAAAAAAI==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.569
b: 3.569
c: 3.569
alpha: 90
beta: 90
gamma: 90
cell_volume: 45.461
crystal_density: 8.160
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 8.02 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAIAAACAAAAAAAAAAAAAAAIAAAAAAAAABAAAQAAAAAAAAAAACAAAAAAAAEAAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.555
b: 3.555
c: 3.555
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.928
crystal_density: 8.256
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 9.90 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAgAAAAAAAAAAAAAABAAAAAAAAAAIAACAAAAAAAAAAAAIAAAAAAAAQAAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.544
b: 3.544
c: 3.544
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.512
crystal_density: 8.334
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 11.48 GPa, T = 1073 K


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.531
b: 3.531
c: 3.531
alpha: 90
beta: 90
gamma: 90
cell_volume: 44.024
crystal_density: 8.426
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 13.36 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAIAAACAAAAAAAAAAAAAAACAAAAAAAAAAIAACAAAAAAAAAAAAIAAAAAAAAQAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.519
b: 3.519
c: 3.519
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.577
crystal_density: 8.512
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 15.37 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAEAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAACAAAAgAAAAAAAAAAAAAAAgAAAAAAAAACAAAgAAAAAAAAAAABAAAAAAAACAAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.507
b: 3.507
c: 3.507
alpha: 90
beta: 90
gamma: 90
cell_volume: 43.133
crystal_density: 8.600
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 17.47 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAACAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAgAAAEAAAAAAAAAAAAAAAEAAAAAAAAAAQAACAAAAAAAAAAAAQAAAAAAAAQAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.495
b: 3.495
c: 3.495
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.692
crystal_density: 8.689
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 19.82 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAIAAABAAAAAAAAAAAAAAABAAAAAAAAAACAAAgAAAAAAAAAAACAAAAAAAACAAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.484
b: 3.484
c: 3.484
alpha: 90
beta: 90
gamma: 90
cell_volume: 42.290
crystal_density: 8.772
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 22.34 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAQAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAACAAAAQAAAAAAAAAAAAAAAQAAAAAAAAAAgAAIAAAAAAAAAAAAIAAAAAAAAQAAAAAAAAA==


formula: Fe
compound: Synthetic
formula_title: <missing>
a: 3.475
b: 3.475
c: 3.475
alpha: 90
beta: 90
gamma: 90
cell_volume: 41.963
crystal_density: 8.840
atoms_sites: ["Fe"]
atoms_x: AAAAAA==
atoms_y: AAAAAA==
atoms_z: AAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Isothermal compression of face-centered cubic iron
 Note: gamma iron, Sample M622, P = 24.37 GPa, T = 1073 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAIAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAAgAAAIAAAAAAAAAAAAAAAEAAAAAAAAAAIAABAAAAAAAAAAAACAAAAAAAACAAAAAAAAA==


formula: Ba Be2 Si2 O7
compound: Yukspor Mountain, Khibiny Massif, Kola Peninsula, Russia
pub_title: Redetermination of clinobarylite, BaBe2Si2O7 Note: polytype barylite-1O
formula_title: <missing>
a: 11.6491
b: 4.9175
c: 4.6746
alpha: 90
beta: 90
gamma: 90
cell_volume: 267.782
crystal_density: 4.012
atoms_sites: ["Ba", "Be", "Si", "O1", "O2", "O3", "O4"]
atoms_x: gIQeAKDXLQCQWCYAmP8mAHhsLwCAhB4AQJ4mAA==
atoms_y: YGYMAFBVCgBANykAgLoVAMAtCABAYy8AcIYsAA==
atoms_z: kAokAJAuBQBAOQQA8FcIACCC7/+Q8QoAQGzv/w==
atoms_occupancy: 0
atoms_u_iso: oJEAAGBtAAAwUgAAEHIAACBnAABQeAAAIIAAAA==
atoms_aniso_label: ["Ba", "Be", "Si", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: MKwAAEBRAADgRwAAUHgAAHB7AABQRgAAMHUAAA==
atoms_aniso_u22: QIgAAPBuAACgQQAA8FUAALBPAAAggAAAUKoAAA==
atoms_aniso_u33: mIAAAPCHAABgbQAAgIkAALBoAADwoAAAAGQAAA==
atoms_aniso_u12: AAAAAHD+//+I+v//8AoAAIDz//8AAAAAAOf//w==
atoms_aniso_u13: AAAAAMDg//8AAAAAYCIAAPAKAAAAAAAAEPX//w==
atoms_aniso_u23: oAAAAJAaAABw/v//MBEAALAEAACA2v//AAAAAA==
qdat:
AAAAAAAAAAAAAAAAAAgAAIAAQAABAABAQAAigAAAAhEABAQEYiUIBAkSEEgAgJUBIBJnKA0UpIAkGAsUxUkCiQmoWFgI+RVw2BBWvFnoEUWYtwoF8ut1B+Dvy0Hjg3V1nx4uGDLOqwyfd5i+f2bDpbT5XZXnT/+ZUu9fGf==


formula: Al2 Be3 Si6 O18
compound: Synthetic
formula_title: <missing>
a: 9.212
b: 9.212
c: 9.187
alpha: 90
beta: 90
gamma: 120
cell_volume: 675.169
crystal_density: 2.644
atoms_sites: ["Al", "Be", "Si", "O1", "O2"]
atoms_x: q7AoAICEHgCwphcA0PkSAAB4HgA=
atoms_y: VVgUAAAAAADwEgcA8H4OAGDsCAA=
atoms_z: QEIPAEBCDwAAAAAAAAAAAKDZCAA=
atoms_occupancy: 0
atoms_u_iso: YDsAAHA1AACQKQAA6GwAAEhJAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural refinement of hydrous and anhydrous synthetic beryl,
 Al2(Be3Si6)O18 and emerald, Al1.9Cr0.1(Be3Si6)O18
 Note: anhydrous beryl

qdat:
AAAAAAAAAAAAAQAAAAAAAADAAAIAAAAAQADAEAAIAEAAAGAMCABgGAAAAYIAYSAAICCAUWIAgQwEGIBBCAzwAQxgBxAx3DjoCOwbiDGYZxDG4TkAZjugzsT4NWGVC/m9DNgcDfGYE3N8ZInTMnaB8WRli6N5rE2TRvB49n==


formula: Al2 Be3 Si6 O19 H2
compound: Synthetic
formula_title: <missing>
a: 9.213
b: 9.213
c: 9.206
alpha: 90
beta: 90
gamma: 120
cell_volume: 676.712
crystal_density: 2.726
atoms_sites: ["Al", "Be", "Si", "O1", "O2", "Wat"]
atoms_x: q7AoAICEHgAgpRcAUO0SAEB+HgAAAAAA
atoms_y: VVgUAAAAAADwEgcA4HAOACDmCAAAAAAA
atoms_z: QEIPAEBCDwAAAAAAAAAAAODfCABAQg8A
atoms_occupancy: 0
atoms_u_iso: sB0AAFBBAAC4FQAA+FwAAHg3AADougcA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural refinement of hydrous and anhydrous synthetic beryl,
 Al2(Be3Si6)O18 and emerald, Al1.9Cr0.1(Be3Si6)O18
 Note: hydrous beryl

qdat:
AAAAAAAAAAAAAQAAAAAAAADAAAIAAAAAQACAEAAIAEAAAEAICABAEAAAAQIAQUAAICCAQUIBgwgIEIBBCAigAQxABhAhmDCIEIgTiDEQRiCEgjIATCMgiYToJkMSE7E5GJAYG6EQE0JsRIkiJkwBMWRJF0bRMEkXxKBItE==


formula: (Al1.9 Cr.1) Be3 Si6 O18
compound: Synthetic
formula_title: <missing>
a: 9.219
b: 9.219
c: 9.198
alpha: 90
beta: 90
gamma: 120
cell_volume: 677.005
crystal_density: 2.649
atoms_sites: ["Al", "Cr", "Be", "Si", "O1", "O2"]
atoms_x: q7AoAKuwKACAhB4AsKYXAAALEwCQeR4A
atoms_y: VVgUAFVYFAAAAAAAgBQHANB7DgAA4wgA
atoms_z: QEIPAEBCDwBAQg8AAAAAAAAAAACg2QgA
atoms_occupancy: wPs5AEANAwAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: KFUAAChVAAB4LQAAuBUAAChLAABwNQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural refinement of hydrous and anhydrous synthetic beryl,
 Al2(Be3Si6)O18 and emerald, Al1.9Cr0.1(Be3Si6)O18
 Note: anhydrous emerald

qdat:
AAAAAAAAAAAAAQAAAAAAAADAAAYAAAAAQACAEAAIAEAAAEAICABAEAAAAYIAQUAAICCAYcIBgxgIGADBCBjgAgxAChBhmDDQEMwziDGwRyGMw1IAzDdBjYjod0ObE7E6GbA4G6M4I+bsTYuiJm0Bs+jLF0bzVEsnjaBR3P==


formula: (Al1.9 Cr.1) Be3 Si6 O19 H2
compound: Synthetic
formula_title: <missing>
a: 9.214
b: 9.214
c: 9.218
alpha: 90
beta: 90
gamma: 120
cell_volume: 677.741
crystal_density: 2.734
atoms_sites: ["Al", "Cr", "Be", "Si", "O1", "O2", "Wat"]
atoms_x: q7AoAKuwKACAhB4AAKIXACD1EgCQeR4AAAAAAA==
atoms_y: VVgUAFVYFAAAAAAAIAsHAFBvDgAA4wgAAAAAAA==
atoms_z: QEIPAEBCDwBAQg8AAAAAAAAAAAAQ2AgAQEIPAA==
atoms_occupancy: wPs5AEANAwAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: AF8AAABfAACALwAA0BEAAOhiAABoMwAAGPUGAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural refinement of hydrous and anhydrous synthetic beryl,
 Al2(Be3Si6)O18 and emerald, Al1.9Cr0.1(Be3Si6)O18
 Note: hydrous emerald

qdat:
AAAAAAAAAAAAAQAAAAAAAACAAAYAAAAAQACAEAAIAEAAAEAICABAEAAAAQIAQUAAICGAQcIBAggIEICBCBigAghACiBhECCIEIgyiCEQRiGMglIASCYhCQTIRkI2EyEyETAwEyEwIkLoRQsiZEwBIWhLFoShIFkWiaBItE==


formula: Ca3 (Al1.94 Fe.06) Si2.04 O10.8 F1.2 H2.64
compound: silicocarbonatite, Afrikanda Complex, Russia
formula_title: <missing>
a: 12.037
b: 12.037
c: 12.037
alpha: 90
beta: 90
gamma: 90
cell_volume: 1744.033
crystal_density: 3.287
atoms_sites: ["Ca", "AlY", "FeY", "SiZ", "O", "O-H", "F"]
atoms_x: AAAAAAAAAAAAAAAAYOMWAMDOAgDAzgIAwM4CAA==
atoms_y: QEIPAAAAAAAAAAAAAAAAANAcCQDQHAkA0BwJAA==
atoms_z: IKEHAAAAAAAAAAAAQEIPABDP/f8Qz/3/EM/9/w==
atoms_occupancy: AAk9AEA0OwDA1AEAAIEpAACBKQCAbQ0AgBoGAA==
atoms_u_iso: QAABAKDwAACg8AAA4KsAAIA4AQCAOAEAgDgBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Fluorine-rich hibschite from silicocarbonatite, Afrikanda Complex, Russia:
 Crystal chemistry and conditions of crystallization

qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAEABAAABABACAIAACAQAAACAgIAAgIECAgQAAECCCBBBABBABCCEAIQQhCEAIBCEIQCEACEQiEQEQgIAIRIBACIAAkQIgBAABAAAAgAAAAAAABIAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca (Si2 Al2) O8
compound: Synthetic
formula_title: <missing>
a: 5.1175
b: 5.1175
c: 14.7716
alpha: 90
beta: 90
gamma: 120
cell_volume: 335.022
crystal_density: 2.758
atoms_sites: ["Ca", "Si", "Al", "O1", "O2"]
atoms_x: AAAAAFVYFABVWBQAVVgUAOCeFwA=
atoms_y: AAAAAKuwKACrsCgAq7AoAAAAAAA=
atoms_z: AAAAADCQCAAwkAgAQEIPAODxBQA=
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQA=
atoms_u_iso: OE8AAOhiAADoYgAAoJ8BAMCTAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Thermally induced phase transformations of Ca-exchanged LTA and FAU zeolite frameworks:
 Rietveld refinement of the hexagonal CaAl2Si2O8 diphyllosilicate structure

qdat:
AAAAAAAAAAAAAAQAAAAAAAACAAAEIAAAAAAABAAAAkEIAAQICJAAAAQQCAAgAEEkYAgACAhBIBCDIAABABSgEUKBAZBAIAEWAAGCIAIrgQFAMwZFAAoAIEQwAUJkCrhBQEglcIGIQRIAKBETMIUFwVIBiEEiIMkgLABDI8==


formula: Ca Zr2.5 Ti O8
compound: Zelenets mine of the South Ural massif's Kusa titanium-
pub_title: Crystal structure of ordered calzirtite Ca2Zr5Ti2O16 magnetite deposit, Russia
formula_title: <missing>
a: 15.189
b: 15.189
c: 10.111
alpha: 90
beta: 90
gamma: 90
cell_volume: 2332.666
crystal_density: 5.057
atoms_sites: ["Ca", "Zr1", "Zr2", "Ti", "O1", "O2", "O3", "O4", "O5"]
atoms_x: YMIoAOBVHwBwKjMAgEMUALDcDgDg/QMAUHslAEBCDwBAQg8A
atoms_y: YAQFAOBwDgCQKg4AQAEFAPB9CgAwawoAsCwKANBGAgDgBQsA
atoms_z: YOMWAOBnNQBA/xUAYOMWAOANKwDQo///4BUAAICEHgAAAAAA
atoms_occupancy: AAk9AICEHgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: uH4AAOAoAQDgyQAA6GwAAHCUAABYmAAAAL4AAGCaAACYigAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAIAABAAAIEECARABAAkEEpgEAmBiQEhJMSTRZMIIDBTQlhaVFGpcC1KLxaCiqpf2J6rjl/mPsp2150NbCfqdfcSHdxO8m49kL0XuY6tJDNOyLU4E0EQpSAIoCgUAABBgAAAAAQAAAAAAAAAAAAAAAAAAAAAAA==


formula: Pb Cr O4
compound: Dundas, Tasmania
pub_title: Four monazite type structures: comparison of SrCrO4, SrSeO4, PbCrO4 (crocoite), and PbSeO4
formula_title: <missing>
a: 7.127
b: 7.438
c: 6.799
alpha: 90
beta: 102.43
gamma: 90
cell_volume: 351.971
crystal_density: 6.099
atoms_sites: ["Pb", "Cr", "O1", "O2", "O3", "O4"]
atoms_x: 0IENALhFDACgfQ8AUJkHAPDMAQCwjRcA
atoms_y: qOAIAOD8CQCgQQAAkOcUAPAYBgBQEQ0A
atoms_z: 4DkYAMDSNQDggAMAIF08AKDbKQAwuS8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Pb", "Cr", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: gB8BAFCRAABg5AEAoAkBAEAZAQBAnAAA
atoms_aniso_u22: sP4AAMCPAABAGQEAoAkBAIA4AQAgxQEA
atoms_aniso_u33: gO0AAICJAADgKAEAAHcBAMBXAQDgKAEA
atoms_aniso_u12: AOf//xD1///gLgAAoA8AAOCx//9g8P//
atoms_aniso_u13: QFEAADAqAADAXQAAoIwAACDR///AXQAA
atoms_aniso_u23: 0O7//yDq//+APgAAQKL//2Dw///A4P//
qdat:
AAAAAAAAAAAAAAAgAAAACQAAAAABQAQEoQEAAhAEIQIABQIYiIgBDQEiqAcCYRhZmAWtAoAQwGotF5BFqIEOF5tDyGcM3M2jxZTnzdhvY+7Go7auef0Uqy/ap/2r4VXvq77v7rHtz/f3bfv2/fz933e/u/577/+37f/vn3==


formula: Pb Se O4
compound: Synthetic
pub_title: Four monazite type structures: comparison of SrCrO4, SrSeO4, PbCrO4 (crocoite), and PbSeO4
formula_title: PbSeO4
a: 7.154
b: 7.407
c: 6.954
alpha: 90
beta: 103.14
gamma: 90
cell_volume: 358.842
crystal_density: 6.481
atoms_sites: ["Pb", "Se", "O1", "O2", "O3", "O4"]
atoms_x: sC4NALj1CwBQoQ4AwEwHAMCJAQDgOhcA
atoms_y: IB0JAJD8CQAQWQAAQLoUAOC5BgCwtgwA
atoms_z: 2IcYAHjUNQCg/QIAICs8ALDQKQAQGjAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Pb", "Se", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: EFMBADALAQAA7gIAgLUBAEAZAQBAGQEA
atoms_aniso_u22: wD4BACD9AABAGQEAIEgBAOClAQBAEwIA
atoms_aniso_u33: IBYBAKC+AADgKAEAYOQBAMBXAQCAOAEA
atoms_aniso_u12: 8PH//3D+///AXQAAIE4AAIDB///gsf//
atoms_aniso_u13: EEAAAHAXAADAXQAA4KsAACDR///gLgAA
atoms_aniso_u23: cP7//1D7//+APgAAYHP//2Dw//+gkv//
qdat:
AAAAAAAAAAAAAAAgAAAACgAAAAABIAggwQgAAoAFAJAAAwFJGBAAlRIEUAWQQJJFkAVloAAQK2yw1wlToIOpF7dWWg6IvXkF6prmTbjX93VSq7ep9+1Haq7v5X7vumxf/dn+379/j+f3f/0/vt+////86vv7/Xvbd2fs/x==


formula: Sr Cr O4
compound: Synthetic
pub_title: Four monazite type structures: comparison of SrCrO4, SrSeO4, PbCrO4 (crocoite), and PbSeO4
formula_title: SrCrO4
a: 7.065
b: 7.375
c: 6.741
alpha: 90
beta: 103.08
gamma: 90
cell_volume: 342.123
crystal_density: 3.953
atoms_sites: ["Sr", "Cr", "O1", "O2", "O3", "O4"]
atoms_x: iOwNAOgQDACAxQ8AkFQHAACQAQAADBcA
atoms_y: wLMJABgQCgDwVQAAUJYUAEAtBgCwTA0A
atoms_z: sEsYAPghNgAgbgMAgCUAANCbKgAQGjAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Sr", "Cr", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: gLsAAFCqAABgZwEAYOoAAGDqAABg6gAA
atoms_aniso_u22: MMAAANC2AADA2gAAQBkBAGBnAQCghgEA
atoms_aniso_u33: sMwAAODEAABAGQEAQJYBACBIAQDgKAEA
atoms_aniso_u12: cP7//1D7//9AHwAAoA8AAECi///A4P//
atoms_aniso_u13: 4BUAACAcAACAPgAAwF0AAIDB///gLgAA
atoms_aniso_u23: kOj//wAAAAAAAAAAINH//6APAACAwf//
qdat:
AAAAAAAAAAAAAAAQAAAABIAAAAAAYAEBUCAgAEIAhCCAAWAjBRBAIVASHIBgFJEhlYA1tBIATAPkTZlAqxEKaa2bD40qKtqvKTXTP3qc/0VXg9eb97f3Xv23juL2N9Aq/9vfrdPznztv3f3e53tf//7v/N/rh3/3/u/u73==


formula: Sr Se O4
compound: Synthetic
pub_title: Four monazite type structures: comparison of SrCrO4, SrSeO4, PbCrO4 (crocoite), and PbSeO4
formula_title: SrSeO4
a: 7.101
b: 7.340
c: 6.874
alpha: 90
beta: 103.48
gamma: 90
cell_volume: 348.412
crystal_density: 4.396
atoms_sites: ["Sr", "Se", "O1", "O2", "O3", "O4"]
atoms_x: UHoNAKDRCwBAKQ8AIAsHAAAsAQCA5hYA
atoms_y: iKAJALATCgBAUQAAcJkUAGCtBgDwOQ0A
atoms_z: oFYYAOARNgCAXgMAwAI9APBTKgAADDAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Sr", "Se", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: 4MQAAHCtAADgpQEAoAkBAKAJAQDA2gAA
atoms_aniso_u22: EKQAAFCRAACAuwAAwNoAACBIAQAAdwEA
atoms_aniso_u33: 0M8AAOCrAAAA+gAAYGcBAAD6AACgCQEA
atoms_aniso_u12: 4Pz//1D7//9AHwAAoA8AAECi//8g0f//
atoms_aniso_u13: sB0AALAdAADgLgAAwF0AAMDg//8gTgAA
atoms_aniso_u23: YPD//wAAAADgLgAAQKL//wAAAABg8P//
qdat:
AAAAAAAAAAAAAAAQAAAABQAAAAAAUAIIMEEAAFABECIAAMBKIQEAEqEgSwBxCguUKQArVIAAhk1rB2iDWgQMrLRomqR0Yvr6Brezvxb56t11Q1qvfO86j/5O3773u+WzPe/d3vyb/1r1/K//+/7/uzv/57897/rX/ntvu7==


formula: Fe4 O5
compound: synthetic, P = 11.5 GPa, T = 1366 K
formula_title: Fe4O5
a: 2.87366
b: 9.6940
c: 12.4116
alpha: 90
beta: 90
gamma: 90
cell_volume: 345.753
crystal_density: 5.828
atoms_sites: ["Fe1", "Fe2", "Fe3", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_y: AAAAADD8DwDw/x4AIBIKABDVFQAQuAUA
atoms_z: AAAAAIAtBwBAQg8AQEIPAFB6IQAAWycA
atoms_occupancy: 0
atoms_u_iso: wNQBAFDvAQAAcQIA4CgBAIAyAgBAlgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 In situ observation of the breakdown of magnetite (Fe3O4) to Fe4O5 and hematite
 at high pressures and temperatures

qdat:
AAAAAAAAAAAAAAAABAAAACAQAAAIAAAAAJAAAAgggCAQgCIIBEjCAABgBAAIIABIFaEsAC5AB4BAkPAgYAUYrSJaqA0YFFjAYFipxCCZSQdGobQ0h9pthCiuDkwTGAEMLgKKmyiMQwENAhQSAGOKMWRQw4ZTAFCFKkQwBh==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.9530
b: 4.9530
c: 13.5884
alpha: 90
beta: 90
gamma: 120
cell_volume: 288.693
crystal_density: 5.245
atoms_sites: ["Cr", "O"]
atoms_x: AAAAACCqEgA=
atoms_y: AAAAAAAAAAA=
atoms_z: sDUVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 0 GPa, data from Ovsyannikov and Dubrovinsky (2011)

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAIAAIAAAQAQAAQAAAAACAAAACAAgIAAAAEAQAQAACABQAAUACCIIAQAIAAYABACAIIAACEAIBBAQIEAgAIAgAgIBBAAkgKBABgTAAIgIAQMAUACYICEKQAQAgIJAAgCA==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.8949
b: 4.8949
c: 13.432
alpha: 90
beta: 90
gamma: 120
cell_volume: 278.714
crystal_density: 5.433
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAIDMEgA=
atoms_y: AAAAAAAAAAA=
atoms_z: kDIVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: cDAAABBAAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 8.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAABAABAAABABAABAAAAAAEAAAAIABAwAAAAIAQAQAAEABQAAUACCIMAIAIAAUAAgBACEAAAjACAQQECBAIACAEAMBAIIAEiAwIAGBIAAiAgBAQBQAEgQEIUgAgBAQTAAg==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.8645
b: 4.8645
c: 13.355
alpha: 90
beta: 90
gamma: 120
cell_volume: 273.685
crystal_density: 5.533
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAODVEgA=
atoms_y: AAAAAAAAAAA=
atoms_z: ADEVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: YFQAAJBlAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 14.0 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAgAAgAAAgAgAAQAAAAABAAAABAAQGAAAABAEAEAAAgASAACQAQIhgBAAgABQACAIAQgAACMAIBAgQIEAgAEAQAYCAQQAJECgIAUCYAAkBACAwBQAEgQEQYgAQBAQTAA==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.8273
b: 4.8273
c: 13.264
alpha: 90
beta: 90
gamma: 120
cell_volume: 267.679
crystal_density: 5.657
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAJDzEgA=
atoms_y: AAAAAAAAAAA=
atoms_z: 4C0VAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: oHMAAFCRAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 20.4 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAIAAIAAAIAEAAEAAAAAAQAAAAQACAwAAAAEAQAQAACABIAAJABAiGAEACAAFAAEAgAhAAAEYAQCBAgQEAgAIAQAQEAQQAJEBgQAMCYAAiAgBAoAoACQICIEQAIAQIEg==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.8152
b: 4.8152
c: 13.242
alpha: 90
beta: 90
gamma: 120
cell_volume: 265.897
crystal_density: 5.695
atoms_sites: ["Cr", "O"]
atoms_x: AAAAACD1EgA=
atoms_y: AAAAAAAAAAA=
atoms_z: UCwVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0GsAAAB9AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 24.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAIAAEAAAEAEAACAAAAAAIAAAAIAAgYAAAAEAIAIAABAAoAAEgAgRCgCABAABQACAIAIQAABGAIAgQIECAQACAEAEBAEEACRAoCADATAAIgIAQGAKAAkCAhBiACAEBBI==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.785
b: 4.785
c: 13.162
alpha: 90
beta: 90
gamma: 120
cell_volume: 260.985
crystal_density: 5.802
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAKAaEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: oCcVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0IQAAIC7AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 29.6 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAACAABAAACABAAAgAAAAACAAAABAAIGAAAAAgBABAAAQAEgAAkAEBEMAIAEAAKAAIBAAhAAAIYAQCBAQQEAgAEAIAYCAIIAEiAwEAGBEAAJAQAgKAMABECAhCiACAEBB==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.756
b: 4.756
c: 13.109
alpha: 90
beta: 90
gamma: 120
cell_volume: 256.793
crystal_density: 5.897
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAPAuEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: 8CIVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: EIsAAOCrAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 35.4 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAABAAAgAABAAQAAIAAAAAAgAAAAQACCQAAAAEAIAIAACABIAAEQAQIhgCAAgAAoAAgEAEIAAASgCAIEBAgQCAAQAgAwIAgQARIDAIAMBMAASAQAgYASABMEAiBEAEAEB==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.737
b: 4.737
c: 13.071
alpha: 90
beta: 90
gamma: 120
cell_volume: 254.007
crystal_density: 5.962
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAIAwEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: 0B8VAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: QJwAACDLAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 39.7 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAgAAQAAAgAIAAEAAAAAAIAAAAIAAgoAAAACAEAEAAAgAUAABIAECIUAgAEAAKAAIBAAiAAACUAQBAgQIEAgACAEAKBAECABIgYBABQJgACQCAEDACQAFQgCIMQAQAQ==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.714
b: 4.714
c: 13.029
alpha: 90
beta: 90
gamma: 120
cell_volume: 250.738
crystal_density: 6.039
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAKAzEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: IBsVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: oIwAAFCqAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 44.8 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAQAAEAAAQAEAABAAAAAAEAAAAEAAISAAAAAgAgBAAAQAJAAARABAhFAIABAABQABAQAEIAAASgEAIEBAgQEAAQAgAwIAQIAIiBgEAFAWAAJAIAQKAFAATCAQQogAgB==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.690
b: 4.690
c: 12.972
alpha: 90
beta: 90
gamma: 120
cell_volume: 247.106
crystal_density: 6.128
atoms_sites: ["Cr", "O"]
atoms_x: AAAAABBLEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: cBYVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: EKQAAODdAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 50.2 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAIAACAAAEABAAAgAAAAABAAAABAACEQAAAAEAIAQAACABIAACIAIEIoBAAEAAKAAICAAhAAACUAQAgQICCAQABACACggBAgASIKAQAMCYAASAQBAoAKAAmEAQgxACA==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.674
b: 4.674
c: 12.941
alpha: 90
beta: 90
gamma: 120
cell_volume: 244.836
crystal_density: 6.185
atoms_sites: ["Cr", "O"]
atoms_x: AAAAAJBXEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: wBEVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: kJcAAFDDAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 55.1 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAEAABAAAEAAgAAQAAAAAAgAAAAgAAiIAAAACACAEAABAAkAABCAEBCSAgABAACgABAgAIQAAAUgEAIEBAggEAAQAQAoIAIIACRBQCACgKgACQCAEDABQAEwgCCGIAQ==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.629
b: 4.629
c: 12.880
alpha: 90
beta: 90
gamma: 120
cell_volume: 239.013
crystal_density: 6.336
atoms_sites: ["Cr", "O"]
atoms_x: AAAAANCPEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: 8AkVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0LYAAAD6AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 63.9 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAACAAAQAABAAIAACAAAAAAEAAAAEAACQgAAAAIAIAQAAIAIgAAEEAICEECAACAADAACCAAEgAAAUgIAECBAQQIAAIAIASEACCABIQoAgAYCoAAUAgCBQARAAZIAQQwg==


formula: Cr2 O3
compound: Synthetic
formula_title: <missing>
a: 4.605
b: 4.605
c: 12.854
alpha: 90
beta: 90
gamma: 120
cell_volume: 236.063
crystal_density: 6.415
atoms_sites: ["Cr", "O"]
atoms_x: AAAAADCyEwA=
atoms_y: AAAAAAAAAAA=
atoms_z: kAAVAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: sLMAAGDqAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 70.4 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAABAAAEAABAACAAAgAAAAABAAAABAAAwIAAAABABAEAACACIAABAgCAQwQgAAQAAoAAIQAAkAAABCBAAgIEBCAgABABACIgAIEACRFACABgGQACQBAEEgBEABkgAghh==


formula: Ba Ti Si3 O9
compound: San Benito, California, USA
formula_title: <missing>
a: 6.6430
b: 6.6430
c: 9.7660
alpha: 90
beta: 90
gamma: 120
cell_volume: 373.229
crystal_density: 3.679
atoms_sites: ["Ba", "Ti", "Si", "O1", "O2"]
atoms_x: q7AoAFVYFACQTQQAoGAxAOBCBQA=
atoms_y: VVgUAKuwKAAQti8AoHgtACAmKAA=
atoms_z: AAAAAAAAAABAQg8AQEIPANCpFwA=
atoms_occupancy: 0
atoms_u_iso: oHMAAAAyAADgFQAAgCUAAPA8AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Second-order P6c2-P31c transition and structural crystallography of
 the cyclosilicate benitoite, BaTiSi3O9, at high pressure
 Note: P = 0.0001 GPa

qdat:
AAAAAAAAAAAAAAAAAAQAAEAAAAAAQAAEAIAAIAQAAAJAAgEAQIAACQCAQBCAAAQgsCHAAkBChRABQAIIoESIdDQCAYQogVCRIwqSiPQFAMMRjQyNVSaLDMSLpMQiIiVPgyTWC6EVYpYgy1Wi0mT1k4GTkmQlzi7xZpxZM0==


formula: Ba Ti Si3 O9
compound: San Benito, California, USA
formula_title: <missing>
a: 6.6094
b: 6.6094
c: 9.7239
alpha: 90
beta: 90
gamma: 120
cell_volume: 367.871
crystal_density: 3.733
atoms_sites: ["Ba", "Ti", "Si", "O1", "O2"]
atoms_x: q7AoAFVYFACwUAQAQHAxAFBBBQA=
atoms_y: VVgUAKuwKABQvC8AQIgtADACKAA=
atoms_z: AAAAAAAAAABAQg8AQEIPAGCrFwA=
atoms_occupancy: 0
atoms_u_iso: QAABACCyAADgkgAAQJwAAGC4AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Second-order P6c2-P31c transition and structural crystallography of
 the cyclosilicate benitoite, BaTiSi3O9, at high pressure
 Note: P = 1.12 GPa

qdat:
AAAAAAAAAAAAAAAAAAIAAEAAAAAAIAACAEAACAIAAAEgAQBAIEAAAkBAEAQgAAEILAhwAJAQoUIAKABBGBCRFQyAQFGFICoiROFSYR6AYBhiMRDJxqJxIJSI3JSCQmLc+DRVYHoRNhVlDLNeHUPHdTQMmJZBTlF3kyTyyZ==


formula: Ba Ti Si3 O9
compound: San Benito, California, USA
formula_title: <missing>
a: 6.6031
b: 6.6031
c: 9.710
alpha: 90
beta: 90
gamma: 120
cell_volume: 366.645
crystal_density: 3.745
atoms_sites: ["Ba", "Ti", "Si", "O1", "O2"]
atoms_x: q7AoAFVYFACgQgQAoGAxALBKBQA=
atoms_y: VVgUAKuwKABgsS8A4JctAIAWKAA=
atoms_z: AAAAAAAAAABAQg8AQEIPABCwFwA=
atoms_occupancy: 0
atoms_u_iso: oIwAAIA+AABgIgAAQB8AAHBJAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Second-order P6c2-P31c transition and structural crystallography of
 the cyclosilicate benitoite, BaTiSi3O9, at high pressure
 Note: P = 2.14 GPa

qdat:
AAAAAAAAAAAAAAAAAAIAAEAAAAAAIAACAEAACAIAAAEQAIBAECAAAkAgEAIgAAEELAgoAFAQkUIAKABBFBCIjwaAQDDEkCoRJGCqMQ+AUAgxGJDJ1VJYsMxEtkxBITFOfBoq0D0ImxKihFk3DqGjlpoEjJEgl2izxnR55N==


formula: Ba Ti Si3 O9
compound: San Benito, California, USA
formula_title: <missing>
a: 6.5689
b: 6.5689
c: 9.6804
alpha: 90
beta: 90
gamma: 120
cell_volume: 361.751
crystal_density: 3.796
atoms_sites: ["Ba", "Ti", "Si", "O1", "O2"]
atoms_x: q7AoAFVYFABwMQQAAFExALAxBQA=
atoms_y: VVgUAKuwKAAwoC8AYFktANDfJwA=
atoms_z: AAAAAAAAAABAQg8AQEIPACClFwA=
atoms_occupancy: 0
atoms_u_iso: 8IcAAIAlAABwFwAAQB8AAHAwAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Second-order P6c2-P31c transition and structural crystallography of
 the cyclosilicate benitoite, BaTiSi3O9, at high pressure
 Note: P = 3.56 GPa

qdat:
AAAAAAAAAAAAAAAAAAIAACAAAAAAIAABACAABAEAAACIAEAgCBAAAKAQBAEIAABBDQIMABQEJDCABgAQQwQiI6EQEAowpAlCKIwpSiGwBgEERjIInKonChiEjcjIIiZs5sLErQWQmTEmKMmbYEULN2SgZOUxBLWJtk2Sky==


formula: Ba Ti Si3 O9
compound: San Benito, California, USA
formula_title: <missing>
a: 6.5605
b: 6.5605
c: 9.6574
alpha: 90
beta: 90
gamma: 120
cell_volume: 359.969
crystal_density: 3.815
atoms_sites: ["Ba", "Ti", "Si", "O1", "O2"]
atoms_x: q7AoAFVYFAAAMwQAgI8xAGBPBQA=
atoms_y: VVgUAKuwKADgpC8AoHgtACDbJwA=
atoms_z: AAAAAAAAAABAQg8AQEIPANCpFwA=
atoms_occupancy: 0
atoms_u_iso: cHsAAEAfAABABgAAoA8AAEAfAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Second-order P6c2-P31c transition and structural crystallography of
 the cyclosilicate benitoite, BaTiSi3O9, at high pressure
 Note: P = 4.01 GPa

qdat:
AAAAAAAAAAAAAAAAAAEAACAAAAAAEAAAgCAABACAAABIAEAQBAgAAJAIAgCIAAAhBoEOAAwCFChABQAIIoIREeCQCAUYUgKhIkYUpRDYBQDCEYmKTlUTiYRCReRkERESY2FRUoLIjViVlDKs+HKNHbJIGjNMglmi7yZJ5Z==


formula: Ba Ti Si3 O9
compound: San Benito, California, USA
formula_title: <missing>
a: 6.5518
b: 6.5518
c: 9.6503
alpha: 90
beta: 90
gamma: 120
cell_volume: 358.751
crystal_density: 3.828
atoms_sites: ["Ba", "Ti", "Si", "O1", "O2"]
atoms_x: q7AoAFVYFABwMQQA4H8xAMA/BQA=
atoms_y: VVgUAKuwKADQry8AoHgtACDbJwA=
atoms_z: AAAAAAAAAABAQg8AQEIPAKCxFwA=
atoms_occupancy: 0
atoms_u_iso: YIYAAEAfAAAgHAAAoA8AAKAPAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Second-order P6c2-P31c transition and structural crystallography of
 the cyclosilicate benitoite, BaTiSi3O9, at high pressure
 Note: P = 4.28 GPa

qdat:
AAAAAAAAAAAAAAAAAAEAACAAAAAAEAAAgBAABACAAABIACAQBAgAAFAIAgCEAAAghYEGAAoCEhRAAoAEEYEJEPBICAKIMQJhEicKkoisAoDBEYSGRyqRTIYhI3IyCImJMbCwqyFkJqwqxhlWfBlDz1kkCJkmQS7Rc4tU02==


formula: Cu4 (As.54 V.46) O6 Cl
compound: Tolbachik volcano, Kamchatka, Russia
formula_title: <missing>
a: 5.440
b: 11.154
c: 10.333
alpha: 90
beta: 90
gamma: 90
cell_volume: 626.983
crystal_density: 4.762
atoms_sites: ["Cu1", "Cu2", "Cu3", "As", "V", "O1", "O2", "O3", "Cl"]
atoms_x: sKEcAHDeFQAAgRAAMAELADABCwCgZxsA4CEXAOA9PADwEgcA
atoms_y: cGEVAJAzGQDAkSEAQEIPAEBCDwCAXyAA8O8QAEBOJgAguyQA
atoms_z: wMYtAEBCDwAgBSEAgIQeAICEHgDQLBcAoNAWAFBmHADAxi0A
atoms_occupancy: AAk9AAAJPQAACT0AgPUgAIATHAAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: oFoAAHBiAACAcAAAcEkAAHBJAAAgTgAAAH0AAKCMAAAA+gAA
atoms_aniso_label: ["Cu1", "Cu2", "Cu3", "As", "V", "O1", "O2", "O3", "Cl"]
atoms_aniso_u11: 4KsAAOCrAAAggAAAwF0AAMBdAAAAfQAAwNoAAOCrAABAnAAA
atoms_aniso_u22: gAwAAEAfAABAagAA0CAAANAgAABAHwAAIE4AAMBdAACAtQEA
atoms_aniso_u33: wF0AAOBgAAAgZwAAEFkAABBZAAAgTgAAIE4AAECcAACAuwAA
atoms_aniso_u12: UOL//1Di///wIwAAAAAAAAAAAABg8P//gD4AACBOAAAgTgAA
atoms_aniso_u13: AAAAAAAAAADQBwAAAAAAAAAAAADA4P//AAAAAGDw//8AAAAA
atoms_aniso_u23: AAAAAAAAAAAgAwAAYAkAAGAJAABAHwAA4C4AAIA+AAAAAAAA
pub_title:
 Crystal chemistry of inorganic compounds based on chains of oxocentered
 tetrahedra II. Crystal structure of Cu4O2[(As,V)O4]Cl

qdat:
AAAAAAAAAAAAAAAAAABIIMACAABCiEAAACQGAUFCGgTMnDBKLAiDkhipOeE9LVDTsgtJV6EXip65x9bf65nZN+700r/Pnfr7/O/F/9r/97/W51+/+d/9vu/7lv/fu/d+v3//7rvv/X63X5+f+T6N7zONurtuVt/dL/879X==


formula: Na4 Ca4 Si6 O18
compound: Mt. Shaheru, Zaire
formula_title: <missing>
a: 10.429
b: 10.429
c: 13.149
alpha: 90
beta: 90
gamma: 120
cell_volume: 1238.536
crystal_density: 2.851
atoms_sites: ["Na1", "Na2", "Ca1", "Ca2", "Si", "O1", "O2", "O3"]
atoms_x: gIQeAAAAAACAhB4AAAAAAKDRMwDAZw8AMHQuACAENgA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAECaKgAAAAAAYN8fAED/LgA=
atoms_z: AAAAAIBIDwCAhB4AAAAAAGCZGgCAhB4AYC8bAMDlEwA=
atoms_occupancy: AAk9AICEHgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: oJ8BAGicAADQjQEA4GoAAMjXAACotAIAYBYCAADbAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Die Kristallstrukturen von naturlichem Na2Ca2Si3O9
 vom Mt.Shaheru (Zaire) und aus dem Mayener Feld (Eifel)
 Note: this is the high-temperature form of combeite

qdat:
AAAAAAAAAAAAAAgAAAACQAABEAAAQAASABFAAAAIQEUASAShAgIREwAAQiMSYREKLgUBASKmsUIJVKBCMsXhoZRUEVnA0WYwwAlbdJM6oQ5jSgXTESNcW1mEU67pUYDqSq5yJp3QLmIUaKuIroyDUBBGEmxDSBUgCLsaQJ==


formula: Hg I2
compound: synthetic, Fluka 83379
formula_title: <missing>
a: 4.358
b: 4.358
c: 12.300
alpha: 90
beta: 90
gamma: 90
cell_volume: 233.604
crystal_density: 6.460
atoms_sites: ["Hg", "I"]
atoms_x: QEIPAEBCDwA=
atoms_y: wMYtAEBCDwA=
atoms_z: QEIPADDlFwA=
atoms_occupancy: 0
atoms_u_iso: UBQAADARAAA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: UBQAAIAlAAA=
atoms_aniso_u22: UBQAAJABAAA=
atoms_aniso_u33: MBEAAIAMAAA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 Neutron diffraction investigation of the temperature dependence of
 crystal structure and thermal motions of red HgI2
 Note: T = 10 K, powder neutron data

qdat:
AAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAgAAgAAAAAABAAAAAAAAAwAwAAAAAgAAAAAAIAwAAAAAAAAAAQDAAAAgAAAAEBgAABAAAABAgAAAAAAAQIAAAAAAAgwAAQAAAQQAAQAAAhgACAAAEIAAAAA==


formula: Hg I2
compound: synthetic, Fluka 83379
formula_title: <missing>
a: 4.358
b: 4.358
c: 12.306
alpha: 90
beta: 90
gamma: 90
cell_volume: 233.718
crystal_density: 6.457
atoms_sites: ["Hg", "I"]
atoms_x: QEIPAEBCDwA=
atoms_y: wMYtAEBCDwA=
atoms_z: QEIPAKDjFwA=
atoms_occupancy: 0
atoms_u_iso: sDYAADAqAAA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: QDgAAABLAAA=
atoms_aniso_u22: QDgAABAOAAA=
atoms_aniso_u33: ADIAABAnAAA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 Neutron diffraction investigation of the temperature dependence of
 crystal structure and thermal motions of red HgI2
 Note: T = 30 K, powder neutron data

qdat:
AAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAgAAgAAAAAABAAAAAAAAAwAwAAAAAgAAAAAAIAwAAAAAAAAAAQCAAAAgAAAAEBgAACAAAABAgAAAAAAAQIAAAAAAAgwAAQAAAQQAAQAAAhgACAAAEIAAAAA==


formula: Hg I2
compound: synthetic, Fluka 83379
formula_title: <missing>
a: 4.359
b: 4.359
c: 12.319
alpha: 90
beta: 90
gamma: 90
cell_volume: 234.072
crystal_density: 6.447
atoms_sites: ["Hg", "I"]
atoms_x: QEIPAEBCDwA=
atoms_y: wMYtAEBCDwA=
atoms_z: QEIPAIDgFwA=
atoms_occupancy: 0
atoms_u_iso: 8G4AABBZAAA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: 8G4AAICJAAA=
atoms_aniso_u22: 8G4AAIA+AAA=
atoms_aniso_u33: 8G4AADBDAAA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 Neutron diffraction investigation of the temperature dependence of
 crystal structure and thermal motions of red HgI2
 Note: T = 60 K, powder neutron data

qdat:
AAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAgAAgAAAAAABAAAAAAAAAgAgAAAAAgAAAAAAIAgAAAAAAAAAAQCAAAAgAAAAEBAAACAAAACAgAAAAAAAQIAAAAAAAggAAQAAAQQAAgAAAhAACAAAIIAAAAA==


formula: Hg I2
compound: synthetic, Fluka 83379
formula_title: <missing>
a: 4.360
b: 4.360
c: 12.337
alpha: 90
beta: 90
gamma: 90
cell_volume: 234.521
crystal_density: 6.435
atoms_sites: ["Hg", "I"]
atoms_x: QEIPAEBCDwA=
atoms_y: wMYtAEBCDwA=
atoms_z: QEIPANDbFwA=
atoms_occupancy: 0
atoms_u_iso: oL4AAPCgAAA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: wMEAAFD1AAA=
atoms_aniso_u22: wMEAAOB5AAA=
atoms_aniso_u33: gLsAAKBzAAA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 Neutron diffraction investigation of the temperature dependence of
 crystal structure and thermal motions of red HgI2
 Note: T = 100 K, powder neutron data

qdat:
AAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAgAAgAAAAAABAAAAAAAABAAgAAAAAgAAAAAAQBAAAAAAAAAAAwGAAABAAAAAECAAACAAAACBAAAAAAAAgQAAAAAABBgAAQAAAQgAAgAAAhAACAAAQQAAAAA==


formula: Hg I2
compound: synthetic, Fluka 83379
formula_title: <missing>
a: 4.365
b: 4.365
c: 12.389
alpha: 90
beta: 90
gamma: 90
cell_volume: 236.050
crystal_density: 6.393
atoms_sites: ["Hg", "I"]
atoms_x: QEIPAEBCDwA=
atoms_y: wMYtAEBCDwA=
atoms_z: QEIPAADUFwA=
atoms_occupancy: 0
atoms_u_iso: AKkBAMBXAQA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: QK8BAEATAgA=
atoms_aniso_u22: QK8BAGDqAAA=
atoms_aniso_u33: gJwBAAD6AAA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 Neutron diffraction investigation of the temperature dependence of
 crystal structure and thermal motions of red HgI2
 Note: T = 200 K, powder neutron data

qdat:
AAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAgADAAAAAAACAAAAAAAADABgAAAABAAAAAAAgGAAAAAAAAAABgUAAABAAAAAIOAAAEAAAAICAAAAAAABBAAAAAAACCAABAAABAgABAAAGCAAEAAAhgAAAAA==


formula: Hg I2
compound: synthetic, Fluka 83379
formula_title: <missing>
a: 4.370
b: 4.370
c: 12.437
alpha: 90
beta: 90
gamma: 90
cell_volume: 237.508
crystal_density: 6.354
atoms_sites: ["Hg", "I"]
atoms_x: QEIPAEBCDwA=
atoms_y: wMYtAEBCDwA=
atoms_z: QEIPAKDKFwA=
atoms_occupancy: 0
atoms_u_iso: 4J8CAKADAgA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: QJACAIAsAwA=
atoms_aniso_u22: QJACAMBXAQA=
atoms_aniso_u33: QJACAECWAQA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 Neutron diffraction investigation of the temperature dependence of
 crystal structure and thermal motions of red HgI2
 Note: T = 293 K, powder neutron data

qdat:
AAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAACAAAAAAAAAAAAABAAFAAAAAAAEAAAAAAAAJADAAAAACAAAAAACAUAAAAAAAAAAFBIAAACAAAAAQsAAAIAAAAQEAAAAAAAECAAAAAAAEKAACAAACDAACAAAEMAAQAACDAAAAAB==


formula: Hg I2
compound: synthetic, Fluka 83379
formula_title: <missing>
a: 4.3675
b: 4.3675
c: 12.470
alpha: 90
beta: 90
gamma: 90
cell_volume: 237.866
crystal_density: 6.344
atoms_sites: ["Hg", "I"]
atoms_x: QEIPAEBCDwA=
atoms_y: wMYtAEBCDwA=
atoms_z: QEIPACC+FwA=
atoms_occupancy: 0
atoms_u_iso: IDwDAOCfAgA=
atoms_aniso_label: ["Hg", "I"]
atoms_aniso_u11: QA0DAKB6AwA=
atoms_aniso_u22: QA0DAGDkAQA=
atoms_aniso_u33: 4JkDAECQAgA=
atoms_aniso_u12: AAAAAAAAAAA=
atoms_aniso_u13: AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAA=
pub_title:
 Neutron diffraction investigation of the temperature dependence of
 crystal structure and thermal motions of red HgI2
 Note: T = 293 K, single crystal X-ray data

qdat:
AAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAACAAAAAAAAAAAAAAgAJAAAAAAAEAAAAAAAARAFAAAAACAAAAAAEAkAAAAAAAAAAFCIAAACAAAAAQsAAAIAAAAQEAAAAAAAEEAAAAAAACSAACAAABDAABAAAKGAAIAACFAAAAAB==


formula: Cu.01 (Mg.99 Al2.01) O4
compound: Synthetic
formula_title: <missing>
a: 8.0853
b: 8.0853
c: 8.0853
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.553
crystal_density: 3.592
atoms_sites: ["CuT", "MgT", "AlT", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgDA/Q8A
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgDA/Q8A
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgDA/Q8A
atoms_occupancy: QJwAAMDGLQBAQg8AAFMHAAC2NQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "MgM", "AlM", "O"]
atoms_aniso_u11: UEYAAFBGAABQRgAA4EcAAOBHAADgeQAA
atoms_aniso_u22: UEYAAFBGAABQRgAA4EcAAOBHAADgeQAA
atoms_aniso_u33: UEYAAFBGAABQRgAA4EcAAOBHAADgeQAA
atoms_aniso_u12: AAAAAAAAAAAAAAAA0P3//9D9//9wAwAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA0P3//9D9//9wAwAA
atoms_aniso_u23: AAAAAAAAAAAAAAAA0P3//9D9//9wAwAA
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl05b

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAAAgAAACAAEAAAAgAEAAACAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAQAAgCAAEAgACAQAAAI==


formula: (Cu.06 Mg.94 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0858
b: 8.0858
c: 8.0858
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.651
crystal_density: 3.634
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AAP8PAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AAP8PAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AAP8PAA==
atoms_occupancy: wNQBAECOLAAApg4AYOoAAKBoBgAAtjUAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_aniso_u11: MEMAADBDAAAwQwAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u22: MEMAADBDAAAwQwAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u33: MEMAADBDAAAwQwAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAASP7//0j+//9I/v//kAEAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAASP7//0j+//9I/v//kAEAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAASP7//0j+//9I/v//kAEAAA==
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl15a2

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAABAAAACAAEAAAAgAEAAAEAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAQAAgCAAEAgACAQAAAI==


formula: (Cu.12 Mg.88 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0857
b: 8.0857
c: 8.0857
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.631
crystal_density: 3.693
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AOP4PAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AOP4PAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AOP4PAA==
atoms_occupancy: wEUEAACBKQBAQg8AoIYBAIAaBgDgZzUAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_aniso_u11: gFcAAIBXAACAVwAAAEsAAABLAAAASwAA0IQAAA==
atoms_aniso_u22: gFcAAIBXAACAVwAAAEsAAABLAAAASwAA0IQAAA==
atoms_aniso_u33: gFcAAIBXAACAVwAAAEsAAABLAAAASwAA0IQAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//0AIAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//0AIAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//0AIAAA==
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl30bw

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAABAAAACAAEAAAAgAEAAAEAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAQAAgCAAEAgACAQAAAI==


formula: (Cu.24 Mg.76 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0867
b: 8.0867
c: 8.0867
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.828
crystal_density: 3.810
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AYP4PAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AYP4PAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AYP4PAA==
atoms_occupancy: gIsIAIDXJQAApg4AQA0DAMBFBAAAtjUAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_aniso_u11: MFwAADBcAAAwXAAAiEoAAIhKAACISgAA8IcAAA==
atoms_aniso_u22: MFwAADBcAAAwXAAAiEoAAIhKAACISgAA8IcAAA==
atoms_aniso_u33: MFwAADBcAAAwXAAAiEoAAIhKAACISgAA8IcAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAACP3//wj9//8I/f//gAIAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAACP3//wj9//8I/f//gAIAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAACP3//wj9//8I/f//gAIAAA==
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl50bw

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAABAAAACAAEAAABAAEAAAEAAgAABAAQAABAAgAAEAEAABABAAAgAgAAAAgABACAAEAQAAgCAAIAgACAQAAAI==


formula: Cu.41 Mg.59 Al1.99 O4
compound: Synthetic
formula_title: <missing>
a: 8.0852
b: 8.0852
c: 8.0852
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.533
crystal_density: 3.973
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AcP0PAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AcP0PAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AcP0PAA==
atoms_occupancy: AKYOAAC9HwAApg4AIDAFAOAiAgDgZzUAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_aniso_u11: sGgAALBoAACwaAAAuFEAALhRAAC4UQAAAJYAAA==
atoms_aniso_u22: sGgAALBoAACwaAAAuFEAALhRAAC4UQAAAJYAAA==
atoms_aniso_u33: sGgAALBoAACwaAAAuFEAALhRAAC4UQAAAJYAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAQPz//0D8//9A/P//kAEAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAQPz//0D8//9A/P//kAEAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAQPz//0D8//9A/P//kAEAAA==
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl70aw

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAAAgAAACAAEAAAAgAEAAACAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAIAAgCAAEAgACAQAAAI==


formula: (Cu.44 Mg.56 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0846
b: 8.0846
c: 8.0846
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.416
crystal_density: 4.011
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AwP0PAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AwP0PAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AwP0PAA==
atoms_occupancy: gN4PAICEHgAApg4AQH4FAMDUAQAAtjUAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "MgM", "AlM", "O"]
atoms_aniso_u11: 0GsAANBrAADQawAA8FUAAPBVAADwVQAAYJ8AAA==
atoms_aniso_u22: 0GsAANBrAADQawAA8FUAAPBVAADwVQAAYJ8AAA==
atoms_aniso_u33: 0GsAANBrAADQawAA8FUAAPBVAADwVQAAYJ8AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAaPz//2j8//9o/P//kAEAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAaPz//2j8//9o/P//kAEAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAaPz//2j8//9o/P//kAEAAA==
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl70bm

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAAAgAAACAAEAAAAgAEAAACAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAIAAgCAAEAgACAIAAAI==


formula: Cu.69 Mg.31 Al2 O4
compound: Synthetic
formula_title: (Cu.69Mg.31)Al2O4
a: 8.0857
b: 8.0857
c: 8.0857
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.631
crystal_density: 4.256
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgBY/A8A
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgBY/A8A
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgBY/A8A
atoms_occupancy: wD4aAMDrEgCA3g8AQO8HAMAZNQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "AlM", "O"]
atoms_aniso_u11: cHsAAHB7AABwewAAwF0AAMBdAAAgsgAA
atoms_aniso_u22: cHsAAHB7AABwewAAwF0AAMBdAAAgsgAA
atoms_aniso_u33: cHsAAHB7AABwewAAwF0AAMBdAAAgsgAA
atoms_aniso_u12: AAAAAAAAAAAAAAAAyPv//8j7//8AAAAA
atoms_aniso_u13: AAAAAAAAAAAAAAAAyPv//8j7//8AAAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAyPv//8j7//8AAAAA
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl90dw


formula: Cu.7 Mg.3 Al2 O4
compound: Synthetic
formula_title: (Cu.70Mg.30)Al2O4
a: 8.0831
b: 8.0831
c: 8.0831
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.122
crystal_density: 4.269
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCo/A8A
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCo/A8A
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCo/A8A
atoms_occupancy: ANsaAIBPEgCA3g8AQO8HAMAZNQAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "AlM", "O"]
atoms_aniso_u11: IIAAACCAAAAggAAAUF8AAFBfAAAgsgAA
atoms_aniso_u22: IIAAACCAAAAggAAAUF8AAFBfAAAgsgAA
atoms_aniso_u33: IIAAACCAAAAggAAAUF8AAFBfAAAgsgAA
atoms_aniso_u12: AAAAAAAAAAAAAAAA8Pv///D7//+QAQAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA8Pv///D7//+QAQAA
atoms_aniso_u23: AAAAAAAAAAAAAAAA8Pv///D7//+QAQAA
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl90dm

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAIAACAAAAAgAAgAAABAAEAAAAgAEAAACAAgAAAgAQAABAAgAAEAEAAAgBAAAQAgAAAAgAAgCAACAIAAgCAAEAgABAIAAAI==


formula: Cu.78 Mg.22 Al2 O4
compound: Synthetic
formula_title: (Cu.78Mg.22)Al2O4
a: 8.0841
b: 8.0841
c: 8.0841
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.318
crystal_density: 4.347
atoms_sites: ["CuT", "MgT", "AlT", "CuM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgAY+w8A
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgAY+w8A
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgAY+w8A
atoms_occupancy: wCAfAIBtDQDAehAAYD0IAKDLNAAACT0A
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "MgT", "AlT", "CuM", "AlM", "O"]
atoms_aniso_u11: kH4AAJB+AACQfgAAUF8AAFBfAABguAAA
atoms_aniso_u22: kH4AAJB+AACQfgAAUF8AAFBfAABguAAA
atoms_aniso_u33: kH4AAJB+AACQfgAAUF8AAFBfAABguAAA
atoms_aniso_u12: AAAAAAAAAAAAAAAAePv//3j7//9w/v//
atoms_aniso_u13: AAAAAAAAAAAAAAAAePv//3j7//9w/v//
atoms_aniso_u23: AAAAAAAAAAAAAAAAePv//3j7//9w/v//
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl95b

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAIAACAAAABAAAgAAABAAEAAAAgAEAAACAAgAABAAQAABAAgAAEAEAAAgBAAAQAgAAAAgAAgCAACAIAAgCAAEAgABAIAAAI==


formula: (Cu Al2) O4
compound: Synthetic
formula_title: CuAl2O4
a: 8.0793
b: 8.0793
c: 8.0793
alpha: 90
beta: 90
gamma: 90
cell_volume: 527.377
crystal_density: 4.572
atoms_sites: ["CuT", "AlT", "CuM", "AlM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAJj4DwA=
atoms_y: IKEHACChBwCAhB4AgIQeAJj4DwA=
atoms_z: IKEHACChBwCAhB4AgIQeAJj4DwA=
atoms_occupancy: wFUrAECzEQCg2QgAYC80AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["CuT", "AlT", "CuM", "AlM", "O"]
atoms_aniso_u11: 4JIAAOCSAADQawAA0GsAALDMAAA=
atoms_aniso_u22: 4JIAAOCSAADQawAA0GsAALDMAAA=
atoms_aniso_u33: 4JIAAOCSAADQawAA0GsAALDMAAA=
atoms_aniso_u12: AAAAAAAAAAAo+///KPv//5ABAAA=
atoms_aniso_u13: AAAAAAAAAAAo+///KPv//5ABAAA=
atoms_aniso_u23: AAAAAAAAAAAo+///KPv//5ABAAA=
pub_title:
 Cation ordering over short-range and long-range scales
 in the MgAl2O4-CuAl2O4 series
 Sample: CuAl100h

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAIAACAAAAAgAAgAAABAAEAAAAgAEAAACAAQAAAgAQAAAgAQAACACAAAgAgAAQAQAAAAgAAgCAACAIAAQBAACAQABAIAAAE==


formula: K1.5 H.5 Mg2 Si2 O7
compound: Synthetic
pub_title: New structural features of the high-pressure synthetic sheet-disilicate Phase-X, K(2-x)Mg2Si2O7Hx
formula_title: <missing>
a: 5.0646
b: 5.0646
c: 13.2379
alpha: 90
beta: 90
gamma: 120
cell_volume: 294.063
crystal_density: 3.116
atoms_sites: ["K", "H", "Mg", "Si", "O1", "O2"]
atoms_x: QJsVAAAAAABVWBQAAAAAAAAAAAAw6hIA
atoms_y: gE4nAIATHACrsCgAAAAAAAAAAAAAAAAA
atoms_z: QEIPAICLCAAAAAAAEIQHAEBCDwBABhkA
atoms_occupancy: QEIPAAgWBQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: AHcBAAASegDwuQAAcHsAAPC5AADgkgAA
atoms_aniso_label: ["K", "Mg", "Si", "O1", "O2"]
atoms_aniso_u11: YOoAAADIAADgkgAAAPoAABCLAAA=
atoms_aniso_u22: QJYBAADIAADgkgAAAPoAAKClAAA=
atoms_aniso_u33: YIYAAGCfAAAASwAAgD4AADCOAAA=
atoms_aniso_u12: AIP//wBkAABwSQAA4HkAANBSAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAPDx//8=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAABAAAAAAABAAAACAACAAAAAAACAIQAIAAHAAIAgQAAAYAAAAA6AQAOAQCCAIECAAI4AAKgwAkEEIACIACcBAIECQIAYADABUEKgBMAIhAIEBCE4gcIkAWAJxBxCBCIAYAQw0SYCYlgGAKEHEMRAGgGAa==


formula: (Co.07 Mg.93 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0851
b: 8.0851
c: 8.0851
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.514
crystal_density: 3.637
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AKP8PAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AKP8PAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AKP8PAA==
atoms_occupancy: gKkDAIC5KgAApg4AIE4AAOAEBwAAtjUAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: AEsAAABLAAAASwAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u22: AEsAAABLAAAASwAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u33: AEsAAABLAAAASwAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAA+P3///j9///4/f//SAMAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAA+P3///j9///4/f//SAMAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAA+P3///j9///4/f//SAMAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl0.5


formula: Co.08 Mg.91 Al2 O4
compound: Synthetic
formula_title: <missing>
a: 8.0848
b: 8.0848
c: 8.0848
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.455
crystal_density: 3.640
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AQAAQAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AQAAQAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AQAAQAA==
atoms_occupancy: wEUEAEAdKgDACQ4AIE4AAMC2BgAgBDYAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: 4EcAAOBHAADgRwAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u22: 4EcAAOBHAADgRwAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u33: 4EcAAOBHAADgRwAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAA+P3///j9///4/f//qAIAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAA+P3///j9///4/f//qAIAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAA+P3///j9///4/f//qAIAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl1


formula: (Co.11 Mg.89 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0840
b: 8.0840
c: 8.0840
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.298
crystal_density: 3.673
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AQAAQAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AQAAQAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AQAAQAA==
atoms_occupancy: QH4FAACBKQDACQ4AQJwAAKBoBgAgBDYAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: cEkAAHBJAABwSQAAUEYAAFBGAABQRgAAwHYAAA==
atoms_aniso_u22: cEkAAHBJAABwSQAAUEYAAFBGAABQRgAAwHYAAA==
atoms_aniso_u33: cEkAAHBJAABwSQAAUEYAAFBGAABQRgAAwHYAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAASP7//0j+//9I/v//qAIAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAASP7//0j+//9I/v//qAIAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAASP7//0j+//9I/v//qAIAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl10

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAIAACAAAABAAAgAAABAAEAAAAgAEAAACAAgAABAAQAABAAgAAEAEAAAgBAAAQAgAAAAgAAgCAACAIAAgCAAEAgABAIAAAI==


formula: (Co.25 Mg.75 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0875
b: 8.0875
c: 8.0875
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.984
crystal_density: 3.790
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AUAQQAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AUAQQAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AUAQQAA==
atoms_occupancy: wAkOAMCRIQCAbQ0AQJwAAIAaBgBAUjYAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: kEwAAJBMAACQTAAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u22: kEwAAJBMAACQTAAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u33: kEwAAJBMAACQTAAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAgP3//4D9//+A/f//WAIAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAgP3//4D9//+A/f//WAIAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAgP3//4D9//+A/f//WAIAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl14

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAABAAAACAAEAAABAAEAAAEAAgAABAAQAABAAgAAEAEAABABAAAgAgAAABAABACAAEAQAAgCAAIAgACAQAAAI==


formula: (Co.34 Mg.66 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0902
b: 8.0902
c: 8.0902
alpha: 90
beta: 90
gamma: 90
cell_volume: 529.514
crystal_density: 3.864
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AaAUQAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AaAUQAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AaAUQAA==
atoms_occupancy: wOsSAABMHQBA0QwAYOoAAEB+BQBgoDYAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: IE4AACBOAAAgTgAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u22: IE4AACBOAAAgTgAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u33: IE4AACBOAAAgTgAAMEMAADBDAAAwQwAAwHYAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAMP3//zD9//8w/f//IAMAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAMP3//zD9//8w/f//IAMAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAMP3//zD9//8w/f//IAMAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl20

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAIAAAAAAIAAAIAAAAAQAAEAAAABAABAAAACAAEAAABAAIAAAEAAgAABAAQAABABAAAEAEAABABAAAgBAAAABAABACAAEAQABACAAIBAACAQAAAQ==


formula: (Co.48 Mg.52 Al2) O4
compound: Synthetic
formula_title: <missing>
a: 8.0914
b: 8.0914
c: 8.0914
alpha: 90
beta: 90
gamma: 90
cell_volume: 529.750
crystal_density: 3.984
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AaAoQAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AaAoQAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AaAoQAA==
atoms_occupancy: ANsaAECVFgDAmAsAgDgBAOCTBACgPDcAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: QFEAAEBRAABAUQAAwEQAAMBEAADARAAA4HkAAA==
atoms_aniso_u22: QFEAAEBRAABAUQAAwEQAAMBEAADARAAA4HkAAA==
atoms_aniso_u33: QFEAAEBRAABAUQAAwEQAAMBEAADARAAA4HkAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//IAMAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//IAMAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//IAMAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl34

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAIAAAAAAIAAAIAAAAAQAAEAAAABAABAAAACAAEAAABAAIAAAEAAgAABAAQAABABAAAEAEAABABAAAgBAAAABAABAEAAEAQABACAAIBAAEAgAAAQ==


formula: (Co.59 Mg.41 Al2) O4
compound: Synthetic
formula_title: (Co.59Mg.41)Al2O4
a: 8.0943
b: 8.0943
c: 8.0943
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.320
crystal_density: 4.075
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AoA4QAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AoA4QAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AoA4QAA==
atoms_occupancy: gPUgAIBPEgBAYAoAoIYBAGBbAwDg2DcAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: AEsAAABLAAAASwAA8DwAAPA8AADwPAAA8G4AAA==
atoms_aniso_u22: AEsAAABLAAAASwAA8DwAAPA8AADwPAAA8G4AAA==
atoms_aniso_u33: AEsAAABLAAAASwAA8DwAAPA8AADwPAAA8G4AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAA4Pz//+D8///g/P//kAEAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAA4Pz//+D8///g/P//kAEAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAA4Pz//+D8///g/P//kAEAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl45


formula: (Co.63 Mg.37 Al2) O4
compound: Synthetic
formula_title: (Co.63Mg.37)Al2O4
a: 8.0957
b: 8.0957
c: 8.0957
alpha: 90
beta: 90
gamma: 90
cell_volume: 530.595
crystal_density: 4.108
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AuAUQAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AuAUQAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AuAUQAA==
atoms_occupancy: AL0fAMB6EABA0QwAYFsDAEANAwBgoDYAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: gFcAAIBXAACAVwAAUEYAAFBGAABQRgAAgIkAAA==
atoms_aniso_u22: gFcAAIBXAACAVwAAUEYAAFBGAABQRgAAgIkAAA==
atoms_aniso_u33: gFcAAIBXAACAVwAAUEYAAFBGAABQRgAAgIkAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//IAMAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//IAMAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAuPz//7j8//+4/P//IAMAAA==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl50

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAACAAIAAABAAIAAAEABAAABAAgAACABAAAIAIAABACAABABAAAACAACAEAAIAgABAEAAQBAAEAgAAAQ==


formula: Co.76 Mg.25 Al2 O4
compound: Synthetic
formula_title: (Co.76Mg.25)Al2O4
a: 8.1010
b: 8.1010
c: 8.1010
alpha: 90
beta: 90
gamma: 90
cell_volume: 531.638
crystal_density: 4.219
atoms_sites: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AqBAQAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AqBAQAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AqBAQAA==
atoms_occupancy: wOQoAEBgCgAAxAkAIL8CAABxAgAAJzgAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "MgT", "AlT", "CoM", "MgM", "AlM", "O"]
atoms_aniso_u11: 2FQAANhUAADYVAAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u22: 2FQAANhUAADYVAAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u33: 2FQAANhUAADYVAAAUEYAAFBGAABQRgAA4HkAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAyPv//8j7///I+///iP///w==
atoms_aniso_u13: AAAAAAAAAAAAAAAAyPv//8j7///I+///iP///w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAyPv//8j7///I+///iP///w==
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl67

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAAEAAIAAACAAIAAAIABAAACAAgAACABAAAIAIAACACAABACAAAACAACAIAAQBAABAIAAgBAAIAgAAAg==


formula: (Co Al2) O4
compound: Synthetic
formula_title: CoAl2O4
a: 8.1047
b: 8.1047
c: 8.1047
alpha: 90
beta: 90
gamma: 90
cell_volume: 532.367
crystal_density: 4.414
atoms_sites: ["CoT", "AlT", "CoM", "AlM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAPgVEAA=
atoms_y: IKEHACChBwCAhB4AgIQeAPgVEAA=
atoms_z: IKEHACChBwCAhB4AgIQeAPgVEAA=
atoms_occupancy: wBk1AEDvBwCg9wMAYBE5AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: ["CoT", "AlT", "CoM", "AlM", "O"]
atoms_aniso_u11: 4FEAAOBRAACAPgAAgD4AAKBzAAA=
atoms_aniso_u22: 4FEAAOBRAACAPgAAgD4AAKBzAAA=
atoms_aniso_u33: 4FEAAOBRAACAPgAAgD4AAKBzAAA=
atoms_aniso_u12: AAAAAAAAAACg+///oPv//+D8//8=
atoms_aniso_u13: AAAAAAAAAACg+///oPv//+D8//8=
atoms_aniso_u23: AAAAAAAAAACg+///oPv//+D8//8=
pub_title:
 Blue spinel crystals in the MgAl2O4-CoAl2O4 series: Part II.
 Cation ordering over short-range and long-range scales
 Sample: CoAl100

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAACAACAAAAEAAIAAACAAQAAAIABAAACABAAAEACAAAQAQAACAEAABACAAAAEAAEAIAAQBAACAIAAgCAAQBAAAAg==


formula: Li Nb O3
compound: Synthetic
pub_title: Crystal structures of ilmenite type LiNbO3 and NaNbO3
formula_title: LiNbO3
a: 5.212
b: 5.212
c: 14.356
alpha: 90
beta: 90
gamma: 120
cell_volume: 337.733
crystal_density: 4.361
atoms_sites: ["Li", "Nb", "O"]
atoms_x: AAAAAAAAAACAzBIA
atoms_y: AAAAAAAAAAAgywAA
atoms_z: 4CEXAJDkCADAhg4A
atoms_occupancy: 0
atoms_u_iso: kBcDAOAoAQDYEwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAABAAIAAIAAAAAAAAAIAAQAARABAgCAAAAABAQAAoABBQACAAgiAEAgEAEgABIAQIjAEACAAMAQgKAIgCAIwBAIoEECAgAIAgSggCECEiCgRAoJgAEgQAgwAwBJhAQikAIAQILBAgEABQKATgAg==


formula: Na Nb O3
compound: Synthetic
pub_title: Crystal structures of ilmenite type LiNbO3 and NaNbO3
formula_title: <missing>
a: 5.335
b: 5.335
c: 15.611
alpha: 90
beta: 90
gamma: 120
cell_volume: 384.796
crystal_density: 4.244
atoms_sites: ["Na", "Nb", "O"]
atoms_x: AAAAAAAAAABArRIA
atoms_y: AAAAAAAAAAAA7gIA
atoms_z: IMoVAGAeCQBglg4A
atoms_occupancy: 0
atoms_u_iso: SJ4AAGA7AABgOwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAQAACAAIAAAAAAAAQAAAIUAAAQBAIAAAASAAAYAIAIEAAAKAAiARAgAAAQAEgEghAAAgAYAhiAAMACBAiAAoBILAAAIAIFEQAEBQMSADAEIJABgCKIACAgckAEFggACARBQAgIJABAgpQAgQkgG==


formula: (Na.95 Li.05) (Al.91 Fe.09) As O4.27 (F.73 H.27)
compound: the Barranca mine, Coneto de Comonfort, Durango, Mexico
pub_title: Redetermination of durangite, NaAl(AsO4)F
formula_title: <missing>
a: 6.5789
b: 8.5071
c: 7.0212
alpha: 90
beta: 115.447
gamma: 90
cell_volume: 354.835
crystal_density: 3.915
atoms_sites: ["Na", "Li", "Al", "Fe", "As", "O1", "O2", "F", "O-H"]
atoms_x: gIQeAICEHgAAAAAAAAAAAAAAAACQHQwAuEYGAAAAAAAAAAAA
atoms_y: SHsKAEh7CgAAAAAAAAAAANgyEwBwkxoA+GQMAKgXBACoFwQA
atoms_z: QEIPAEBCDwAAAAAAAAAAAEBCDwCoXBkACOcGAMDGLQDAxi0A
atoms_occupancy: wPs5AEANAwDAijcAQH4FAAAJPQAACT0AAAk9AECOLADAehAA
atoms_u_iso: 4M4AAODOAACQVgAAkFYAAMBOAAA4lQAA8IIAAFhwAABYcAAA
atoms_aniso_label: ["Na", "Li", "Al", "Fe", "As", "O1", "O2", "F", "O-H"]
atoms_aniso_u11: IJkAACCZAACYWAAAmFgAAHBJAACAcAAAkJcAAACWAAAAlgAA
atoms_aniso_u22: cGIAAHBiAABAUQAAQFEAABhHAABQkQAA8G4AALBoAACwaAAA
atoms_aniso_u33: AEUBAABFAQBIWAAASFgAAPhXAADwoAAA8KAAAIBXAACAVwAA
atoms_aniso_u12: AAAAAAAAAAAIBwAACAcAAAAAAABg1///UPv//wAAAAAAAAAA
atoms_aniso_u13: 8DwAAPA8AABoJAAAaCQAABgfAABAHwAAUF8AAEA4AABAOAAA
atoms_aniso_u23: AAAAAAAAAABAAQAAQAEAAAAAAAAAzv//wOD//wAAAAAAAAAA
qdat:
AAAAAAAAAAAAAAAAAAAAAEAACAAAACAIAgAIAAAAAwAgAIBAAIAQgAIIASAIEABgkAiAgBEAgBKHYAAAAxWAgE0cghDAISQFUYGRQUoZCjwMWAbARY8EOAXgAYxXxC1ElqAlTooClxiCC9qa+kZAR6HVqHVBDknR4q3MJ1==


formula: Fe2.97 Ni.027 Mn.024 Si
compound: cosmic dust found in placers, Yanshan, China
pub_title: Two new minerals gupeiite and xifengite in cosmic dusts from Yanshan
formula_title: <missing>
a: 5.670
b: 5.670
c: 5.670
alpha: 90
beta: 90
gamma: 90
cell_volume: 182.284
crystal_density: 7.173
atoms_sites: ["Fe1", "Ni1", "Mn1", "Fe2", "Ni2", "Mn2", "Si"]
atoms_x: gIQeAICEHgCAhB4AQEIPAEBCDwBAQg8AAAAAAA==
atoms_y: gIQeAICEHgCAhB4AQEIPAEBCDwBAQg8AAAAAAA==
atoms_z: gIQeAICEHgCAhB4AQEIPAEBCDwBAQg8AAAAAAA==
atoms_occupancy: wGw8AKCMAAAAfQAAwGw8AKCMAAAAfQAAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAgAAAAAAAAAAAAAAQAAAAAAAAIAAgAAAAAAAABAAAAAAEACAAAAAAAEAAAAAgAAAAAAAEAAAAQBAAAAABAAAAQEAAAAAgAABAQAAAAQAAAgAAAABAAAQIAAABAABAgAAAQ==


formula: Fe Si2
compound: Luobusha, Tibet, China
pub_title: Linzhiite, FeSi2, a redefined and revalidated new mineral species from Luobusha, Tibet, China
formula_title: <missing>
a: 2.696
b: 2.696
c: 5.147
alpha: 90
beta: 90
gamma: 90
cell_volume: 37.411
crystal_density: 4.972
atoms_sites: ["Fe", "Si"]
atoms_x: gIQeAAAAAAA=
atoms_y: gIQeAAAAAAA=
atoms_z: AAAAAFCVEAA=
atoms_occupancy: 0
atoms_u_iso: YG0AAOAuAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAAAAABACAABAAAAAAAAAAAgQACAAgAAAAAAIAAAIAAAACAAIIQAAABCAQQAAAABAARAABAAAAQAAhACEAACEQIgAAhEECAAwEAEADAACQAAQEUACBAKADAACACICAAEUExARQ==


formula: Si.73 (Y.78 Yb.12 Er.05 Dy.03 Gd.02) O4 H2
compound: Stetind quarry, Tysfjord, Norway
pub_title: Atelisite-(Y), a new rare earth defect silicate of the KDP structure type
formula_title: <missing>
a: 6.947
b: 6.947
c: 6.133
alpha: 90
beta: 90
gamma: 90
cell_volume: 295.984
crystal_density: 4.331
atoms_sites: ["Si", "Y", "Yb", "Er", "Dy", "Gd", "O", "H"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAkBoyAADUMAA=
atoms_y: gIQeAICEHgCAhB4AgIQeAICEHgCAhB4AUGEhAACBKQA=
atoms_z: QEIPAMDGLQDAxi0AwMYtAMDGLQDAxi0AQDMFAMAnCQA=
atoms_occupancy: QI4sAICbLwAAUwcAQA0DAMDUAQCAOAEAAAk9AICEHgA=
atoms_u_iso: wHYAAGCGAABghgAAYIYAAGCGAABghgAAENYAAABxAgA=
atoms_aniso_label: ["Si", "Y", "Yb", "Er", "Dy", "Gd", "O"]
atoms_aniso_u11: kH4AALCaAACwmgAAsJoAALCaAACwmgAAUJEAAA==
atoms_aniso_u22: kH4AALCaAACwmgAAsJoAALCaAACwmgAAYDUBAA==
atoms_aniso_u33: sGgAADBcAAAwXAAAMFwAADBcAAAwXAAAoL4AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgPP//w==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQO3//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgD4AAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAABAAAAAAAQAAAAAABAAIACAAAACIAAAAIAAAgCAIIAAEAAIIAAAEACCBIAAEAAoQICBAAExAIIIiAgAAQFACiFACQApAphAAJAhFQCAYIEBpCgJICRiGAEhhJAwGkChUMDQOTEQFsNJYwYxgV==


formula: (Ca2.19 Na.81) V2.781 As.024 Si.21 Mn1.978 O12
compound: Molinello mine, Italy
pub_title: Palenzonaite, berzeliite, and manganberzeliite:(As5+,V5+,Si4+)O4 tetrahedra in garnet structures
formula_title: <missing>
a: 12.5433
b: 12.5433
c: 12.5433
alpha: 90
beta: 90
gamma: 90
cell_volume: 1973.492
crystal_density: 3.745
atoms_sites: ["Ca", "Na", "V", "As", "Si", "Mn", "O"]
atoms_x: IKEHACChBwBg4xYAYOMWAGDjFgAAAAAAIGUCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQE4DAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwAAAAAA0C8oAA==
atoms_occupancy: QI4sAMB6EABglDgAAH0AAMBFBAAgXTwAAAk9AA==
atoms_u_iso: kMkAAJDJAACgcwAAoHMAAKBzAABwrQAAQM4AAA==
atoms_aniso_label: ["Ca", "Na", "V", "As", "Si", "Mn", "O"]
atoms_aniso_u11: oKUAAKClAADAdgAAwHYAAMB2AABwrQAAsMwAAA==
atoms_aniso_u22: UNwAAFDcAAAQcgAAEHIAABByAABwrQAAcN8AAA==
atoms_aniso_u33: UNwAAFDcAAAQcgAAEHIAABByAABwrQAAoL4AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAw+P//AAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAw+P//IAMAAA==
atoms_aniso_u23: ABkAAAAZAAAAAAAAAAAAAAAAAAAw+P//gAwAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAEAACAAAAAAAQAIAAAIAQBAEAACAQAAAEBAQACBAgQIEAACBBBBBBABCAEIIQAhCEIQgEARCEQCEACIhERAIkAgBERAQAiAASIEQBAACAAACAAAAAAAASAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Ca2.19 Na.81) V2.7 As.132 Si.18 Mn1.978 O12
compound: Gambatesa mine, Italy
pub_title: Palenzonaite, berzeliite, and manganberzeliite:(As5+,V5+,Si4+)O4 tetrahedra in garnet structures
formula_title: <missing>
a: 12.5359
b: 12.5359
c: 12.5359
alpha: 90
beta: 90
gamma: 90
cell_volume: 1970.001
crystal_density: 3.773
atoms_sites: ["Ca", "Na", "V", "As", "Si", "Mn", "O"]
atoms_x: IKEHACChBwBg4xYAYOMWAGDjFgAAAAAAIGUCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAkE4DAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwAAAAAAyC0oAA==
atoms_occupancy: QI4sAMB6EACA7jYAgK8CAICpAwAgXTwAAAk9AA==
atoms_u_iso: iK4AAIiuAAA4YwAAOGMAADhjAABIlAAAYLgAAA==
atoms_aniso_label: ["Ca", "Na", "V", "As", "Si", "Mn", "O"]
atoms_aniso_u11: 8IcAAPCHAACAVwAAgFcAAIBXAABIlAAA4MQAAA==
atoms_aniso_u22: wMEAAMDBAAAAaQAAAGkAAABpAABIlAAA4MQAAA==
atoms_aniso_u33: wMEAAMDBAAAAaQAAAGkAAABpAABIlAAAgKIAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAACg9v//cP7//w==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAACg9v//oPb//w==
atoms_aniso_u23: sBgAALAYAAAAAAAAAAAAAAAAAACg9v//oPb//w==
qdat:
AAAAAAAAAAAAAAAAAAAAEAACAAAAAAAQAIAAAIAQAgCAABAIAAAEBAQACBAgIIEAABBBBAhBABCAEEIQAhCEIQgCAQhEICEACIREJAIiAgAiIgQAiAARIEQAgABAAACAAAAAAAASAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Ca2.04 Na.96) V1.563 As1.38 Si.03 Mn1.936 O12
compound: Fianel mine, Switzerland
pub_title: Palenzonaite, berzeliite, and manganberzeliite:(As5+,V5+,Si4+)O4 tetrahedra in garnet structures
formula_title: <missing>
a: 12.5342
b: 12.5342
c: 12.5342
alpha: 90
beta: 90
gamma: 90
cell_volume: 1969.200
crystal_density: 3.953
atoms_sites: ["Ca", "Na", "V", "As", "Si", "Mn", "O"]
atoms_x: IKEHACChBwBg4xYAYOMWAGDjFgAAAAAAoGwCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAiEcDAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwAAAAAAODYoAA==
atoms_occupancy: AIEpAACIEwCgzB8AgBMcAECcAAAAFTsAAAk9AA==
atoms_u_iso: 8NIAAPDSAABwhQAAcIUAAHCFAACgvgAAYOoAAA==
atoms_aniso_label: ["Ca", "Na", "V", "As", "Si", "Mn", "O"]
atoms_aniso_u11: 4KsAAOCrAABwewAAcHsAAHB7AACgvgAA0AEBAA==
atoms_aniso_u22: sOUAALDlAAAgigAAIIoAACCKAACgvgAAEO8AAA==
atoms_aniso_u33: sOUAALDlAAAgigAAIIoAACCKAACgvgAA0M8AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAACg9v//0AcAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAACg9v//EPX//w==
atoms_aniso_u23: sB0AALAdAAAAAAAAAAAAAAAAAACg9v//8AoAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAEAACAAAAAAAIAEAAAIAQAgCAABAIAAAEBAQACBAgIIEAABBBBAhBABCAEEIQAhCEIQgCAQhEICEACEREIgIiAgAiIgQASAARIEQAgABAAACAAAAAAAAJAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Na.9 Ca2.1) (Mg1.762 Mn.238) As2.847 Si.12 O12
compound: Langban, Sweden
pub_title: Palenzonaite, berzeliite, and manganberzeliite:(As5+,V5+,Si4+)O4 tetrahedra in garnet structures
formula_title: <missing>
a: 12.3450
b: 12.3450
c: 12.3450
alpha: 90
beta: 90
gamma: 90
cell_volume: 1881.366
crystal_density: 4.021
atoms_sites: ["NaX", "CaX", "MgY", "MnY", "AsT", "Si", "O"]
atoms_x: IKEHACChBwAAAAAAAAAAAGDjFgBg4xYA2GECAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAyCADAA==
atoms_z: QEIPAEBCDwAAAAAAAAAAAEBCDwBAQg8AABQoAA==
atoms_occupancy: gE8SAIC5KgCgxTUAYEMHACDsOQAAcQIAAAk9AA==
atoms_u_iso: OJoAADiaAACQfgAAkH4AABBPAAAQTwAACI4AAA==
atoms_aniso_label: ["NaX", "CaX", "MgY", "MnY", "AsT", "Si", "O"]
atoms_aniso_u11: EHIAABByAACQfgAAkH4AAPhNAAD4TQAAMI4AAA==
atoms_aniso_u22: YK4AAGCuAACQfgAAkH4AAIhPAACITwAAgKIAAA==
atoms_aniso_u33: YK4AAGCuAACQfgAAkH4AAIhPAACITwAA4HkAAA==
atoms_aniso_u12: AAAAAAAAAACo+P//qPj//wAAAAAAAAAAUBQAAA==
atoms_aniso_u13: AAAAAAAAAACo+P//qPj//wAAAAAAAAAAUOL//w==
atoms_aniso_u23: gCAAAIAgAACo+P//qPj//wAAAAAAAAAAYAkAAA==
qdat:
AAAAAAAAAAAAAAAAAAAABAAAgAAAAAACAAgAAAgBAEAIAAEAgAAAICAgAEBAgQIEAABBAgggggAhACCEEAQQhCEIAgEIRCAQgARCIREBEICACIiBABEAAkQIgCAACAAACAAAAAAAAJAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Na.99 Ca2.01) (Mn1.554 Mg.446) (As2.544 V.456) O12
compound: Varenche, Italy
pub_title: Palenzonaite, berzeliite, and manganberzeliite:(As5+,V5+,Si4+)O4 tetrahedra in garnet structures
formula_title: <missing>
a: 12.4829
b: 12.4829
c: 12.4829
alpha: 90
beta: 90
gamma: 90
cell_volume: 1945.120
crystal_density: 4.134
atoms_sites: ["NaX", "CaX", "MnY", "MgY", "AsT", "VT", "O"]
atoms_x: IKEHACChBwAAAAAAAAAAAGDjFgBg4xYAOGsCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAcDwDAA==
atoms_z: QEIPAEBCDwAAAAAAAAAAAEBCDwBAQg8AaDMoAA==
atoms_occupancy: QCQUAMDkKACgbC8AYJwNAADCMwAARwkAAAk9AA==
atoms_u_iso: uKsAALirAABQkQAAUJEAAHhpAAB4aQAAAK8AAA==
atoms_aniso_label: ["NaX", "CaX", "MnY", "MgY", "AsT", "VT", "O"]
atoms_aniso_u11: cHsAAHB7AABQkQAAUJEAAMhkAADIZAAAILIAAA==
atoms_aniso_u22: UMMAAFDDAABQkQAAUJEAANBrAADQawAA4MQAAA==
atoms_aniso_u33: UMMAAFDDAABQkQAAUJEAANBrAADQawAAkJcAAA==
atoms_aniso_u12: AAAAAAAAAAAQ+v//EPr//wAAAAAAAAAAwBIAAA==
atoms_aniso_u13: AAAAAAAAAAAQ+v//EPr//wAAAAAAAAAAkOj//w==
atoms_aniso_u23: 0CAAANAgAAAQ+v//EPr//wAAAAAAAAAAgAwAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAEAACAAAAAAAIAEAAAEAIAQBAAAgEAAACAgIABAQIECBAAAgQQQQQQAQgBBCEAIQgiEIAgEIQiAQgAREIiICEQEAEiICAEQACRAiAIAAIAAAQAAAAAAABIAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Ca2.01 Na.99) (Mn1.696 Mg.304) As2.889 O12
compound: Gozaisho mine, Japan
pub_title: Palenzonaite, berzeliite, and manganberzeliite:(As5+,V5+,Si4+)O4 tetrahedra in garnet structures
formula_title: <missing>
a: 12.4929
b: 12.4929
c: 12.4929
alpha: 90
beta: 90
gamma: 90
cell_volume: 1949.799
crystal_density: 4.172
atoms_sites: ["CaX", "NaX", "MnY", "MgY", "AsT", "O"]
atoms_x: IKEHACChBwAAAAAAAAAAAGDjFgDIbAIA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAADIPgMA
atoms_z: QEIPAEBCDwAAAAAAAAAAAEBCDwDAOigA
atoms_occupancy: wOQoAEAkFAAAwjMAAEcJAODGOgAACT0A
atoms_u_iso: 6K0AAOitAACokwAAqJMAAIhjAACArAAA
atoms_aniso_label: ["CaX", "NaX", "MnY", "MgY", "AsT", "O"]
atoms_aniso_u11: 0IQAANCEAACokwAAqJMAAAhhAAAArwAA
atoms_aniso_u22: OMIAADjCAACokwAAqJMAAMhkAABQwwAA
atoms_aniso_u33: OMIAADjCAACokwAAqJMAAMhkAADgkgAA
atoms_aniso_u12: AAAAAAAAAACA+P//gPj//wAAAAAAGQAA
atoms_aniso_u13: AAAAAAAAAACA+P//gPj//wAAAABQ4v//
atoms_aniso_u23: QBoAAEAaAACA+P//gPj//wAAAADwCgAA
qdat:
AAAAAAAAAAAAAAAAAAAAEAACAAAAAAAIAEAAAEAIAgCAABAEAAACAgIABAgIECCAAAggQQQQQAggBCCEAQQhCEIBAEIhEAhAAhERCICIgIAIiIEAEQAESAkAIAAQAAAQAAAAAAACQAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Pb2 (O F) Cl
compound: Merehead quarry, Somerset, England
formula_title: <missing>
a: 4.065
b: 4.065
c: 12.631
alpha: 90
beta: 90
gamma: 90
cell_volume: 208.717
crystal_density: 7.715
atoms_sites: ["Pb", "OF", "FO", "Cl"]
atoms_x: AAAAAICEHgCAhB4AgIQeAA==
atoms_y: AAAAAAAAAAAAAAAAgIQeAA==
atoms_z: UPcIAEBCDwBAQg8AAAAAAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AA==
atoms_u_iso: ILkDAKD9AgCg/QIAAGsDAA==
atoms_aniso_label: ["Pb", "OF", "FO", "Cl"]
atoms_aniso_u11: oPcDAKD9AgCg/QIAwMgDAA==
atoms_aniso_u22: oPcDAKD9AgCg/QIAwMgDAA==
atoms_aniso_u33: gCwDAEANAwBADQMA4J8CAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAA==
pub_title:
 Rumseyite, [Pb2OF]Cl, the first naturally occurring fluoroxychloride
 mineral with the parent crystal structure for layered lead oxychlorides

qdat:
AAAAAAAAAAAAAAAACAAAAAAAAAAgAAAAAQABEAAAgAAAAAAABKAEAAQAAAQAAKBEAAIAAAAiBACCACBAgVBQgAACwAEAAQIESCEAACAgIgEEIcMAAA0QYAARggEAAEABARAYUgAIAQAgFIgABCCQBEIQABkMBEyAQAZBQQ==


formula: Fe5 Si3
compound: Synthetic
formula_title: <missing>
a: 6.7522
b: 6.7522
c: 4.740
alpha: 90
beta: 90
gamma: 120
cell_volume: 187.154
crystal_density: 6.450
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUACB3DgAg7SQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3
 Note: P = 0.0001 GPa

qdat:
AAAAAAAAAAAAAAAAABAAAAAAAAAAAAAgAAABAAQAAAAAQAAKAAAAICgABAAAAAgAFBAAQEACAQAAQAoAAUQAQgAAIGRAEyBKAIADIAYkEEAEgkARACqCQFAGUAAAQNiMoUgiEyBYUqAhTBUxIUKoRBGAI5EhXSAQi2xAQX==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 1.8 GPa
formula_title: <missing>
a: 6.7472
b: 6.7472
c: 4.716
alpha: 90
beta: 90
gamma: 120
cell_volume: 185.931
crystal_density: 6.493
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUALB4DgDgzSQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAgAAABAAQAAAAAIAAFAAAAIBQAAgAAAAgACggAICACAEAAIAYAARQAIQAABFCgBYhDAIABiASRCCAEIxAJAAUJIGICqgAAQGQaGQoRAyIpDQwEjK1KgkjoowRICaGyVjEYFvMEQJ==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 3.6 GPa
formula_title: <missing>
a: 6.7277
b: 6.7277
c: 4.695
alpha: 90
beta: 90
gamma: 120
cell_volume: 184.035
crystal_density: 6.560
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUAGAyDgAgcCQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAQAAAAgAIAAAAACAAEgAAAEBIAAIAAAAIABQQAEAgBABAAEAKAAEYACIAAARQoAWEQwCAAoQEkQgQBBMICQAFBKBSApUAAEBmDQyKEIFQmIcGAoY3KIFCbDFEIgVI2ScYRAa5QSB==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 4.5 GPa
formula_title: <missing>
a: 6.7169
b: 6.7169
c: 4.696
alpha: 90
beta: 90
gamma: 120
cell_volume: 183.483
crystal_density: 6.579
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUANDlDQAgcCQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAQAAAAgAIAAAAACAACQAAACAkAAIAAAAIABIQACAgAgBAACAFAAEUACEAAAQwkAWEQQBAAMQCSIQQAhGIBEAGhJAxAU0AACAyCoxFCEDQioZGASMrUqESPCTBEgJEnRVMQwT6YQg==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 5.7 GPa
formula_title: <missing>
a: 6.7108
b: 6.7108
c: 4.688
alpha: 90
beta: 90
gamma: 120
cell_volume: 182.838
crystal_density: 6.602
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUADDWDQBgjyQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAQAAAAgAIAAAAACAACQAAACAkAAIAAAAEAAoIACAQAgBAABAFAACUABEAAAIYSALCIYBAAKIBKEIIAQjEBEADQkgYgSWAABAZA0UihCBoJiLBgRKNyVCRHQxRCQFULkmiEYG7MEQ==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 7.5 GPa
formula_title: <missing>
a: 6.7031
b: 6.7031
c: 4.676
alpha: 90
beta: 90
gamma: 120
cell_volume: 181.952
crystal_density: 6.635
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUAGAADgCA3SQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAQAAAAgAEAAAAABAACIAAACASAAEAAAAEAAkIABAQAQAQABACgABGAAiAAAEUKAGhEMAgAGEAlCEEAISiAiABoKQMQJTAAAgMwKGgwiAqExCgQFCmZIgYTUIohEBZCRJxBMBdlhI==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 8.8 GPa
formula_title: <missing>
a: 6.6904
b: 6.6904
c: 4.667
alpha: 90
beta: 90
gamma: 120
cell_volume: 180.914
crystal_density: 6.673
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUALAUDgAgcCQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAIAAAAQAEAAAAABAABIAAABASAACAAAACAASEAAgIAIAQAAgBQABFAARAAABKEgCwiGAQADCASRCCAEEwgRAAUEoGICUwAAQFYFBIUQgTBMRIEBQxuUQKJWCKERAkgsk0QTAXZQS==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 11 GPa
formula_title: <missing>
a: 6.6752
b: 6.6752
c: 4.649
alpha: 90
beta: 90
gamma: 120
cell_volume: 179.398
crystal_density: 6.729
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUAODzDQCAYCQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAIAAAAQACAAAAAAgABEAAAAgJAABAAAABAAJCAAgEAEAEAAIAoAARgAIgAAAVAwA0JBQEABQgJIQggCBUIEQALAqBhBGMAAEBmBQaFEIEYKEVAgUMaimCRMwyRCIFiNEnGBwDrTB==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 14.4 GPa
formula_title: <missing>
a: 6.6496
b: 6.6496
c: 4.638
alpha: 90
beta: 90
gamma: 120
cell_volume: 177.604
crystal_density: 6.797
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUABDTDQBgjyQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAEAAAAIABAAAAAAQAASAAAAQEgAAgAAAAgAEggAIBACACAAEAKAAEoACIAAAIwUANCQYBAAUICREIIAQTCBEABoSQMQJTAAAgMwKGQwhAqCRCwYChSckQKJaESIRAqRsiYQTAXZQ==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 18.7 GPa
formula_title: <missing>
a: 6.6193
b: 6.6193
c: 4.621
alpha: 90
beta: 90
gamma: 120
cell_volume: 175.344
crystal_density: 6.885
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUAMDwDQAgcCQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAIAAAAAAAAAAAACAAAAEAAgAAAAAIAAJAAAAIBIAAQAAAAIABQQACAQAgAgABACgABKAAiAAACKFACwiCAIACiASQhBACEYgIgAKCSBiApYAAEBmBIyFCICwREOBASKJySBQmowwhICRGyTRCMBtT==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 22.6 GPa
formula_title: <missing>
a: 6.5771
b: 6.5771
c: 4.593
alpha: 90
beta: 90
gamma: 120
cell_volume: 172.066
crystal_density: 7.016
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUAODzDQCAYCQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAABAAQAAAAACAACQAAACASAACAAAACAAKCAAQEAEAEAAIAUAAIwAEIAAAQwkAVCIYAgAKIBJEEEAIJhARAA0IoFECUwAAIDECRUKEIDQjIWDASMWyWCRHQxIiICqCSLxBMBv==


formula: Fe5 Si3
compound: Synthetic
pub_title: Iron silicides and their corresponding oxides: a high-pressure study of Fe5Si3 Note: P = 30 GPa
formula_title: <missing>
a: 6.5412
b: 6.5412
c: 4.558
alpha: 90
beta: 90
gamma: 120
cell_volume: 168.896
crystal_density: 7.147
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: VVgUANDlDQBAviQA
atoms_y: q7AoAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAgAEAAAAAAgABEAAAAgEgAAgAAAAgACQgAEAgAgAgABACgABGAAhAAAAlCgBoJBQEAAwQEkIgQAgmEBEACwKgUQJJgAAgGYFBoUIgJgkIsCAoUTFECRMgxJCICiCxTRAsB==


formula: Fe2 Si
compound: Synthetic
formula_title: Fe2Si
a: 4.052
b: 4.052
c: 5.085
alpha: 90
beta: 90
gamma: 120
cell_volume: 72.304
crystal_density: 6.420
atoms_sites: ["Fe1", "Fe", "Fe3", "Si"]
atoms_x: AAAAAAAAAABVWBQAVVgUAA==
atoms_y: AAAAAAAAAACrsCgAq7AoAA==
atoms_z: AAAAAICEHgCAmy8AABcRAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural stability of Fe5Si3 and Ni2Si studied by high-pressure
 X-ray diffraction and ab initio total-energy calculations

qdat:
AAAAAAAAAAAAAAAAAAAACAAAAAAAABAAAAAAIAAAAQAAAAAAAABCAAACAAACABAQAAgACAAAEAAAAAAgEEIAABACAkABAAAAAIEAICAoAIASBEAIAAQQAAAoESAEQAIgABgCQAoEGQIAAABAwgiIAwiACRBgoCgSIkARKB==


formula: Mg2 Si O4
compound: Synthetic
formula_title: <missing>
a: 10.20141
b: 5.98348
c: 4.75534
alpha: 90
beta: 90
gamma: 90
cell_volume: 290.266
crystal_density: 3.219
atoms_sites: ["MgM1", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAEDrEAAQuAUAUIwFAOBtGwBw2wkA
atoms_y: AAAAAEBCDwBAQg8AQEIPAEBCDwDgOwIA
atoms_z: AAAAAKCCPABAABoAMI0uAMBzDQDg+hAA
atoms_occupancy: 0
atoms_u_iso: 2NEAANjHAAAYsAAAGLAAAOjLAACY3wAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Rietveld refinement of site-occupancy parameters of Mg2-xMnxSiO4
 using a new weight function in least-squares fitting
 Note: e = 1

qdat:
AAAAAAAAAAAAAAAAAAAAEAAAIAAgQAwAAABgABAACiCAiQUAGBAGACgBcxMBUCCAyIjCIbxMBgQ2SXAFBwTL4+hAaNfK8ZBpH+Fegwq/WoV102Xml7Lqmthj02qO35UrrUD9fObav8s+/l3ep1v1/3tcet32eV1/c+9775==


formula: Mg2 Si O4
compound: Synthetic
formula_title: <missing>
a: 10.20141
b: 5.98348
c: 4.75534
alpha: 90
beta: 90
gamma: 90
cell_volume: 290.266
crystal_density: 3.219
atoms_sites: ["MgM1", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAANDsEADAvAUAQJcFANBGGwAw7gkA
atoms_y: AAAAAEBCDwBAQg8AQEIPAEBCDwDABgIA
atoms_z: AAAAADCEPACABhoA0LUuALB+DQCg9BAA
atoms_occupancy: 0
atoms_u_iso: oIIAAMB2AADoYgAA0HAAAPhmAADQcAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Rietveld refinement of site-occupancy parameters of Mg2-xMnxSiO4
 using a new weight function in least-squares fitting
 Note: e = eo

qdat:
AAAAAAAAAAAAAAAAAAAAEAAAIAAgQAwAAABgABAACiCAiQUAGBAGACgBcxMBUCCAyIjCITxMBgQ2SXAFBwTL4+hAaNfK8ZBpH+Fegwq/WoV102Xml7Lqmthj02qO35UrrUD9fObav8s+/l3ep1v1/3tcet32eV1/c+9775==


formula: (Mg Mn) Si O4
compound: Synthetic
formula_title: <missing>
a: 10.45100
b: 6.12446
c: 4.80757
alpha: 90
beta: 90
gamma: 90
cell_volume: 307.717
crystal_density: 3.698
atoms_sites: ["Mg1", "Mn1", "MgM2", "MnM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADwCBEA8AgRAACqBQCgbgUAQJAbAPDOCQA=
atoms_y: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAIBkAgA=
atoms_z: AAAAAAAAAADwSzwA8Es8ALDlGQBANy4A0MwNAOD6EAA=
atoms_occupancy: oAcrAGABEgBgARIAoAcrAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: GLoAABi6AABgmgAAYJoAAMB2AAAIwAAAaJwAAFiiAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Rietveld refinement of site-occupancy parameters of Mg2-xMnxSiO4
 using a new weight function in least-squares fitting
 Note: e = 1

qdat:
AAAAAAAAAAAAAAAAAAAAgAAAgAICAGAAAAQAAQAChBAGCSABiAFACgCqKoBQQCEokQYEuQUIkG+oWBMqQz8m5EEXZdUwZSYbH+pIcnmknNxyr8Sf/wvV07nTL+266q3Clk72xP36rRrttr9Lyu2tt9tlzJO2fn6zs/9vnz==


formula: (Mn1.4 Mg.6) Si O4
compound: Synthetic
formula_title: <missing>
a: 10.52411
b: 6.17903
c: 4.83927
alpha: 90
beta: 90
gamma: 90
cell_volume: 314.692
crystal_density: 3.875
atoms_sites: ["MnM1", "MgM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADAEBEAwBARAIC2BQBQcwUA0KobALDICQA=
atoms_y: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPABB/AgA=
atoms_z: AAAAAAAAAACwRTwAsEU8APDrGQBQEy4A0GgNABAlEQA=
atoms_occupancy: oE8fAGC5HQBgIzYAoOUGAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: MKwAADCsAABIqAAASKgAAKh6AAD4uwAAqIQAAIiQAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAABAAABAAQEAYAAABgABAAJCEAIJIAGIAUAMAKxVAHCAQlEkCgVSCiFhVZDQSkSI9luRBH233OEZ2Oy/SUHTzqbV59Y2Vv74XsadtRl+2Z1eSilyVW5FzevT/Pr3pfzck357fPX+Jvv/W/Z97Vvm7==


formula: Mn2 Si O4
compound: Synthetic
formula_title: <missing>
a: 10.60016
b: 6.25753
c: 4.90338
alpha: 90
beta: 90
gamma: 90
cell_volume: 325.245
crystal_density: 4.124
atoms_sites: ["MnM1", "MnM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAHAVEQCA6AUAgJ0FAKDkGwDQ5AkA
atoms_y: AAAAAEBCDwBAQg8AQEIPAEBCDwDQ3AIA
atoms_z: AAAAALBFPABgHBoA8PAtALABDQCQfBEA
atoms_occupancy: 0
atoms_u_iso: 4MkAABC4AABokgAA4MkAAEieAAB46wAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAABAAAEABAQBQAAAEAAEABEQgDBIgAggEgBgBuUoCwIEDgpBYS4RhEoMsAoRiQlv5qlBJrPXJEOs3e1kIHX6hM09rXSm1rwvflXqnn/nTbb4l3X/+Df19R7q758tY86Ms7Xn/NP+f+373/973Tb72==


formula: Mn2 Si O4
compound: Synthetic
formula_title: <missing>
a: 10.60016
b: 6.25753
c: 4.90338
alpha: 90
beta: 90
gamma: 90
cell_volume: 325.245
crystal_density: 4.124
atoms_sites: ["MnM1", "MnM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAALAbEQBg5QUAsK4FAADVGwBA/AkA
atoms_y: AAAAAEBCDwBAQg8AQEIPAEBCDwCQiwIA
atoms_z: AAAAAIBNPACwFxoAED8uAODgDACgihEA
atoms_occupancy: 0
atoms_u_iso: ELgAADikAAB4jAAA+MUAALB8AAAQuAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAABAAAEABAQBQAAAEAAEABEQgDBIgAggEgBgBuUoCwIEDgpBYS4RhEoMsIoRiQlv5qlBJrPXJEOs3e1kIHX6hM09rXTm1rwvflXqnn/nTbb4l3X/+Df19R7q758tY86Ms/Xn/NP+f+373/973Tb72==


formula: Mg2 Si O4
compound: Synthetic
pub_title: X-ray determination of electron distributions in forsterite, fayalite and tephroite
formula_title: <missing>
a: 4.7534
b: 10.1902
c: 5.9783
alpha: 90
beta: 90
gamma: 90
cell_volume: 289.577
crystal_density: 3.227
atoms_sites: ["Mg1", "Mg2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAACiHPABIBxoA0L8uACCHDQAY8BAA
atoms_y: AAAAADjuEAA4vQUAoJYFAChJGwBw9AkA
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBABAIA
atoms_occupancy: 0
atoms_u_iso: cFgAAIBXAAAoPAAAYE8AALBPAAAYVgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAMAAAAAAAQAgAAABkAAAACaCAgQQEGBACAFoAMxKAsiBARAgDMaxGAk51ZTADgwSs8eRAarNJ7JRtLolawcndHgN9q6X3l6t3idxjUT3lateup8H12vdKXUOvXT3f43X6vz9ueW/6XC3du/V/99==


formula: Mn2 Si O4
compound: Synthetic
pub_title: X-ray determination of electron distributions in forsterite, fayalite and tephroite
formula_title: <missing>
a: 4.9023
b: 10.5964
c: 6.2567
alpha: 90
beta: 90
gamma: 90
cell_volume: 325.015
crystal_density: 4.127
atoms_sites: ["Mn1", "Mn2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAEBMPAB4GBoAAEAuAADfDABQhREA
atoms_y: AAAAAGgdEQC44gUA+LYFAOiwGwAAAAoA
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwDghgIA
atoms_occupancy: 0
atoms_u_iso: qHoAAChpAACgSwAAQGoAADBrAACIcgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAFAAAAAAAQBAAAAEgAAABGQgCBIBAggEgRwAOUoC4IEBQIAYy8RRU4K6IgJSQlqJmjRNrm3NEJq1130YHW3g+09pXS21rx9ejXqUn/n7fb2U3T/+DXX/x/p75stI06O6/bn/PH/fv33z79//Tb53==


formula: (Mn1.4 Fe.6) Si O4
compound: Synthetic
pub_title: Fe-Mn cation ordering in fayalite-tephroite (FexMn1-x)2SiO4 olivines: A neutron diffraction study
formula_title: <missing>
a: 4.87890
b: 10.60587
c: 6.20468
alpha: 90
beta: 90
gamma: 90
cell_volume: 321.061
crystal_density: 4.189
atoms_sites: ["MnM1", "FeM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAgwTwAIME8AFAnGgBgbC4A4PkMAPCFEQA=
atoms_y: AAAAAAAAAAAQDBEAEAwRAADcBQDgpgUAgK8bAND9CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPADBpAgA=
atoms_occupancy: QFMhAMC1GwDAHzQAQOkIAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: QEcAAEBHAADgagAA4GoAADBNAACIhgAAqHoAANhyAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAADgAAAAUoQAgiAQYgBQCwADlYAuQCAUEAUMeQMLUDfIoBYUhjZHiQrI3c/FkppubzFD28aOduOVaiy92H7zK7tG7tPvPuifwtRZLrXf5vdfj7Pufp+b9Nrn82t/e9n37v6Z5n9==


formula: (Mn Fe) Si O4
compound: Synthetic
pub_title: Fe-Mn cation ordering in fayalite-tephroite (FexMn1-x)2SiO4 olivines: A neutron diffraction study
formula_title: <missing>
a: 4.86184
b: 10.58358
c: 6.16950
alpha: 90
beta: 90
gamma: 90
cell_volume: 317.456
crystal_density: 4.245
atoms_sites: ["MnM1", "FeM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACgujsAoLo7ABAhGgBAmy4AQAMNAMCNEQA=
atoms_y: AAAAAAAAAACAPBEAgDwRAJDdBQCgoAUAgK8bAGD/CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAABYAgA=
atoms_occupancy: wGIUAECmKABApigAwGIUAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: GFEAABhRAAAYUQAAGFEAAEBHAACoegAAwHYAALh0AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAABwAAAAMYIAgRAIIQAoBYABqcAOoBAJCAKDHoCC6g70KAWFQp0J5CKyFbLyaGSrT8aZqrFilfh3es23vZ72Sunwfr7/pfkJ+n7PRfqt/71M8fI/z8l6b23/+k7d/xVO3P35nl/==


formula: (Mn.6 Fe1.4) Si O4
compound: Synthetic
pub_title: Fe-Mn cation ordering in fayalite-tephroite (FexMn1-x)2SiO4 olivines: A neutron diffraction study
formula_title: <missing>
a: 4.84857
b: 10.55545
c: 6.14054
alpha: 90
beta: 90
gamma: 90
cell_volume: 314.266
crystal_density: 4.295
atoms_sites: ["MnM1", "FeM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADQFjwA0BY8AEAyGgAQvC4AwPYMADCMEQA=
atoms_y: AAAAAAAAAABAHREAQB0RAGDlBQDAowUA8K0bADAHCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAFBTAgA=
atoms_occupancy: oNMJAGA1MwBgyxoAoD0iAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 8GQAAPBkAAA4TwAAOE8AADBNAAC4fgAAqHoAANhyAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAAA4AAAAGMEAQIgEEIAUAcAA0qAG0AQEggDAjyBAsodeFAFBoKpEchBoh+m9Kh0rkfGiSbholX4dXyt9/ze0lq48Hpf/+W9gu1+78Tv5f+3dvRdlWfk2r/3fuvJU/dNp37vda8d==


formula: (Mg.88 Fe.12) Ca Si O4
compound: Crestmore, California, USA
formula_title: <missing>
a: 11.1098
b: 6.3894
c: 4.8281
alpha: 90
beta: 90
gamma: 90
cell_volume: 342.722
crystal_density: 3.106
atoms_sites: ["Mg1", "Fe1", "Ca2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACg5RAAYPoEAJi9BADIZxsAKAEJAA==
atoms_y: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AEMoCAA==
atoms_z: AAAAAAAAAACon/7/kBUZAJB68P/AAw8AUK4QAA==
atoms_occupancy: ALY1AABTBwAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["Mg1", "Fe1", "Ca2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: gHAAAIBwAAAwXAAA4GAAALCaAAAwXAAAkH4AAA==
atoms_aniso_u22: UF8AAFBfAABwYgAAgFcAANCdAADAjwAAQGoAAA==
atoms_aniso_u33: gFcAAIBXAADwbgAAMEMAAHBJAADQawAAMHUAAA==
atoms_aniso_u12: oPb//6D2//8AAAAAAAAAAAAAAAAAAAAAUBQAAA==
atoms_aniso_u13: gPP//4Dz//+wBAAAIAMAAFD7//9w/v//QAYAAA==
atoms_aniso_u23: AOf//wDn//8AAAAAAAAAAAAAAAAAAAAAIAMAAA==
pub_title:
 Thermal parameters for minerals of the olivine group:
 their implication on vibrational spectra,
 thermodynamic functions and transferable force fields

qdat:
AAAAAAAAAAAAAAAAAABAAAACAgAQDAAABQACADAQEQAOIAEIIAgBCCMQEkBBGIhAgPQRRGAshUC6Bw2wbEwGR8b1Fp4KP06OjgZX5VeHjoLVf6Y5oPn2rac+9MOrT7Tw4xV/8wV08zbs50x36u3OGa973xmudf6nPW57yu==


formula: Ni Rh As
compound: Synthetic
pub_title: Zaccariniite, RhNiAs, a new platinum-group mineral from Loma Peguera, Dominican Republic
formula_title: <missing>
a: 3.5498
b: 3.5498
c: 6.1573
alpha: 90
beta: 90
gamma: 90
cell_volume: 77.589
crystal_density: 10.124
atoms_sites: ["Ni", "Rh", "As"]
atoms_x: wMYtAEBCDwBAQg8A
atoms_y: QEIPAEBCDwBAQg8A
atoms_z: AAAAAED/FQBA0y0A
atoms_occupancy: 0
atoms_u_iso: +FwAAIgxAACQKQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAgAAAAAAAgAIAAAAAAwAAAAAAAAAgAAAAEAwAAAAwAAAAAABAAAAgEAAACAAAAAAAAABgwAABAAAAAEAABBgAAwAAAAIAAAEAAMAAAAQAAhAACAAAAgA==


formula: Fe Si2
compound: Luobusha, Tibet
pub_title: X-ray diffraction investigation of native Si-Fe alloy minerals from Luobusha, Tibet
formula_title: <missing>
a: 2.725
b: 2.725
c: 5.202
alpha: 90
beta: 90
gamma: 90
cell_volume: 38.628
crystal_density: 4.815
atoms_sites: ["Fe", "Si"]
atoms_x: gIQeAAAAAAA=
atoms_y: gIQeAAAAAAA=
atoms_z: AAAAABCPEAA=
atoms_occupancy: 0
atoms_u_iso: QB8AAMBdAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAAAAAEAIAAIAAAAAAAAAAICAAgAIAAAAAACAAACAAAABAAEEQAAAAhAIQAAAAAgASAACAAAAgACCAEIAAIJAhAABEQQIADAgAQAMAAKAAEAjAAQIBQAQAAwAhAgABFBMgEkIS==


formula: Be2 B O3.96 H.96 F.04
compound: Anjanabonoina mine, Madagascar
pub_title: A single-crystal neutron diffraction study of hambergite, Be2BO3(OH,F)
formula_title: <missing>
a: 9.762
b: 12.201
c: 4.430
alpha: 90
beta: 90
gamma: 90
cell_volume: 527.640
crystal_density: 2.365
atoms_sites: ["Be1", "Be2", "B", "O1", "O2", "O3", "O4", "H", "F4"]
atoms_x: yCgAAOB6DgDoegYAgEsCAEAtBgB4aAsAwLwUACAnEwDAvBQA
atoms_y: mIQLAMgfBACAiAYAMHQLALBJBgAQGwIAcI8KAECZDQBwjwoA
atoms_z: UOEPAMjqEADQLS8AEMolAOABBQDIqCUAABESAODqGwAAERIA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAJg6AACYOgAAcQIA
atoms_u_iso: uGUAAJBlAAB4RgAA6GwAAOhnAAA4cgAAGIMAAOBzAQAYgwAA
atoms_aniso_label: ["Be1", "Be2", "B", "O1", "O2", "O3", "O4", "H", "F4"]
atoms_aniso_u11: gHAAAOB5AADgRwAA0J0AAJB+AABAnAAAkGUAAPBoAQCQZQAA
atoms_aniso_u22: wF0AADBcAAAQQAAAgFcAAIBwAABAagAAkH4AACBhAQCQfgAA
atoms_aniso_u33: cGIAAKBaAAAQQAAAQFEAAHBJAACwTwAAoKUAACCTAQCgpQAA
atoms_aniso_u12: sAQAAIAMAABwFwAAoCgAAKAoAADwPAAAcOX//5Do//9w5f//
atoms_aniso_u13: 4Pz//yADAABw/v//YPD//+D8//8QDgAAMBEAAMBdAAAwEQAA
atoms_aniso_u23: SP7//3D+//+wBAAA4Pz//3D+//8QDgAAkOj//0BX//+Q6P//
qdat:
AAAAAAAAAAAAAAAAAQAAAEAQAAAMAQAQAkIAUAAAFiBmAARMkS4EiEDpCTmbGgSBu0SpjoiU/1CCy8tdbmlqqTpm++eWOe28yqv//5Lbf6k/br+bfYrXVPF+9832311e99r6Zs5f2+ssa79+3v9vcehv/FN2rFin3nFYyR==


formula: Ca10 P6 O24 Se
compound: Synthetic
pub_title: The chalcogenide phosphate apatites Ca10(PO4)6S, Sr10(PO4)6S, Ba10(PO4)6S and Ca10(PO4)6Se
formula_title: Ca10(PO4)6Se
a: 9.5007
b: 9.5007
c: 6.8406
alpha: 90
beta: 90
gamma: 120
cell_volume: 534.732
crystal_density: 3.259
atoms_sites: ["Ca11", "Ca12", "Ca2", "P", "O1", "O2", "O31", "O32", "Se"]
atoms_x: VVgUAFVYFACQPQ8AkGsYABDhEwBwvCMAcHMSAADtFwAAAAAA
atoms_y: q7AoAKuwKACANDwAAKgWAPC6HQBQmBwAQEgOAGDPEQAAAAAA
atoms_z: UFkBAKAdHwBAQg8AwBwPABBKDwBgwQsAgM8FAEBFGwCAhB4A
atoms_occupancy: 0
atoms_u_iso: sDYAALA2AACwNgAA4HkAAKCMAACgjAAAoIwAAKCMAABgVAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAACAAIAAABAAgAAEBAACCAASAAAiQBAQAAgFiCIgBgESAUAkIKIQEKBlYJEhDA1AwEMbFGGkKOFUAAZ80hiqUYSJCMLxyk4sMYzNYqoz8VjW3M3EvWb9do+5xlb2XvqX9+y/Mlu67NUmzHT7P7p/m5Bv3li1==


formula: Sr10 P6 O24 S
compound: Synthetic
pub_title: The chalcogenide phosphate apatites Ca10(PO4)6S, Sr10(PO4)6S, Ba10(PO4)6S and Ca10(PO4)6Se
formula_title: Sr10(PO4)6S
a: 9.8077
b: 9.8077
c: 7.2089
alpha: 90
beta: 90
gamma: 120
cell_volume: 600.529
crystal_density: 4.087
atoms_sites: ["Sr11", "Sr12", "Sr2", "P", "O1", "O2", "O31", "O32", "S"]
atoms_x: VVgUAFVYFACo/Q4A4E0YAJA4FACQdCMA0McSAND6FgAAAAAA
atoms_y: q7AoAKuwKACQPTwAkJAWAPBvHQBwNxwAcNYOAEA2EQAAAAAA
atoms_z: 8E8BAKCBHwBgvQ8AMBsPAGA/EABw4gwAoIcFANBMGgCAhB4A
atoms_occupancy: 0
atoms_u_iso: sG0AALBtAACwbQAAYDsAAODEAADgxAAA4MQAAODEAACQsAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAIAEAAAAgAIAACBAACgAECAACggQCAACCEYBgEIgKASECEQYIAzQcgTDATQYMSSkuakMWJsYASZudkjchg0zRPvCmzCpLmrZXXXOpVpvo/DVRbV+J9e6k21H+vqbpu14u7e/wvdbLT9/n+LqvfDqbvxf9k6==


formula: Ba10 P6 O24 S
compound: Synthetic
pub_title: The chalcogenide phosphate apatites Ca10(PO4)6S, Sr10(PO4)6S, Ba10(PO4)6S and Ca10(PO4)6Se
formula_title: Ba10(PO4)6S
a: 10.252
b: 10.252
c: 7.659
alpha: 90
beta: 90
gamma: 120
cell_volume: 697.140
crystal_density: 4.705
atoms_sites: ["Ba11", "Ba12", "Ba2", "P", "O1", "O2", "O31", "O32", "S"]
atoms_x: VVgUAFVYFADo9A4AoHkYAACVFQBQ8SIAAP8UAKCRFAAAAAAA
atoms_y: q7AoAKuwKACg9jsAoLcWANCFHQCwKhsAQPcOAJCVEQAAAAAA
atoms_z: 4N0AACAqHwDg5w8AABAOAMBuEgBgJQwAwLwFAACcGACAhB4A
atoms_occupancy: 0
atoms_u_iso: MMAAADDAAAAwwAAAoHMAAMBRAgDAUQIAwFECAMBRAgDAXQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAABACAAAAgAEAACEAAIABAQAAwIQAgABkGQCBAYAQEMAQ2BgBYkEINhAzAxYIBb4jCxBoECMD3iMsQ1AsYLcSLKVF8wPy5qliewr7ytVLOj+o66FSj/P7WzoT/vj77DuXt29r++79Svz/eG1dNu75H3Judbvd==


formula: Li.91 Mn.8 Fe.183 P O4
compound: Koktokay No. 3 granitic pegmatite, Altai Mountains, northwestern China
pub_title: A structural study of the lithiophilite-sicklerite series Sample 1, colorless
formula_title: <missing>
a: 4.736
b: 10.432
c: 6.088
alpha: 90
beta: 90
gamma: 90
cell_volume: 300.783
crystal_density: 3.433
atoms_sites: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_x: AAAAAOBSOwDgUjsA4AsZABCvLABw4gwAgPEQAA==
atoms_y: AAAAADAyEQAwMhEAYKkFAEjpBQAo1RsAgOQJAA==
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBAQg8AoP0CAA==
atoms_occupancy: wIo3AADUMABgKwsAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: APoAADBwAAAwcAAAGGUAALCaAACAiQAAcJQAAA==
atoms_aniso_label: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_aniso_u11: YOoAAJB+AACQfgAAMFwAAIBXAAAggAAAYIYAAA==
atoms_aniso_u22: oAkBAABkAAAAZAAAwF0AAPCgAABgbQAAoKUAAA==
atoms_aniso_u33: oAkBAPBuAADwbgAAMHUAABDWAAAArwAAMI4AAA==
atoms_aniso_u12: 4LH///gHAAD4BwAA4Pz///Dx//+gDwAAsB0AAA==
atoms_aniso_u13: oJL//wAAAAAAAAAAAAAAAAAAAAAAAAAAoPb//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA8CMAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAwAAAAAAAgBAAAAOAAAABRQQAQMAEEgBEFkAAwsAGQAQCCAFAnoBGpgL6CIJGMJOg3gKYlpz2oeiky3zWbOr66W6tqnmhv7qj5MTuDXv77y/6PdXley5ouf2+dfvf0m7LTO/dv42i/nv5HsRf/Z==


formula: Li.86 Mn.8 Fe.183 P O4
compound: Koktokay No. 3 granitic pegmatite, Altai Mountains, northwestern China
pub_title: A structural study of the lithiophilite-sicklerite series Sample 2, light yellow
formula_title: <missing>
a: 4.7340
b: 10.423
c: 6.0940
alpha: 90
beta: 90
gamma: 90
cell_volume: 300.693
crystal_density: 3.426
atoms_sites: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_x: AAAAADBTOwAwUzsA8AoZAGCqLACg2gwAAP4QAA==
atoms_y: AAAAAFgyEQBYMhEAeKoFAIDtBQCY0xsA+OQJAA==
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBAQg8AoP0CAA==
atoms_occupancy: gH00AADUMABgKwsAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: UNwAAJB+AACQfgAAIHYAACCyAADQnQAA8KAAAA==
atoms_aniso_label: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_aniso_u11: YOoAADCOAAAwjgAA8G4AAMB2AACgjAAAUJEAAA==
atoms_aniso_u22: APoAAFhwAABYcAAAoHMAADDAAABwewAA4MQAAA==
atoms_aniso_u33: 4KsAAAB9AAAAfQAAkH4AAHDfAABg0QAAEIsAAA==
atoms_aniso_u12: 0KP//+gIAADoCAAAIAMAAHD+//9wFwAAkBoAAA==
atoms_aniso_u13: IJ///wAAAAAAAAAAAAAAAAAAAAAAAAAAcP7//w==
atoms_aniso_u23: gPP//wAAAAAAAAAAAAAAAAAAAAAAAAAAwCsAAA==
qdat:
AAAAAAAAAAAAAAAAAAABQAAAAAAAgBAAAAOAAAABRQQAQMAEGgBEFUAAxsAHIAQCCAAhG4BG5ALqCIJGKJKg3wMUmpzqoeiky7yWXV62a25dmnqx/3qj5MT2DPvv7y36Wva3+z4t6fv+b+n35n7NjP//vp/z1nv5H8Tf2R==


formula: Li.84 (Mn.8 Fe.2) P O4
compound: Koktokay No. 3 granitic pegmatite, Altai Mountains, northwestern China
pub_title: A structural study of the lithiophilite-sicklerite series Sample 3, yellow
formula_title: <missing>
a: 4.7403
b: 10.4145
c: 6.0795
alpha: 90
beta: 90
gamma: 90
cell_volume: 300.132
crystal_density: 3.451
atoms_sites: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_x: AAAAAFhOOwBYTjsA8A8ZAMCaLACQswwAkOsQAA==
atoms_y: AAAAAAAwEQAAMBEAsK4FAFj8BQDI0BsAUOwJAA==
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBAQg8AoP0CAA==
atoms_occupancy: AEUzAADUMAAANQwAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: EAgBAAiEAAAIhAAAaG8AALCzAADwoAAA8KoAAA==
atoms_aniso_label: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_aniso_u11: 4CgBALiSAAC4kgAAEGgAAOB5AABAnAAA0J0AAA==
atoms_aniso_u22: 0AEBADB6AAAwegAAQG8AAMDaAAAAfQAAIMsAAA==
atoms_aniso_u33: YOoAAFh/AABYfwAAEHcAAHDGAAAgywAAIJkAAA==
atoms_aniso_u12: MK3//ygFAAAoBQAA+AIAAMD5//8QDgAAsB0AAA==
atoms_aniso_u13: MJT//wAAAAAAAAAAAAAAAAAAAAAAAAAAsAQAAA==
atoms_aniso_u23: EPX//wAAAAAAAAAAAAAAAAAAAAAAAAAAkDMAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAwAAAAAAAgBAAAAGAAAABQwQAQKAEEgBEC0AAw8AHIAQDBAEgn0BKtgLZBIIlEFNgvwKcYs3bYZTsxrzOPKb+ZK+s+zlR9/5T4sTuirv9YrVuJ32zfr047vt85tvf63XJrPZtv4/r3SvdG+F/+z==


formula: Li.76 Mn.8 Fe.18 P O4
compound: Koktokay No. 3 granitic pegmatite, Altai Mountains, northwestern China
pub_title: A structural study of the lithiophilite-sicklerite series Sample 4, orange
formula_title: <missing>
a: 4.7670
b: 10.403
c: 6.0720
alpha: 90
beta: 90
gamma: 90
cell_volume: 301.117
crystal_density: 3.402
atoms_sites: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_x: AAAAAOg7OwDoOzsAcBIZALCMLADgYwwAMN0QAA==
atoms_y: AAAAAMgrEQDIKxEA2LgFAHAlBgAIzRsAMP0JAA==
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBAQg8AkAgDAA==
atoms_occupancy: AGMuAADUMACA/AoAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 4CgBABB8AAAQfAAAcHsAABDWAADgxAAAsMwAAA==
atoms_aniso_label: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_aniso_u11: gDgBAGCGAABghgAAcGIAAEBqAADgxAAA8KAAAA==
atoms_aniso_u22: APoAADB1AAAwdQAA0IQAAIAfAQCwmgAAgAYBAA==
atoms_aniso_u33: IEgBAFB4AABQeAAAEIsAAOD2AAAQ7wAAEL0AAA==
atoms_aniso_u12: YHP//4j///+I////AAAAAGDw//8gAwAA8CMAAA==
atoms_aniso_u13: IFT//wAAAAAAAAAAAAAAAAAAAAAAAAAAQO3//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQDgAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAwAAAAAAAgCAAAAFAAAAApQQAgUAQIgBIC4ABxcALIAgFBAFBT0BhdQO1CgFRMFNhfQRXUlZ7JoNpnPxZi62MtN+nu3o63+xd5ZW7kVm87zdqlWh326P1+Vq/9dw7J+2ble7N/pWn93z7N7XW3/==


formula: Li.748 Mn.8 Fe.195 P O4
compound: Koktokay No. 3 granitic pegmatite, Altai Mountains, northwestern China
pub_title: A structural study of the lithiophilite-sicklerite series Sample 5, deep orange
formula_title: <missing>
a: 4.7651
b: 10.3379
c: 6.0595
alpha: 90
beta: 90
gamma: 90
cell_volume: 298.498
crystal_density: 3.449
atoms_sites: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_x: AAAAAJA0OwCQNDsACBYZAMCBLACQNgwAoNYQAA==
atoms_y: AAAAAHApEQBwKREAsL0FAHg7BgC4xxsAIAMKAA==
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBAQg8AwAADAA==
atoms_occupancy: gKctAADUMADg5gsAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: wFcBAHiRAAB4kQAAqIQAAGDqAACA1AAAMN4AAA==
atoms_aniso_label: ["Li1", "Mn2", "Fe2", "P", "O1", "O2", "O3"]
atoms_aniso_u11: 4CgBAKCbAACgmwAA0HAAAGCGAACA7QAAEL0AAA==
atoms_aniso_u22: 4CgBAAiOAAAIjgAAyJEAAOBBAQBQqgAAcBEBAA==
atoms_aniso_u33: 4KUBAJiKAACYigAAiIsAAFD1AACw5QAAsMwAAA==
atoms_aniso_u12: YIz//2D6//9g+v//AAAAAKD2//9ABgAAIBwAAA==
atoms_aniso_u13: AGr//wAAAAAAAAAAAAAAAAAAAAAAAAAAoPb//w==
atoms_aniso_u23: UOL//wAAAAAAAAAAAAAAAAAAAAAAAAAAcEkAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAoAAAAAAAgCAAAAEgAAAAkoQAgSAQIQAoBMAA5TAFRAQCgQAgz4hQk4O+QwCYYhHpNSIpUW9bxxGsbn+w4ennhjlx7ZsLK3sbmmZ21Ez/OrPtidYf1sVNvfd77b4bo2X9X3Pkm+djZv+9te7P3W==


formula: Fe.96 Si2
compound: <missing>
pub_title: Rietveld structure refinement of new mineral luobusaite (beta-FeSi2)
formula_title: <missing>
a: 9.8362
b: 7.8301
c: 7.8655
alpha: 90
beta: 90
gamma: 90
cell_volume: 605.788
crystal_density: 4.815
atoms_sites: ["Fe1", "Fe2", "Si1", "Si2"]
atoms_x: iIkvAAAAAACwNAcAACEWAA==
atoms_y: AAAAAGBhDAAA+g8AwIcDAA==
atoms_z: AAAAAEj1MAAQQgMASAUNAA==
atoms_occupancy: AAk9AAAnOAAACT0AAAk9AA==
atoms_u_iso: 0BYAAPAZAACwOwAAyEsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAKAAAACAABACAAwACSAAAAEOAAAAgIYAlsAQlLAjAgANQgCF66kDBYxsFCHRoKC48af8iO1JcSa04jHbvksEzau3e1cpq5fc7lQ161rvTv35sh/xs+/9v+s95//H5t2XxufOu9kO5v6x78X0kl==


formula: Cd1.58 Ag1.994 Pb.426 As2 S6
compound: Lengenbach, Binntal, Switzerland
pub_title: Quadratite, AgCdAsS3:Chemical composition, crystal structure and OD character
formula_title: <missing>
a: 5.5229
b: 5.5229
c: 33.399
alpha: 90
beta: 90
gamma: 90
cell_volume: 1018.750
crystal_density: 5.367
atoms_sites: ["CdM1", "AgM1", "CdM2", "AgM3", "PbM3*", "As", "S1", "S2", "S3"]
atoms_x: UNMOAFDTDgBgDi0AgKctAIAqLQBwng8AwIwNAGCQKADgPg4A
atoms_y: UNMOAFDTDgBgDi0AgGcOAEDFDgCwbS0AQPIsAJA+LABA4wkA
atoms_z: IKEHACChBwAgoQcAkA4CAJCLAgD4BAMASD0HAKDkAgD43AIA
atoms_occupancy: gGYjAICiGQAACT0A4AgwACAADQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: UHIBAFByAQAwbwEAAHcBAAB3AQAARQEAEDoBAOCMAQAARQEA
atoms_aniso_label: ["CdM1", "AgM1", "CdM2", "AgM3", "PbM3'", "As", "S1", "S2", "S3"]
atoms_aniso_u11: YIABAGCAAQCwYgEA8IEBAPCBAQDgQQEAAHcBAIC1AQAA+gAA
atoms_aniso_u22: YIABAGCAAQCwYgEA4L4BAOC+AQBASwEAQBkBAMBXAQCgAwIA
atoms_aniso_u33: wFcBAMBXAQAQhQEA4CgBAOAoAQBQQAEA4CgBAECWAQDA2gAA
atoms_aniso_u12: oA8AAKAPAABg8P//QO3//0Dt//9g8P//QB8AAEAfAABAHwAA
atoms_aniso_u13: cP7//3D+//9Q+///YPD//2Dw//8Q9f//4C4AAIA+AADgLgAA
atoms_aniso_u23: kAEAAJABAACwBAAA4C4AAOAuAACQAQAAQB8AAGDw//+gDwAA
qdat:
AAAAAAAAAAAAEAAAAAAwgQCACgDgEiAkAAiACAkgggNFQUIJAYAgCCEhBywwqoxFAgICOkRBBAgRVEexM0wYR6JEIIEAAAByTdlRCC9JEQhKoEWqSL1PtYiEsutYiIAdUSIgDqerPy+uREAAOsSR0yJH17skvUpEA69d0k==


formula: Mg2 Si O4
compound: Synthetic
pub_title: High-temperature structural behaviors of anhydrous wadsleyite and forsterite Note: T = 297 K
formula_title: <missing>
a: 5.7016
b: 11.4427
c: 8.2491
alpha: 90
beta: 90
gamma: 90
cell_volume: 538.185
crystal_density: 3.473
atoms_sites: ["Mg1", "Mg2", "Mg3", "Si1", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAAAAAAAAAAAAAAAEEAA=
atoms_y: AAAAAEBCDwBg2QcAsD4HAEBCDwBAQg8AEJo8ADB9BwA=
atoms_z: AAAAAOBcOwBAQg8AcLAlAJBJDQAw0SsAQI0PABCzPAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAACAAIAAAIAAIAABAQICAAACAAQgiJAGAgmIABBAChEkCAOkICAQIioEchICVF28GJFABQpkCmVQYR2WhUyONOapVIWnL1OkEZvhevHa8XzocH0q6jv/Qu541xYzwflJXmYd3HNlT50uENcfYLzNgaJzX==


formula: Mg2 Si O4
compound: Synthetic
pub_title: High-temperature structural behaviors of anhydrous wadsleyite and forsterite Note: T = 728 K
formula_title: <missing>
a: 5.7214
b: 11.4789
c: 8.2924
alpha: 90
beta: 90
gamma: 90
cell_volume: 544.607
crystal_density: 3.432
atoms_sites: ["Mg1", "Mg2", "Mg3", "Si1", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAAAAAAAAAAAAAPAOEAA=
atoms_y: AAAAAEBCDwAA0AcAwEwHAEBCDwBAQg8AMIQ8AKB7BwA=
atoms_z: AAAAAHBFOwBAQg8AcLAlAEAcDQAw6isAkKEPAGCuPAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAEAAQAAAQAAIAABAQQEAAAGAAhBESAMBCMgAECAGFKIEA5IQIBAxKQRyEQI0PXoVkUADDmQG5VjhNacFzIw85svkis8+1cghO8O955sm2aHAun3MZ/+DstOnTM+DspY4vDspn80WNPwjNj9B4xoDkcd1==


formula: Mg2 Si O4
compound: Synthetic
pub_title: High-temperature structural behaviors of anhydrous wadsleyite and forsterite Note: T = 929 K
formula_title: <missing>
a: 5.7321
b: 11.4998
c: 8.3163
alpha: 90
beta: 90
gamma: 90
cell_volume: 548.194
crystal_density: 3.409
atoms_sites: ["Mg1", "Mg2", "Mg3", "Si1", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAAAAAAAAAAAAAHAbEAA=
atoms_y: AAAAAEBCDwDQ8AcAQEAHAEBCDwBAQg8AsHc8ALCJBwA=
atoms_z: AAAAAJAvOwBAQg8AsJ0lAEA1DQAwnysAoH0PALCpPAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAEAAQAAAQAAQAACAgQEAAAEABCBIiAICCYgAICAMKUQEAyQgQCBmUgjkIghoevQqIsAGHtgJSzGEy14SmRjZzaeJJZy6yxDCv41z1nbPdcOC9fcpl9sPyyuaqxoX6lzksfXkezJUy9iLUP4HjPgORplV==


formula: Mg2 Si O4
compound: Synthetic
pub_title: High-temperature structural behaviors of anhydrous wadsleyite and forsterite Note: T = 1084 K
formula_title: <missing>
a: 5.7391
b: 11.5134
c: 8.3350
alpha: 90
beta: 90
gamma: 90
cell_volume: 550.748
crystal_density: 3.394
atoms_sites: ["Mg1", "Mg2", "Mg3", "Si1", "O1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAABAQg8AAAAAAAAAAAAAAAAAAAAAAJA3EAA=
atoms_y: AAAAAEBCDwBg2QcAsFcHAEBCDwBAQg8AgH88APCoBwA=
atoms_z: AAAAAGAFOwBAQg8AgKUlAIAiDQAgqisA8JEPALCpPAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAEAAQAAAQAAQAACAggIAAAMABCBJCAYCEZAAIEAMUkQIByxAwEDGUhFIZAhw3dg2pYAMXagajWKFU6wjMjCzmi8SU3V2liGFeh7vvO6ua48Fq+5XP7IfFlU1ZHg9pGrJofs43WVTJ+EpU3wPObA9FTP1==


formula: K3 Na Fe Cl6
compound: Synthetic
formula_title: <missing>
a: 8.3376
b: 8.3376
c: 8.3376
alpha: 92.29
beta: 92.29
gamma: 92.29
cell_volume: 578.166
crystal_density: 2.348
atoms_sites: ["K", "Na", "Fe", "Cl"]
atoms_x: cLAHAEBCDwCAhB4AkJwZAA==
atoms_y: ENQWAEBCDwCAhB4A8PgMAA==
atoms_z: wMYtAEBCDwCAhB4AAEghAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal and molecular structures of rinneite, sodium tripotassium hexachloroferrate(II),
 and hexaamminecobalt(III) hexachloroferrate(III). Comparison of iron-chloride distances
 in hexachloroferrates(II) and -(III)

qdat:
AAAAAAAAAAAAAAAAAAQAAAAAAAAACAABAAAAICAQAABAAAAACAAAIBEAAQAQAAACAAkAiAUACAAEEAKAQAQBADAIAEBAMAgEAQDAIBgIBAYCAgIBAQODAIOCBIIBAAAkGKkwQiSEkZiAUgAiIqUEQRCEREQBEEgJICEYIM==


formula: Fe Co Cl6 N6 H18
compound: Synthetic
formula_title: Co(NH3)6FeCl6
a: 11.2506
b: 11.2506
c: 11.2506
alpha: 90
beta: 90
gamma: 90
cell_volume: 1424.056
crystal_density: 2.004
atoms_sites: ["Fe", "Co", "Cl", "N", "H1", "H2", "H3"]
atoms_x: AAAAAICEHgBgmvv/cJ0kAKA3IwDg5ygAMLAkAA==
atoms_y: AAAAAICEHgAwDggAMIsmAKAHKwBgHyYA4PMmAA==
atoms_z: AAAAAICEHgAALgkA4AkbAHBQHAAgbhwAMG4WAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal and molecular structures of rinneite, sodium tripotassium hexachloroferrate(II),
 and hexaamminecobalt(III) hexachloroferrate(III). Comparison of iron-chloride distances
 in hexachloroferrates(II) and -(III)

qdat:
AAAAAAAAAAAAAAAAQACABABAAAIAgABAQEBAAQIEECCCACEEIAQgCEIhCIBCIhEQERERECQECIEiRJAkiSQJJJIJJBQSSUgpKSApKQpIkKEqEpUiVChVAgVUiKpBVSCIoiCigiERBQAEkQAgAiBAAACQAAAAgAAAAQAAAA==


formula: K3 Na Mn Cl6
compound: Salton Sea, California, USA
pub_title: Saltonseaite, K3NaMn2+Cl6, the Mn analogue of rinneite from the Salton Sea, California
formula_title: <missing>
a: 12.0966
b: 12.0966
c: 13.9555
alpha: 90
beta: 90
gamma: 120
cell_volume: 1768.490
crystal_density: 2.298
atoms_sites: ["K", "Na", "Mn", "Cl"]
atoms_x: YLsRAAAAAAAAAAAAuBQLAA==
atoms_y: VVgUAAAAAAAAAAAA6KcBAA==
atoms_z: CBYFAEBCDwAAAAAAQKUGAA==
atoms_occupancy: 0
atoms_u_iso: iKMBAFDCAQDgAAEAIGsBAA==
atoms_aniso_label: ["K", "Na", "Mn", "Cl"]
atoms_aniso_u11: eJoBAIAZAgCoCwEAAEUBAA==
atoms_aniso_u22: sI8BAIAZAgCoCwEASMoBAA==
atoms_aniso_u33: sLwBACAWAQAA6wAA0FEBAA==
atoms_aniso_u12: 2McAAHAMAQDohQAAsNsAAA==
atoms_aniso_u13: MNX//wAAAAAAAAAASMz//w==
atoms_aniso_u23: YKr//wAAAAAAAAAAUPb//w==
qdat:
AAAAAAAAAAAAAAAAAIgAAAAAAgAEIAoCAACAhAAggICAQhRAQAggxEQgTGJAhIGaRCoZSKoE1CUnUi1ModWag6DVJU0TwPpCGSFiqdmx6NpSbDpibXMtLXTQIbUzJ4XOEqzAeqQOCENiZApRAyAZkGoIwAiBJFBgEASACQ==


formula: Ca3 Ge S2 O17 H12
compound: Tsumeb, Namibia
pub_title: Schaurteite, Ca3Ge(SO4)2(OH)6*3H2O
formula_title: <missing>
a: 8.5253
b: 8.5253
c: 10.8039
alpha: 90
beta: 90
gamma: 120
cell_volume: 680.034
crystal_density: 2.642
atoms_sites: ["Ca", "Ge", "S", "O1", "O2", "O3", "O4", "H1", "H2"]
atoms_x: +IsSAAAAAABVWBQAVVgUACA2HQBwGwYAIP0eAMCqCABgJCEA
atoms_y: 6EUJAAAAAACrsCgAq7AoABCbDgCQNgwA4AseAIBVEQCg5BsA
atoms_z: QEIPAAAAAACYGiAAIMAGAAg6BADwswYAwMYtAOCTBABgayoA
atoms_occupancy: 0
atoms_u_iso: +KwAABB3AAB4lgAA8AQBAOAoAQCgpQAA4CgBAIC1AQDgHAMA
atoms_aniso_label: ["Ca", "Ge", "S", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: IJkAADCJAADAqAAAEFMBACCyAACwzAAAcHUBAA==
atoms_aniso_u22: sMwAADCJAADAqAAAEFMBALB7AQBghgAAcHUBAA==
atoms_aniso_u33: MI4AANBSAAAQcgAAsGgAABAIAQDwhwAAcN8AAA==
atoms_aniso_u12: uEwAAJhEAAAQVAAAUKoAABBZAAAwQwAA4PYAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAPA8AADA+f//AAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAEAfAACA8///AAAAAA==
qdat:
AAAAAAAAAAAAAAQAAQAIAAAAkAAAIAgIIAIAAEBACIMCABCEgQEUhAiASERBgJGSXiABKYFUgmCiSEFkl4EIVzZYuZCjD1igSlw6xwKlxjt0jPHyM1cwueAixXLKqxn2p9stRUM6iY7nxhWTt4j5mebJXZG50a0xcqXHmR==


formula: Ca3 V2 O8
compound: synthetic at 11 GPa and 1373 K
pub_title: Crystal structure of Ca3(VO4)2 synthesized at 11 GPa and 1373 K
formula_title: Ca3(VO4)2
a: 9.6715
b: 5.43276
c: 7.0713
alpha: 90
beta: 116.949
gamma: 90
cell_volume: 331.201
crystal_density: 3.511
atoms_sites: ["Ca1", "Ca2", "V", "O1", "O2", "O3"]
atoms_x: AAAAAFDPMABgKyQAwMwsAEAjKQAQmR8A
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAgaxAA
atoms_z: AAAAACBtGADAui8A4CYrAECQAgAgqhIA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAACAAAAABAIAAAAAAIAQAQAAEAAQgACEAACJRAQAAAAAgiAAliEAEAICUAFAQYJgBApBFjiAAQAQKfJhACMQEHGBBgsLdkAASqdagCpAx6vEdHinwKEdl4FtFIiYsOdDvREmQJMVvwyLVibGTERHxF6L==


formula: Fe1.27 Si.62 Ni.05 Cr.01 P.06
compound: lunar meteorite Dhofar 280 from Oman
pub_title: Space weathering on airless planetary bodies: Clues from the lunar mineral hapkeite
formula_title: <missing>
a: 2.831
b: 2.831
c: 2.831
alpha: 90
beta: 90
gamma: 90
cell_volume: 22.689
crystal_density: 6.854
atoms_sites: ["Fe", "Si", "Fe", "Ni", "Cr", "P"]
atoms_x: AAAAAICEHgCAhB4AgIQeAICEHgCAhB4A
atoms_y: AAAAAICEHgCAhB4AgIQeAICEHgCAhB4A
atoms_z: AAAAAICEHgCAhB4AgIQeAICEHgCAhB4A
atoms_occupancy: AAk9AIDXJQDAehAAQA0DAECcAACAqQMA
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAIAAAAAAAAAAAgAAAAAAAAAgAAAAAAACAAAAAAACAAAAAAAAAAAAACAAAAAAgAAAAAgAAAACAAAAAQAAAAIAAAAIAAAAAAAABAAAAEAAABAAAAQAAAI==


formula: Fe3 Si
compound: Synthetic
formula_title: <missing>
a: 5.644
b: 5.644
c: 5.644
alpha: 90
beta: 90
gamma: 90
cell_volume: 179.788
crystal_density: 7.227
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: gIQeAEBCDwAAAAAA
atoms_y: gIQeAEBCDwAAAAAA
atoms_z: gIQeAEBCDwAAAAAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Stability of crystal structure of (Fe,V)3M and (Fe,Ni)3M (M=Si,Ge,Sn)
 and its analysis based on rigid band model

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAQAAAAAAAAAAAAAAEAAAAAAAAEAAIAAAAAAAAAQAAAAABAAgAAAAAABAAAAAEAAAAAAAAgAAABAIAAAAAIAAACAgAAAAEAAAEBAAAABAAAEAAAAAEAABAgAAAEAACCAAAA==


formula: Fe3 Si
compound: Synthetic
pub_title: Magneto-optical properties of metallic ferromagnetic materials
formula_title: <missing>
a: 5.662
b: 5.662
c: 5.662
alpha: 90
beta: 90
gamma: 90
cell_volume: 181.514
crystal_density: 7.159
atoms_sites: ["Fe1", "Fe2", "Si"]
atoms_x: gIQeAEBCDwAAAAAA
atoms_y: gIQeAEBCDwAAAAAA
atoms_z: gIQeAEBCDwAAAAAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAgAAAAAAAAAAAAAAIAAAAAAAAIAAgAAAAAAAAAgAAAAACACAAAAAAACAAAAAQAAAAAAACAAAAEAgAAAAAgAAAICAAAAAQAAAQIAAAAIAAAgAAAABAAAEEAAABAAAQQAAAI==


formula: Ag1.87 Cu.13 (Zn.61 Fe.36 Cd.03) Sn S4
compound: Pirquitas, Jujuy Province, Argentina
pub_title: Pirquitasite, Ag2ZnSnS4
formula_title: <missing>
a: 5.7757
b: 5.7757
c: 10.8696
alpha: 90
beta: 90
gamma: 90
cell_volume: 362.596
crystal_density: 4.766
atoms_sites: ["Ag1", "Ag2", "Cu", "Zn", "Fe", "Cd", "Sn", "S"]
atoms_x: AAAAAAAAAAAAAAAAgIQeAICEHgCAhB4AgIQeAFC1LAA=
atoms_y: AAAAAICEHgCAhB4AAAAAAAAAAAAAAAAAgIQeAOBqDwA=
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBAQg8AAAAAAFjXBwA=
atoms_occupancy: AAk9AMAZNQBA7wcAQDslAAD5FQDA1AEAAAk9AAAJPQA=
atoms_u_iso: wDgCAFDWAQBQ1gEAwFcBAMBXAQDAVwEAwLcAAGBOAQA=
atoms_aniso_label: ["Ag1", "Ag2", "Cu", "Zn", "Fe", "Cd", "Sn", "S"]
atoms_aniso_u11: gDICACCsAQAgrAEAgIMBAICDAQCAgwEAILIAAKCGAQA=
atoms_aniso_u22: gDICACCsAQAgrAEAgIMBAICDAQCAgwEAILIAAEBLAQA=
atoms_aniso_u33: QEUCALAqAgCwKgIAsP4AALD+AACw/gAAUMMAANAaAQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAANBSAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABDc//8=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAMBEAAA=
qdat:
AAAAAAAAAAAAAAAAAAAIEAAAACAAAAAAgAQAIAEAAiAAAAIAABAMAgBQAJAAECAwQAgAQhAEGAAoAoCIQ0QIAQiAChAQFAkS4AQCSBOgIDAED0GBUgmEMCCCMggYAnAIYKTAYNQRIAwkXAg6EoMAQuRBADEwxUiAKgYIYJ==


formula: Fe.85 Mg.49 Mn1.66 P2 O8
compound: La Empleada pegmatite, San Luis Province, Argentina
formula_title: <missing>
a: 6.088
b: 4.814
c: 10.484
alpha: 90
beta: 89.42
gamma: 90
cell_volume: 307.245
crystal_density: 3.681
atoms_sites: ["Fe2+M1", "MgM1", "Mn2+M2", "MgM2", "P", "O1", "O2", "O3", "O4"]
atoms_x: gIQeAICEHgCQHhAAkB4QANCUDgDwUg0AQBAPAND7AQCwyCIA
atoms_y: AAAAAAAAAACQyQAAkMkAALCm5f/wXw8AoKDs/6DG7v/g6BMA
atoms_z: gIQeAICEHgAgvy8AIL8vAMCYJADA4yQAYEIcAMBOKAAQfRMA
atoms_occupancy: QOEzAMAnCQDAqDIAQGAKAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: cJQAAHCUAAAAlgAAAJYAAAB9AADAqAAA0LYAAICiAACgvgAA
atoms_aniso_label: ["Fe2+M1", "MgM1", "Mn2+M2", "MgM2", "P", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: wMEAAMDBAABgnwAAYJ8AADCOAAAgywAAAPoAAIC7AACAuwAA
atoms_aniso_u22: 8G4AAPBuAAAQpAAAEKQAAEBqAACgjAAAIMsAAAB9AACAuwAA
atoms_aniso_u33: MI4AADCOAACwgQAAsIEAAAB9AADgqwAAwF0AAIC7AACAuwAA
atoms_aniso_u12: 0AcAANAHAACQAQAAkAEAAEAGAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u13: MN///zDf///g/P//4Pz//0Dt//9g8P//YPD//+AuAACAwf//
atoms_aniso_u23: kAEAAJABAAAw+P//MPj//8D5//9g8P//YPD//2Dw//+Awf//
pub_title:
 Zavaliaite, (Mn2+,Fe2+,Mg)3(PO4)2, a new member of the sarcopside group from
 La Empleada pegmatite, San Luis Province, Argentina

qdat:
AAAAAAAAAAAAAAAAAQAAgAAAgAQCAMAAAAoAAgACiBAMCUBBEAJCFAEUpgBogERJQhwEdAYFRTahMBaVCO5TkImsb5ZgkMnfHwYRqeS08vl0+6ertinjrrXKfJ/l6f2A+ve3k30vu37u/T4rsvUflup9atFzeetvJz17t8==


formula: Ba Cu2 Si2 O7
compound: Wessels mine, Kalahari Manganese Fields, South Africa
formula_title: <missing>
a: 6.8556
b: 13.1725
c: 6.8901
alpha: 90
beta: 90
gamma: 90
cell_volume: 622.213
crystal_density: 4.618
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3", "O4"]
atoms_x: mMsAANDxEADIXx4AwK4YAFCHCgBgHiIA0F0TAA==
atoms_y: QEIPAChBAACwLggAQEIPABApCACQ1wYAQKMDAA==
atoms_z: wOIbAJiXDADgLCAAcIkfAKD4BwDgsC0AIG4cAA==
atoms_occupancy: 0
atoms_u_iso: kJcAAJBvAAAQWQAA8IcAAICiAABwrQAA4HkAAA==
atoms_aniso_label: ["Ba", "Cu", "Si", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: EIsAABCLAAAgZwAAQIMAAKC+AACA7QAAEKQAAA==
atoms_aniso_u22: wKgAABBZAABwSQAAEFkAAEBqAAAgmQAAwHYAAA==
atoms_aniso_u33: cJQAAEBqAAAQWQAAgLsAAKC+AACwgQAA0FIAAA==
atoms_aniso_u12: AAAAAOAVAAAYBgAAAAAAAGAiAAAASwAAoN3//w==
atoms_aniso_u13: gPP//xDc//9ABgAAwPn//zCt//+Qz///8AoAAA==
atoms_aniso_u23: AAAAAIDz//8AAAAAAAAAAFD7//9w5f//YPD//w==
pub_title:
 Scottyite, the natural analog of synthetic BaCu2Si2O7,
 a new mineral from the Wessels mine, Kalahari Manganese Fields, South Africa

qdat:
AAAAAAAAAAAAAAABAQAAAEAgAABAIAMFQA8gAGJAAGERwQuCqoTEIHBkGTCDlSP2K6E73BsA7GWZXN5/IVevxb+Xy9e715//XvV9v+uvvuDeu969+29b+tq70u////by9/6/2bT+/79+fr9T//+rv/////8/n/3////L/9==


formula: U As2 (O12 H10)
compound: Jachymov, Czech Republic
formula_title: <missing>
a: 10.9867
b: 10.9867
c: 32.9271
alpha: 90
beta: 90
gamma: 90
cell_volume: 3974.551
crystal_density: 3.944
atoms_sites: ["U", "As", "Wat1", "O-H2", "Wat3", "O4", "O5", "O6", "Wat7"]
atoms_x: cMcJAADvFQDAxi0AEPsXAICEHgDAyBwAUCwVAJARDgAQIgUA
atoms_y: 8EsoAHhSNQDAUTQA4N0yAICEHgBQRjIAsGs+ANANMQAQyjQA
atoms_z: AAAAAAiBAwAgoQcAYHsGAGBPBQCwrQEAoJMDAEDCAgBAwf7/
atoms_occupancy: 0
atoms_u_iso: cK0AAKCMAABgZwEAoIYBAGDkAQDgKAEAIMsAACDLAAAA+gAA
atoms_aniso_label: ["U", "As", "Wat1", "O-H2", "Wat3", "O4", "O5", "O6", "Wat7"]
atoms_aniso_u11: sJoAAICJAAAAcQIAwNQBAMBRAgAgywAA4CgBAIC7AAAA+gAA
atoms_aniso_u22: sJoAALCBAACAuwAAQJYBAMBRAgCgCQEA4KsAACDLAABAnAAA
atoms_aniso_u33: YNEAALCaAABg6gAAQBkBAEAZAQCAtQEAQJwAAGDqAAAgSAEA
atoms_aniso_u12: cP7//8Dg//8AAAAAoBX//2Dw///A4P//AAAAAKAPAABg8P//
atoms_aniso_u13: 2P///9Du//9Aov//QKL//wAAAAAAfQAAYPD//+AuAABAov//
atoms_aniso_u23: KAAAAIAMAAAAAAAAAH0AAAAAAAAg0f//QB8AAKAPAABg8P//
pub_title:
 Stepite, U(AsO3OH)2*4H2O, from Jachymov, Czech Republic:
 the first natural arsenate of tetravalent uranium

qdat:
AAAAAAAAAAAACABAAAAgAEBIAECgABBBAAECAhQEUgKBGRABCiQESDAKgQjCYTSgilAKCEgQBIEgRKETpFygVQcAoomIuAqZcw6ElJmWINCjDAJRAQhRKkMBAEjACIAAMQQIAABIAQAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ti1.47 Fe.26 O4 H1.25
compound: Konigshain, northeast Germany
pub_title: Kleberite, Fe3+Ti6O11(OH)5, a new ilmenite alteration product, from Konigshain, northeast Germany
formula_title: <missing>
a: 7.537
b: 4.5795
c: 9.885
alpha: 90
beta: 131.02
gamma: 90
cell_volume: 257.419
crystal_density: 3.875
atoms_sites: ["TiM1", "TiM2", "FeM2", "O1", "O-H2", "O2", "O-H3", "O3", "O4"]
atoms_x: ICQHAOC2EwDgthMAwC0IAMDNFwDAzRcAgNEmAIDRJgBA2zQA
atoms_y: YGECAEAZAQBAGQEAwIYOAGCWDgBglg4AoKkQAKCpEABgDRAA
atoms_z: oMcLAGCbIgBgmyIA4KoVAMDGLQDAxi0A4IcGAOCHBgDgAxwA
atoms_occupancy: QI4sAIAqLQCA3g8AAAk9AICEHgCAhB4AwMYtAEBCDwAACT0A
atoms_u_iso: wCoBAMAqAQDAKgEAkDwBAJA8AQCQPAEAkDwBAJA8AQCQPAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAIAAAAAAABAgIAAAAAARIAAAAEIACABIIAAECEQQACRGAUEABAAASgiMLTECRABmAAJQwGI2ICGkIHTUZSJjoBhIgBc+wETdEL7LGYr1NpTJQluFFi3irYqjTKIY2uWllmP52TghZ96zUm1uuVa0X==


formula: Ca2 B2 O5
compound: Fuka, Okayama Prefecture, Japan
formula_title: <missing>
a: 3.5485
b: 6.352
c: 19.254
alpha: 90
beta: 92.393
gamma: 90
cell_volume: 433.608
crystal_density: 2.784
atoms_sites: ["Ca1", "Ca2", "B1", "B2", "O1", "O2", "O3", "O4", "O5"]
atoms_x: 0JsRAFD6LQCgUAoAIIkLAMBDLgDgDi8AIGURAIBTOwDgYwwA
atoms_y: 0PA5AEDwCwCgYRwAIHEPAFBMMQDAXjYAwGEQAPCJIQCQKSMA
atoms_z: ENkMAJDGAwCQkwkAoHMZANDoAACAJwgAEAoJADDtBQAwQA0A
atoms_occupancy: 0
atoms_u_iso: IGcAACBnAABAnAAAoIwAAMCPAACAVwAAQGoAAOAoAQCgcwAA
atoms_aniso_label: ["Ca1", "Ca2"]
atoms_aniso_u11: sIEAADB1AAA=
atoms_aniso_u22: gHAAADB1AAA=
atoms_aniso_u33: oEEAAOBHAAA=
atoms_aniso_u12: cBcAAKAoAAA=
atoms_aniso_u13: oPb//yDq//8=
atoms_aniso_u23: oPb//yADAAA=
pub_title:
 Shimazakiite-4M and shimazakiite-4O, Ca2B2O5, two polytypes of a new mineral
 from Fuka, Okayama Prefecture, Japan
 Note: polytype Shimazakiite-4M

qdat:
AAAAAAAAAABAAAAAAIABABAQAAAIAEABClGBDEQEBECEZhEDABKDiCmCVCh4UJmjQRxiymSZM1JBWqRpiB+SisBlvOVS6bE3EZJeJfOdeSgaySOpVKLV/O0689evrsaK+rLl57S75XQ8JUrC/mVGH15v79ruWNrdZ3t8z7==


formula: Ca2 B2 O5
compound: Fuka, Okayama Prefecture, Japan
formula_title: <missing>
a: 3.55645
b: 6.35194
c: 19.2534
alpha: 90
beta: 90
gamma: 90
cell_volume: 434.941
crystal_density: 2.776
atoms_sites: ["Ca1", "Ca2", "B1", "B2", "O1", "O2", "O3", "O4", "O5"]
atoms_x: KCoSABCrMADwXgsAILQIACC+MADghTAA0EQTANA5AABwsAwA
atoms_y: QEUMAIBGGwBQ1CsAELgeAFhoAwBQuwgAWKYfADDbMADwjDIA
atoms_z: ONkMAEDBAwBwkAkAsIEZAMDuAAAINggA6AkJACjhBQCIRw0A
atoms_occupancy: 0
atoms_u_iso: SHYAAJh7AABwewAAoHMAAOCSAAAwjgAAEKQAACCyAACQlwAA
atoms_aniso_label: ["Ca1", "Ca2", "B1", "B2", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: IIAAAOB5AABQXwAAYG0AAICiAABQkQAA0LYAAGA1AQAwwAAA
atoms_aniso_u22: gHAAAICJAACgjAAAsE8AAKClAAAgmQAAUJEAAPBuAAAwjgAA
atoms_aniso_u33: sHIAAIBwAABAgwAA0J0AAPBuAAAggAAAEKQAAIBwAADgeQAA
atoms_aniso_u12: wP7//7gBAADQ7v//wBIAADARAADQIAAA4C4AAEA4AABA7f//
atoms_aniso_u13: KAAAADACAACg9v//oPb//+D8///Q7v//4BUAACDR///A+f//
atoms_aniso_u23: 4Pf//wj9//+gKAAAEPX//5AaAACAwf//sB0AABD1//8gAwAA
pub_title:
 Shimazakiite-4M and shimazakiite-4O, Ca2B2O5, two polytypes of a new mineral
 from Fuka, Okayama Prefecture, Japan
 Note: polytype Shimazakiite-4O

qdat:
AAAAAAAAAABAAAAAAAAAABAAAAAAAAAICkSEDEAEQACMkEIwAIJBEAKgABLlAdxKhAxvIsRI50gmR2Kw4HQMIFCSah06EFcmKCVVIvOvVk+A5A6EtEJyKRM7z49tR6HLVHrpvrL9jRlkeJiLfOYrv6LPlveexvHzpuxcl3==


formula: (Ni.623 Al.377) C.34 O3.02 H2
compound: Agoudal mine, Bou Azzer district, Tazenakht, Morocco
formula_title: <missing>
a: 3.0290
b: 3.0290
c: 22.5995
alpha: 90
beta: 90
gamma: 120
cell_volume: 179.568
crystal_density: 2.806
atoms_sites: ["Ni", "Al", "C", "O1", "O2", "H"]
atoms_x: AAAAAAAAAABVWBQAVVgUAABBCgBVWBQA
atoms_y: AAAAAAAAAACrsCgAq7AoAABBCgCrsCgA
atoms_z: AAAAAAAAAAAAeB4AcKsCAICEHgBgBAUA
atoms_occupancy: YAYmAKACFwBAYAoAAAk9AEBgCgAACT0A
atoms_u_iso: cJQAAHCUAABg2AMAAPoAAIAyAgDgKAEA
atoms_aniso_label: ["Ni", "Al", "C", "O1", "O2"]
atoms_aniso_u11: UHgAAFB4AABAhAQAIBYBAABxAgA=
atoms_aniso_u22: UHgAAFB4AABAhAQAIBYBAABxAgA=
atoms_aniso_u33: QM4AAEDOAAAAcQIAwMEAAMBXAQA=
atoms_aniso_u12: eDwAAHg8AAAgQgIAEIsAAGDqAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAGAJAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAKD2//8=
pub_title:
 Contribution to the crystallography of hydrotalcites:
 the crystal structures of woodallite and takovite
 Note: polytype 3R
 Note: calculated chemical formula differs from expected

qdat:
AAAAAAAAAAAAABAAAAAAAAAAAAABAAAAAAAAAAAAQiAAgAQAAAAEAAEAAAAAAQAAAAAAAQEAAAEAAAAAqAgQAAQAgAAAIAAAAAAAAAAAACgQQAEBAAAIAAABEABAAABAAAAAAAAAAAIgAgAAoRAECAAQAAAAAAABBIBAgA==


formula: (Mg.75 Cr.124 Al.039 Fe.087) O2.851 H2 C.07 Cl.11
compound: Mount Keith Nickel Mine, Western Australia, Australia
formula_title: <missing>
a: 3.10124
b: 3.10124
c: 23.6817
alpha: 90
beta: 90
gamma: 120
cell_volume: 197.249
crystal_density: 2.095
atoms_sites: ["Mg1", "Cr", "Al", "Fe", "O1", "H1", "O2", "C1", "Cl1"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAFVYFABVWBQAIJ4UAAAAAAAAAAAA
atoms_y: AAAAAAAAAAAAAAAAAAAAAKuwKACrsCgAIJ4UAAAAAAAAAAAA
atoms_z: AAAAAAAAAAAAAAAAAAAAANiJAgBA/AQAgIQeAICEHgCAhB4A
atoms_occupancy: wMYtAICRBwBgYQIAYE8FAAAJPQAACT0AMKkIAMBFBADAtgYA
atoms_u_iso: 2NEAANjRAADY0QAA2NEAANjRAADY0QAAyIsBAMiLAQDIiwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Contribution to the crystallography of hydrotalcites:
 the crystal structures of woodallite and takovite
 Note: polytype 3R
 Note: calculated chemical formula differs from expected

qdat:
AAAAAAAAAAAAAIAAAAAAAAAAAAEAAAAAAAAAAAARgABABAAAABAACAAAAAAgAAAAAAAEBAAACAAAAAcAggAAgCAAACAAAAAAAAAAAAAMCEACAgAAQAAAAiAAgAAEAAAAAAAAAAAiACAADCIAggAIAAAAAAAAxEAhAAQAAA==


formula: Fe3 P2 O8
compound: Synthetic
formula_title: <missing>
a: 6.0186
b: 4.7768
c: 10.4192
alpha: 90
beta: 90.952
gamma: 90
cell_volume: 299.507
crystal_density: 3.964
atoms_sites: ["FeM1", "FeM2", "P", "O1", "O2", "O3", "O4"]
atoms_x: gIQeAEB6DgCg4Q8AEPMQALByDwBwYwQAwJYcAA==
atoms_y: AAAAACAJ//+gbRoAoA4uAND3CgAg1hMAsGYRAA==
atoms_z: AAAAAGA5EQDAIAYAIFwGAABSHABQHQsAgOkJAA==
atoms_occupancy: 0
atoms_u_iso: QB8AAAAZAAAwKgAAMPj//xAnAABwFwAA4C4AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic structure of iron(II) phosphate, sarcopside, Fe3(PO4)2
 Sample: FE3(PO4)2
 Note: T = 59.7 K

qdat:
AAAAAAAAAAAAAAAAAIAAQAAAQABAgBAAAADAAIAAUYEBghgQYQAIQSBAyjAGIAQhUIOAz6woJnNSpwAUMgvpj4Ei4O9irUM5ekdRmg7FeEncj249tfz9bWysXnwd+fkPVV/fHr7R92+37s3/Ct2bbfcXi93rau/z7k+/99==


formula: Fe3 P2 O8
compound: Synthetic
formula_title: <missing>
a: 6.01037
b: 4.7727
c: 10.4052
alpha: 90
beta: 90.944
gamma: 90
cell_volume: 298.440
crystal_density: 3.978
atoms_sites: ["FeM1", "FeM2", "P", "O1", "O2", "O3", "O4"]
atoms_x: gIQeAPB+DgCg4Q8AoPQQANB1DwDAXgQAgJAcAA==
atoms_y: AAAAAIAS///waBoAMBAuACAMCwBQzhMAQGgRAA==
atoms_z: AAAAANA3EQBQIgYAIFwGAOBOHADAGwsAMO4JAA==
atoms_occupancy: 0
atoms_u_iso: sB0AAMASAABgIgAAcBcAANAgAACwHQAAgCUAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Magnetic structure of iron(II) phosphate, sarcopside, Fe3(PO4)2
 Sample: FE3(PO4)2
 Note: T = 10.1 K

qdat:
AAAAAAAAAAAAAAAAAEAAQAAAQABAgBAAAADAAIAAMYEBQhQQIIAMIKBA6jgGMAQQqEHARawUJlGqZYAWGgT0h8CRYP0zZ2M1WUW5jQfitC1uR9Yuuv52prRWXW4O2PUPta+3jydo+7PlbT5Xhm7Nd+/FzbfvdNP5I6XPn9==


formula: Na.68 (Fe.67 Mn.33) P O4
compound: the Malpensata pegmatite, Lecco Province, Italy
formula_title: <missing>
a: 4.882
b: 10.387
c: 6.091
alpha: 90
beta: 90
gamma: 90
cell_volume: 308.871
crystal_density: 3.573
atoms_sites: ["NaM1", "FeM2", "MnM2", "P", "O1", "O2", "O3"]
atoms_x: AAAAAGAxPABgMTwA4HMaAABpLQDAIQoAYH4SAA==
atoms_y: AAAAADBBEQAwQREAoE8GAGDGBgCAXhwAEJoKAA==
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwBAQg8AgCwDAA==
atoms_occupancy: AIEpAMDkKABAJBQAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: QBkBAPCgAADwoAAAoL4AAOAoAQCAOAEA4CgBAA==
atoms_aniso_label: ["NaM1", "FeM2", "MnM2", "P", "O1", "O2", "O3"]
atoms_aniso_u11: AH0AAKAJAQCgCQEAoAkBAOAoAQAgQgIAQJYBAA==
atoms_aniso_u22: oIYBAECcAABAnAAAIMsAAAB3AQBAnAAAoIYBAA==
atoms_aniso_u33: IEgBACBOAAAgTgAAYG0AAGDqAAAgywAAIE4AAA==
atoms_aniso_u12: QB8AAIDz//+A8///QB8AAMBdAAAgVP//wF0AAA==
atoms_aniso_u13: oJL//wAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: INH//wAAAAAAAAAAAAAAAAAAAAAAAAAAAH0AAA==
pub_title:
 Karenwebberite, Na(Fe2+,Mn2+)PO4, a new member of the triphylite group
 from the Malpensata pegmatite, Lecco Province, Italy

qdat:
AAAAAAAAAAAAAAAAAAAAwAAAAAAEAIAAAApAAAABNBBAgIQIBAEAEoAxBUFJEIBECAWpbCgCz2TKQBYhCrOspRMHyV97MizEaqROb18Qfp9N3WuzXcrZLzC3D3vZ9/hr29fua+1bvtu9W88ban+dxSd/Xa1q93mdu/9N31==


formula: Ca S O4.5 H
compound: Synthetic
formula_title: <missing>
a: 6.937
b: 6.937
c: 6.345
alpha: 90
beta: 90
gamma: 120
cell_volume: 264.427
crystal_density: 2.735
atoms_sites: ["Ca", "S", "O1", "O2", "Wat"]
atoms_x: 8D4hAACYIQCQbiQAcEIWAPAFNwA=
atoms_y: AAAAAAAAAABgLzQAIDw1AAAAAAA=
atoms_z: yNwyAFVYFABQZhwAkIcLAMjcMgA=
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AICEHgA=
atoms_u_iso: 0
atoms_aniso_label: ["Ca", "S", "O1", "O2", "Wat"]
atoms_aniso_u11: MAUCAADhAAAAXgEAUKQBAICcAQA=
atoms_aniso_u22: IP0AACCyAAAAkAEAgO0AAIBLAgA=
atoms_aniso_u33: gLsAAIC7AACASwIA4PYAAODsCgA=
atoms_aniso_u12: wPn//+AuAADwTwEA0NX//yBa/v8=
atoms_aniso_u13: 4Pz//3AXAACgQQAA8Nj//6Au//8=
atoms_aniso_u23: kH4AABBZAACA7QAAQO3//8AlAQA=
pub_title:
 Bestimmung der Kristallstruktur von CaSO4(H2O)0.5 mit
 Rontgenbeugungsmethoden und mit Potentialprofil-Rechnungen

qdat:
AAAAAAAAAAAAAAAAAEAAAAAAgAAAAAQAAAJAAIEAAAAACAQAgkAAMABACAgAMBDAAgACJCAiiACAgSgBkEBAYEERCEGQoSkAkikgOAMOGhgIh6QgwKJGhoAqjRkTNSFYAAsHiQZaSSKNegyKiwW5ErJ9rIMtRWXR8onRnC==


formula: Ca S O4
compound: <missing>
pub_title: A more accurate determination of the crystal structure of anhydrite, CaSO4
formula_title: <missing>
a: 6.23
b: 6.98
c: 6.97
alpha: 90
beta: 90
gamma: 90
cell_volume: 303.093
crystal_density: 2.983
atoms_sites: ["Ca", "S", "O1", "O2"]
atoms_x: QB4VAEBmCQAAERIAgDgBAA==
atoms_y: wMYtAEBCDwAA4gQAQEIPAA==
atoms_z: AAAAAAAAAAAAAAAAII8KAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAgAAgAACAAAAAAAAEAAwAAAAIAAASAAAAAwAAAABAYBIAAACAwAAMEAQAAAgCAAQwKAAAgUAAADgAAAUAEYEAAMKAGIMAEwYADDgBMYAYBABcYBTOAJhgMggCJgC4wCpwGDAGjADGA2c==


formula: Ca S O4.81 H1.62
compound: Synthetic
pub_title: Calcium sulfat subhydrat, CaSO4.0,8H2O
formula_title: <missing>
a: 6.968
b: 6.968
c: 6.410
alpha: 90
beta: 90
gamma: 120
cell_volume: 269.529
crystal_density: 2.786
atoms_sites: ["Ca", "S", "O1", "O2", "Wat"]
atoms_x: ABshABB0IQAAVCQAUIoWAPDNNwA=
atoms_y: AAAAAAAAAABARTQAMEo1AAAAAAA=
atoms_z: yNwyAFVYFAAAaxwAEJQLAMjcMgA=
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AEBwMQA=
atoms_u_iso: EHYBAAjAAAC4kQEAcEgBAACsAwA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAIAAAAABAAAAAAgAAASAAgIAAAAAIBACCgAAgAEAIEAAwEMACAASEIEMgAgCCMAFAQEEAghgLAUDCOAJDEgGgEngwMBQKUEoCRgyKAU0QODRSTUAAZIxoWYuFTHNSUklwuaooWc5Upvi5mzlQpuDpN==


formula: Ca S O4
compound: Synthetic
formula_title: CaSO4
a: 6.9694
b: 6.9694
c: 6.3033
alpha: 90
beta: 90
gamma: 120
cell_volume: 265.149
crystal_density: 2.558
atoms_sites: ["Ca", "S", "O"]
atoms_x: gIQeAICEHgCgNRsA
atoms_y: AAAAAAAAAACwOAgA
atoms_z: AAAAAICEHgCg1hUA
atoms_occupancy: 0
atoms_u_iso: 8MMAAJDnAAAAHQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A crystallographic study of the low-temperature dehydration products of gypsum
 CaSO4*2H2O: hemihydrate CaSO4*0.50H2O, and gamma-CaSO4
 Note: gamma-CaSO4

qdat:
AAAAAAAAAAAAAAAAAIAAAAAAgAAAAAgAAAKAAEEAAAAABBAAhBAAhACACAQASBMACAABCIBIhAAiAogEhQCAFISAIE0LBJAgSCgCiQUi0MBAKbCAsJAkKOEIQMCFSxQsAEQxwQ6cWJLFTCCgYxVcQU9Y1FRgZxKzlSWAtU==


formula: Ge Fe (O6 H6)
compound: Tsumeb mine, Nambia
formula_title: <missing>
a: 7.5520
b: 7.5520
c: 7.4694
alpha: 90
beta: 90
gamma: 90
cell_volume: 426.000
crystal_density: 3.594
atoms_sites: ["Ge", "Fe", "O-H1", "O-H2", "O-H3"]
atoms_x: gIQeAICEHgDgSxAAwNYiANBnIgA=
atoms_y: AAAAAAAAAACAXgMAUCQOANBX+/8=
atoms_z: gIQeAAAAAACQjSMAYGkiAJC7LAA=
atoms_occupancy: 0
atoms_u_iso: sGgAAOB5AAAQvQAA8LkAAGCfAAA=
atoms_aniso_label: ["Ge", "Fe", "O-H1", "O-H2", "O-H3"]
atoms_aniso_u11: kGUAAOB5AAAAfQAAgLsAAIC7AAA=
atoms_aniso_u22: 0GsAAKBzAAAgywAAAH0AAOCrAAA=
atoms_aniso_u33: QGoAAJB+AABg6gAAYOoAAAB9AAA=
atoms_aniso_u12: AAAAAJABAACgDwAAAAAAAKAPAAA=
atoms_aniso_u13: cP7//3D+//9g8P//wOD//wAAAAA=
atoms_aniso_u23: cP7//yADAACgDwAAwOD//2Dw//8=
pub_title:
 Phase transitions in hydroxide perovskites: a Raman spectroscopic study
 of stottite, FeGe(OH)6, to 21 GPa

qdat:
AAAAAAAAAAAAAAAAAAACAAAAAAACgAAAAAwAAAAUAAABIAAAQAAAwAAEQABYAA0AAYAAkAD0AAAAiAFABUAaQGYDEBUAhApAEA8QpBqhUDEAAbQgSzOkWCJOUkFIoSC4W0qHrAGyheuURMrwyFzAurLRgNoCxhicXzUukL==


formula: Fe1.5 Ca.5 Si2 O6
compound: Synthetic
formula_title: <missing>
a: 9.793
b: 9.078
c: 5.238
alpha: 90
beta: 106.27
gamma: 90
cell_volume: 447.014
crystal_density: 3.804
atoms_sites: ["FeM1", "FeM2", "CaM2*", "SiT", "O1", "O2*", "O2**", "O3*", "O3**"]
atoms_x: AAAAAAAAAAAAAAAAgOYRAGhtBwBgAhYA4DoXAAB8FQDwbRUA
atoms_y: ID83AAAqEgBgDRAA2HcFANh3BQBwCA8AQHoOAIDUAACgZwIA
atoms_z: QEIPAEBCDwBAQg8AgNAOAHBeCQAAiBMAIMQWAKBBAABQTP//
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQCAhB4AgIQeAICEHgCAhB4A
atoms_u_iso: wI8AAFDDAABQwwAAGIgAAPCgAACgpQAAoKUAACCAAAAggAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Local structure in C2/c clinopyroxenes on the hedenbergite (CaFeSi2O6)-
 ferrosilite (Fe2Si2O6) join: A new interpretation for the Mossbauer spectra
 of Ca-rich C2/c clinopyroxenes and implications for pyroxene exsolution
 Note split-M2-O2-O3 model
 Sample: Hd50Fs50

qdat:
AAAAAAAAAAAAAAAAgAAAAAIgAAAACAAQgAAIIAAAAGAEEEQGQASQEAAAhKBgAIQIQGDEA1CQKJAiAKBURUIoBOnJ4YAgpyC4QvVHJQMm1Ay0KgDM1/laAv2YsULTMiKmKlqe27LGiLuzFIZz6VSmAHFRRov9CVphorQIgS==


formula: Fe1.4 Ca.6 Si2 O6
compound: Synthetic
formula_title: <missing>
a: 9.806
b: 9.068
c: 5.238
alpha: 90
beta: 105.92
gamma: 90
cell_volume: 447.903
crystal_density: 3.773
atoms_sites: ["FeM1", "FeM2", "CaM2*", "SiT", "O1", "O2*", "O2**", "O3*", "O3**"]
atoms_x: AAAAAAAAAAAAAAAA4NERAHBqBwCgCBYAgDEXAEBQFQAgfxUA
atoms_y: GEc3AIBPEgCAEBAAAIcFACB7BQCAYQ8AIPoNAFBnAgDQ6AAA
atoms_z: QEIPAEBCDwBAQg8A6KQOAOBcCQDgthMAYGYWACAi//9wFwAA
atoms_occupancy: AAk9AABqGAAAnyQAAAk9AAAJPQAAnyQAAGoYAACfJAAAahgA
atoms_u_iso: QJwAAGC4AABguAAA4JIAADCnAADAjwAAwI8AANCEAADQhAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Local structure in C2/c clinopyroxenes on the hedenbergite (CaFeSi2O6)-
 ferrosilite (Fe2Si2O6) join: A new interpretation for the Mossbauer spectra
 of Ca-rich C2/c clinopyroxenes and implications for pyroxene exsolution
 Note split-M2-O2-O3 model
 Sample: Hd60Fs40

qdat:
AAAAAAAAAAAAAAAAgAAAAAQQAAAAEAAggAAIIAAAAMAIEIQMgAiIQAABCUDAAQQIQEGICKEgNRBIAKFQhkKYA6PHRgCBs0CwRssaaIWOMFUw4QMlfus0A9Tg2Q+Zapxcdhxz1qNYhZ8s7BrfYuYsBauFDjHbhGsTUyCYE0==


formula: Fe1.3 Ca.7 Si2 O6
compound: Synthetic
formula_title: <missing>
a: 9.819
b: 9.056
c: 5.242
alpha: 90
beta: 105.61
gamma: 90
cell_volume: 448.931
crystal_density: 3.741
atoms_sites: ["FeM1", "FeM2", "CaM2*", "SiT", "O1", "O2*", "O2**", "O3*", "O3**"]
atoms_x: AAAAAAAAAAAAAAAASL8RAJBeBwDgDhYAAD4XAEAYFgDwIhUA
atoms_y: OE83AGBMEgCwCBAAkI0FAMh9BQBAEA8AIHcOAOAoAQBggAEA
atoms_z: QEIPAEBCDwBAQg8ASIYOAKBWCQAgixMAkNsWAOCrAAAgVP//
atoms_occupancy: AAk9AIBPEgCAuSoAAAk9AAAJPQCAuSoAgE8SAIC5KgCATxIA
atoms_u_iso: cIoAAPCgAADwoAAA+H8AAACWAACwmgAAsJoAAPCgAADwoAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Local structure in C2/c clinopyroxenes on the hedenbergite (CaFeSi2O6)-
 ferrosilite (Fe2Si2O6) join: A new interpretation for the Mossbauer spectra
 of Ca-rich C2/c clinopyroxenes and implications for pyroxene exsolution
 Note split-M2-O2-O3 model
 Sample: Hd70Fs30

qdat:
AAAAAAAAAAAAAAAAgAAAAAQQAAAAEAAggAAQEAAAAMAIIQIUgAiIgAABEsFABAQIgYOgIqJAdCCgAMNAhiMwB4aNCAIEs4NwSZjiqIkY2kVvQRSE/XhyDnOk1DZZNrlUoDueWMaIrDS84NPxZjQoJ/0oOZU6zxRc54pBFT==


formula: Ca C O3
compound: theoretical
pub_title: A new structural model for disorder in vaterite from first-principles calculations
formula_title: <missing>
a: 8.4905
b: 6.3905
c: 4.5026
alpha: 90
beta: 90
gamma: 90
cell_volume: 244.305
crystal_density: 2.721
atoms_sites: ["Ca", "C", "O1", "O2"]
atoms_x: gIQeAEBCDwCYcxcAQEIPAA==
atoms_y: AAAAAADPCAAIIAoA2HEGAA==
atoms_z: IAwfAACeOQDwtQQAAH0oAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAACAAAEAAgBAAgACAAAgAAAAGAAIAACAIBBgQSAAgAAFCBABgCCEgJAAAIKowAgYokHAhBJoMAQAPYAKiog4ACJUoEThlBsm9GgMi6igVqDEP3aIRN0Spu8KLZompruJmMQ5ekwuiiNbCbs1==


formula: Ca C O3
compound: theoretical
pub_title: A new structural model for disorder in vaterite from first-principles calculations
formula_title: <missing>
a: 4.3668
b: 6.5831
c: 8.4282
alpha: 90
beta: 90
gamma: 90
cell_volume: 242.286
crystal_density: 2.744
atoms_sites: ["Ca", "C", "O1", "O2", "O3"]
atoms_x: OKwRAJjXDQDQ0DsAuBsTAEATBwA=
atoms_y: EF48ALiZJgCIcCAAkEwoAAgJEgA=
atoms_z: KGgfACAcDwCYpQ0A4BYYAFCJJgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAABAAAAAAJAAUAAAgAICAAAAAwgiEAgAlQIEBgAADCBQACNxBAohGAwOIDihEE2AC0jhgjVjwHZIiarlsmZYJX4S4GDdtdKJyBU3mH6bF9KXvvCbZI6779J/obda7va1B8wrX23vn/X+Rb39==


formula: Ca.8 Co1.2 Si2 O6
compound: Synthetic
formula_title: CaCoSi2O6
a: 9.794
b: 8.953
c: 5.243
alpha: 90
beta: 105.66
gamma: 90
cell_volume: 442.671
crystal_density: 3.825
atoms_sites: ["CaM2", "CoM2", "CoM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAKJQRAKAwBwBYFBYAiGwVAA==
atoms_y: QGISACCdEABoYDcA0KIFADBmBQBgLA8AiDUBAA==
atoms_z: QEIPAEBCDwBAQg8A2C0OAJD9CADwxBMAULk8AA==
atoms_occupancy: ANQwAAA1DAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: gHAAAJB4AQDwXwAAeFAAAPBuAADwoAAAAH0AAA==
atoms_aniso_label: ["CaM2", "CoM1", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: AJYAALBoAABgVAAA8FUAAFDDAACAcAAA
atoms_aniso_u22: AEsAAIBXAADgRwAAwHYAABByAADwoAAA
atoms_aniso_u33: QFEAABBZAABgVAAAAH0AALCzAABAagAA
atoms_aniso_u12: AAAAAAAAAAAg+f//0AcAALDS//8gAwAA
atoms_aniso_u13: sOv//6gRAABQFAAAcBcAADBDAACgKAAA
atoms_aniso_u23: AAAAAAAAAABY+P//sAQAAJDo//8w3///
pub_title:
 The structure of (Ca,Co)CoSi2O6 pyroxenes and the Ca-M2+
 substitution in (Ca,M2+)M2+Si2O6 pyroxenes (M2+=Co,Fe,Mg)
 Sample: Ca0.8Co0.2

qdat:
AAAAAAAAAAAAAAAAQAAAAAQIAAAAEAAIIAAIBAAAAEACEIBSIAQRgAAASSiEAgEAkKGYEIyIIyJQABmgCECiAK1MNAEFFFGRSKw6aILFUZpbmAagd3xJgtH7GRYae6rY3wTr3gbnJzKmzij+A53QGSJDiLHGbOwzKJpgkD==


formula: Ca.6 Co1.4 Si2 O6
compound: Synthetic
formula_title: CaCoSi2O6
a: 9.7754
b: 8.9686
c: 5.2421
alpha: 90
beta: 106.302
gamma: 90
cell_volume: 441.106
crystal_density: 3.896
atoms_sites: ["CaM2", "CoM2", "CoM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAA2LYRAJg9BwDgQBYAGHMVAA==
atoms_y: MFQSAKAsEACQUTcAwJQFAMBnBQDgHw8AcFwBAA==
atoms_z: QEIPAEBCDwBAQg8AEHgOANADCQBwThQAQN08AA==
atoms_occupancy: AJ8kAABqGAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: UJEAAOAPAQAIawAA0GEAAJB+AAAA4QAAQJwAAA==
atoms_aniso_label: ["CaM2", "CoM2", "CoM1", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: wKgAAFDDAAAQcgAA4GAAAGBtAADwBAEAAGQAAA==
atoms_aniso_u22: AH0AAIC1AQBgbQAAUF8AACCZAAAAlgAAoAkBAA==
atoms_aniso_u33: cHsAALCaAAAAZAAAEHIAADB1AADgQQEAEHIAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAACPP//xAOAABgpf//AAAAAA==
atoms_aniso_u13: 0AcAAAAAAAD4IAAAADIAANAgAAAArwAA4C4AAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAWO7//yADAAAAtf//cMz//w==
pub_title:
 The structure of (Ca,Co)CoSi2O6 pyroxenes and the Ca-M2+
 substitution in (Ca,M2+)M2+Si2O6 pyroxenes (M2+=Co,Fe,Mg)
 Sample: Ca0.6Co0.4

qdat:
AAAAAAAAAAAAAAAAQAAAAAIIAAAACAAIIAAEBAAAACACCCCGEAIREAAAIlgUAEEAiBCsAixCBWISAAwsBGEogDUVfMAIpVAmgl5jl0I0ZqaVrAI6Ke7CSBXrS2Fk70Zzl+A/HZDPlRUtXZEfKdY9CDNMzp1e5lnVoLYCwS==


formula: Ca.4 Co1.6 Si2 O6
compound: Synthetic
formula_title: CaCoSi2O6
a: 9.747
b: 8.982
c: 5.249
alpha: 90
beta: 107.46
gamma: 90
cell_volume: 438.365
crystal_density: 3.977
atoms_sites: ["CaM2", "CoM2", "CoM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAIPERALBXBwCwkxYAcIkVAA==
atoms_y: YBoSAEC/DwAgPzcAyH0FAABpBQAQ/w4A8GgBAA==
atoms_z: QEIPAEBCDwBAQg8AwBwPAFApCQAgNBUAsHE9AA==
atoms_occupancy: AGoYAACfJAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: YLgAAADhAABYmAAAgJgAABCkAACgIgEAgDgBAA==
atoms_aniso_label: ["CaM2", "CoM2", "CoM1", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: gNQAAFDcAAAwpwAAYJ8AAHCtAADwTwEAYJ8AAA==
atoms_aniso_u22: oIwAAKC+AACwgQAA8G4AAJCXAAAArwAAIMUBAA==
atoms_aniso_u33: wKgAANDoAAAQpAAAAMgAAFCqAAAgxQEAoDsBAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAsOv//xAOAABgjP//MBEAAA==
atoms_aniso_u13: cP7//1AUAABAOAAAcEkAAEA4AADwBAEAQDgAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAA0O7//5ABAAAAg///MEn//w==
pub_title:
 The structure of (Ca,Co)CoSi2O6 pyroxenes and the Ca-M2+
 substitution in (Ca,M2+)M2+Si2O6 pyroxenes (M2+=Co,Fe,Mg)
 Sample: Ca0.4Co0.6

qdat:
AAAAAAAAAAAAAAAAQAAAAAEIAAAAAgAIEAACBAAAABQBAgKBCACRAQAABE4JAASAhAKsgAmEQlMCIAYCkkYSUBJhdkUAFY4FiIjzJUwGh+QaJwQAuGl1qgOrDPLR0v0T1rVfGdhHiIBFXJsPJnZqpQjzHHUpfyDbMmSsgB==


formula: La (Al2.85 Fe.15) (As1.86 P.14) O14 H6
compound: Grupendity Lake cirque, Komi Republic, Russia
formula_title: <missing>
a: 7.0147
b: 7.0147
c: 16.4461
alpha: 90
beta: 90
gamma: 120
cell_volume: 700.829
crystal_density: 4.250
atoms_sites: ["La", "Al", "Fe", "As", "P", "O1", "O2", "O-H3"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAAAAAAAAEHUMAGCOBwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA8Irz/6Bx+P8=
atoms_z: AAAAAICEHgCAhB4AsEETALBBEwCQpiMAQJv8/2BvCAA=
atoms_occupancy: AAk9AMD7OQBADQMAQMM4AMBFBAAACT0AAAk9AAAJPQA=
atoms_u_iso: oNcAAMDzAADA8wAAkLAAAJCwAABg6gAAQJwAAICJAAA=
atoms_aniso_label: ["La", "Al", "Fe", "As", "P", "O1", "O2", "O-H3"]
atoms_aniso_u11: oNcAAGDqAABg6gAA0J0AANCdAABg6gAAoIwAAECcAAA=
atoms_aniso_u22: oNcAAGDqAABg6gAA0J0AANCdAABg6gAAoIwAAECcAAA=
atoms_aniso_u33: ENYAAAD6AAAA+gAAoNcAAKDXAAAA+gAAoAkBAOCrAAA=
atoms_aniso_u12: 0GsAABByAAAQcgAAIE4AACBOAAAAfQAAAH0AAAB9AAA=
atoms_aniso_u13: AAAAAEAGAABABgAAAAAAAAAAAAAAAAAAcOX//6APAAA=
atoms_aniso_u23: AAAAAKAPAACgDwAAAAAAAAAAAAAAAAAAkBoAAGDw//8=
pub_title:
 Elasticity and high-pressure structure of arsenoflorencite-(La):
 insights into the high-pressure behaviour of the alunite supergroup
 note: P = 1.6 GPa

qdat:
AAAAAAAAAAAAAAAAAAIQAEAAAAAAABBAAAAkRAQAAABAAAgpEAACQBASIIACAEGFKAgQIJRAIEAI0QIoIUSAACIZAlBLQBCATqEIQUAEEzITCMIIASoRCEQIBsiIloBAKBQkkAJKFg8CQPwIigApIsvAkLhpVAiVIEEQEp==


formula: La (Al2.85 Fe.15) (As1.86 P.14) O14 H6
compound: Grupendity Lake cirque, Komi Republic, Russia
formula_title: <missing>
a: 6.9822
b: 6.9822
c: 16.3379
alpha: 90
beta: 90
gamma: 120
cell_volume: 689.781
crystal_density: 4.318
atoms_sites: ["La", "Al", "Fe", "As", "P", "O1", "O2", "O-H3"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAAAAAAAA0G4MACChBwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAMJHz/+Be+P8=
atoms_z: AAAAAICEHgCAhB4A0E4TANBOEwAwnSMAELz8/9BtCAA=
atoms_occupancy: AAk9AMD7OQBADQMAQMM4AMBFBAAACT0AAAk9AAAJPQA=
atoms_u_iso: wNoAAEDnAABA5wAAAK8AAACvAADA2gAAAPoAAMCPAAA=
atoms_aniso_label: ["La", "Al", "Fe", "As", "P", "O1", "O2", "O-H3"]
atoms_aniso_u11: ENYAAMDaAADA2gAAUKoAAFCqAABAnAAAQBkBAECcAAA=
atoms_aniso_u22: ENYAAMDaAADA2gAAUKoAAFCqAABAnAAAQBkBAECcAAA=
atoms_aniso_u33: IOQAAKAJAQCgCQEA8LkAAPC5AADAVwEAYOoAAECcAAA=
atoms_aniso_u12: QGoAAEBqAABAagAAYFQAAGBUAAAgTgAA4KsAAMBdAAA=
atoms_aniso_u13: AAAAAEAfAABAHwAAAAAAAAAAAAAAAAAAwOD//7AdAAA=
atoms_aniso_u23: AAAAAIA+AACAPgAAAAAAAAAAAAAAAAAAQB8AAFDi//8=
pub_title:
 Elasticity and high-pressure structure of arsenoflorencite-(La):
 insights into the high-pressure behaviour of the alunite supergroup
 note: P = 3.6 GPa

qdat:
AAAAAAAAAAAAAAAAAAEQAEAAAAAAAAggAAASEgEAAAAQAAIShAAAkAQIiCAAgBBiSgIECCUIBBABNCBJBCkQAARFQEoJsAIQCtQhCCgBAmZCYRRBACNBIQhAgFSJCsgEBIKCSQApIWDwJA+giMABmSxUCQtDisCFOQQIgJ==


formula: La (Al2.85 Fe.15) (As1.86 P.14) O14 H6
compound: Grupendity Lake cirque, Komi Republic, Russia
formula_title: <missing>
a: 6.9538
b: 6.9538
c: 16.2436
alpha: 90
beta: 90
gamma: 120
cell_volume: 680.232
crystal_density: 4.379
atoms_sites: ["La", "Al", "Fe", "As", "P", "O1", "O2", "O-H3"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAAAAAAAA8HEMAFCyBwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEI7z/7BN+P8=
atoms_z: AAAAAICEHgCAhB4AWFgTAFhYEwCwkCMAoNb8/6B1CAA=
atoms_occupancy: AAk9AMD7OQBADQMAQMM4AMBFBAAACT0AAAk9AAAJPQA=
atoms_u_iso: kPsAAFD1AABQ9QAA0M8AANDPAABAGQEAAPoAAACWAAA=
atoms_aniso_label: ["La", "Al", "Fe", "As", "P", "O1", "O2", "O-H3"]
atoms_aniso_u11: sP4AAEAZAQBAGQEAIMsAACDLAADAXQAAgDgBACDLAAA=
atoms_aniso_u22: sP4AAEAZAQBAGQEAIMsAACDLAADAXQAAgDgBACDLAAA=
atoms_aniso_u33: wPMAAOCrAADgqwAAUNwAAFDcAACArwIAgLsAAGBtAAA=
atoms_aniso_u12: IIAAADCOAAAwjgAAkGUAAJBlAADgLgAAIMsAAAAAAAA=
atoms_aniso_u13: AAAAADARAAAwEQAAAAAAAAAAAAAAAAAAINH///AKAAA=
atoms_aniso_u23: AAAAAEAfAABAHwAAAAAAAAAAAAAAAAAA4C4AABD1//8=
pub_title:
 Elasticity and high-pressure structure of arsenoflorencite-(La):
 insights into the high-pressure behaviour of the alunite supergroup
 note: P = 5.7 GPa

qdat:
AAAAAAAAAAAAAAAAAAEIACAAAAAAAAQQAAAJCgCAAAAIAAEFIgAASAECQggAQAQokoBBARFCAQQAjIgSgQoiAACRSBKCLABEAmsEQQkAIE1ILCMIIARoIiEIEBqRITkAgFAoSKAElBoOAkF8CIwAKaLHgJCsWKwIU4hAiA==


formula: La (Al2.85 Fe.15) (As1.86 P.14) O14 H6
compound: Grupendity Lake cirque, Komi Republic, Russia
formula_title: <missing>
a: 6.9280
b: 6.9280
c: 16.1770
alpha: 90
beta: 90
gamma: 120
cell_volume: 672.426
crystal_density: 4.430
atoms_sites: ["La", "Al", "Fe", "As", "P", "O1", "O2", "O-H3"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAAAAAAAAoKgMAADQBwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAYFfz/wAw+P8=
atoms_z: AAAAAICEHgCAhB4AkFcTAJBXEwDgViMAQLT8/zCQCAA=
atoms_occupancy: AAk9AMD7OQBADQMAQMM4AMBFBAAACT0AAAk9AAAJPQA=
atoms_u_iso: gLUBAAB3AQAAdwEAAHcBAAB3AQAA9AEAAPQBAEAZAQA=
atoms_aniso_label: ["La", "Al", "Fe", "As", "P"]
atoms_aniso_u11: oIACAABxAgAAcQIAYOQBAGDkAQA=
atoms_aniso_u22: oIACAKCGAQCghgEAYOQBAGDkAQA=
atoms_aniso_u33: 4C4AAEAfAABAHwAAQJwAAECcAAA=
atoms_aniso_u12: MD0BACDLAAAgywAAMPIAADDyAAA=
atoms_aniso_u13: AAAAAMDg///A4P//AAAAAAAAAAA=
atoms_aniso_u23: AAAAAIDB//+Awf//AAAAAAAAAAA=
pub_title:
 Elasticity and high-pressure structure of arsenoflorencite-(La):
 insights into the high-pressure behaviour of the alunite supergroup
 note: P = 7.4 GPa

qdat:
AAAAAAAAAAAAAAAAAACEACAAAAAAAAQQAAAEhQBAAAAEAACCkQAAIgCBIQIAEAEUKSAggIRhAEEAI0IEoEKQgABEUgKglQARAJqhCEJABBMxCoSiBACWBIQhBANUJCsgEAoFCSQAkoNBQEgvQRGAAzJYqBITRpOAiTiEEI==


formula: Fe2 Ti O4
compound: Synthetic
formula_title: <missing>
a: 8.4480
b: 8.4480
c: 8.4480
alpha: 90
beta: 90
gamma: 90
cell_volume: 602.923
crystal_density: 4.926
atoms_sites: ["Fe1", "Ti2", "Fe2", "O"]
atoms_x: AAAAAKAlJgCgJSYAIIwXAA==
atoms_y: AAAAAKAlJgCgJSYAIIwXAA==
atoms_z: AAAAAKAlJgCgJSYAIIwXAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure phase transitions of Fe3-xTixO4 solid solution
 up to 60 GPa correlated with electronic spin transition
 Note: P = 5.58 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAQAAAAAAAEAAAAgAAAAACAAAEAAAAAQAAIAAAAIAAIAAABAAEAAABAAQAAAQAEAAAQAIAABAAgAAIAQAAEAIAAEAIAAAAgABAEAAQAgAEAQACAIABAIAAAQACAQAAB==


formula: Fe2 Ti O4
compound: Synthetic
formula_title: <missing>
a: 8.521
b: 8.521
c: 8.521
alpha: 90
beta: 90
gamma: 90
cell_volume: 618.688
crystal_density: 4.800
atoms_sites: ["Fe1", "Ti2", "Fe2", "O"]
atoms_x: AAAAAKAlJgCgJSYAUCYWAA==
atoms_y: AAAAAKAlJgCgJSYAUCYWAA==
atoms_z: AAAAAKAlJgCgJSYAUCYWAA==
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure phase transitions of Fe3-xTixO4 solid solution
 up to 60 GPa correlated with electronic spin transition
 Note: P = 7 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAQAAAEAAAAAAQAABAAAAAEAACAAAACAACAAAAQABAAAAgAIAAAIACAAAIAEAABAAgAAIAIAAEAIAAIAQAAABAACAIAAgCAAIAgAEAgAEAgAABAAQCAAAEA==


formula: Fe2 Ti O4
compound: Synthetic
formula_title: <missing>
a: 5.9052
b: 5.9052
c: 8.1834
alpha: 90
beta: 90
gamma: 90
cell_volume: 285.367
crystal_density: 5.204
atoms_sites: ["Fe1", "Ti2", "O"]
atoms_x: AAAAAAAAAAAAAAAA
atoms_y: AAAAAMDGLQDQyQEA
atoms_z: gIQeACChBwCgZA8A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure phase transitions of Fe3-xTixO4 solid solution
 up to 60 GPa correlated with electronic spin transition
 Note: P = 14 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAFAAAAACIAAAAAAAQQAACQAAAAACIAASIAAAAiAASIAAAMBAEQAAAEAEEIAAogKQgAIAIgQAMEKIgASAsiEASDABAIFohBhFoiAACgEFAiQAgOSIQikiFBiQCoSRCgQCCB0i==


formula: Fe2 Ti O4
compound: Synthetic
formula_title: <missing>
a: 2.685
b: 9.228
c: 9.099
alpha: 90
beta: 90
gamma: 90
cell_volume: 225.448
crystal_density: 6.587
atoms_sites: ["Fe1", "Ti2", "Fe2", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_y: gCsYACAeCAAgHggAIKcGACDuDwCAhB4A
atoms_z: QEIPAIAmBACAJgQAQEIPAGAGJgAAAAAA
atoms_occupancy: AAk9AICEHgCAhB4AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-pressure phase transitions of Fe3-xTixO4 solid solution
 up to 60 GPa correlated with electronic spin transition
 Note: P = 50 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAACgAEAAAAAAIAAAAAAACIQAAIjAAABJAoAACgAAAJQACAAARpEBCIAAIogAQYzCEAIAMaVkkaBhC0AGCJCEQGikAYgKQeuxAMWDSptGsASSJItShCVBYJU0RI0wIUWICYCgCihKimqdAKnA0C==


formula: Cu2 Cl O3 H3
compound: Synthetic
formula_title: <missing>
a: 6.02797
b: 6.86383
c: 9.11562
alpha: 90
beta: 90
gamma: 90
cell_volume: 377.158
crystal_density: 3.761
atoms_sites: ["Cu1", "Cu2", "Cl", "O1", "O2", "H1", "H2"]
atoms_x: AAAAAOjACwCgchUAoCQJAKDRGgCgtCMAIL4XAA==
atoms_y: AAAAAEBCDwDAxi0AQEIPAMDhAwDAxi0A4FYjAA==
atoms_z: AAAAAHigDwDQcgMAMJT//zCMEQDgmQMAIB4IAA==
atoms_occupancy: 0
atoms_u_iso: AH0AAGCGAADQzwAAIGcAALBoAAAgZwAAIGcAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Antiferromagnetic transitions in polymorphous minerals of
 the natural cuprates atacamite and botallackite Cu2Cl(OH)3

qdat:
AAAAAAAAAAAAAAAAAAAQBAAgABAABAEACACACiyCAGgAIAoSAwIOAIgUAvCnglEAOQA8BkcQy1CNJcK4A1I/mGJLCjzelXb9hhfYDSNZ9LzN/1/jZ/v/RVZ6zo9x/vfsu3tXmy/4ib6/fP+271bfT373Xds3fX27/vX69V==


formula: Cu2 Cl O3 H3
compound: Synthetic
formula_title: <missing>
a: 5.7165
b: 6.1182
c: 5.6283
alpha: 90
beta: 93.1161
gamma: 90
cell_volume: 196.557
crystal_density: 3.608
atoms_sites: ["Cu1", "Cu2", "Cl", "O1", "O2", "H1", "H2"]
atoms_x: kOMdAICEHgDwDAgAUOcTAJATFgBAvTkAwAMPAA==
atoms_y: QEIPAICEHgBAQg8AwMYtAPD/HgBAQg8AYLgyAA==
atoms_z: wOk8AICEHgCgBxIAIKsWADD4MQAAtyAA4MA7AA==
atoms_occupancy: 0
atoms_u_iso: AH0AAAB9AAAQCAEAgIkAAICJAAAA+gAAAPoAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Antiferromagnetic transitions in polymorphous minerals of
 the natural cuprates atacamite and botallackite Cu2Cl(OH)3

qdat:
AAAAAAAAAAAAAAAAAAKAAAAAAYBAAAABAAQACIBgEgoEAKAAAASAACWhICkhAEQWBEKAdATgAMMJWCtEMgoAxLElIGFGIYCtXFEYLx7MoScGl6y5jU9fl3Vslel1IM1vdG/fbTRaS5+P1brfutL/t5nxv+o//+tzLnjevy==


formula: Fe C2 O6 H4
compound: Synthetic
formula_title: <missing>
a: 12.011
b: 5.557
c: 9.920
alpha: 90
beta: 128.53
gamma: 90
cell_volume: 517.958
crystal_density: 2.307
atoms_sites: ["Fe", "C", "O1", "O2", "O3", "H1", "H2"]
atoms_x: AAAAALALAwAALQUAcEQFAND3CgBgDRAAYDEKAA==
atoms_y: gGYKAMDLKABgphwAwDI1AJDYCgDgjQUAQO8HAA==
atoms_z: QEIPAPBtFQCwzBkAwNoZAFC0DwAgTRUAgIUJAA==
atoms_occupancy: 0
atoms_u_iso: AB0BAED7AABwSAEAQGQBAGCtAQCoVgYAqLQCAA==
atoms_aniso_label: ["Fe", "C", "O1", "O2", "O3"]
atoms_aniso_u11: gIMBAHCOAQCgAwIAAKkBAMAMAQA=
atoms_aniso_u22: kJcAABDvAADgxAAAAA0CAIDtAAA=
atoms_aniso_u33: IP0AANDPAABA5wAA8B0BABDWAAA=
atoms_aniso_u12: AAAAACAcAABg8P//IE4AAHD+//8=
atoms_aniso_u13: MKcAAOB5AABwrQAA4MQAAGCGAAA=
atoms_aniso_u23: AAAAAFAUAADg4///QDgAAFD7//8=
pub_title:
 Single-crystal X-ray diffraction and spectroscopic studies on
 humboldtine and lindbergite: weak Jahn-Teller effect of Fe2+ ion

qdat:
AAAAAAAAAAAAAAAAAAAAABIAAAAgAQAAAAAAACIBgAABGAIQACABAAgIACJACAAAJDFCEIgQAAIoFJEMokQCBMYEB4IIDB9ANIAknSgnFRBkxmDEeRccuCAKdFIxGobQaRpre6FY3CHgee35ovItFTb/o50Pa1mUa2hJ13==


formula: (Mg.93 Fe.07) Si O3
compound: Synthetic
pub_title: Single-crystal structure determination of (Mg,Fe)SiO3 postperovskite Note: P = 120 GPa
formula_title: Mg.93Fe.07SiO3
a: 2.466
b: 8.130
c: 6.108
alpha: 90
beta: 90
gamma: 90
cell_volume: 122.457
crystal_density: 5.565
atoms_sites: ["Mg", "Fe", "Si", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_y: AKAPAACgDwAAAAAAoLM4AGAAJwA=
atoms_z: QEIPAEBCDwAAAAAAQEIPACCsGgA=
atoms_occupancy: QMM4AMBFBAAACT0AAAk9AAAJPQA=
atoms_u_iso: QJwAAECcAAAAfQAAwFcBAGDqAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAABAAAAAgAAIAAAAAAABAIAAEAAAEAAIAQEAAgBAAAABBEAAABQAAA4AwACAAEhAACEICDAAQEAAKhQD4EogACQABwAB8gBABCgCNCBAA3QiUE6yBAViEAIC6QMlACSYCAA6S4k6BGICIdA==


formula: (N H4) As4 O6 Br
compound: Synthetic
formula_title: NH4As4O6Br
a: 5.265
b: 5.265
c: 9.148
alpha: 90
beta: 90
gamma: 120
cell_volume: 219.611
crystal_density: 3.732
atoms_sites: ["NM", "H1M", "H2M", "H3M", "H4M", "As", "O", "BrX"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABVWBQAgIQeAAAAAAA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACrsCgAAAAAAAAAAAA=
atoms_z: gIQeAICEHgCAhB4AgIQeAICEHgAQawwAQN8SAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["NM", "H1M", "H2M", "H3M", "H4M", "As", "O", "BrX"]
atoms_aniso_u11: YIABAGCAAQBggAEAYIABAGCAAQCAiQAAYNEAAPA2AQA=
atoms_aniso_u22: YIABAGCAAQBggAEAYIABAGCAAQCAiQAA4GAAAPA2AQA=
atoms_aniso_u33: gFEBAIBRAQCAUQEAgFEBAIBRAQDwBAEAQGQBABB/AgA=
atoms_aniso_u12: MMAAADDAAAAwwAAAMMAAADDAAADARAAAwBIAAHibAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 The compounds KAs4O6X (X=Cl,Br,I) and NH4As4O6X (X=Br,I):
 Hydrothermal syntheses and structure determinations

qdat:
AAAAAAAAAAAEAAAAAAAAAABgACAAAAAAEAIAAAABAIAAABgIAAAYEAAAAYAADDAABgAADDAAKIAAQgAMYADOAAiAAGADMAKAAIgBTAGgAvACIBaABAHcCQALAdgOwCIBIDQAcDIDADoGwMgHAUDsAQPg4BMGAOA8BwZAcO==


formula: (N H4) As4 O6 I
compound: Synthetic
formula_title: NH4As4O6I
a: 5.290
b: 5.290
c: 9.338
alpha: 90
beta: 90
gamma: 120
cell_volume: 226.306
crystal_density: 3.967
atoms_sites: ["NM", "H1M", "H2M", "H3M", "H4M", "As", "O", "IX"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABVWBQAgIQeAAAAAAA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACrsCgAAAAAAAAAAAA=
atoms_z: gIQeAICEHgCAhB4AgIQeAICEHgAY2wwAsCgTAAAAAAA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["NM", "H1M", "H2M", "H3M", "H4M", "As", "O", "IX"]
atoms_aniso_u11: 0H4BANB+AQDQfgEA0H4BANB+AQBghgAAcPgAANDoAAA=
atoms_aniso_u22: 0H4BANB+AQDQfgEA0H4BANB+AQBghgAAwF0AANDoAAA=
atoms_aniso_u33: IEgBACBIAQAgSAEAIEgBACBIAQAw2QAAcCoBALBiAQA=
atoms_aniso_u12: aL8AAGi/AABovwAAaL8AAGi/AAAwQwAAAEsAAGh0AAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 The compounds KAs4O6X (X=Cl,Br,I) and NH4As4O6X (X=Br,I):
 Hydrothermal syntheses and structure determinations

qdat:
AAAAAAAAAAAQAAAAAAAAAAFAAEAAAAAAgCAAAAAECQAABGAgAAJAgAAARAABEEAAkAAIGUAQYAAIIAkQgJsQAIgBCiFoUBQAQogSLBQFRYIQYQhERFtAECD6V1hkEEBqYwIuCIRAUTK0BJKQ+MSARHqEGOEDEFqD4DJMt0==


formula: K As4 O6 Cl
compound: Synthetic
formula_title: <missing>
a: 5.252
b: 5.252
c: 8.880
alpha: 90
beta: 90
gamma: 120
cell_volume: 212.126
crystal_density: 3.681
atoms_sites: ["KM", "As", "O", "ClX"]
atoms_x: AAAAAFVYFACAhB4AAAAAAA==
atoms_y: AAAAAKuwKAAAAAAAAAAAAA==
atoms_z: gIQeAEiIDAAAJBMAAAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["KM", "As", "O", "ClX"]
atoms_aniso_u11: ICkCAGDqAAAQ0AEAMOwBAA==
atoms_aniso_u22: ICkCAGDqAADgxAAAMOwBAA==
atoms_aniso_u33: UNYBAMAMAQCQXwEAYLkEAA==
atoms_aniso_u12: kBQBADB1AABwrQAAGPYAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAA==
pub_title:
 The compounds KAs4O6X (X=Cl,Br,I) and NH4As4O6X (X=Br,I):
 Hydrothermal syntheses and structure determinations

qdat:
AAAAAAAAAAABAAAAAAAAAAAiABAAAAAAAgAIAAABAEQAAAgUAAACEIAAAAggBBgIAIgAAglQAAJAAiABCQEzFCIQAARCTIMkAQDQIhKkAkaCCoBIIIBWYlACVBJGeCDgWIqBCohYCBSgVWsCII0RhCJMtAh4DAQVIyTIBh==


formula: K As4 O6 Br
compound: Synthetic
formula_title: KAs4O6Br
a: 5.257
b: 5.257
c: 8.955
alpha: 90
beta: 90
gamma: 120
cell_volume: 214.325
crystal_density: 3.988
atoms_sites: ["KM", "As", "O", "BrX"]
atoms_x: AAAAAFVYFACAhB4AAAAAAA==
atoms_y: AAAAAKuwKAAAAAAAAAAAAA==
atoms_z: gIQeAGCxDACwWhMAAAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["KM", "As", "O", "BrX"]
atoms_aniso_u11: 0MkBAACWAABQ9QAAQDIBAA==
atoms_aniso_u22: 0MkBAACWAABwewAAQDIBAA==
atoms_aniso_u33: kMMBAHD4AACQRgEAUIUCAA==
atoms_aniso_u12: 6OQAAJBMAADQIAAAIJkAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAA==
qdat:
AAAAAAAAAAACAAAAAAAAAAAoABAAAAAABAAQAAABAEgAAAxEAAACQQAAABEABEhAASAAAgxABBIABIACGBAqogQgAAkgpFAwIAFAJGgwQIwiigCiEAJqsoAUUHJU0jCAskYRhkhhIQkBtVEKYuSFJhBriEhhEEiZImRQhJ==


formula: K As4 O6 I
compound: Synthetic
formula_title: KAs4O6I
a: 5.281
b: 5.281
c: 9.169
alpha: 90
beta: 90
gamma: 120
cell_volume: 221.455
crystal_density: 4.212
atoms_sites: ["KM", "As", "O", "IX"]
atoms_x: AAAAAFVYFACAhB4AAAAAAA==
atoms_y: AAAAAKuwKAAAAAAAAAAAAA==
atoms_z: gIQeANgfDQAQlhMAAAAAAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["KM", "As", "O", "IX"]
atoms_aniso_u11: 0BQCAJCXAADQZQEAgAYBAA==
atoms_aniso_u22: 0BQCAJCXAADgeQAAgAYBAA==
atoms_aniso_u33: AMIBAMAlAQAAXgEA0LABAA==
atoms_aniso_u12: aAoBAMhLAACwgQAAQIMAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAA==
qdat:
AAAAAAAAAAAEAAAAAAAAAABAACAAAAAAIAIAAAACAYAAADAQAAAQIAAAAQAAEGAACAAAGGAAIQABBAAYwAEYACIAAIAOYAYAAjADMAZABsAIgDYAGAdgGAAsB2A7AJAFgNABgMgIAbA+BUA8BQPgBA0DAFgwBIDgODQBg0==


formula: Ca6.12 Al7 O16 F.99
compound: Synthetic
pub_title: Refinement of the structure of 11CaO*7Al2O3*CaF2
formula_title: <missing>
a: 11.97
b: 11.97
c: 11.97
alpha: 90
beta: 90
gamma: 90
cell_volume: 1715.072
crystal_density: 2.746
atoms_sites: ["Ca1", "Ca2", "Al1", "Al2", "O1", "O2", "F"]
atoms_x: cLsGAKApBABg4xYAIBMOAHC2CwCwKBMA4Gc1AA==
atoms_y: AAAAAAAAAAAAAAAAIBMOABBwEQCwKBMAAAAAAA==
atoms_z: QEIPAEBCDwBAQg8AIBMOAHAMBgCwKBMAQEIPAA==
atoms_occupancy: gCotAAAXEQAACT0AAAk9AAAJPQAACT0AQCQUAA==
atoms_u_iso: 0HAAADhFAACoJQAAcDUAAEieAABIngAAULMBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAACAAAAAAACAAgAAAQAgBACAABAEAAAAgICAAICBAQIEAABAgQQQQIAIIAQQQgBCCEIQgCAEQhCAQgAIhAQiARCAgAiIgEAIgAERASACAAEAAACAAAAAAAACQAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca6 Al7 O16 F.87
compound: Synthetic
pub_title: Improved powder X-ray data for the cement phase Ca12Al14O32F2 (C11A7f)
formula_title: <missing>
a: 11.96269
b: 11.96269
c: 11.96269
alpha: 90
beta: 90
gamma: 90
cell_volume: 1711.932
crystal_density: 2.723
atoms_sites: ["Ca1", "Ca2", "Al1", "Al2", "O1", "O2", "F"]
atoms_x: 4LkGAOD9AwDAGA4AYOMWADDJCwDANhMA4Gc1AA==
atoms_y: AAAAAAAAAADAGA4AAAAAAMB0EQDANhMAAAAAAA==
atoms_z: QEIPAEBCDwDAGA4AQEIPAIAaBgDANhMAQEIPAA==
atoms_occupancy: oA0qAGD7EgAACT0AAAk9AAAJPQAACT0AQLMRAA==
atoms_u_iso: IGcAACBnAAAAEnoAABJ6AAASegAAEnoAwNQBAA==
atoms_aniso_label: ["Al1", "Al2", "O1", "O2"]
atoms_aniso_u11: 0GsAAMBdAADwBAEA4KsAAA==
atoms_aniso_u22: 0GsAAECcAABgbQAA4KsAAA==
atoms_aniso_u33: 0GsAAECcAADgLgAA4KsAAA==
atoms_aniso_u12: 0O7//wAAAADgsf//QB8AAA==
atoms_aniso_u13: 0O7//wAAAAAAAAAAQB8AAA==
atoms_aniso_u23: 0O7//wAAAADAXQAAQB8AAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAEAABAAAAAAACAAgAAAQAgBACAAAgEAAAAgICAAICBAQIEAAAggQQQIIAIIAQQQgBCCEIIQBAEIRCAQgAIhAIhAQiAgAREQEAEQACIgRACAACAAACAAAAAAAACQAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca6 Al7 O16 F
compound: Synthetic
formula_title: <missing>
a: 11.981
b: 11.981
c: 11.981
alpha: 90
beta: 90
gamma: 90
cell_volume: 1719.805
crystal_density: 2.720
atoms_sites: ["Ca", "Al1", "Al2", "O1", "O2", "F"]
atoms_x: AL0GAGDjFgBALw4A0AgEALDuCwDAJwkA
atoms_y: AAAAAAAAAABALw4A0AgEAEBoEQAgoQcA
atoms_z: QEIPAEBCDwBALw4A0AgEAMAgBgCAhB4A
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAIFgUA
atoms_u_iso: YIYAAEB+BQAAcQIA4CgBAMDaAAAAdwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 On the preparation of single crystals of 11CaO*7Al2O3*CaF2
 and the confirmation of its crystal structure

qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAACAAgAAAQAgBAEAABAEAAABAICAAIEBAgQIAABAgggQQQAQQAggggBCEEIQgCAIQhEARAAQiERCAiEBABCIgIAJAAESAiAEAAEAAAEAAAAAAAAEgAAAAAAAAAAAAAAAAAAAAAAA==


formula: Na6.88 Fe4 As6 O24
compound: Synthetic
formula_title: <missing>
a: 13.807
b: 13.807
c: 18.354
alpha: 90
beta: 90
gamma: 120
cell_volume: 3030.121
crystal_density: 3.995
atoms_sites: ["Na1", "Na2", "Fe1", "Fe2", "As", "O1", "O2", "O3", "O4"]
atoms_x: AAAAADBPMAAAAAAAwKEvAMBDCwBwOCAAoIQrAEAoJAAwiAEA
atoms_y: AAAAAGADAQAAAAAAAAAAAHBYPADAyAMAkFMDACBwCwDACAoA
atoms_z: AAAAABBHAwBAQg8AQEIPAHDhCAAA/AgA0N4KACBIAQAAtgMA
atoms_occupancy: AAk9AIDQOwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: OAMBAGBYAQC4dAAA+FwAAMhuAAAIwAAA+MUAADiuAACg4QAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of Na7Fe4(AsO4)6 and alpha-Na3Al2(AsO4)3,
 two sodium ion conductors structurally related to II-Na3Fe2(AsO4)3

qdat:
AAAAAAAAAAAAAAIQAAAABABBEBIABAIAUERABEChQBESEWWCDYhSGFGUEukGKXK4U0VyKOwiyeWrEWrWo0xSNw+2I0dzdJq9MuVNzaSNE6WWTorLBhnB4owMDJWRGlQIg2jhQAYoFyCGBgEAKBggQCASCAAkAAAAQAAAAA==


formula: Ba3 V2 O8
compound: Synthetic
pub_title: Crystal growth of alkaline earth vanadates from hydroxide fluxes
formula_title: <missing>
a: 5.7733
b: 5.7733
c: 21.339
alpha: 90
beta: 90
gamma: 120
cell_volume: 615.961
crystal_density: 5.191
atoms_sites: ["Ba1", "Ba2", "V", "O1", "O2"]
atoms_x: AAAAALin6/9VWBQAYBMoAFVYFAA=
atoms_y: AAAAAFVYFAC4p+v/MIX1/7in6/8=
atoms_z: AAAAACDTBwAYhAQAaC0GALCv//8=
atoms_occupancy: 0
atoms_u_iso: EDoBAOD2AAAQ1gAAsDABABDpAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAACAAAAAAEAQAAAACEAAIAAAIAAQQAQgUAKAEAAAAIQCIUBACABAEQABAIAAEAgCRAoEAAAgowgIAAkJEIEAg0AIIAACBSEEBBQpFEACikQQAUAgACEFBRBCgYQACKhEAEBAAhChiAEbIgEggAhABAACyI==


formula: Ba5 V3 O13 H
compound: Synthetic
pub_title: Crystal growth of alkaline earth vanadates from hydroxide fluxes
formula_title: Ba5(VO4)3OH
a: 10.4589
b: 10.4589
c: 7.8476
alpha: 90
beta: 90
gamma: 120
cell_volume: 743.429
crystal_density: 4.684
atoms_sites: ["Ba1", "Ba2", "V", "O1", "O2", "O3", "O4", "H"]
atoms_x: VVgUAPDNDwAobBYA8FwcAJBmHQDwkQ8AAAAAAAAAAAA=
atoms_y: q7AoAIj0AACAdhgAwAIkANDzEwBQLBUAAAAAAAAAAAA=
atoms_z: gPj//0BCDwBAQg8AQEIPAEBCDwBAnQQAgC4LAICjBAA=
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgIQeAICEHgA=
atoms_u_iso: MOMAABDlAADAsgAAACwBADAkAQDwaAEAsMYBAEANAwA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAEAAAAACAAgAAQgACAAQEAAICIAQAAiCQDBAYAQEIAQoCAChQIQUCCIDKCAKKEQcIRAhCAowkKESAcIFcJGESE4gJixiKCxA1NGRImYNmHIo2QbHM2i5CZTEo8hsxo55C5TJmSNnbKWRpXTlIWZMjUb1pkkU==


formula: Sr5 V3 O13 H
compound: Synthetic
pub_title: Crystal growth of alkaline earth vanadates from hydroxide fluxes
formula_title: Sr5(VO4)3OH
a: 10.0570
b: 10.0570
c: 7.4349
alpha: 90
beta: 90
gamma: 120
cell_volume: 651.242
crystal_density: 4.079
atoms_sites: ["Sr1", "Sr2", "V", "O1", "O2", "O3", "O4", "H"]
atoms_x: sCsuAKuwKAC4uSQAQKApAGC+GADwLSgAAAk9AAAAAAA=
atoms_y: iKkAAFVYFADIlOn/8HPi/xBx4/9Qv/D/AAAAAAAAAAA=
atoms_z: wMYtAACRHgDAxi0AwMYtAMDGLQDgpyIAABcqAICjBAA=
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgIQeAICEHgA=
atoms_u_iso: kJcAAFCvAACYcQAAwNoAAKDwAAAwVgEAYFUEAEANAwA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAgAAAAAEABAAAgQABQACBAABgggCAACEIgFAQiAYCJAIWJCAM0JECiQIoEGgUSUckIsJQwBGKUoSliMJVMFQkVYkMTMKuZjFzU3V3KqHUz4+4Ty1Fsuafn3r5Gn6OTXK8bN9tOtfrVyZLWfktxN7TNnpalp==


formula: Ba K V O4
compound: Synthetic
pub_title: Crystal growth of alkaline earth vanadates from hydroxide fluxes
formula_title: KBaVO4
a: 7.802
b: 5.908
c: 10.376
alpha: 90
beta: 90
gamma: 90
cell_volume: 478.274
crystal_density: 4.046
atoms_sites: ["Ba", "K", "V", "O1", "O2", "O3"]
atoms_x: wPMeACA5MwA4bBAAMMEdAEC+CwBwTAwA
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwAArwAA
atoms_z: EJwSADBhIwAIjiMAQC4jAGgUGgBIUygA
atoms_occupancy: 0
atoms_u_iso: cLwAAFCWAADgMgEA4FoBAHARAQBgNQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAABAAAYAAAYABACAgAQSAUAEgQNEEgUyQANAICQHSZE8EHsSjQcQR9UGxUraVz0CsAe/X2hzxh+0dx823lf/eqJ15PXu//77b/b//Wl+ff30vddZf+v/v7+f//b73/+9/bO/OP/ff3/9fz/32p/69/t7==


formula: Mn C2 O6 H4
compound: Synthetic
pub_title: The monoclinic polymorph of catena-poly [[diaquamanganese(II)]-mu-oxalato-4O1,O2:O1',O2']
formula_title: <missing>
a: 11.7648
b: 5.6440
c: 9.6367
alpha: 90
beta: 125.843
gamma: 90
cell_volume: 518.704
crystal_density: 2.292
atoms_sites: ["Mn", "C", "O1", "O2", "O3", "H1", "H2"]
atoms_x: gIQeACidIQDo1SMAmOQjAGBpEwCgUQ4AgCoUAA==
atoms_y: GLsiALhIBABIPDUA+FYQAMiIIgAQdSUAEBgoAA==
atoms_z: wMYtACjlMwDwWTgAMEw4ABhQLgBA3icAcNkzAA==
atoms_occupancy: 0
atoms_u_iso: aIMAAECDAADwoAAACJgAAEC1AADA2gAAwNoAAA==
atoms_aniso_label: ["Mn", "C", "O1", "O2", "O3"]
atoms_aniso_u11: OKQAAAB9AADAwQAAwMEAABC9AAA=
atoms_aniso_u22: 8FAAANCdAACwaAAAkGUAABC9AAA=
atoms_aniso_u33: 8H0AAGBtAADQhAAAAH0AAGCGAAA=
atoms_aniso_u12: AAAAAJABAACwBAAAMPj//9AHAAA=
atoms_aniso_u13: CEgAAMBEAAAwQwAAcEkAAJBMAAA=
atoms_aniso_u23: AAAAAJABAADwCgAAoPb///Dx//8=
qdat:
AAAAAAAAAAAAAAAAAAAAAEgAAABAEAAAAAAAARAUAAAVABQABAAgACCAKUgBAAAECVIRBBAAAUQKaoRRKAIKECopCJAUMkEsBCMwlU4URV0xBFdM1MMlAK6OHnUViBRozd/SXI5GDLdmNr86DcMt21xMOtn8dl2SJlfSaN==


formula: Mn C2 O6
compound: Synthetic
formula_title: <missing>
a: 12.0155
b: 5.6323
c: 9.9609
alpha: 90
beta: 128.37
gamma: 90
cell_volume: 528.509
crystal_density: 2.199
atoms_sites: ["Mn", "C", "O1", "O2", "O3"]
atoms_x: AAAAAGDeAgBgTwUAYE8FAKDNCgA=
atoms_y: YK4KAOAyKQCABx4AQF40AGCuCgA=
atoms_z: QEIPAAB8FQBAgxkAQIMZAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Contribution a l'etude des oxalates de certains metaux bivalents.
 III. - Structure cristalline des oxalates dihydrates de manganese,
 de cobalt, de nickel et de zinc. Polymorphisme des oxalates dihydrates
 de cobalt et de nickel

qdat:
AAAAAAAAAAAAAAAAAAAAACQAAABABAAAAAAAAQQEAAAIUBBAAIAIACBABKiAgAAAitCJBCEAAEMCLHCgkwCANEmAOiCDAmAFEAFJwhJxiAUeMUEaovWUwQGmwZZBIao5BU/3iCd6DdC9H1+SatSVK/vT0szz5k8wYg0xdN==


formula: Co C2 O6
compound: Synthetic
formula_title: CoC2O4*2H2O
a: 11.7750
b: 5.4160
c: 9.8590
alpha: 90
beta: 127.85
gamma: 90
cell_volume: 496.467
crystal_density: 2.394
atoms_sites: ["Co", "C", "O1", "O2", "O3"]
atoms_x: AAAAAICvAgCAIAUAgCAFAKDNCgA=
atoms_y: YK4KAOAyKQBgPB0AwBk1AGCuCgA=
atoms_z: QEIPACDQFABAgxkAQIMZAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Contribution a l'etude des oxalates de certains metaux bivalents.
 III. - Structure cristalline des oxalates dihydrates de manganese,
 de cobalt, de nickel et de zinc. Polymorphisme des oxalates dihydrates
 de cobalt et de nickel

qdat:
AAAAAAAAAAAAAAAAAAAAAAMAAABAAEAAAAAAAACgggAAFgAUAAEBABABABAsAAQAIQKWRIgAIAAKAbMDHVAAkBiUJdQCAA2kQpwSBRPaK0yCnwQhDGuJ3FSlEZTEWqA9SJdEGt0JGVJlxI+rD03IkMbGsd+UXi6tDuTjhg==


formula: Ni C2 O6
compound: Synthetic
formula_title: NiC2O4*2H2O
a: 11.7748
b: 5.3328
c: 9.8326
alpha: 90
beta: 127.21
gamma: 90
cell_volume: 491.724
crystal_density: 2.414
atoms_sites: ["Ni", "C", "O1", "O2", "O3"]
atoms_x: AAAAACBCAgAgMAUAIDAFAIB/CgA=
atoms_y: YK4KAEAjKQBgvxwAIIc1AMCeCgA=
atoms_z: QEIPAGByFACAohkAgKIZAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Contribution a l'etude des oxalates de certains metaux bivalents.
 III. - Structure cristalline des oxalates dihydrates de manganese,
 de cobalt, de nickel et de zinc. Polymorphisme des oxalates dihydrates
 de cobalt et de nickel

qdat:
AAAAAAAAAAAAAAAAAAAAAAKAAACAAEAAAAAAAABJAEAAiQAUAABCAEAAQEA0gABAkAKjJIAABAAFCGECzSAgDNAE8aoQAQK0KDTBCGKadrAzk4BDYxslODumxBYmtH2EpGK1uKxNKDCYfHW64nCrIidEmLBwTmy7ZC7YNh==


formula: Zn C2 O6
compound: Synthetic
formula_title: ZnC2O4*2H2O
a: 11.8039
b: 5.4028
c: 9.9213
alpha: 90
beta: 127.70
gamma: 90
cell_volume: 500.625
crystal_density: 2.460
atoms_sites: ["Zn", "C", "O1", "O2", "O3"]
atoms_x: AAAAAGDeAgDAPwUAwD8FAODsCgA=
atoms_y: YK4KAIBCKQDgeh0AQNs0AGCuCgA=
atoms_z: QEIPAIA9FQAgshkAILIZAEBCDwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAMAAACAAIAAAAAAAABCAgAARAAoAAEEAIACACCYAAQBCAkbCoAAIAAUEXCEjggAwEQYS+AgAIUUoCAoQwOg1hiB2EAswUVc+sGaGKpg6IZiqM/FMsYbaVhj4d93ZkzRSSNGsdMyXdHxa/0Fyw==


formula: Al1.99 Fe.07 Zn.94 O4
compound: Jemaa, Kaduna State, Nigeria
formula_title: <missing>
a: 8.0850
b: 8.0850
c: 8.0850
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.494
crystal_density: 4.602
atoms_sites: ["AlM", "Fe2+M", "Fe3+M", "ZnT", "Fe2+T", "AlT", "O"]
atoms_x: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMB8QAA==
atoms_y: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMB8QAA==
atoms_z: gIQeAICEHgCAhB4AIKEHACChBwAgoQcAMB8QAA==
atoms_occupancy: gNA7AGDqAAAgTgAAgF85AMDUAQDA1AEAAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["AlM", "Fe2+M", "Fe3+M", "ZnT", "Fe2+T", "AlT", "O"]
atoms_aniso_u11: 2EAAANhAAADYQAAAGEwAABhMAAAYTAAAoEYAAA==
atoms_aniso_u22: 2EAAANhAAADYQAAAGEwAABhMAAAYTAAAoEYAAA==
atoms_aniso_u33: 2EAAANhAAADYQAAAGEwAABhMAAAYTAAAoEYAAA==
atoms_aniso_u12: iPr//4j6//+I+v//AAAAAAAAAAAAAAAA8Pv//w==
atoms_aniso_u13: iPr//4j6//+I+v//AAAAAAAAAAAAAAAA8Pv//w==
atoms_aniso_u23: iPr//4j6//+I+v//AAAAAAAAAAAAAAAA8Pv//w==
pub_title:
 Crystallographic and spectroscopic characterization of a natural Zn-rich spinel
 approaching the endmember gahnite (ZnAl2O4) composition


formula: Pb.92 Ca.87 Mn.09 Sr.01 Na.05 (Sb1.73 Fe.27) O7
compound: Harstigen mine, Varmland, Sweden
formula_title: <missing>
a: 10.3783
b: 10.3783
c: 10.3783
alpha: 90
beta: 90
gamma: 90
cell_volume: 1117.837
crystal_density: 6.776
atoms_sites: ["PbA", "CaA", "MnA", "SrA", "NaA", "SbB", "Fe3+B", "O1", "O2"]
atoms_x: gIQeAICEHgCAhB4AgIQeAICEHgAAAAAAAAAAAMCzEwBg4xYA
atoms_y: gIQeAICEHgCAhB4AgIQeAICEHgAAAAAAAAAAACChBwBg4xYA
atoms_z: gIQeAICEHgCAhB4AgIQeAICEHgAAAAAAAAAAACChBwBg4xYA
atoms_occupancy: gBMcAOCMGgAgvwIAIE4AAKCGAQCgyzQAYD0IAAAJPQAACT0A
atoms_u_iso: 4CgBAOAoAQDgKAEA4CgBAOAoAQCwgQAAsIEAAACWAADA1AEA
atoms_aniso_label: ["PbA", "CaA", "MnA", "SrA", "NaA", "SbB", "Fe3+B", "O1", "O2"]
atoms_aniso_u11: 4CgBAOAoAQDgKAEA4CgBAOAoAQCwgQAAsIEAAOCrAADA1AEA
atoms_aniso_u22: 4CgBAOAoAQDgKAEA4CgBAOAoAQCwgQAAsIEAADCOAADA1AEA
atoms_aniso_u33: 4CgBAOAoAQDgKAEA4CgBAOAoAQCwgQAAsIEAADCOAADA1AEA
atoms_aniso_u12: YM3//2DN//9gzf//YM3//2DN///Y9f//2PX//wAAAAAAAAAA
atoms_aniso_u13: YM3//2DN//9gzf//YM3//2DN///Y9f//2PX//wAAAAAAAAAA
atoms_aniso_u23: YM3//2DN//9gzf//YM3//2DN///Y9f//2PX//zBDAAAAAAAA
pub_title:
 Oxyplumboromeite, Pb2Sb2O7, a new mineral species of the pyrochlore supergroup
 from Harstigen mine, Varmland, Sweden

qdat:
AAAAAAAAAAQAAAIAAEAAQAEACAAAEAIBAEAgIBAAICBAgQQIAEEEEAIIAghCEIQBCIQiEAiIhEQEREBECIiRECRIkQRIkkCSQJBJJFApJJAKSSElBIUkpCUpQUoUJSBAlShEqgSpgQihECiQRBCIKAAKIgAgAIgQAAAIgA==


formula: K Cu Cl3
compound: Synthetic
pub_title: Crystal strucutres of KCuCl3 and NH4CuCl3
formula_title: <missing>
a: 4.029
b: 13.785
c: 8.736
alpha: 90.
beta: 97.33
gamma: 90.
cell_volume: 481.230
crystal_density: 2.885
atoms_sites: ["K", "Cu", "Cl1", "Cl2", "Cl3"]
atoms_x: kMIvAICyDgAgzxAA4GQpADAI9f8=
atoms_y: 6GwKAIAJAwB4IQwAmIv///gGBgA=
atoms_z: 4P0hAPCcCQBgDRAAuKITAJjx/f8=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["K", "Cu", "Cl1", "Cl2", "Cl3"]
atoms_aniso_u11: gOMAAOCrAACQ9gAA4KYAABADAQA=
atoms_aniso_u22: oKkBALgUAQBwNAEACG8BAHBDAQA=
atoms_aniso_u33: 8CYCADBlAQAwugEAYF0BAPhgAQA=
atoms_aniso_u12: EOH//wglAABwMAAA+CUAAIAlAAA=
atoms_aniso_u13: 8Pb//5DP///4t///QBoAAGD///8=
atoms_aniso_u23: INv//xDc//+IOwAAOA4AAPDd//8=
qdat:
AAAAAAAAAAAAAAIQAAAEAAAAQJQIEAIQCRCAAhDJRABAQkQYsiCCMmGBIZYZH04QOKUjAcFfFSyKy6Wi8PUa73+raF1pu0mm+vMO6MsLX5xeT99+Fn/f7Ns2hdL1KYb/PW/x+r/qXf/ld4f7asYXFS8e/51Zwvp7f7xahn==


formula: Pt Cu As S2
compound: Tao and Ma districts, Fengning County, Chengde Prefecture, Hebei Province, China
pub_title: Determination of daomanite crystal structure
formula_title: <missing>
a: 5.852
b: 15.876
c: 3.756
alpha: 90
beta: 90.
gamma: 90
cell_volume: 348.956
crystal_density: 7.570
atoms_sites: ["Pt", "Cu", "As", "S1", "S2"]
atoms_x: QEIPAKAyDwDg6jQAQKwnAECsJwA=
atoms_y: gPwKAMC1GwDACQ4AAGQZAIAUBwA=
atoms_z: IDwDAIAsAwCALAMAQA0DAEANAwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAQAAAAAgAAAAAAKAAABAABABAEcEAAAAEACQIEAAFIQBBYAiRDgjAAwUpCBOBAEgZSgBgRAITBIDAiRCkUiJAcByCYAAWyEIQEFmYQmRAzICgijLwMhKslAg0UIQqROAhpkSOkuB0cLYiqRpIuLBhTUEEJ==


formula: Pt Cu As S2
compound: Tao and Ma districts, Fengning County, Chengde Prefecture, Hebei Province, China
pub_title: Determination of daomanite crystal structure
formula_title: <missing>
a: 3.756
b: 15.876
c: 5.852
alpha: 90
beta: 90.
gamma: 90
cell_volume: 348.956
crystal_density: 7.570
atoms_sites: ["Pt", "Cu", "As", "S1", "S2"]
atoms_x: IDwDAIAsAwCALAMAQA0DAEANAwA=
atoms_y: gPwKAMC1GwDACQ4AAGQZAIAUBwA=
atoms_z: QEIPAKAyDwDg6jQAQKwnAECsJwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAQAAAAAAAAQAAAIACAABABQBAAUEAAAUEBCAAEAABIgLRIABhCADSCyEpACMBACoZwFIABACjhpBQjFSAegFC5AiAKkBWgQISEM1aCFBgRIKwiCLehlIkFhokQMQ4FIERMmSoMhTsEDU6iRLJmiBRDEcEB==


formula: Co.42 Cu3.33 Mn.17 Ni.07 Mg.01 Cl2 O6 H6
compound: Torrecillas mine, Iquique Provence, Chile
formula_title: <missing>
a: 6.8436
b: 6.8436
c: 14.0637
alpha: 90
beta: 90
gamma: 120
cell_volume: 570.426
crystal_density: 3.694
atoms_sites: ["CoM1", "CuM1", "MnM1", "NiM1", "MgM1", "CuM2", "Cl", "O", "H"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AAAAAAACZDABgPQgA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABn8/+gwvf/
atoms_z: gIQeAICEHgCAhB4AgIQeAICEHgAAAAAAWNgLAEC8AwBAhAQA
atoms_occupancy: gKIZAEAkFABAYAoAwEUEAECcAAAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: wKgAAMCoAADAqAAAwKgAAMCoAACwzAAAoAkBALD+AABg2AMA
atoms_aniso_label: ["CoM1", "CuM1", "MnM1", "NiM1", "MgM1", "CuM2", "Cl", "O"]
atoms_aniso_u11: gLsAAIC7AACAuwAAgLsAAIC7AAAgywAAQBkBAGDqAAA=
atoms_aniso_u22: gLsAAIC7AACAuwAAgLsAAIC7AACAuwAAQBkBAGDqAAA=
atoms_aniso_u33: oIwAAKCMAACgjAAAoIwAAKCMAABg6gAAYOoAAOAoAQA=
atoms_aniso_u12: wF0AAMBdAADAXQAAwF0AAMBdAADAXQAAoIwAAGBtAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAACgDwAAAAAAAMDg//8=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAABAHwAAAAAAAMDg//8=
pub_title:
 Leverettite from the Torrecillas mine, Iquique Provence, Chile:
 the Co-analogue of herbertsmithite

qdat:
AAAAAAAAAAAAAAAAAAAQAAIQAAAAAACAAACAQBIAAQAACAQIAgAIAgQkAEABAQQgQUAgAIoQQDADGIEBAgMAgMARCEBBExGBAIyECAjAAwkyMAJMECAkhAAmACJJMIAyIQLACEQIATRESUwgJEQWAIKSApTEJREpEEyIAU==


formula: W2 O7 H2
compound: Synthetic
formula_title: <missing>
a: 10.305
b: 10.305
c: 10.305
alpha: 90
beta: 90
gamma: 90
cell_volume: 1094.319
crystal_density: 5.848
atoms_sites: ["W", "O", "Wat"]
atoms_x: AAAAAAALEwBg4xYA
atoms_y: AAAAACChBwBg4xYA
atoms_z: AAAAACChBwBg4xYA
atoms_occupancy: 0
atoms_u_iso: uDIBAPjFAACQFwMA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Direct synthesis and single crystal structure determination of cubic
 pyrochlore-type tungsten trioxide hemihydrate, WO3*0.5H2O

qdat:
AAAAAAAAAAQAAAIAACAAIACABAAACAEAQCAQCAgACBAQIEECABBBBACCAEIQQhCAIhCIQgIRCIiAiIgIgJEREgREiRBEkSIJEgkEiSSCSSUAklIJSCglKSEpSQpQkKUCApUiFKgUqQIiREEigRBCIKAAGIQAQAEQIAAAEQ==


formula: Ag2 (Se.49 S.42 Te.09)
compound: San Carlos mine, Guanajuato, Mexico
pub_title: On the symmetry and crystal structure of aguilarite, Ag4SeS
formula_title: <missing>
a: 4.2478
b: 6.9432
c: 8.0042
alpha: 90
beta: 100.103
gamma: 90
cell_volume: 232.410
crystal_density: 7.984
atoms_sites: ["Ag1", "Ag2", "Se", "S", "Te"]
atoms_x: 0AsuAECaEQCw/RUAsP0VALD9FQA=
atoms_y: UNcAAFB0EwAwtw4AMLcOADC3DgA=
atoms_z: oGESAEBVGgCw9wcAsPcHALD3BwA=
atoms_occupancy: AAk9AAAJPQBA6B0AgKIZAEB+BQA=
atoms_u_iso: UBMBALgZAQDQUQEA0FEBANBRAQA=
atoms_aniso_label: ["Ag1", "Ag2", "Se", "S", "Te"]
atoms_aniso_u11: 0BoBAEggAQDwTwEA8E8BAPBPAQA=
atoms_aniso_u22: MBUBAFAdAQDgWgEA4FoBAOBaAQA=
atoms_aniso_u33: aAoBAOAPAQAASgEAAEoBAABKAQA=
atoms_aniso_u12: IP7//1AAAADY+v//2Pr//9j6//8=
atoms_aniso_u13: sDEAAIgxAAAoPAAAKDwAACg8AAA=
atoms_aniso_u23: AAAAAPgCAADY////2P///9j///8=
qdat:
AAAAAAAAAAAAAAAAAAAAQAAAAgEAAQUAAhAAAAAUQALAAAAQABwCNQEQQAEgaRGAIIgFQFFAYgAWGIJVr4CAycBGAxHXLBJNJBjs2KMPGqMKt71gRI4WR/yDWPfdK64r9VrH965l5Zu8/fzir36vC/98v5Gk33r39TrPHu==


formula: Ca1.06 Na.82 (Ta1.79 Nb.21) O6.21 F.79 H.27
compound: Volta Grande pegmatite, Nazareno, Minas Gerais, Brazil
formula_title: <missing>
a: 10.4191
b: 10.4191
c: 10.4191
alpha: 90
beta: 90
gamma: 90
cell_volume: 1131.073
crystal_density: 6.100
atoms_sites: ["CaA", "NaA", "TaB", "NbB", "OX", "O-HX", "FY", "O-HY"]
atoms_x: AAAAAAAAAAAAAAAAAAAAACChBwAgoQcAIKEHACChBwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAACChBwAgoQcAIKEHACChBwA=
atoms_z: gIQeAICEHgAAAAAAAAAAAHBtEwBwbRMAoCUmAKAlJgA=
atoms_occupancy: QFkgAEAGGQBgoDYAoGgGAMBsPABAnAAAwDcwAEDRDAA=
atoms_u_iso: IMsAACDLAABwRAAAcEQAAPCHAADwhwAAEL0AABC9AAA=
atoms_aniso_label: ["CaA", "NaA", "TaB", "NbB", "OX", "O-HX", "FY", "O-HY"]
atoms_aniso_u11: IMsAACDLAABwRAAAcEQAACCAAAAggAAAEL0AABC9AAA=
atoms_aniso_u22: IMsAACDLAABwRAAAcEQAACCAAAAggAAAEL0AABC9AAA=
atoms_aniso_u33: IMsAACDLAABwRAAAcEQAAJCXAACQlwAAEL0AABC9AAA=
atoms_aniso_u12: 8L////C///9Q9v//UPb//7BPAACwTwAAAAAAAAAAAAA=
atoms_aniso_u13: 8L////C///9Q9v//UPb//wAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u23: 8L////C///9Q9v//UPb//wAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 Fluorcalciomicrolite, (Ca,Na,_)2Ta2O6F, a new microlite-group mineral
 from Volta Grande pegmatite, Nazareno, Minas Gerais, Brazil

qdat:
AAAAAAAAAAgAAAQAAIAAQAEACAAAEAQBAIBAQCAAQECBAggQAIIQQAQgBCCEIQgEIQiEQCISERAREQEQIiJEQJEiSBEkSQJJAkEkkkEkkoBJKQUkJCUlISUpClCRKQIEqUIlUCVUCEUIgoUEIIiCgABhEAEACICAAACIAA==


formula: Te Cu3 O6
compound: the Gambatesa mine, Val Graveglia, eastern Liguria, Italy
pub_title: Mcalpineite from the Gambatesa mine, Italy, and redefinition of the species
formula_title: <missing>
a: 9.53928
b: 9.53928
c: 9.53928
alpha: 90
beta: 90
gamma: 90
cell_volume: 868.054
crystal_density: 6.339
atoms_sites: ["Te", "Cu", "O"]
atoms_x: QEIPAAgcOwAgYBYA
atoms_y: QEIPAAAAAABgrgoA
atoms_z: QEIPAEBCDwCQIBgA
atoms_occupancy: AAk9ALAIPQCwCD0A
atoms_u_iso: kEYBABCeAQDQlwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAABAAAAgAAAAAAgAAgABAAEAAQAEABAAgAAAQAQAgBACAIAQBAEAgCAQCAQAAAEBAQEBAQECAgQICBAgQAEECBBAgggQAQQIQQAQQAQgghBCCAEIQAgCCIIQhAEIgAAIhAEQBEAAAIAAAh==


formula: Ni5 P4
compound: Synthetic
pub_title: Redetermination of Ni5P4
formula_title: <missing>
a: 6.7921
b: 6.7921
c: 10.9922
alpha: 90
beta: 90
gamma: 120
cell_volume: 439.161
crystal_density: 6.312
atoms_sites: ["Ni1", "Ni2", "Ni3", "Ni4", "P1", "P2", "P3", "P4"]
atoms_x: GMwgACCrDACo+iAAAAAAAKDxMQBA4goAAAAAAFVYFAA=
atoms_y: 6DwcAOBdMABYDhwAAAAAAGAXCwDAJjIAAAAAAKuwKAA=
atoms_z: QG8FAGB4DgBgKRcAqEEMALAjDgB4AxsAAAAAALieAwA=
atoms_occupancy: 0
atoms_u_iso: MFcAADBXAACYUwAAqFcAAOBHAAAwTQAAYFQAADBcAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAABAgQAAAAAgAAABAACACJAQAIAgAACAQggBAQEAQCQAFECAAViAoAgQRECSCRCYBhGSBQCkEAkgoFkWQZjkSxiIQIFRQPQwWhMFGCUIlQQFMDkwZKRo0FFtBg0QuMImSbqYoEIaIsMVdNJXJNKNYOY==


formula: Y F3
compound: Synthetic
pub_title: The structures of yttrium and bismuth trifluorides by neutron diffraction
formula_title: <missing>
a: 6.3537
b: 6.8545
c: 4.3953
alpha: 90
beta: 90
gamma: 90
cell_volume: 191.422
crystal_density: 5.063
atoms_sites: ["Y", "F1", "F2"]
atoms_x: EGsWADDnHwBAFQoA
atoms_y: QEIPAEBCDwCw7AMA
atoms_z: cJsDAGASJAAw6xYA
atoms_occupancy: 0
atoms_u_iso: SEkAABiwAADQcAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAIgEACgAAIAAACAQEAgACAAFCCARAGggggYBAAEgCSEYGCdAwEECU4KWSVBFQQBAmwogdWJVCpHjOCKxsE3TDBYtLLJbhRS02Xnt7HjIxX65Kf5Rk9+G/3Kf/hbp8u7Jnd32zsm7Z79==


formula: B1.1 N.9
compound: deposit 31, Luobusa ophiolite, Yarlung Zangbu suture, southern Tibet
pub_title: Qingsongite, natural cubic boron nitride: The first boron mineral from the Earth's mantle
formula_title: <missing>
a: 3.61
b: 3.61
c: 3.61
alpha: 90
beta: 90
gamma: 90
cell_volume: 47.046
crystal_density: 3.459
atoms_sites: ["B", "N", "B"]
atoms_x: AAAAAEBCDwBAQg8A
atoms_y: AAAAAEBCDwBAQg8A
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: AAk9AIDuNgCAGgYA
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAAAgAAAAAAAAAAAABAAAAAAAAAAAAgAAAAAAAAAAAAAAAAAAAAAgA==


formula: K (Al.89 Fe.11) S2 O8
compound: Tolbachik volcano, Kamchatka, Russia
formula_title: <missing>
a: 4.7281
b: 4.7281
c: 7.9936
alpha: 90
beta: 90
gamma: 120
cell_volume: 154.756
crystal_density: 2.805
atoms_sites: ["K", "Al", "Fe", "S", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAq7AoAKuwKABwSBUA
atoms_y: AAAAAAAAAAAAAAAAVVgUAFVYFADg+hAA
atoms_z: gIQeAAAAAAAAAAAAMJowAICMJQAAcTQA
atoms_occupancy: AAk9AEBSNgDAtgYAAAk9AAAJPQAACT0A
atoms_u_iso: kF8BACCAAAAggAAA0IQAACAWAQCg1wAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Steklite, KAl(SO4)2: the find at Tolbachik volcano (Kamchatka, Russia).
 Validation as a mineral species and crystal structure

qdat:
AAAAAAAAAAAAAQAAAAAAAAAAAEQACAAAAAAACAAIAAAAIARAAAAUJAAAAEIQAAAAEEACCgIACQAACBMQAACQACQACEQCZSQRAgAAJBIyBigBAFQEQRlACRUCSUASCAgFMpkgBGQIkZcEDQFiJQEORCYDAokCVVUBYFSIUI==


formula: Al F2.52 O.48 H.48
compound: Eldfell volcano, Heimaey, Iceland
pub_title: Oskarssonite, AlF3, a new fumarolic mineral from Eldfell volcano, Heimaey, Iceland
formula_title: <missing>
a: 4.9817
b: 4.9817
c: 12.387
alpha: 90
beta: 90
gamma: 120
cell_volume: 266.227
crystal_density: 3.107
atoms_sites: ["Al", "F", "O-H"]
atoms_x: AAAAAIAyGwCAMhsA
atoms_y: AAAAAAAAAAAAAAAA
atoms_z: AAAAAEBCDwBAQg8A
atoms_occupancy: AAk9AABFMwAAxAkA
atoms_u_iso: qJcBADAoAgAwKAIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAACgAAAAAAQCIAAAAAAAQAAAABBIAAAABDAAABAAAAAAIQABJiQAAAJAAAUUAAABAACQQAACoAIgAAAIAASMAACwACEAABABYwAAoAKAAAUANEAAUAHQAAAAZgAJACA==


formula: Mg Al F5 O2 H4
compound: Synthetic
formula_title: <missing>
a: 7.0637
b: 10.1308
c: 6.7745
alpha: 90
beta: 90
gamma: 90
cell_volume: 484.790
crystal_density: 2.498
atoms_sites: ["Mg", "Al", "F1", "F2", "O", "H"]
atoms_x: AAAAAEBCDwCQWQwAAAAAAAAAAABAQ/r/
atoms_y: AAAAAEBCDwCwogcAQEIPAJijIwDgzSQA
atoms_z: AAAAAEBCDwBwSgQAgN8TAHAuEQAgyhUA
atoms_occupancy: 0
atoms_u_iso: 0M8AACCZAABQDgEAQOcAABC3AQBAfgUA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The thermal dehydration of magnesium aluminum pentafluoride dihydrate:
 crystal structures of MgAlF5(H2O)2 and MgAlF5

qdat:
AAAAAAAAAAAAAAAAAACACEAAAAAAADBAAAChQQAAAIBAACUkCABGBAgRgAAMAF7RMSBEGMhCIApOlBnCwsyIALoFZ5Jclwd0ur5URNRIllA3v04b3CZWpkPy+/DX/rISfO45WHZpt+KlvMmUkncdNL/v93cnxvOj661nkv==


formula: Mg Al F5
compound: Synthetic
formula_title: MgAlF5
a: 7.268
b: 6.123
c: 3.543
alpha: 90
beta: 90
gamma: 90
cell_volume: 157.670
crystal_density: 3.081
atoms_sites: ["Mg", "Al", "Fl", "F2", "F3"]
atoms_x: AAAAAAAAAACAKi0AgIQeAAAAAAA=
atoms_y: AAAAAICEHgAAAAAAAAAAAEDRDAA=
atoms_z: AAAAAICEHgAAAAAAgIQeAICEHgA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The thermal dehydration of magnesium aluminum pentafluoride dihydrate:
 crystal structures of MgAlF5(H2O)2 and MgAlF5

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAABAAABAQAAAAAAAAACAEEAAAAIIAAACAQAAEQABAgMAAAAAwRABAEAAGAAgWAENMAAgDhQACAAAOCFgMaAAUBFQIQAGUI8DA4A4GqBGBGQwwArIEHJAIERAHCtyOHYE8KNmAdBDBGEU==


formula: Cu5 Al5
compound: Synthetic
pub_title: Kristallstruktur von Cu3Al2+ (h) und CuAl (r)
formula_title: <missing>
a: 9.889
b: 4.105
c: 6.913
alpha: 90
beta: 89.996
gamma: 90
cell_volume: 280.629
crystal_density: 5.357
atoms_sites: ["Cu1", "Cu2", "Cu3", "Al1", "Al2", "Al3"]
atoms_x: AAAAAACgDwAgpwYAAAAAAOB1CQDAUBcA
atoms_y: AAAAAAAAAAAAAAAAgIQeAAAAAAAAAAAA
atoms_z: AAAAAAD6AACgkRQAgIQeAECaKgDgGxgA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAQAAAAAQAAAAgCAAIEAAAAAgAABgIEAkAAAARggQAQAIBIGgQkQIaAoAIEBgoCAIaRKEhg2AhBQDjIAqMhQBTTqEiUQIsiXkXuUCURgGGM0Yyy8hghtA6VaW7DvA4lQqqSJlS1OBbGKxkQ7sNXN7UAsb==


formula: Cu5 Al5
compound: Synthetic
pub_title: Kristallstruktur von Cu3Al2+ (h) und CuAl (r)
formula_title: <missing>
a: 12.066
b: 4.105
c: 6.913
alpha: 90
beta: 55.04
gamma: 90
cell_volume: 280.621
crystal_density: 5.357
atoms_sites: ["Cu1", "Cu2", "Cu3", "Al1", "Al2", "Al3"]
atoms_x: AAAAAACgDwAgpwYAAAAAAOB1CQDAUBcA
atoms_y: AAAAAAAAAAAAAAAAgIQeAAAAAAAAAAAA
atoms_z: AAAAAABjLgCA6g0AgIQeAGAkIQAgywAA
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAEAAQAAAAACACIAAAAQEgAABgIAAACAAABiwAI0QABIEAgkQAaQARYABggqEIoQhEzgmAFBRhlMsoAgGBXCLEiGQEsCs5HwUAESwkWIURwioAwlsoxkGQTIjWagsKgaJkylIjHEDx8wptFRganItJ==


formula: Ba Cu Si2 O6
compound: Synthetic
formula_title: <missing>
a: 9.97511
b: 9.97511
c: 22.2887
alpha: 90
beta: 90
gamma: 90
cell_volume: 2217.789
crystal_density: 4.229
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAAAAAACA8RAAYKIMAMDTFgDATxMA
atoms_y: 4G88AEBCDwDQ7S0AoAEsAIB3NQAwoC8A
atoms_z: gIQeAMjZAwCAdzUAQNQxAHCINADQ7wMA
atoms_occupancy: 0
atoms_u_iso: 2AkAAOALAADYCQAA0BEAAOALAADoAwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Hydrothermal synthesis and properties of pigments
 Chinese purple BaCuSi2O6 and dark blue BaCu2Si2O7

qdat:
AAAAAAAAAAAAAAAAAEBAAgAAgAAIQCABAQEQACQAIAgkEEghIISACAIAKEIIUQogiKIIigMRAIRCMSgEkAQQlJiJKhBgqBKFDBASgRQEIimimCUGUWmAoFSawRIhCAEQtAKAIIlACAAEAKgQAgAIECAAAQAAAAAAAAAAAA==


formula: Ba Cu2 Si2 O7
compound: Synthetic
formula_title: <missing>
a: 6.86317
b: 13.1773
c: 6.86317
alpha: 90
beta: 90
gamma: 90
cell_volume: 620.692
crystal_density: 4.629
atoms_sites: ["Ba", "Cu", "Si", "O1", "O2", "O3", "O4"]
atoms_x: MDD//wB6DQDQ1f//oOsFAKDU9P9Auvv/IBIKAA==
atoms_y: QEIPACA1AABQSAgAQEIPAAA0CABAqgYAgNsDAA==
atoms_z: UGE6AHBVMADw2RwAIJodADBZJgAwbA4A4GggAA==
atoms_occupancy: 0
atoms_u_iso: 6AMAAOgDAADwBQAACAIAAOgDAADoAwAA+AcAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Hydrothermal synthesis and properties of pigments
 Chinese purple BaCuSi2O6 and dark blue BaCu2Si2O7

qdat:
AAAAAAAAAAAAAAABAQAAAEAgAABAIAEFQAYgACKAACERgQmCRIRCIDAiCLCCikEsLcCZTgsA5SKIrH41oIeOhcuJws9Nx4+zHnz5XqOVNmATSt88VC8kU4ic1U545rxgtPO/0M0qOe9qTley9n2JXsc77O93avtdem9w8R==


formula: (Mg.758 Fe.242) (Al1.758 Cr.242) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.1334
b: 8.1334
c: 8.1334
alpha: 90
beta: 90
gamma: 90
cell_volume: 538.042
crystal_density: 3.850
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_y: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_z: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_occupancy: wEMuAEDFDgBgpjUAoGIHAAAJPQA=
atoms_u_iso: cGIAAHBiAAAwQwAAMEMAALCBAAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: cGIAAHBiAAAwQwAAMEMAALCBAAA=
atoms_aniso_u22: cGIAAHBiAAAwQwAAMEMAALCBAAA=
atoms_aniso_u33: cGIAAHBiAAAwQwAAMEMAALCBAAA=
atoms_aniso_u12: AAAAAAAAAADw+///8Pv//+D8//8=
atoms_aniso_u13: AAAAAAAAAADw+///8Pv//+D8//8=
atoms_aniso_u23: AAAAAAAAAADw+///8Pv//+D8//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-BI2

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAACAAAAAAAAEAAAAQAAAAAAQAAAgAAAABAAAQAAAAEAAEAAAAQAAgAAAIABAAAAgAIAAAQAEAAAQAIAABABAAAQAQAAIAQAAAAgAAgBAACAIAAQBAAEAQACAIAAAIA==


formula: (Mg.75 Fe.25) (Al1.6 Cr.4) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.1454
b: 8.1454
c: 8.1454
alpha: 90
beta: 90
gamma: 90
cell_volume: 540.427
crystal_density: 3.937
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_y: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_z: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_occupancy: wMYtAEBCDwAA1DAAADUMAAAJPQA=
atoms_u_iso: YG0AAGBtAAAQWQAAEFkAAJB+AAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: YG0AAGBtAAAQWQAAEFkAAJB+AAA=
atoms_aniso_u22: YG0AAGBtAAAQWQAAEFkAAJB+AAA=
atoms_aniso_u33: YG0AAGBtAAAQWQAAEFkAAJB+AAA=
atoms_aniso_u12: AAAAAAAAAACA+P//gPj//wAAAAA=
atoms_aniso_u13: AAAAAAAAAACA+P//gPj//wAAAAA=
atoms_aniso_u23: AAAAAAAAAACA+P//gPj//wAAAAA=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-BI4


formula: Mg.714 Fe.287 (Al1.206 Cr.794) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.2021
b: 8.2021
c: 8.2021
alpha: 90
beta: 90
gamma: 90
cell_volume: 551.792
crystal_density: 4.122
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAHgJEAA=
atoms_y: IKEHACChBwCAhB4AgIQeAHgJEAA=
atoms_z: IKEHACChBwCAhB4AgIQeAHgJEAA=
atoms_occupancy: QJQrAGCEEQDgzSQAIDsYAAAJPQA=
atoms_u_iso: 4EcAAOBHAADIMgAAyDIAABhgAAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: 4EcAAOBHAADIMgAAyDIAABhgAAA=
atoms_aniso_u22: 4EcAAOBHAADIMgAAyDIAABhgAAA=
atoms_aniso_u33: 4EcAAOBHAADIMgAAyDIAABhgAAA=
atoms_aniso_u12: AAAAAAAAAABI+f//SPn//6jz//8=
atoms_aniso_u13: AAAAAAAAAABI+f//SPn//6jz//8=
atoms_aniso_u23: AAAAAAAAAABI+f//SPn//6jz//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-BI16

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAQAAAAAIAAAAAAAAgAAACAAAAAAEAAAIAAAAAQAAEAAAACAACAAAAEAAQAAAEAAgAAAQAEAAAIAEAAAQAIAABABAAAgAgAAQAQAAAAgABAEAAIAQABAEAAIBAAEAgAAAgAE==


formula: (Mg.694 Fe.306) (Al1.38 Cr.62) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.1727
b: 8.1727
c: 8.1727
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.879
crystal_density: 4.074
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAFAJEAA=
atoms_y: IKEHACChBwCAhB4AgIQeAFAJEAA=
atoms_z: IKEHACChBwCAhB4AgIQeAFAJEAA=
atoms_occupancy: wFsqAECtEgBAHSoAwOsSAAAJPQA=
atoms_u_iso: cHsAAHB7AABgVAAAYFQAAOB5AAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: cHsAAHB7AABgVAAAYFQAAOB5AAA=
atoms_aniso_u22: cHsAAHB7AABgVAAAYFQAAOB5AAA=
atoms_aniso_u33: cHsAAHB7AABgVAAAYFQAAOB5AAA=
atoms_aniso_u12: AAAAAAAAAABw+f//cPn//6D2//8=
atoms_aniso_u13: AAAAAAAAAABw+f//cPn//6D2//8=
atoms_aniso_u23: AAAAAAAAAABw+f//cPn//6D2//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-BI24

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAQAAAAAEAAAAAAAAIAAABAAAAAABAAAEAAAAAEAABAAAAAgAAgAAABAAEAAABAAEAAAEABAAACAAgAAEACAAAQAQAAEAEAACAEAAAAIAAIAgAAgCAAEAgABAIAAgEAAAEAA==


formula: (Mg.76 Fe.24) (Al1.718 Cr.282) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.1339
b: 8.1339
c: 8.1339
alpha: 90
beta: 90
gamma: 90
cell_volume: 538.141
crystal_density: 3.873
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAKAJEAA=
atoms_y: IKEHACChBwCAhB4AgIQeAKAJEAA=
atoms_z: IKEHACChBwCAhB4AgIQeAKAJEAA=
atoms_occupancy: AGMuAACmDgDgbTQAIJsIAAAJPQA=
atoms_u_iso: UF8AAFBfAAAgTgAAIE4AAJB+AAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: UF8AAFBfAAAgTgAAIE4AAJB+AAA=
atoms_aniso_u22: UF8AAFBfAAAgTgAAIE4AAJB+AAA=
atoms_aniso_u33: UF8AAFBfAAAgTgAAIE4AAJB+AAA=
atoms_aniso_u12: AAAAAAAAAADw+///8Pv//+D8//8=
atoms_aniso_u13: AAAAAAAAAADw+///8Pv//+D8//8=
atoms_aniso_u23: AAAAAAAAAADw+///8Pv//+D8//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle
 xenoliths of the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):
 Mineralogical evidence of a cooler mantle beneath the West African Craton.
 Note:Sample MAR-TF6

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAACAAAAAAAAEAAAAQAAAAAAQAAAgAAAABAAAQAAAAEAAEAAAAQAAgAAAIABAAAAgAIAAAQAEAAAQAIAABABAAAQAQAAIAQAAAAgAAgBAACAIAAQBAAEAQACAIAAAIA==


formula: (Mg.764 Fe.236) (Al1.76 Cr.24) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.13510
b: 8.13510
c: 8.13510
alpha: 90
beta: 90
gamma: 90
cell_volume: 538.380
crystal_density: 3.842
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_y: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_z: IKEHACChBwCAhB4AgIQeALgKEAA=
atoms_occupancy: gKEuAIBnDgAAtjUAAFMHAAAJPQA=
atoms_u_iso: wF0AAMBdAADAPwAAwD8AAChzAAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: wF0AAMBdAADAPwAAwD8AAChzAAA=
atoms_aniso_u22: wF0AAMBdAADAPwAAwD8AAChzAAA=
atoms_aniso_u33: wF0AAMBdAADAPwAAwD8AAChzAAA=
atoms_aniso_u12: AAAAAAAAAAD4+P//+Pj//4D9//8=
atoms_aniso_u13: AAAAAAAAAAD4+P//+Pj//4D9//8=
atoms_aniso_u23: AAAAAAAAAAD4+P//+Pj//4D9//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-TF7

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAQAAAAAAgAABAAAAABAAAQAAAAEAAEAAAAQAAgAAAIABAAAAgAIAAAQAEAAAQAIAABABAAAQAgAAQAQAAAAgAAgCAAEAIAAQBAAEAQACAIAAAIA==


formula: (Mg.7 Fe.3) (Al1.42 Cr.58) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.1704
b: 8.1704
c: 8.1704
alpha: 90
beta: 90
gamma: 90
cell_volume: 545.419
crystal_density: 4.049
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeANALEAA=
atoms_y: IKEHACChBwCAhB4AgIQeANALEAA=
atoms_z: IKEHACChBwCAhB4AgIQeANALEAA=
atoms_occupancy: gLkqAIBPEgDAVSsAQLMRAAAJPQA=
atoms_u_iso: 0GsAANBrAAAASwAAAEsAAKBzAAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: 0GsAANBrAAAASwAAAEsAAKBzAAA=
atoms_aniso_u22: 0GsAANBrAAAASwAAAEsAAKBzAAA=
atoms_aniso_u33: 0GsAANBrAAAASwAAAEsAAKBzAAA=
atoms_aniso_u12: AAAAAAAAAABw/v//cP7//xD1//8=
atoms_aniso_u13: AAAAAAAAAABw/v//cP7//xD1//8=
atoms_aniso_u23: AAAAAAAAAABw/v//cP7//xD1//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-TF8


formula: (Mg.732 Fe.268) (Al1.6 Cr.4) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.1391
b: 8.1391
c: 8.1391
alpha: 90
beta: 90
gamma: 90
cell_volume: 539.174
crystal_density: 3.960
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAAgLEAA=
atoms_y: IKEHACChBwCAhB4AgIQeAAgLEAA=
atoms_z: IKEHACChBwCAhB4AgIQeAAgLEAA=
atoms_occupancy: gK0sAIBbEAAA1DAAADUMAAAJPQA=
atoms_u_iso: 0GsAANBrAADQUgAA0FIAAMB2AAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: 0GsAANBrAADQUgAA0FIAAMB2AAA=
atoms_aniso_u22: 0GsAANBrAADQUgAA0FIAAMB2AAA=
atoms_aniso_u33: 0GsAANBrAADQUgAA0FIAAMB2AAA=
atoms_aniso_u12: AAAAAAAAAAB4+///ePv///D7//8=
atoms_aniso_u13: AAAAAAAAAAB4+///ePv///D7//8=
atoms_aniso_u23: AAAAAAAAAAB4+///ePv///D7//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-TF21

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAIAAAAACAAAAAAAAEAAAAQAAAAAAgAABAAAAABAAAQAAAAIAAIAAAAQABAAAAIABAAAAgAIAAAQAIAAAQAQAACACAAAgAgAAQAgAAAAgABACAAEAIAAgCAAEAgACAQAAAIA==


formula: (Mg.766 Fe.234) (Al1.612 Cr.388) O4
compound: Middle Atlas Neogene-Quaternary Volcanic Field of Morocco
formula_title: <missing>
a: 8.1499
b: 8.1499
c: 8.1499
alpha: 90
beta: 90
gamma: 90
cell_volume: 541.324
crystal_density: 3.911
atoms_sites: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeACAHEAA=
atoms_y: IKEHACChBwCAhB4AgIQeACAHEAA=
atoms_z: IKEHACChBwCAhB4AgIQeACAHEAA=
atoms_occupancy: wMAuAEBIDgDAMTEAQNcLAAAJPQA=
atoms_u_iso: IGcAACBnAABgVAAAYFQAANCEAAA=
atoms_aniso_label: ["MgT", "FeT", "AlM", "CrM", "O"]
atoms_aniso_u11: IGcAACBnAABgVAAAYFQAANCEAAA=
atoms_aniso_u22: IGcAACBnAABgVAAAYFQAANCEAAA=
atoms_aniso_u33: IGcAACBnAABgVAAAYFQAANCEAAA=
atoms_aniso_u12: AAAAAAAAAAAQ+v//EPr//yD5//8=
atoms_aniso_u13: AAAAAAAAAAAQ+v//EPr//yD5//8=
atoms_aniso_u23: AAAAAAAAAAAQ+v//EPr//yD5//8=
pub_title:
 Low intra-crystalline closure temperatures of Cr-bearing spinels from the mantle xenoliths of
 the Middle AtlasNeogene-Quaternary Volcanic Field (Morocco):Mineralogical evidence of a cooler
 mantle beneath the West African Craton.
 Note:Sample MAR-TF28

qdat:
AAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAAAIAAAAACAAAAAAAAIAAAAgAAAAAAgAABAAAAACAAAgAAAAQAAQAAAAgACAAAAQACAAABAAQAAAgAIAABAAgAAEACAABABAAAgAgAAABAABAEAAIAgABAEAAQCAAEAgAAAgA==


formula: Fe2.134 Ti.866 O4
compound: Synthetic
formula_title: <missing>
a: 8.5139
b: 8.5139
c: 8.5139
alpha: 90
beta: 90
gamma: 90
cell_volume: 617.143
crystal_density: 4.835
atoms_sites: ["FeT", "FeM", "TiM", "O"]
atoms_x: IKEHAICEHgCAhB4ACN4PAA==
atoms_y: IKEHAICEHgCAhB4ACN4PAA==
atoms_z: IKEHAICEHgCAhB4ACN4PAA==
atoms_occupancy: AAk9AGCbIgCgbRoAAAk9AA==
atoms_u_iso: iK4AACCAAAAggAAAgOgAAA==
atoms_aniso_label: ["FeT", "FeM", "TiM", "O"]
atoms_aniso_u11: iK4AACCAAAAggAAAgOgAAA==
atoms_aniso_u22: iK4AACCAAAAggAAAgOgAAA==
atoms_aniso_u33: iK4AACCAAAAggAAAgOgAAA==
atoms_aniso_u12: AAAAAAj4//8I+P//oNj//w==
atoms_aniso_u13: AAAAAAj4//8I+P//oNj//w==
atoms_aniso_u23: AAAAAAj4//8I+P//oNj//w==
pub_title:
 Static positional disorder in ulvospinel: A single-crystal neutron diffraction study.
 Note:Crystal 1

qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAQAAACAAAAAAIAABAAAAACAABAAAABAACAAAAQABAAAAgAEAAAIACAAAIAEAAAgAgAAIAIAAEAIAAEAQAAABAABAEAAQBAAEAgACAQACAQAAAgAIBAAAEA==


formula: Fe2.111 Ti.889 O4
compound: Synthetic
formula_title: <missing>
a: 8.5139
b: 8.5139
c: 8.5139
alpha: 90
beta: 90
gamma: 90
cell_volume: 617.143
crystal_density: 4.832
atoms_sites: ["FeT", "FeM", "TiM", "O"]
atoms_x: IKEHAICEHgCAhB4AcN8PAA==
atoms_y: IKEHAICEHgCAhB4AcN8PAA==
atoms_z: IKEHAICEHgCAhB4AcN8PAA==
atoms_occupancy: AAk9ANDqIQAwHhsAAAk9AA==
atoms_u_iso: AK8AAOB5AADgeQAAYOoAAA==
atoms_aniso_label: ["FeT", "FeM", "TiM", "O"]
atoms_aniso_u11: AK8AAOB5AADgeQAAYOoAAA==
atoms_aniso_u22: AK8AAOB5AADgeQAAYOoAAA==
atoms_aniso_u33: AK8AAOB5AADgeQAAYOoAAA==
atoms_aniso_u12: AAAAAPjz///48///INb//w==
atoms_aniso_u13: AAAAAPjz///48///INb//w==
atoms_aniso_u23: AAAAAPjz///48///INb//w==
pub_title:
 Static positional disorder in ulvospinel: A single-crystal neutron diffraction study.
 Note:Crystal 2

qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAQAAACAAAAAAIAABAAAAACAABAAAABAACAAAAQABAAAAgAEAAAIACAAAIAEAAAgAgAAIAIAAEAIAAEAQAAABAABAEAAQBAAEAgACAQACAQAAAgAIBAAAEA==


formula: Fe2.134 Ti.864 O4
compound: Synthetic
formula_title: <missing>
a: 8.5139
b: 8.5139
c: 8.5139
alpha: 90
beta: 90
gamma: 90
cell_volume: 617.143
crystal_density: 4.833
atoms_sites: ["FeT", "FeM", "TiM", "O"]
atoms_x: IKEHAICEHgBA6B0ACN4PAA==
atoms_y: IKEHAICEHgBA6B0ACN4PAA==
atoms_z: IKEHAICEHgBA6B0ACN4PAA==
atoms_occupancy: AAk9AGCbIgAALw0AAAk9AA==
atoms_u_iso: AK8AAPCgAAAQiwAA0OgAAA==
atoms_aniso_label: ["FeT", "FeM", "O"]
atoms_aniso_u11: AK8AAPCgAADQ6AAA
atoms_aniso_u22: AK8AAPCgAADQ6AAA
atoms_aniso_u33: AK8AAPCgAADQ6AAA
atoms_aniso_u12: AAAAAEgXAAB42P//
atoms_aniso_u13: AAAAAEgXAAB42P//
atoms_aniso_u23: AAAAAEgXAAB42P//
pub_title:
 Static positional disorder in ulvospinel: A single-crystal neutron diffraction study.
 Note:Refinement with Ti at .49, .49, .49

qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAQAAACAAAAAAIAABAAAAACAABAAAABAACAAAAQABAAAAgAEAAAIACAAAIAEAAAgAgAAIAIAAEAIAAEAQAAABAABAEAAQBAAEAgACAQACAQAAAgAIBAAAEA==


formula: K (Fe2.79 Al.21) S2 O14 H6
compound: Jaroso Ravine, Sierra Almagrera, Andalusia, Almeria, Spain
pub_title: Looking for jarosite on Mars: The low-temperature crystal structure of jarosite Note: T = 297 K
formula_title: <missing>
a: 7.2913
b: 7.2913
c: 17.1744
alpha: 90
beta: 90
gamma: 120
cell_volume: 790.719
crystal_density: 3.117
atoms_sites: ["K", "Fe", "Al", "S", "O1", "O2", "O3", "H1"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAABYmg0AaMIHAIB5CwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAACoZfL/mD34/4CG9P8=
atoms_z: AAAAAICEHgCAhB4AMNYSAJAEJQDIs/z/qEUIAADWBgA=
atoms_occupancy: AAk9AEDDOADARQQAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: APoAAIBXAACAVwAAoHMAAHDGAAAgsgAAYJ8AAICvAgA=
atoms_aniso_label: ["K", "Fe", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: ECEBAEA4AABAOAAAMFwAAHDfAACwzAAA4GAAAA==
atoms_aniso_u22: ECEBACAcAAAgHAAAMFwAAHDfAACwzAAA4GAAAA==
atoms_aniso_u33: AK8AAMCoAADAqAAAYJ8AAHCUAACgvgAAABMBAA==
atoms_aniso_u12: wI8AAMANAADADQAAaC4AAIBwAAAAlgAAoCgAAA==
atoms_aniso_u13: AAAAAHD+//9w/v//AAAAAAAAAACg9v//0CAAAA==
atoms_aniso_u23: AAAAAOD8///g/P//AAAAAAAAAABgCQAAMN///w==
qdat:
AAAAAAAAAAAAAAAAACIACAAAAAAACEAAACiICAAAAQAAIlEAACQEAkhAAEAgYxgQECCUQICAEsQQoQVEAAIRoIUQ6AQgFSCEQKAEIyQlEYhAAlCEgiBALRCS0AgGCREoASkTBwRAqBIYAJcSLgiFxZNAiXIQJAKlgiAJgU==


formula: K (Fe2.79 Al.21) S2 O14 H6
compound: Jaroso Ravine, Sierra Almagrera, Andalusia, Almeria, Spain
pub_title: Looking for jarosite on Mars: The low-temperature crystal structure of jarosite Note: T = 253 K
formula_title: <missing>
a: 7.2931
b: 7.2931
c: 17.1456
alpha: 90
beta: 90
gamma: 120
cell_volume: 789.783
crystal_density: 3.121
atoms_sites: ["K", "Fe", "Al", "S", "O1", "O2", "O3", "H1"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAAAAmA0AGL0HAEBaCwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAaPL/6EL4/8Cl9P8=
atoms_z: AAAAAICEHgCAhB4AANkSAAgAJQBYtfz/4EQIAKDlBgA=
atoms_occupancy: AAk9AEDDOADARQQAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: ENYAANhFAADYRQAAIGcAAGCfAACgpQAAoIwAAMDUAQA=
atoms_aniso_label: ["K", "Fe", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: 8OsAAKAoAACgKAAAYFQAADCnAACwswAAgFcAAA==
atoms_aniso_u22: 8OsAAFAUAABQFAAAYFQAADCnAACwswAAgFcAAA==
atoms_aniso_u33: wKgAADCOAAAwjgAAMI4AAKCMAABwxgAA0OgAAA==
atoms_aniso_u12: wHYAACgKAAAoCgAAMCoAAGBUAADwhwAA0CAAAA==
atoms_aniso_u13: AAAAAHgAAAB4AAAAAAAAAAAAAAAQ9f//UBQAAA==
atoms_aniso_u23: AAAAABgBAAAYAQAAAAAAAAAAAADwCgAAsOv//w==
qdat:
AAAAAAAAAAAAAAAAACIACAAAAAAACEAAACiICAAAAQAAIVEAACQCAkQgAEAgYpgIECCUQECAEsQQoQVEAAIRoEYQ6AQgFaCEQKAEI1QlEYhAAtCEgiBAbJCS0AgKCREoASoVBwRB6BIoAJcSLgiFRZNAirIQRAKlgiAJgV==


formula: K (Fe2.79 Al.21) S2 O14 H6
compound: Jaroso Ravine, Sierra Almagrera, Andalusia, Almeria, Spain
pub_title: Looking for jarosite on Mars: The low-temperature crystal structure of jarosite Note: T = 213 K
formula_title: <missing>
a: 7.2918
b: 7.2918
c: 17.1235
alpha: 90
beta: 90
gamma: 120
cell_volume: 788.484
crystal_density: 3.126
atoms_sites: ["K", "Fe", "Al", "S", "O1", "O2", "O3", "H1"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAADQlQ0AwL8HAIB5CwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAwavL/QED4/4CG9P8=
atoms_z: AAAAAICEHgCAhB4AkNoSADD7JADYt/z/eEMIAKDlBgA=
atoms_occupancy: AAk9AEDDOADARQQAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0LYAAGA7AABgOwAAEFkAAECcAACAiQAAIIAAAAD0AQA=
atoms_aniso_label: ["K", "Fe", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: cMYAAEAfAABAHwAAwEQAABCkAAAgmQAA0FIAAA==
atoms_aniso_u22: cMYAABAOAAAQDgAAwEQAABCkAAAgmQAA0FIAAA==
atoms_aniso_u33: IJkAAJB+AACQfgAA0IQAAKCMAADQnQAA8NIAAA==
atoms_aniso_u12: cGIAAOAGAADgBgAAOCIAANBSAACAcAAAYCIAAA==
atoms_aniso_u13: AAAAADj///84////AAAAAAAAAACQAQAAMBEAAA==
atoms_aniso_u23: AAAAAHD+//9w/v//AAAAAAAAAABw/v//0O7//w==
qdat:
AAAAAAAAAAAAAAAAACIACAAAAAAACEAAAChICAAAAQAAIVEAACQCAkQgAEAQYpgICCCUQCCAEsQIoIUkAAERoEUI6AQgFbCEIKAEEzIlEYggAlCEQiBAbIiKyAgGCQkoASkTBwJA+BIUAJaSLgSFxZNAiXIIIgKTgiAJgT==


formula: K (Fe2.79 Al.21) S2 O14 H6
compound: Jaroso Ravine, Sierra Almagrera, Andalusia, Almeria, Spain
pub_title: Looking for jarosite on Mars: The low-temperature crystal structure of jarosite Note: T = 173 K
formula_title: <missing>
a: 7.2918
b: 7.2918
c: 17.1026
alpha: 90
beta: 90
gamma: 120
cell_volume: 787.521
crystal_density: 3.130
atoms_sites: ["K", "Fe", "Al", "S", "O1", "O2", "O3", "H1"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAACIlw0AwL8HACCJCwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAB4aPL/QED4/+B29P8=
atoms_z: AAAAAICEHgCAhB4AmNwSAHj0JABoufz/iEIIAKDlBgA=
atoms_occupancy: AAk9AEDDOADARQQAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: kJcAAHAwAABwMAAAQFEAABCLAAAAfQAAEHIAAIAyAgA=
atoms_aniso_label: ["K", "Fe", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: oKUAAOAVAADgFQAAgD4AANCEAACwgQAAEEAAAA==
atoms_aniso_u22: oKUAAEAGAABABgAAgD4AANCEAACwgQAAEEAAAA==
atoms_aniso_u33: cHsAAIBwAACAcAAAwHYAACCZAAAQpAAA0M8AAA==
atoms_aniso_u12: 0FIAAEgDAABIAwAAQB8AADBDAACQZQAAkBoAAA==
atoms_aniso_u13: AAAAANj////Y////AAAAAAAAAADg/P//wBIAAA==
atoms_aniso_u23: AAAAANj////Y////AAAAAAAAAAAgAwAAQO3//w==
qdat:
AAAAAAAAAAAAAAAAACIACAAAAAAACEAAAChIBAAAAQAAIUiAACICAkQQAEAQYpQECBCUQCCAEsQIoIUiAAERoCUI6AIgE7CEIKAEEzIlEYggAlBEQiBAbIiKyAgFBQkoASkSBwJA/BIUAJaSLgSFw5NAiXIIIgKTgiAJgT==


formula: K (Fe2.79 Al.21) S2 O14 H6
compound: Jaroso Ravine, Sierra Almagrera, Andalusia, Almeria, Spain
pub_title: Looking for jarosite on Mars: The low-temperature crystal structure of jarosite Note: T = 133 K
formula_title: <missing>
a: 7.2907
b: 7.2907
c: 17.0900
alpha: 90
beta: 90
gamma: 120
cell_volume: 786.704
crystal_density: 3.133
atoms_sites: ["K", "Fe", "Al", "S", "O1", "O2", "O3", "H1"]
atoms_x: AAAAAICEHgCAhB4AAAAAAAAAAAAIlQ0A6L8HAIB5CwA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAD4avL/GED4/4CG9P8=
atoms_z: AAAAAICEHgCAhB4A8N4SANDxJADAu/z/IEEIAED1BgA=
atoms_occupancy: AAk9AEDDOADARQQAAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: wHYAAGAnAABgJwAA4EcAAOB5AADQawAAAGQAAEAZAQA=
atoms_aniso_label: ["K", "Fe", "Al", "S", "O1", "O2", "O3"]
atoms_aniso_u11: AH0AAIAMAACADAAAADIAAGBtAADgYAAAEEAAAA==
atoms_aniso_u22: AH0AAAAAAAAAAAAAADIAAGBtAADgYAAAEEAAAA==
atoms_aniso_u33: IGcAAJBlAACQZQAAMHUAAFCRAAAgmQAAsLMAAA==
atoms_aniso_u12: gD4AACgAAAAoAAAAsBgAALA2AAAQQAAAgCUAAA==
atoms_aniso_u13: AAAAABD///8Q////AAAAAAAAAAAAAAAAwBIAAA==
atoms_aniso_u23: AAAAAEj+//9I/v//AAAAAAAAAAAAAAAAQO3//w==
qdat:
AAAAAAAAAAAAAAAAACIACAAAAAAACCAAACRIBAAAAQAAIUiAABIBAkQQAEAQYpQECBCUQCCAEsIIoIUiAAERkCUI6AIQE7BEIKAEEzIVEYQgAnBEQhBAKoiKyAgFBQkkASUTB4JA/BEUAJaKLgSFo0tAiVEIIgKTQyAJgS==


formula: Si2 Al2 Ca.946 O9 H2
compound: Rio Pian del Foco, Genova province, Italy
formula_title: <missing>
a: 9.434
b: 9.0440
c: 9.6950
alpha: 90
beta: 89.040
gamma: 90
cell_volume: 827.072
crystal_density: 2.362
atoms_sites: ["Si", "Al", "Ca1", "Ca2", "O1", "O2", "O3", "O4", "Wat1"]
atoms_x: IGQDAKgOCAA4FPX/AOgDALBu+v9ADQMAsNMDAOBfCwBAQg8A
atoms_y: AJITAJDeBAAwlgwAQPQCAHDmFwDAsxMAGDkJAPCHGQBA5fj/
atoms_z: kI8XAAAOCwCAZQsAAKsiADAHFAA4tSEACGEUAPD2EwCAhB4A
atoms_occupancy: AAk9AAAJPQAgvhcAgCAFAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: YBcBAIAVAQBwVgIA4PABAGCAAQCgAwIAENABADBQAgCAkQcA
atoms_aniso_label: ["Si", "Al"]
atoms_aniso_u11: MCQBAMAlAQA=
atoms_aniso_u22: wAwBALD+AAA=
atoms_aniso_u33: sBcBAGAcAQA=
atoms_aniso_u12: wBwAALD1//8=
atoms_aniso_u13: wMf//xjU//8=
atoms_aniso_u23: cO///4Du//8=
pub_title:
 Topotactic transformation and dehydration of the zeolite gismondine
 to a novel Ca feldspar structure
 Note: T = 225 C, Path 2

qdat:
AAAAAAAAAAAAAAAAgAAQACQQAEBAAACCgCAImAkBAgIQIIoESwQ4MEIMeGBxMEGI5mTUTGuUj+4AiylTZbVrM+Ym70WtfSjxXP+4fx3SV7Q23vf+L/0/s//faXTc7tnzu/+8uD//+cOnT4Nbfr4r0TpRKvgpI2MaaCwKkC==


formula: (Ca.5 U.5) O2
compound: Jabel Harmun, Palestinian Autonomy, Israel
pub_title: Vorlanite, (CaU6+)O4, from Jabel Harmun, Palestinian Autonomy, Israel
formula_title: <missing>
a: 5.3647
b: 5.3647
c: 5.3647
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.396
crystal_density: 7.359
atoms_sites: ["Ca", "U", "O"]
atoms_x: AAAAAAAAAABAQg8A
atoms_y: gIQeAICEHgBAQg8A
atoms_z: AAAAAAAAAABAQg8A
atoms_occupancy: gIQeAICEHgAACT0A
atoms_u_iso: wCABAMAgAQBgvwMA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAgAAAAAAAAAAAAAAAQAAAAAAAACAACAAAAAAAAAAgAAAAAAQAIAAAAAAACAAAAAEAAAAAAAAIAAAAEAQAAAAAEAAAAgEAAAAAIAAAEBAAAAAQAAAgAAAAAQAABAgAAAC==


formula: Na Fe3 S2 O14 H6
compound: Londonderry Li deposit, Nepean, Western Australia, Australia
formula_title: <missing>
a: 7.3170
b: 7.3170
c: 16.5955
alpha: 90
beta: 90
gamma: 120
cell_volume: 769.462
crystal_density: 3.138
atoms_sites: ["Na", "Fe", "S", "O1", "O2", "O-H3"]
atoms_x: AAAAAMjcMgCrsCgAq7AoABBrLwBAvQcA
atoms_y: AAAAADgsCgBVWBQAVVgUAPCdDQCAeg8A
atoms_z: AAAAADgsCgAARQEAENv7/2AQAwCwHwgA
atoms_occupancy: 0
atoms_u_iso: IDwDAKClAACAuwAAgLsAAEAZAQAA+gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The alunite supergroup under high pressure: the case of natrojarosite,
 NaFe3(SO4)2(OH)6
 Note: P = 0.00010 GPa

qdat:
AAAAAAAAAAAAAAAAACAgBAAAAAAACAQAACIKABAAACAAQGAUAEEAAxAQBIAApAYCCQJMCABQIQQKJAyECABSGBJCsAAoJjCFBIgQCogygoQBERgKFAMBohGNkBAJCIQhAWIVNADJmSEkANI2KAUtiRqECMiIQJQbFCBLCN==


formula: Na Fe3 S2 O20 H6
compound: Londonderry Li deposit, Nepean, Western Australia, Australia
formula_title: <missing>
a: 7.2791
b: 7.2791
c: 16.2837
alpha: 90
beta: 90
gamma: 120
cell_volume: 747.204
crystal_density: 3.872
atoms_sites: ["Na", "Fe", "S", "O1", "O2", "O-H3"]
atoms_x: AAAAAMjcMgCrsCgAq7AoAIBpLwDQvgcA
atoms_y: AAAAADgsCgBVWBQAVVgUAACTDQAQfA8A
atoms_z: AAAAADgsCgBQJwEA8KX7/2D3AgBwGQgA
atoms_occupancy: 0
atoms_u_iso: QJACAMCoAAAgywAAgLsAAAD6AABg6gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The alunite supergroup under high pressure: the case of natrojarosite,
 NaFe3(SO4)2(OH)6
 Note: P = 1.738 GPa

qdat:
AAAAAAAAAAAAAAAAABAIAgAAAAAABACAABCCQAEAAAgAEBQAwBBAAEkAgFAAKYAgCQKCgIAQKFAgZBEwICAIgIIhVgACGKEChDBCAVBDIlhAAyCBCKAQGhBhmEEAiIFQhBIRJuAIiIYGIAkRp0ATYlJSQGMhIgGgcqBCjC==


formula: Na Fe3 S2 O14 H6
compound: Londonderry Li deposit, Nepean, Western Australia, Australia
formula_title: <missing>
a: 7.2473
b: 7.2473
c: 16.0061
alpha: 90
beta: 90
gamma: 120
cell_volume: 728.062
crystal_density: 3.316
atoms_sites: ["Na", "Fe", "S", "O1", "O2", "O-H3"]
atoms_x: AAAAAMjcMgCrsCgAq7AoAFBxLwDgzAcA
atoms_y: AAAAADgsCgBVWBQAVVgUALCXDQAwmA8A
atoms_z: AAAAADgsCgAwCwEAoHj7/2DeAgDwDAgA
atoms_occupancy: 0
atoms_u_iso: IL8CAACWAACAuwAAoIwAAGDqAABg6gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The alunite supergroup under high pressure: the case of natrojarosite,
 NaFe3(SO4)2(OH)6
 Note: P = 3.368 GPa

qdat:
AAAAAAAAAAAAAAAAAAgCAQAAAAAABAAgAAghCAAIAAIACAiACAgIABAgCBBAEkgCACAkkBACAlICEIBBAgECFAiEFMAAgVQQEBEEQCqERAiEADQIECQCQsCCFogQCEgEiBEwkjYAi4QgEQCYklQBHSSFFAUQhJAWAoUBFC==


formula: Na Fe3 S2 O14 H6
compound: Londonderry Li deposit, Nepean, Western Australia, Australia
formula_title: <missing>
a: 7.2205
b: 7.2205
c: 15.9139
alpha: 90
beta: 90
gamma: 120
cell_volume: 718.525
crystal_density: 3.360
atoms_sites: ["Na", "Fe", "S", "O1", "O2", "O-H3"]
atoms_x: AAAAAMjcMgCrsCgAq7AoAEB8LwBwtQcA
atoms_y: AAAAADgsCgBVWBQAVVgUAMCMDQBwbA8A
atoms_z: AAAAADgsCgDg9gAA0Ff7/5C9AgAQEAgA
atoms_occupancy: 0
atoms_u_iso: IEICAADhAAAA+gAAgLsAAKAJAQBg6gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The alunite supergroup under high pressure: the case of natrojarosite,
 NaFe3(SO4)2(OH)6
 Note: P = 4.729 GPa

qdat:
AAAAAAAAAAAAAAAAAAgCAIAAAAAAAgAQAAQQhAAEAACABAQgAgQEAAgQAggQCJIBABgJLAQAgJSAhCAYgIBAhQIhBMgAEFUEBgJBEAqgkYEwgAqBAgSAiKggQvCEAQkAkQImEkbACVCEAiASikbAI2JQkUCRCEkBYFhQEU==


formula: Na Fe3 S2 O14 H6
compound: Londonderry Li deposit, Nepean, Western Australia, Australia
formula_title: <missing>
a: 7.2049
b: 7.2049
c: 15.8254
alpha: 90
beta: 90
gamma: 120
cell_volume: 711.445
crystal_density: 3.394
atoms_sites: ["Na", "Fe", "S", "O1", "O2", "O-H3"]
atoms_x: AAAAAMjcMgCrsCgAq7AoAGB/LwBwtQcA
atoms_y: AAAAADgsCgBVWBQAVVgUAKCJDQDgag8A
atoms_z: AAAAADgsCgDw6wAAAFD7/2DFAgCQAwgA
atoms_occupancy: 0
atoms_u_iso: APQBAACWAADA2gAAYG0AAAD6AADA2gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The alunite supergroup under high pressure: the case of natrojarosite,
 NaFe3(SO4)2(OH)6
 Note: P = 5.701 GPa

qdat:
AAAAAAAAAAAAAAAAAAgBAIAAAAAAAgAIAAQQgQACAACABAIQAYICAAQMAQQEBEiAQAoEMgIAQEZARBgGIEAQQkGQgnYACCJBAYCQSAKoJGDMIATAQQFgIiwIESxBAEKAJECRRSLQBFohgIgEopnYCKikPFAiQgpAOBY0Ap==


formula: Na Fe3 S2 O14 H6
compound: Londonderry Li deposit, Nepean, Western Australia, Australia
formula_title: <missing>
a: 7.1960
b: 7.1960
c: 15.7640
alpha: 90
beta: 90
gamma: 120
cell_volume: 706.935
crystal_density: 3.416
atoms_sites: ["Na", "Fe", "S", "O1", "O2", "O-H3"]
atoms_x: AAAAAMjcMgCrsCgAq7AoAJCQLwBAvQcA
atoms_y: AAAAADgsCgBVWBQAVVgUAOB2DQDweA8A
atoms_z: AAAAADgsCgDw6wAAcE77/+C4AgBwAAgA
atoms_occupancy: 0
atoms_u_iso: QBMCAADhAABAGQEAIMsAAMBXAQDAVwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The alunite supergroup under high pressure: the case of natrojarosite,
 NaFe3(SO4)2(OH)6
 Note: P = 6.454 GPa

qdat:
AAAAAAAAAAAAAAAAAAgAgEAAAAAAAQAEAAQIQQABAABAAgIIAMEBAAQGAIQBAkhAIAUEEoEAIEMgIgwEqCAEISDIQVMABBEggMBIJAJkEjBWIAIgYICQIRYCFJYggCFAGRBJIpDoAhYQQEQCUUzYBEpSCygJIIUQJAWKAS==


formula: Na Fe3 S2 O14 H6
compound: Londonderry Li deposit, Nepean, Western Australia, Australia
formula_title: <missing>
a: 7.1594
b: 7.1594
c: 15.6003
alpha: 90
beta: 90
gamma: 120
cell_volume: 692.495
crystal_density: 3.487
atoms_sites: ["Na", "Fe", "S", "O1", "O2", "O-H3"]
atoms_x: AAAAAMjcMgCrsCgAq7AoAGCYLwDAyQcA
atoms_y: AAAAADgsCgBVWBQAVVgUAKBwDQCAkw8A
atoms_z: AAAAADgsCgCA1AAAICH7/0CpAgDA+wcA
atoms_occupancy: 0
atoms_u_iso: IMUBAECcAAAgywAAQJwAAEAZAQBg6gAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The alunite supergroup under high pressure: the case of natrojarosite,
 NaFe3(SO4)2(OH)6
 Note: P = 8.779 GPa

qdat:
AAAAAAAAAAAAAAAAAAQAQEAAAAAAAQACAAEEIEAAIAAQAQCCABiAQAEBIBEAIJIEDAERBVAgCAhUBIJAiwIASEIZCCrQAII0GBQDgoAsIUUJogAjBggFggmgIUnRCAIUAVECSSSNgBIwhQMQIkyr4CJjkLlARIQZATBMkA==


formula: Mg.135 Fe1.929 Ti.94 O4
compound: Synthetic
pub_title: Crystal chemistry of the ulvospinel-qandilite series. Note: sample T1
formula_title: <missing>
a: 8.5271
b: 8.5271
c: 8.5271
alpha: 90
beta: 90
gamma: 90
cell_volume: 620.018
crystal_density: 4.714
atoms_sites: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAICEHgCA6A8A
atoms_y: IKEHACChBwCAhB4AgIQeAICEHgCA6A8A
atoms_z: IKEHACChBwCAhB4AgIQeAICEHgCA6A8A
atoms_occupancy: IEICAODGOgCg/QIA4HodAMCvHAAACT0A
atoms_u_iso: KKoAACiqAACAhAAAgIQAAICEAAAg5AAA
atoms_aniso_label: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_aniso_u11: KKoAACiqAACAhAAAgIQAAICEAAAg5AAA
atoms_aniso_u22: KKoAACiqAACAhAAAgIQAAICEAAAg5AAA
atoms_aniso_u33: KKoAACiqAACAhAAAgIQAAICEAAAg5AAA
atoms_aniso_u12: AAAAAAAAAACg9v//oPb//6D2//+gzv//
atoms_aniso_u13: AAAAAAAAAACg9v//oPb//6D2//+gzv//
atoms_aniso_u23: AAAAAAAAAACg9v//oPb//6D2//+gzv//
qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAACAAAAACAAAAAAAAQAAAEAAAAAAQAABAAAAAEAACAAAACAAEAAAAQACAAAAgAIAAAQAEAAAQAIAABABAAAQAQAAIAQAAIAgAAACAAEAQAAgCAAQBAAIAgAEBAAABAAQEAAAIA==


formula: Mg.531 Fe1.511 Ti.96 O4
compound: Synthetic
pub_title: Crystal chemistry of the ulvospinel-qandilite series. Note: sample T3
formula_title: <missing>
a: 8.5104
b: 8.5104
c: 8.5104
alpha: 90
beta: 90
gamma: 90
cell_volume: 616.382
crystal_density: 4.467
atoms_sites: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAICEHgDw6w8A
atoms_y: IKEHACChBwCAhB4AgIQeAICEHgDw6w8A
atoms_z: IKEHACChBwCAhB4AgIQeAICEHgDw6w8A
atoms_occupancy: YDEKAKDXMgDAGwsA4LAUAABMHQAACT0A
atoms_u_iso: UKoAAFCqAAD4hAAA+IQAAPiEAACY2gAA
atoms_aniso_label: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_aniso_u11: UKoAAFCqAAD4hAAA+IQAAPiEAACY2gAA
atoms_aniso_u22: UKoAAFCqAAD4hAAA+IQAAPiEAACY2gAA
atoms_aniso_u33: UKoAAFCqAAD4hAAA+IQAAPiEAACY2gAA
atoms_aniso_u12: AAAAAAAAAADA9P//wPT//8D0//940///
atoms_aniso_u13: AAAAAAAAAADA9P//wPT//8D0//940///
atoms_aniso_u23: AAAAAAAAAADA9P//wPT//8D0//940///
qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAQAAACAAAAAAIAAAgAAAACAABAAAABAACAAAAQABAAAAgAEAAAEACAAAEAEAAAgAQAAEAIAAEAEAAEAIAAAAgABAEAAQBAAEAgACAQACAIAAAQAEAgAAEA==


formula: Mg.79 Fe1.228 Ti.98 O4
compound: Synthetic
pub_title: Crystal chemistry of the ulvospinel-qandilite series. Note: sample T4
formula_title: <missing>
a: 8.5021
b: 8.5021
c: 8.5021
alpha: 90
beta: 90
gamma: 90
cell_volume: 614.580
crystal_density: 4.295
atoms_sites: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAICEHgCo7Q8A
atoms_y: IKEHACChBwCAhB4AgIQeAICEHgCo7Q8A
atoms_z: IKEHACChBwCAhB4AgIQeAICEHgCo7Q8A
atoms_occupancy: ABcRAADyKwBgkA8AwIAPAEDoHQAACT0A
atoms_u_iso: eKoAAHiqAAB4ggAAeIIAAHiCAACA1AAA
atoms_aniso_label: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_aniso_u11: eKoAAHiqAAB4ggAAeIIAAHiCAACA1AAA
atoms_aniso_u22: eKoAAHiqAAB4ggAAeIIAAHiCAACA1AAA
atoms_aniso_u33: eKoAAHiqAAB4ggAAeIIAAHiCAACA1AAA
atoms_aniso_u12: AAAAAAAAAACo8///qPP//6jz//+g0///
atoms_aniso_u13: AAAAAAAAAACo8///qPP//6jz//+g0///
atoms_aniso_u23: AAAAAAAAAACo8///qPP//6jz//+g0///
qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAIAAACAAAAAAIAAAgAAAACAABAAAAAgABAAAAIAAgAAAQACAAAEABAAAEACAAAQAQAAEAEAACAEAACAIAAAAQABACAAIAgACAQABAIABAIAAAIACAgAABA==


formula: Mg.918 Fe1.106 Ti.98 O4
compound: Synthetic
pub_title: Crystal chemistry of the ulvospinel-qandilite series. Note: sample T5
formula_title: <missing>
a: 8.4946
b: 8.4946
c: 8.4946
alpha: 90
beta: 90
gamma: 90
cell_volume: 612.955
crystal_density: 4.226
atoms_sites: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAICEHgBg7w8A
atoms_y: IKEHACChBwCAhB4AgIQeAICEHgBg7w8A
atoms_z: IKEHACChBwCAhB4AgIQeAICEHgBg7w8A
atoms_occupancy: AHwVAACNJwDgRREAIPoNAEDoHQAACT0A
atoms_u_iso: 6KgAAOioAABIhQAASIUAAEiFAABAzgAA
atoms_aniso_label: ["MgT", "FeT", "MgM", "FeM", "TiM", "O"]
atoms_aniso_u11: 6KgAAOioAABIhQAASIUAAEiFAABAzgAA
atoms_aniso_u22: 6KgAAOioAABIhQAASIUAAEiFAABAzgAA
atoms_aniso_u33: 6KgAAOioAABIhQAASIUAAEiFAABAzgAA
atoms_aniso_u12: AAAAAAAAAACQ8v//kPL//5Dy///41f//
atoms_aniso_u13: AAAAAAAAAACQ8v//kPL//5Dy///41f//
atoms_aniso_u23: AAAAAAAAAACQ8v//kPL//5Dy///41f//
qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAIAAACAAAAAAIAAAgAAAACAABAAAAAgABAAAAIAAgAAAIACAAACABAAACABAAAIAIAACAEAABACAACAEAAAAQAAgCAAEAQACAIABAEAAgEAAAEABAQAAAg==


formula: (Mg.931 Cr.138) Si.931 O3
compound: Synthetic
formula_title: <missing>
a: 4.8213
b: 4.9368
c: 6.9132
alpha: 90
beta: 90
gamma: 90
cell_volume: 164.547
crystal_density: 4.196
atoms_sites: ["Mg", "Cr1", "Cr2", "Si", "O1", "O2"]
atoms_x: 8Es8APBLPAAAAAAAAAAAAJBBBgDQ0ykA
atoms_y: YG4EAGBuBACAhB4AgIQeAOBUGwBAERMA
atoms_z: QEIPAEBCDwAAAAAAAAAAAEBCDwBADQMA
atoms_occupancy: 4NI4ACA2BAAgNgQA4NI4AAAJPQAACT0A
atoms_u_iso: ECEBABAhAQBwQwEAcEMBALB7AQBwjgEA
atoms_aniso_label: ["Mg", "Cr1", "Cr2", "Si", "O1", "O2"]
atoms_aniso_u11: kC0BAJAtAQBQQAEAUEABAGBnAQCghgEA
atoms_aniso_u22: MAsBADALAQAQOgEAEDoBAKBUAQAgkwEA
atoms_aniso_u33: ACwBAAAsAQDwTwEA8E8BAKC4AQAAkAEA
atoms_aniso_u12: AAAAAAAAAABABgAAQAYAAAAZAABw/v//
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAACwBAAA
atoms_aniso_u23: AAAAAAAAAADg/P//4Pz//wAAAABQ+///
pub_title:
 Chromium solubility in perovskite at high pressure: The structure of
 (Mg1-xCrx)(Si1-xCrx)O3 (with x = 0.07) synthesized at 23 GPa and 1600 C

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAkAAAIAAAgAAIAAAAJEAAgAIA6AQgCAEgAAGAFAIFIhAgQBABkhAkXUAQREBBBIRl3EoEIJmhnAqJCgQClS+KIDFxWbdeESEWZec6RMaG9+nBEOBfu3JqkWqpQFQTr3yY78f+ngaT9+s2==


formula: Fe2.42 Ni.52 Cr.03 Al.01 Co.02 O4
compound: Bon Accord, South Africa
formula_title: <missing>
a: 8.3626
b: 8.3626
c: 8.3626
alpha: 90
beta: 90
gamma: 90
cell_volume: 584.822
crystal_density: 5.285
atoms_sites: ["FeT", "NiM", "CrM", "AlM", "CoM", "FeM", "O"]
atoms_x: IKEHAICEHgCAhB4AgIQeAICEHgCAhB4AMJgPAA==
atoms_y: IKEHAICEHgCAhB4AgIQeAICEHgCAhB4AMJgPAA==
atoms_z: IKEHAICEHgCAhB4AgIQeAICEHgCAhB4AMJgPAA==
atoms_occupancy: AAk9AIDeDwBg6gAAIE4AAECcAADAVSsAAAk9AA==
atoms_u_iso: EEAAAGBUAABgVAAAYFQAAGBUAABgVAAAsGgAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Trevorite: Ni-rich spinel formed by metasomatism and desulfurization processes
 at Bon Accord, South Africa?

qdat:
AAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAAAAIAAAAAEAAAAAAAAQAAACAAAAAAIAAAgAAAABAAAQAAAAQAAQAAABAAEAAACAAQAAAQAEAAAQAEAAAgAgAAEAEAACACAACAEAAAAQAAQAgACAIAAQCAAIBAAEBAAABAAIBAA==


formula: (Ba.5 Sr.5) Cu Si4 O10
compound: Synthetic
formula_title: <missing>
a: 7.2958
b: 7.2958
c: 15.396
alpha: 90
beta: 90
gamma: 90
cell_volume: 819.509
crystal_density: 3.634
atoms_sites: ["Ba", "Sr", "Cu", "Si", "O1", "O2", "O3"]
atoms_x: QEIPAEBCDwBAQg8A8K4fAIAZGwAg9SsAYC4XAA==
atoms_y: wMYtAMDGLQBAQg8AgBQ5AAAZAAAQszwAEGwBAA==
atoms_z: AAAAAAAAAABATAUAcCwJAODUDgCg+AcAIBcFAA==
atoms_occupancy: gIQeAICEHgAACT0AAAk9AICEHgAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Equation of state and a high-pressure structural phase transition
 in the gillespite-structured phase Ba0.5Sr0.5CuSi4O10
 Note: P = 4.13 GPa

qdat:
AAAAAAAAAAAAACAAAAAAIAAAEAAQCAABAAgAAAAEDABAANAIBBAAAgEACEggBkIEUDCJgCFgCdIAwAgQiTIDxCQYigJ5A0BMIiAFgHMGIlghAtQYSIlSCgsQQFUXRYEitQ6UJMJAdjJEJgyGaoelFYISwNGQwkLBAGKjyh==


formula: Fe2 C O5 H2
compound: Synthetic
formula_title: <missing>
a: 12.5
b: 9.5
c: 3.2
alpha: 90
beta: 97.6
gamma: 90
cell_volume: 376.662
crystal_density: 3.628
atoms_sites: ["Fe1", "Fe2", "C1", "O1", "O2", "O3", "O-H4", "O-H5"]
atoms_x: UN8MAPBbGABgtAkAYLoIAKCcDgAguQMAwAsWAEAAGgA=
atoms_y: gMH//zDYLgCg+O7/AMz3/zB26//AXuv/IJQ3ALDoJQA=
atoms_z: YM07ACASIwCAAR8AAFgbAGCzHgAg5yUAYN4CAMA/BQA=
atoms_occupancy: 0
atoms_u_iso: gDICAOAiAgAguQMAoAMCACBCAgBAkAIAYGECAECQAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A multi-technique, micrometer- to atomic-scale description of
 a synthetic analogue of chukanovite, Fe2(CO3)(OH)2

qdat:
AAAAAAAAEAAAABAABAAAQAgCAIADAAAAADREBQACMGICRECaQIDVACBdIChQWgEQKpz3MGLQoDLIhjn1DQQq1Tkd6/VS5E+tNZDWrVLod5zbK9c+Rev/0t2w874DV3fOE+KLnvkrTX3+eqKTrsyO6weqmuy6UXtTJ6YMYX==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 23.5 GPa
formula_title: <missing>
a: 5.493
b: 6.520
c: 3.453
alpha: 90
beta: 90
gamma: 90
cell_volume: 123.667
crystal_density: 12.847
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: gN4PACBZEwBgTwUA
atoms_y: gBoGAKD2GABAHhUA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAIAAAQAAIAAAAAACBAIAAAAAgIACEAAIAAAGAACAECAQAkACASCABIAZAQAIAgQYEDCgACjQAACiBCAABJEGCLJgIHgQEURUEEQAIihg5QSAAk4WARyBGIQPJAlIwCXKchOQ0==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 29.0 GPa
formula_title: <missing>
a: 5.464
b: 6.468
c: 3.415
alpha: 90
beta: 90
gamma: 90
cell_volume: 120.690
crystal_density: 13.164
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: wIAPAGByFABgVQQA
atoms_y: gBoGAGBUGQAgRxYA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIACAAAIAACAAAAAAAQQCAAAAAEBAAJAACAAAAoAAIAQICAIQAQEQQACQCUBAAECBAwQGIgAIlgAAFEBEAABiQKBmRQGNhABUMUIIkAUkRIWwSAAJGEgIYgnBCLQgOQlCBtGKLZ==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 39.0 GPa
formula_title: <missing>
a: 5.426
b: 6.389
c: 3.362
alpha: 90
beta: 90
gamma: 90
cell_volume: 116.549
crystal_density: 13.632
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: QL8PAEChFAAguQMA
atoms_y: YEkGAADbGgAA/xQA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAQAACAAAgAAAAAACCAQAAAAAQEAAMAAEAAABIAAIAgQQBAIAQJBAACIEEEAABBCAIQEYIAECoAAAyAEAABJgBAswKAKjAADCZUEgEESBIGZhgAAQrFBCZC9Ak6TFKAMoip2i==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 62.7 GPa
formula_title: <missing>
a: 5.343
b: 6.290
c: 3.295
alpha: 90
beta: 90
gamma: 90
cell_volume: 110.737
crystal_density: 14.348
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: oK8PAAD/FACAOAEA
atoms_y: gJcGAABkGQCglxMA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIABAAAQAAEAAAAAAAEEAQAAAAAQEAAEAACAAAAiAACAEIIAQBAEEQQAARBAggAABIQBhAJgEAQKIAABCAMAAEGABBTkGAMzAABmEyRQARJAUAmEwAAEBIMEKwdiBHhJpCAOEK==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 75.1 GPa
formula_title: <missing>
a: 5.298
b: 6.239
c: 3.269
alpha: 90
beta: 90
gamma: 90
cell_volume: 108.054
crystal_density: 14.704
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: AKAPAKAIFgBgYQIA
atoms_y: IKcGACA1GQBApxMA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAQAAEAAAgAAAAAABBAEAAAAACAgAAgAAQAAACIAAIAQggBAEAQJBAABECBCAAAEQQDBATAIAQUQAABEAMAACLABhSoCAKxAABmCRRIAIkgKATCYAABA2FCFMHRAz4iqQgBh==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 93 GPa
formula_title: <missing>
a: 5.246
b: 6.194
c: 3.228
alpha: 90
beta: 90
gamma: 90
cell_volume: 104.890
crystal_density: 15.147
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: YJAPAIBDFACgdAQA
atoms_y: YMYGAABkGQDgORMA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAACAABAAAIAAAAAAAEIAQAAAAAQEAAFAACAAAAIQAAQAkBACAIAgSBAAEEEGCAAABggFBAKQEAIhEAADCAJAABGgCQVpBgFxoAAQRLRUAApoCAGoaAAAwCoIISRooDOCEpCA==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 105 GPa
formula_title: <missing>
a: 5.215
b: 6.167
c: 3.211
alpha: 90
beta: 90
gamma: 90
cell_volume: 103.269
crystal_density: 15.385
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: 4M4PAAD/FABg0gQA
atoms_y: oOUGAGDXGAAAERIA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgABAAAQAACAAAAAAACCAEAAAAAEBAABQABAAAACEAACAFAIAQBAICQIAAggQwQAAAIEBIEBSAQAkYgAAIIBIAAEqARBWkGAPFgADBDEkoACagGAaRYAADAFJQQxFhQD+EIxE==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 120 GPa
formula_title: <missing>
a: 5.128
b: 6.108
c: 3.183
alpha: 90
beta: 90
gamma: 90
cell_volume: 99.697
crystal_density: 15.936
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: 4FEPAAD5FQBg0gQA
atoms_y: IKcGAIAfGgDgsBQA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAQAABAAAIAAAAAAAEIAQAAAAAgCAADAAEAAAAEQAAEAJACAECAIASCABAgEgEAAAUAhEBATAQAKKQAAEBAEAAAVCIIBwxQCsCAAIhxhgYAhQIYBQNEAAgRQpANSKigQ4IM==


formula: Pb O2
compound: Synthetic
pub_title: Crystal structure and compressibility of lead dioxide up to 140 GPa Note: P = 140 GPa
formula_title: <missing>
a: 5.083
b: 6.046
c: 3.152
alpha: 90
beta: 90
gamma: 90
cell_volume: 96.867
crystal_density: 16.402
atoms_sites: ["Pb", "O1", "O2"]
atoms_x: YJAPAOAtFQDAtgYA
atoms_y: wLYGAADbGgAgWRMA
atoms_z: QEIPAEBCDwDAxi0A
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAEAAAQAACAAAAAAAAhACAAAAACAQAAMAAIAAAAQgAAQAiAEAQEAQBIEABBAJgIAAAUAhEBALAQAJKIAACBAGAAAKRCEA4YkArBQACIcYYKAIMECAMDJAACEGNICZQ0UAnh==


formula: Si O2 He
compound: calculated structure
formula_title: <missing>
a: 8.062
b: 4.797
c: 9.491
alpha: 90
beta: 120.43
gamma: 90
cell_volume: 316.488
crystal_density: 2.690
atoms_sites: ["Si1", "Si2", "O1", "O2", "O3", "O4", "He1", "He2"]
atoms_x: oAwmAGBCNQCQ1TAA4CwqACCTGgDQRgIAgJ8mALBqCAA=
atoms_y: MLMXAHBqBwCQHhAAECcZAICrCwAAbxMAcDkkALA7FAA=
atoms_z: 4CgzAHBzKwAQWTIA0MkBANCiLQCgnSsAgHggAABZHwA=
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structures and stabilities of cristobalite-helium phases at high pressures
 Note: P = 10 GPa

qdat:
AAAAAAAAAAAAAAAgAAAAAAAAAKEAAAQACCACAQAAABACwUQAIAyQEwACIQwAYAREyQicEBIYgBOJlEEFEUASRIUoegKkYsYLDDYPvQqADex7IV+rVWdPtVS5X8fwaudg6dZ929Nd9/d2r+2bd9rbZT+7xsHv5ur+7/3r/2==


formula: Si O2 He
compound: calculated structure
formula_title: <missing>
a: 9.080
b: 9.080
c: 9.080
alpha: 31.809
beta: 31.809
gamma: 31.809
cell_volume: 184.735
crystal_density: 2.304
atoms_sites: ["Si", "O1", "O2", "He"]
atoms_x: YFAiAICEHgAwBTQAoEEyAA==
atoms_y: YFAiAICEHgBQiCcAoEEyAA==
atoms_z: YFAiAICEHgBAQg8AoEEyAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structures and stabilities of cristobalite-helium phases at high pressures
 Note: P = 4 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAACAAAQACAAAAEIAAAAABAAAACABQCAACAAkAACAIIAAAAIQChBiAhAIAAAAAaAACABAqIEQgMQAAIUUFYYhAAGAMgABAjYISwEAEwiFAiEAEAYAAgBIiUYAJgRSBAAABgCECVA4IAECIIE==


formula: Na Mg F3
compound: Synthetic
formula_title: <missing>
a: 5.32517
b: 5.47795
c: 7.62732
alpha: 90
beta: 90
gamma: 90
cell_volume: 222.497
crystal_density: 3.113
atoms_sites: ["Na", "Mg", "F1", "F2"]
atoms_x: MFcFAAAAAACwrgUAwDISAA==
atoms_y: EI0hAAAAAACwMjsAsHUMAA==
atoms_z: QEIPAAAAAABAQg8AGBI6AA==
atoms_occupancy: 0
atoms_u_iso: 0E0AAAgHAAAIIAAAUCgAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 A high-resolution powder neutron diffraction study of
 the crystal structure of neighborite (NaMgF3) between 9 and 440 K
 Note: T = 9 K

qdat:
AAAAAAAAAAAAAAAAAAAAAAAEgAAEAACAABAAAARIACACAbAggEAiAABAEgIkkIQEAgElCGTOgJGEECCRT9ZKCEjVH0VKlIQI2P9ooYoZeq8xIjmbra6GKy3+40jF//d2qm/3QRke13rv+fXXQ13L3vfH8tL9Xe9bt3v3W3==


formula: Na Cr Si2 O6
compound: Synthetic
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 2.1 GPa
formula_title: <missing>
a: 9.524
b: 8.672
c: 5.2411
alpha: 90
beta: 107.36
gamma: 90
cell_volume: 413.156
crystal_density: 3.652
atoms_sites: ["NaM2", "CrM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABQ2hEAEP0GADDxFQCQ5AgA
atoms_y: oGsSABCfBQAQnwUAENcEAEDYDwCg2B0A
atoms_z: QEIPAMDGLQBgSw4A4GIIABC1EgDQiv//
atoms_occupancy: 0
atoms_u_iso: wNoAACBOAABgbQAAAH0AAECcAAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAACAAAAAAgQAAAAIAAgIAACAgAABBAAgQgYAgAiEAAAATggkBAgAiIwSBEkQgq4gAQCWAGIJIUqA5OQQgx+BBIbIosqomngrKHoA8cXPxB1UllYnAruRjA233olKEa6xXTUmWpmTNQ6HODF4VxOqY6up==


formula: Na Cr Si2 O6
compound: Synthetic
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 18.5 GPa
formula_title: <missing>
a: 9.197
b: 8.327
c: 5.0572
alpha: 90
beta: 106.23
gamma: 90
cell_volume: 371.863
crystal_density: 4.057
atoms_sites: ["NaM2", "CrM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAA+BEAoP4GAEDmFQAgaQgA
atoms_y: oOgSAIBrBQAQ0QUAQDMFACBSEAAQ9hwA
atoms_z: QEIPAMDGLQAAdA4A4HsIAMD+EwAwQwAA
atoms_occupancy: 0
atoms_u_iso: oIwAACBOAADAXQAAwF0AAAB9AABgbQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAIAAAAACAQAAAAQAAQEAACAEAAAQQACEQEoBACCCAAABTAiAoAIAEaQQMEIEJAcwAAgngANQRxaQY6JiIBRNyABKWC4spFqzMQGJEPSrO5JVkZVj/GDLOpZQg5Zp+IwAt0r9aqFBWtheOUo6A0Gcxj==


formula: Na Cr Si2 O6
compound: Synthetic
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 31.3 GPa
formula_title: <missing>
a: 9.084
b: 8.077
c: 4.9544
alpha: 90
beta: 105.70
gamma: 90
cell_volume: 349.950
crystal_density: 4.311
atoms_sites: ["NaM2", "CrM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADA8REAANYGAKDWFQCAWQgA
atoms_y: gBcTAMBYBQBQ8AUA8IIFAGCKEABQZhwA
atoms_z: QEIPAMDGLQDAuA4AQGwIABDbFAAQWQAA
atoms_occupancy: 0
atoms_u_iso: 4KsAACBOAADAXQAAoIwAAECcAAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAACAAAAAAgAgAAACAAAgIAAQACAABBAABCAQhAgEIIQAAA4QMAQgAgANVAQSBIDAIxoABbAgBSKAvqRBlAqASkQwiIslUGg1irBuCYMGKkN98Ix5mEb9fCiXKxHcVT9tbAE1iXuZlGjgvjEnZ4wxo8D==


formula: Na Cr Si2 O6
compound: Synthetic
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 35.3 GPa
formula_title: <missing>
a: 9.076
b: 7.971
c: 4.9309
alpha: 90
beta: 105.56
gamma: 90
cell_volume: 343.651
crystal_density: 4.390
atoms_sites: ["NaM2", "CrM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABw9hEAoOUGAEC0FQBAUwgA
atoms_y: 0BITABBUBQAA9QUAUIwFAOCvEACAXhwA
atoms_z: QEIPAMDGLQDQ3w4AUGEIAPAJFQCQTAAA
atoms_occupancy: 0
atoms_u_iso: AH0AAMBdAAAAfQAAwF0AAECcAAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAABAAAAAAgAIAAACAAAIEAAQAAQAAgQABSAEIEICEAiAAAMCEgQBACAIfAIBgEBREGBIANABARgYC+xAZUNBIZIDIikWfCNCph4xnMALBjFTEYMQ7QB9MNypM63eNrue8KgWRAz855L0rto2Z40Dk88==


formula: Na Cr Si2 O6
compound: Synthetic
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 40.2 GPa
formula_title: <missing>
a: 9.011
b: 7.918
c: 4.8955
alpha: 90
beta: 105.10
gamma: 90
cell_volume: 337.229
crystal_density: 4.474
atoms_sites: ["NaM2", "CrM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACg7hEA0N0GAHCTFQAggggA
atoms_y: wE8TADA+BQAg+AUAsK4FAIDYEADwdRwA
atoms_z: QEIPAMDGLQAwAg8AQGwIAMAqFQBAagAA
atoms_occupancy: 0
atoms_u_iso: YG0AAGBtAAAgTgAAwF0AAECcAACgjAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAABAAAAAAgAEAAABAAAEBAAEAAEAAIQAAVACCBCAiAIQAAGAhIIAQAgEHwEAIBAkJBwYgE4AECMFAlcgFKiIJCUAVDDEa0RYY0LGKpgAmbQb4rxFEzAH0Q6YVORuNlW1e6FDYkUHrKTxjYsiVbjQFEy==


formula: Na Al Si2 O6
compound: Clear Creek, San Benito County, California, USA
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 1.9 GPa
formula_title: <missing>
a: 9.368
b: 8.539
c: 5.1975
alpha: 90
beta: 107.44
gamma: 90
cell_volume: 396.653
crystal_density: 3.385
atoms_sites: ["NaM2", "AlM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAwvhEA8K4GAOD1FQBQ3ggA
atoms_y: YGUSABC4BQDgvwUAUKsEAIApEACQ/B0A
atoms_z: QEIPAMDGLQAw7w0AEN4HAIAEEgDArv//
atoms_occupancy: 0
atoms_u_iso: wNoAAGBtAAAAfQAAYG0AAECcAABgbQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAgAAAAAEEAAAACAAIAgAAQCAAAIEACBCDgBABEYAAAApBAkCCAAhhwKBEkEQmZAAQBSgFCC0iXgMLyQEhvQQJHpDUhRJacKigLIDJ4/fiGjNJrbtC21cKArXpt44QNZSc30PMnJt7IuSZAosY9ZPw8==


formula: Na Al Si2 O6
compound: Clear Creek, San Benito County, California, USA
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 5.6 GPa
formula_title: <missing>
a: 9.300
b: 8.447
c: 5.157
alpha: 90
beta: 107.14
gamma: 90
cell_volume: 387.127
crystal_density: 3.468
atoms_sites: ["NaM2", "AlM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABQwREA0KsGABAHFgBwyAgA
atoms_y: kHYSADCiBQAgxgUAcK4EAFBKEABAzx0A
atoms_z: QEIPAMDGLQDA8A0AwOIHAFBwEgDg4///
atoms_occupancy: 0
atoms_u_iso: YOoAAGBtAAAAfQAAwF0AAIC7AACgjAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAQAAAAAEBAAAABAACAQAAEAgAAEBAAgQg0AIAIpAAAAKQIIQgIACEKCIQkIiIKoABAGYAmIEUM0hUTKBCFtUAEuyhkFRCxYkYwtAKtjmtRjBsD21wTDuyOB6P+VNJAHOss3aM4LK2xivl0CT4y85Pg==


formula: Na Al Si2 O6
compound: Clear Creek, San Benito County, California, USA
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 8.2 GPa
formula_title: <missing>
a: 9.243
b: 8.407
c: 5.1220
alpha: 90
beta: 106.85
gamma: 90
cell_volume: 380.922
crystal_density: 3.525
atoms_sites: ["NaM2", "AlM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADAvxEA8K4GALDkFQBwrwgA
atoms_y: wKASABCfBQAQ0QUAQM8EANBWEABQqx0A
atoms_z: QEIPAMDGLQDQ/g0AoPgHAMBuEgCw6///
atoms_occupancy: 0
atoms_u_iso: gLsAAGBtAABgbQAAYG0AAKCMAABgbQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAQAAAAACAgAAAAgABAIAACAQAACAgAIIgVAEAEUQAAACkCEIQCAAiCgiIRCJECsAAQCrAIhBklFIVESgQhXLABJ6kNgsI6bNBGK4AtMVvqK0Mg5WeCKbyJQLx3xV4oAcrTXbJjAtj3Ca2noQtDbUpX==


formula: Na Al Si2 O6
compound: Clear Creek, San Benito County, California, USA
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 12.4 GPa
formula_title: <missing>
a: 9.163
b: 8.340
c: 5.0739
alpha: 90
beta: 106.52
gamma: 90
cell_volume: 371.739
crystal_density: 3.612
atoms_sites: ["NaM2", "AlM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAgyREAIKcGAAD5FQBAnggA
atoms_y: 8LESABCGBQDA1QUAwNsEAGBxEACQfx0A
atoms_z: QEIPAMDGLQDACQ4AMPoHANDHEgDwIwAA
atoms_occupancy: 0
atoms_u_iso: YOoAAECcAABAnAAAAH0AAKCMAAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAIAAAAABAQAAAAQAAgCAABAEAAAgQAECIFQAgBDCAAAApAhBEAQAEIkEJCIJEgNgABATYATIKSUkhYjqCBDesACtlg1BorVasCMRoDmZ7fKKoqi7qcCdrmLIezeiWwwAu2S6qXDA7npBmnpkgvhO2p==


formula: Na Al Si2 O6
compound: Clear Creek, San Benito County, California, USA
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 18.3 GPa
formula_title: <missing>
a: 9.082
b: 8.200
c: 5.020
alpha: 90
beta: 106.12
gamma: 90
cell_volume: 359.152
crystal_density: 3.738
atoms_sites: ["NaM2", "AlM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABAzBEAoJoGAKDvFQBwlggA
atoms_y: EOcSAPCCBQDQ4wUAsOYEADCrEABwSh0A
atoms_z: QEIPAMDGLQBwJw4AYAsIAOA5EwBwYgAA
atoms_occupancy: 0
atoms_u_iso: 4KsAAAB9AACgjAAAAH0AAECcAAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAEAAAAAAgEAAAAIAAEAgAAQAQAAECAAQiBIgEAIUEAAAFMBIBgAgAE0QgYIQGUAaoABCTgBCYQUzINcEoICKjkQCM0hWFhI8LQEFiETw01TQWmCuUPsILBTCNTOl5bsaAg6Xc1Jwshe2RCuZpwMMJW==


formula: Na Al Si2 O6
compound: Clear Creek, San Benito County, California, USA
pub_title: High-pressure single-crystal X-ray diffraction study of jadeite and kosmochlor Note: P = 21.5 GPa
formula_title: <missing>
a: 9.034
b: 8.184
c: 4.9875
alpha: 90
beta: 106.02
gamma: 90
cell_volume: 354.427
crystal_density: 3.788
atoms_sites: ["NaM2", "AlM1", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABAzBEAEJkGAMDyFQBAhQgA
atoms_y: MOoSAGCBBQBg5QUAQAEFAFCVEACADR0A
atoms_z: QEIPAMDGLQDwMw4AIAUIANB2EwCwaAAA
atoms_occupancy: 0
atoms_u_iso: 4KsAAMBdAAAAfQAAwF0AAAB9AABgbQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAEAAAAAAQCAAAAEAACAQAAIAQAACBAAIRASQCACGEAAABjAkAQAIACJkIECEBFAH0AAQSYAJKEOmqCOgvCARVZIATcwLhcZKxbARMREdHmycJ4oYph3iBePULRQWbEtiIBNlK6pHjRF7ocS4qegJwz==


formula: (Ca1.52 Na.48) (Al.5 Fe.3 Mg.2) Si2 O7
compound: Oldoinyo Lengai, northern Tanzania
formula_title: <missing>
a: 7.7661
b: 7.7661
c: 5.0297
alpha: 90.
beta: 90.
gamma: 90.
cell_volume: 303.353
crystal_density: 3.013
atoms_sites: ["Ca1", "Na1", "Al2", "Fe2", "Mg2", "Si", "O1", "O2", "O3"]
atoms_x: MIQoADCEKAAAAAAAAAAAAAAAAAAAdjQAgIQeACBgNABA+zcA
atoms_y: UAkzAFAJMwAAAAAAAAAAAAAAAACAFycAAAAAAGAtJwAo8TEA
atoms_z: 4PwdAOD8HQAAAAAAAAAAAAAAAAB4egMAAEsyALA7LQCgXQwA
atoms_occupancy: AGMuAACmDgCAhB4AgE8SAAA1DAAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: YBwBAGAcAQBQwwAAUMMAAFDDAACotgAAUHIBAGCAAQCQkQEA
atoms_aniso_label: ["Ca1", "Na1", "Al2", "Fe2", "Mg2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: wD4BAMA+AQBwrQAAcK0AAHCtAACgvgAA0MkBAFDWAQBARQIA
atoms_aniso_u22: wD4BAMA+AQBwrQAAcK0AAHCtAACgvgAA0MkBAFDWAQCgIgEA
atoms_aniso_u33: oNcAAKDXAACg8AAAoPAAAKDwAACgpQAAgLsAAIDUAABgTgEA
atoms_aniso_u12: cGIAAHBiAAAAAAAAAAAAAAAAAADgFQAAYPb+/3BiAABgjP//
atoms_aniso_u13: AOf//wDn//8AAAAAAAAAAAAAAAAgAwAAAAAAABAnAADQUgAA
atoms_aniso_u23: AOf//wDn//8AAAAAAAAAAAAAAAAgAwAAAAAAABAnAACwuf//
pub_title:
 Alumoakermanite, (Ca,Na)2(Al,Mg,Fe2+)(Si2O7), a new mineral from the active
 carbonatite-nephelinite-phonolite volcano Oldoinyo Lengai, northern Tanzania

qdat:
AAAAAAAAAAAAAAAAAAAgBAAAAAAgQAQAAAgACAQAACCEABAECCAIBAgCERAKJAEBgIAEyMFBCYAGIACwAokOCIJFFgEihEApEKUaYgTQxLGdqBHQEwtWppjQ6Ccxqoq3niOx1F/du9DxJX9aFzar1XHr6DqZtavYNTbONz==


formula: Zn Se O3
compound: Synthetic
pub_title: The crystal structure of beta-zinc selenite
formula_title: <missing>
a: 7.188
b: 6.225
c: 11.976
alpha: 90
beta: 90
gamma: 90
cell_volume: 535.870
crystal_density: 4.768
atoms_sites: ["Zn", "Se", "O1", "O2", "O3"]
atoms_x: oBIlANA7IQBgyCcAcGogAJBsHAA=
atoms_y: AEQWAKCxFwCg8AAAYL0UAEAwEgA=
atoms_z: 0FskAHBWNADANCQAEIUaAMDMLAA=
atoms_occupancy: 0
atoms_u_iso: QJwAAAB9AACAuwAAwNoAAIC7AAA=
atoms_aniso_label: ["Zn", "Se", "O1", "O2", "O3"]
atoms_aniso_u11: wNoAAECcAACAuwAA4KUBAEAZAQA=
atoms_aniso_u22: oIwAAMBdAADgqwAAwF0AAAB9AAA=
atoms_aniso_u33: AH0AAGBtAAAgywAAoIwAAOCrAAA=
atoms_aniso_u12: QB8AAAAAAACAwf//gMH//wAAAAA=
atoms_aniso_u13: YPD//2Dw///A4P//4C4AAAAAAAA=
atoms_aniso_u23: oA8AAAAAAACgDwAAINH//+AuAAA=
qdat:
AAAAAAAAAAAAAAAAAEAAAABBAAAAIQAAACpgADgACECAEcAjEgiCEKEZihOgjoIRgYgJptouRPSrRzIxbVUgXLTUC9eqdSzfWpdczoq/d6HP9Q+r77a1nl/0yPf21rX557Kfe/ruu5v33v9nv7Tb1vvHq99z7l3TO3XX5X==


formula: Ca2 Si O4
compound: Synthetic
formula_title: <missing>
a: 5.5051
b: 6.7551
c: 9.3108
alpha: 90
beta: 94.513
gamma: 90
cell_volume: 345.172
crystal_density: 3.314
atoms_sites: ["Ca1", "Ca2", "Si", "O1", "O2", "O3", "O4"]
atoms_x: cHgNAJDfDQCANQ4AwEIRAEBLAQCwtB0AEIcJAA==
atoms_y: gNr//yDpFABQKxEAkEEfAJAkDwCwRQoAAHMKAA==
atoms_z: wNgqAHBDGgAA+wQAgKkDAHC2CwDQbQgAMJP7/w==
atoms_occupancy: 0
atoms_u_iso: oIwAAMCoAABgbQAAoKUAACCyAADgqwAAAK8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of larnite beta-Ca2SiO4 and specific features
 of polymorphic transitions in dicalcium orthosilicate

qdat:
AAAAAAAAAAAAAAAAAAAwAAEACAAKAACgAgIAIQcAAQAmARADIQKTCABaAMEYQdh4J4xCOUOCJVUOKxcFPVap9Go8NqxLlrhvKXbiuvb+nLwkLX76Nrn3KlertWrW///6mX/c+Pf9fd8fz9rbe8X/8VVO3e22fn7z7///y3==


formula: Cu1.918 Ag1.468 Fe.022 Te
compound: the Campbell orebody, Bisbee, Arizona, USA
formula_title: <missing>
a: 12.1987
b: 12.1987
c: 12.1987
alpha: 90
beta: 90
gamma: 90
cell_volume: 1815.267
crystal_density: 5.987
atoms_sites: ["CuM1", "AgM1", "CuM2", "AgM2", "FeM2", "Te"]
atoms_x: IKEHACChBwDgZzUA4Gc1AOBnNQAAAAAA
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAAAAAA
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAAAAAA
atoms_occupancy: gIodAMBWFgDg/RwAAHYWAOCrAAAACT0A
atoms_u_iso: YNgDAGDYAwAA6AMAAOgDAADoAwCAJgQA
atoms_aniso_label: ["CuM1", "AgM1", "CuM2", "AgM2", "FeM2", "Te"]
atoms_aniso_u11: YNgDAGDYAwCg9wMAoPcDAKD3AwCAJgQA
atoms_aniso_u22: YNgDAGDYAwBg2AMAYNgDAGDYAwCAJgQA
atoms_aniso_u33: YNgDAGDYAwBg2AMAYNgDAGDYAwCAJgQA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAABg8P//
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAABg8P//
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAABg8P//
pub_title:
 Chemical and structural characterization of henryite, (Cu,Ag)3+xTe2 (x ~ 0.40):
 A new structure type in the (Ag)-Cu-Te system

qdat:
AAAAAAAACAAAQABAAQAQAgAAICAQECAgQAIIEEIIIAghCAQgEIhEQgIiIiQESJEQRIgkCSRJBJJJBKSSElBQUpKEpSgKlQpQoVSoVUoqRRVBA0qJVQVVCIoiFGCQSIUABiQBABIIAAAkAAABAAAACAAAAAAAAAAAAAAAAA==


formula: Si.9 Fe.4 Mg.7 Na.03 Ca.02 Mn.01 O3
compound: Tenham L6 Chondrite;
pub_title: Discovery of bridgmanite, the most abundant mineral in Earth, in a shocked meteorite
formula_title: <missing>
a: 5.05
b: 6.92
c: 4.82
alpha: 90
beta: 90
gamma: 90
cell_volume: 168.440
crystal_density: 4.522
atoms_sites: ["Si", "Fe1", "Mg", "Fe2", "Na", "Ca", "Mn", "O1", "O2"]
atoms_x: AAAAAAAAAAAg/yEAIP8hACD/IQAg/yEAIP8hAODSOAAAvgoA
atoms_y: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBgGCMA
atoms_z: gIQeAICEHgCgTx8AoE8fAKBPHwCgTx8AoE8fACBBFwAAxAkA
atoms_occupancy: gO42AIAaBgCAuSoAgE8SAMDUAQCAOAEAQJwAAAAJPQAACT0A
atoms_u_iso: 6GwAAOhsAAAoVQAAKFUAAChVAAAoVQAAKFUAALh0AAAwTQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAEAAAoAACAAAAAAAECEQABAQQMIAgEBBAAAkEgAARQsEAgAEIFJEICEgKQgIKJgIuTogCNiKkUBbAzAgklw1DSmcKLRYqIUYSlpLa4anBaxvR0crHO00IrS80SOZXXv92vzfOfV1lh451==


formula: Ca Cl2 O4
compound: Synthetic
pub_title: Crystal structure of calcium chloride tetrahydrate
formula_title: <missing>
a: 6.593
b: 6.364
c: 8.557
alpha: 97.77
beta: 93.52
gamma: 110.56
cell_volume: 330.776
crystal_density: 1.757
atoms_sites: ["Ca", "Cl1", "Cl2", "O1", "O2", "O3", "O4"]
atoms_x: QEAHAODCEQCQxfD/kN/0/4AS//9AOR0AUDcPAA==
atoms_y: QCX///AM7//wZPH/kJT0/3CrEQAQtA4AsK/w/w==
atoms_z: 8PUPAIATAwAgNRkAIKYCADCSEADwQBAAoFoZAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: ["Ca", "Cl1", "Cl2", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: +GoBAFC4AQDYdgEAiKMBAHAaAgDA/AEAWCMCAA==
atoms_aniso_u22: 4B4BALBdAQDgWgEA8G0BALBdAQCgwgEAoKQBAA==
atoms_aniso_u33: yNEBAFByAQBQnwEAuGMCAKD+AQBIuwEAiMYBAA==
atoms_aniso_u12: cBwAAAhNAAAw1f//0BYAAIB6AACQu///gKIAAA==
atoms_aniso_u13: aBAAAFBBAACoIAAAyCgAAGjj///IggAAaBAAAA==
atoms_aniso_u23: KMn//zD4///I2P//6Kn//1gbAAAYov//sNz//w==
qdat:
AAAAAAAAAAAAEAAAARAAAAIIBAAABAABAoQCAKACAQBBlABEECAwAFUjBCAEgjyUARLEIAVMLRKMKCFcIOVEkbmhkVCDmeo9OSBGjBVlzolio94dW9N+5xzzf3i/rs8+NvMz96/t3TOs95n68f/712b4r9c/yN2xcsv7v3==


formula: Mn5 P3 O12.1 (Cl.9 H.1)
compound: Synthetic
pub_title: The crystal structure of hydrothermally grown manganese chlorapatite, Mn5(PO4)3Cl0.9(OH)0.1
formula_title: <missing>
a: 9.532
b: 9.532
c: 6.199
alpha: 90
beta: 90
gamma: 120
cell_volume: 487.776
crystal_density: 4.039
atoms_sites: ["Mn1", "Mn2", "P", "O1", "O2", "O3", "Cl", "O-H"]
atoms_x: VVgUAPjxEACg0xgAePkVAMhjJAAY9hQAAAAAAAAAAAA=
atoms_y: q7AoAJgVAgDIPhcA4EsfAPjwGwDoYRAAAAAAAAAAAAA=
atoms_z: AGkAAEBCDwBAQg8AQEIPAEBCDwBAIQMAQEIPAEBCDwA=
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgO42AIAaBgA=
atoms_u_iso: 0
atoms_aniso_label: ["Mn1", "Mn2", "P", "O1", "O2", "O3", "Cl", "O-H"]
atoms_aniso_u11: YLgAAADIAAAwdQAAsMwAAAB9AADw6wAAQLUAAEC1AAA=
atoms_aniso_u22: YLgAAGCfAACAcAAAEKQAAECcAACAogAAQLUAAEC1AAA=
atoms_aniso_u33: wHYAAACWAABwewAAUKoAABDWAAAAlgAAcI4BAHCOAQA=
atoms_aniso_u12: MFwAALBPAACgQQAAQIMAAMBEAADQawAAoFoAAKBaAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAABA1P//AAAAAAAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAACg3f//AAAAAAAAAAA=
qdat:
AAAAAAAAAAAACAAAAAAAAQgAAIACAAEAAFAAQEgAICIAgCAiBADAQEAcDBQAFgAMBCg8qQCjSAQ0QUowC0AYVIRJRVJEKg4xgOEQGt1DWSRxITXbDO5HJWEix/9HUiRKjnUVmnVai9MWLZrm805d2O9Ger77Hl3cI3tZuj==


formula: Fe.49 Ru.34 Os.1 Ir.05
compound: Chirynaisky Massif, Koryak Mts, Far-Eastern Region, Russia
pub_title: Hexaferrum (Fe,Ru),(Fe,Os),(Fe,Ir) - a new mineral Note: sample 48-126
formula_title: <missing>
a: 2.64
b: 2.64
c: 4.20
alpha: 90
beta: 90
gamma: 120
cell_volume: 25.351
crystal_density: 11.838
atoms_sites: ["Fe", "Ru", "Os", "Ir"]
atoms_x: VVgUAFVYFABVWBQAVVgUAA==
atoms_y: q7AoAKuwKACrsCgAq7AoAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAA==
atoms_occupancy: QOgdAIDAFACAGgYAQA0DAA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAABAAQAAAAAAAAAAAAAACAAAAAAAAAAAIAAAAAAACAAACACAgAAACAAAAIAAAABAAAAAAAAIAAQACAAAIAAAgBAAIAIAAAAEAAAQAACAAAACAFACAAAAAAQ==


formula: (Fe.69 Os.18 Ru.06 Ir.05 Ni.02)
compound: Chirynaisky Massif, Koryak Mts, Far-Eastern Region, Russia
pub_title: Hexaferrum (Fe,Ru),(Fe,Os),(Fe,Ir) - a new mineral Note: sample 117-8
formula_title: <missing>
a: 2.591
b: 2.591
c: 4.168
alpha: 90
beta: 90
gamma: 120
cell_volume: 24.232
crystal_density: 12.283
atoms_sites: ["Fe", "Os", "Ru", "Ir", "Ni"]
atoms_x: VVgUAFVYFABVWBQAVVgUAFVYFAA=
atoms_y: q7AoAKuwKACrsCgAq7AoAKuwKAA=
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwA=
atoms_occupancy: QB0qAID8CgCAqQMAQA0DAIA4AQA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAIAAgAAAAAAAAAAAAAAEAAAAAAAAAAABAAAAAAACAAAAIAQCAAAEAAAAAgAAABAAAAAAAAAgAAEAAgAAgAAAIgAAQAAgAAACAAACABAAAAAEBAQACAAAA==


formula: Ru
compound: Synthetic
pub_title: Hexaferrum (Fe,Ru),(Fe,Os),(Fe,Ir) - a new mineral Note: sample 6-0663
formula_title: <missing>
a: 2.7058
b: 2.7058
c: 4.2819
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.149
crystal_density: 12.364
atoms_sites: ["Ru"]
atoms_x: VVgUAA==
atoms_y: q7AoAA==
atoms_z: QEIPAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAgAgAAAAAAAAAAAAAAQAAAAAAAAAAIAAAAAAAAgAAIAECAAAABAAABAAAAAEAAAAAAACAAQABAAACAAAgAQAEAQAAAAQAACAAACAAAAEAMBAAAAAAgIgAB==


formula: Os
compound: Synthetic
pub_title: Hexaferrum (Fe,Ru),(Fe,Os),(Fe,Ir) - a new mineral Note: sample 6-0662
formula_title: <missing>
a: 2.7341
b: 2.7341
c: 4.3197
alpha: 90
beta: 90
gamma: 120
cell_volume: 27.965
crystal_density: 22.588
atoms_sites: ["Os"]
atoms_x: VVgUAA==
atoms_y: q7AoAA==
atoms_z: QEIPAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAEAEAAAAAAAAAAAAAACAAAAAAAAAACAAAAAAAAQAAEACCAAAAAgAABAAAAAEAAAAAAAEAAgAEAAAEAACAAgAQCAAAABAAAIAAAEAAAAgAgIAAAAAECIAAMA==


formula: (Pb.997 Fe.003) Cr O4
compound: Red Lead mine, Dundas, Tasmania, Australia
formula_title: <missing>
a: 7.098
b: 7.410
c: 6.779
alpha: 90
beta: 102.4
gamma: 90
cell_volume: 348.232
crystal_density: 6.156
atoms_sites: ["Pb", "Fe", "Cr", "O1", "O2", "O3", "O4"]
atoms_x: 8LYNAPC2DQAAHAwAkKEPAJBUBwAgrAEAsI0XAA==
atoms_y: MD8JADA/CQAwBwoAcEkAAPDXFADwYwYAgCINAA==
atoms_z: wK4YAMCuGABQ/DUAgHcDAPCm//+g2ykAAAwwAA==
atoms_occupancy: INo8AOAuAAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Effects of high-pressure on the structural, vibrational, and electronic
 properties of monzanite-type PbCrO4

qdat:
AAAAAAAAAAAAAAAQAAAACQAAAAAAoAQCoICAARAEEIIAA4EMREQAhkCRVAOBMEwaRALWwKAEMDqORqQRbCDFhefQ8jnDNyNo8Wc583YV9L3xlO/f339Dvsf35b/1/C3+6W2t/fZ9+792zb/+v7e/ue/3//7Lf9/3P//90d==


formula: Ca (O2 H2)
compound: Synthetic
formula_title: <missing>
a: 5.8882
b: 6.8408
c: 8.9334
alpha: 90
beta: 104.798
gamma: 90
cell_volume: 347.902
crystal_density: 2.829
atoms_sites: ["Ca1", "Ca2", "O-H1", "O-H2", "O-H3", "O-H4"]
atoms_x: ALIMAMBVKwDAzRcAYF8sAAAuIgCASRMA
atoms_y: AAAAAADsLADgSxAA4NMjAAAM/v8AaS0A
atoms_z: wBUMALBFCgCgXAgAYNcYAGBmFgBg0gQA
atoms_occupancy: 0
atoms_u_iso: 4HkAAOB5AABAlgEAQJYBAECWAQBAlgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of the high-pressure phase of calcium hydroxide, portlandite:
 In situ powder and single crystal X-ray diffraction study
 Note: P = 8.9 GPa

qdat:
AAAAAAAAAAAAQAAAAAAAAAAAoAAABACAAgAAJIAgAEAAAAANEkACgAAAAawACYEAQFAFgIAVGEkQAEfCYhAaJASACEwFGQayAhBiBCzpaIyAPRphcsuE6TRW10HpzyTHcPCfAOR9qDppx41SMkddn2uGjVUuXsm5uCKKtS==


formula: Ca3 P2 O8
compound: Synthetic
formula_title: <missing>
a: 5.2522
b: 5.2522
c: 18.690
alpha: 90
beta: 90
gamma: 120
cell_volume: 446.501
crystal_density: 3.461
atoms_sites: ["Ca1", "Ca2", "P", "O1", "O2"]
atoms_x: AAAAAAAAAAAAAAAAAAAAADiaCgA=
atoms_y: AAAAAAAAAAAAAAAAAAAAAHA0FQA=
atoms_z: AAAAABhtDABguRgAIMITALASBgA=
atoms_occupancy: 0
atoms_u_iso: yMgAAGicAAA4XgAA8OsAACCyAAA=
atoms_aniso_label: ["Ca1", "Ca2", "P", "O1", "O2"]
atoms_aniso_u11: QAABAEC1AAAAZAAAkC0BAMDaAAA=
atoms_aniso_u22: QAABAEC1AAAAZAAAkC0BABByAAA=
atoms_aniso_u33: MFwAAEBqAABAUQAAIGcAAKClAAA=
atoms_aniso_u12: 0H8AAKBaAABQMgAAkJcAAEA4AAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAJgDAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAANAHAAA=
pub_title:
 A comparison of the Ca3(PO4)2 and CaSiO3 systems, with a new structure refinement
 of tuite synthesized at 15 GPa and 1300 deg C

qdat:
AAAAAAAAAAAAAAAABAAAAAACACAAAAAAQCAAIAABAAAIAEIIAAMQQBAAAAAAEQgAJAAgAgAQEAACBAABAECRAEkCAAABJAJAIAAA0gJAQEBDABCAAABSAoECBCoFIgAAqBQQAAQBAAQRUBRCBEAiAABkKEAAgEAEIyBkAB==


formula: Pb4.695 Ca.01 P2.913 O12 Cl.956
compound: Daoping mine, Guangxi, China
formula_title: <missing>
a: 9.986
b: 9.986
c: 7.3378
alpha: 90
beta: 90
gamma: 120
cell_volume: 633.694
crystal_density: 6.757
atoms_sites: ["Pb1", "Ca1", "Pb2", "Ca2", "P", "O1", "O2", "O3", "Cl"]
atoms_x: VVgUAFVYFADwjA8A8IwPAEgNGQDQ2RQAWPIjADAKFgAAAAAA
atoms_y: q7AoAKuwKACYXQAAmF0AANAnFwAovx0AsPEcAEi7EAAAAAAA
atoms_z: YEoAAGBKAABAQg8AQEIPAEBCDwBAQg8AQEIPAOjqBAAAAAAA
atoms_occupancy: 4E85AEAfAADgTzkAQB8AAOBDOwAACT0AAAk9AAAJPQCAWToA
atoms_u_iso: YOoAAGDqAAAA+gAAAPoAAAB9AABg6gAAQBkBAGBnAQCgCQEA
atoms_aniso_label: ["Pb1", "Ca1", "Pb2", "Ca2", "P", "O1", "O2", "O3", "Cl"]
atoms_aniso_u11: uBQBALgUAQDwpQAA8KUAAPiOAABIdQEAGJcAADD7AQBoBQEA
atoms_aniso_u22: uBQBALgUAQDYzAAA2MwAAFB9AAAg2gAA4JcAABBnAQBoBQEA
atoms_aniso_u33: oJsAAKCbAADwfAEA8HwBAEiAAABY/AAAONUBALAhAQBIDAEA
atoms_aniso_u12: SIoAAEiKAAAoVQAAKFUAAFhIAADw8AAAaCQAAIAGAQCgggAA
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAALhD//8AAAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEBh//8AAAAA
pub_title:
 Relationships among channel typology and atomic displacements in the structures
 of Pb5(BO4)3Cl with B = P (pyromorphite), V (vanadinite), and As (mimetite)

qdat:
AAAAAAAAAAAAQAAAAACAAgAAQIAAUAAggAAoIEAgAAhCMAwCEQGARECEQYIAlQ4gmGAmggRBKS5qQiwnjACSpztIekYJM0S7RZZQal1VtV9qqpVpvo9Fri2r8T725LX6f6+p6lVfl1f29G33r8XNr+j8zbxut3o//m9bi1==


formula: Pb4.695 Ca.01 P2.913 O12 Cl.956
compound: Daoping mine, Guangxi, China
formula_title: <missing>
a: 9.9791
b: 9.9791
c: 7.3439
alpha: 90
beta: 90
gamma: 120
cell_volume: 633.345
crystal_density: 6.761
atoms_sites: ["Pb1", "Ca1", "Pb2", "Ca2", "P", "O1", "O2", "O3", "Cl"]
atoms_x: VVgUAFVYFABAiA8AQIgPAJAGGQAA/xQAYPQjAJgQFgAAAAAA
atoms_y: q7AoAKuwKACgWgAAoFoAADgpFwAY1B0A8PIcAKimEAAAAAAA
atoms_z: cEkAAHBJAABAQg8AQEIPAEBCDwBAQg8AQEIPAND4BAAAAAAA
atoms_occupancy: 4E85AEAfAADgTzkAQB8AAOBDOwAACT0AAAk9AAAJPQCAWToA
atoms_u_iso: YOoAAGDqAAAA+gAAAPoAAAB9AADgKAEAgDgBAIA4AQCgCQEA
atoms_aniso_label: ["Pb1", "Ca1", "Pb2", "Ca2", "P", "O1", "O2", "O3", "Cl"]
atoms_aniso_u11: yA4BAMgOAQD4ogAA+KIAAMCAAADopwEAEK4AAMA5AQDoAgEA
atoms_aniso_u22: yA4BAMgOAQAwzwAAMM8AAEhnAACgRQEAqMoAAMA+AQDoAgEA
atoms_aniso_u33: CI4AAAiOAACgcgEAoHIBAMCZAACIMAEAIBACAGgtAQDIDgEA
atoms_aniso_u12: UIcAAFCHAADwVQAA8FUAAHA6AADAKgEAGD0AAOCNAABggQAA
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAGhm//8AAAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIBO//8AAAAA
pub_title:
 Relationships among channel typology and atomic displacements in the structures
 of Pb5(BO4)3Cl with B = P (pyromorphite), V (vanadinite), and As (mimetite)

qdat:
AAAAAAAAAAAAQAAAAACAAgAAQIAAUAAggAAYIEAgAAhCMAwCEQGARECEQoIAlQ0gWGAmgwRBKSZqQiQnjACSt15IekYMs0T7Q55Qcl2Vtq1Lqk1pvo6FnS2v8V619LVOP67puqz/jXL3fG12T6Xf67Tcyvw3Nt8Xv2dJjV==


formula: Pb4.51 V2.976 P.012 O12 Cl.915
compound: Mibladen, Morocco
formula_title: <missing>
a: 10.3231
b: 10.3231
c: 7.3399
alpha: 90
beta: 90
gamma: 120
cell_volume: 677.394
crystal_density: 6.427
atoms_sites: ["Pb1", "Pb2", "V", "P", "O1", "O2", "O3", "Cl"]
atoms_x: VVgUAMCPDwCQ/BgAkPwYAJBqFABQsyQAAPkVAAAAAAA=
atoms_y: q7AoAOC/AABQaxcAUGsXAHB2HgDgrB0AoHcQAAAAAAA=
atoms_z: UHgAAEBCDwBAQg8AQEIPAEBCDwBAQg8AIOsDAAAAAAA=
atoms_occupancy: wA03AMANNwAAjDwAgD4AAAAJPQAACT0AAAk9AODYNwA=
atoms_u_iso: YOoAAKAJAQAAfQAAAH0AAOAoAQAAdwEA4KUBAEAZAQA=
atoms_aniso_label: ["Pb1", "Pb2", "V", "P", "O1", "O2", "O3", "Cl"]
atoms_aniso_u11: uB4BAMi5AABAoQAAQKEAAFADAgBwjwAAcEICACAqAQA=
atoms_aniso_u22: uB4BAIj+AABwewAAcHsAAMB1AQDQHwEAECoCACAqAQA=
atoms_aniso_u33: CIkAACBXAQAIcAAACHAAANCdAABICwIAWEcBAJgCAQA=
atoms_aniso_u12: cI8AAEhsAABQUAAAUFAAAIBRAQA49f//WKEBABCVAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA4On+/wAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACn//wAAAAA=
pub_title:
 Relationships among channel typology and atomic displacements in the structures
 of Pb5(BO4)3Cl with B = P (pyromorphite), V (vanadinite), and As (mimetite)

qdat:
AAAAAAAAAAACAAAAAAEAIAAEBAAEEABgAAQwBAgACAQgMIBIBiAgBiBMAgMgdCkGAwCoSAoyORcpFB8EAR9UVKrCqcEuNinHCqwTz16y1roLvSeqWrS9s1vPVSb93u+8P9vX2/n/m67yV/vz/8/rLXzF/3V/juy9PI/O9d==


formula: Pb4.51 V2.976 P.012 O12 Cl.915
compound: Mibladen, Morocco
formula_title: <missing>
a: 10.3217
b: 10.3217
c: 7.3407
alpha: 90
beta: 90
gamma: 120
cell_volume: 677.284
crystal_density: 6.428
atoms_sites: ["Pb1", "Pb2", "V", "P", "O1", "O2", "O3", "Cl"]
atoms_x: VVgUALCQDwCA/RgAgP0YAFAyFABAviQAYOkVAAAAAAA=
atoms_y: q7AoAKjAAACobRcAqG0XAKBVHgAwqB0AwHoQAAAAAAA=
atoms_z: gHoAAEBCDwBAQg8AQEIPAEBCDwBAQg8A8AsEAAAAAAA=
atoms_occupancy: wA03AMANNwAAjDwAgD4AAAAJPQAACT0AAAk9AODYNwA=
atoms_u_iso: oAkBAOAoAQBAnAAAQJwAAKAJAQCghgEAIMUBAIA4AQA=
atoms_aniso_label: ["Pb1", "Pb2", "V", "P", "O1", "O2", "O3", "Cl"]
atoms_aniso_u11: iDABAKDIAAA4pAAAOKQAANAzAQDAewAAuHICANhJAQA=
atoms_aniso_u22: iDABABgZAQA4nwAAOJ8AAID8AADoBwEAuDECANhJAQA=
atoms_aniso_u33: aL8AAEiYAQDgnAAA4JwAACBcAQD4wwIAWGUBAFAnAQA=
atoms_aniso_u12: MJgAAJh2AAAIVwAACFcAAIDtAADoIQAAiLIBANikAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAiKv+/wAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAcPD+/wAAAAA=
qdat:
AAAAAAAAAAACAAAAAAEAIAAEBAAEEABgAAQwBAgACAYgKIBIBiAgBiBMAgMgdCkGAwDoSAo6ORcpFB8EAR9cVKrCmcEuNinHCqwS118yVroLrSerWrS9s13PVSb93u+8P9vX37n/m67yV/vT/8/rLf7Fv/V/ju29PI/O9d==


formula: Pb5 As2.775 P.036 O12 Cl
compound: Pingtouling mine, Guangdong, China
formula_title: <missing>
a: 10.2382
b: 10.2382
c: 7.4502
alpha: 90
beta: 90
gamma: 120
cell_volume: 676.310
crystal_density: 7.231
atoms_sites: ["Pb1", "Pb2", "As", "P", "O1", "O2", "O3", "Cl"]
atoms_x: VVgUANBSDwAAABkAAAAZAKAtFACgfCQAsC8WAAAAAAA=
atoms_y: q7AoAHhBAADoeBcA6HgXABA7HgDAqR0A8L0QAAAAAAA=
atoms_z: 0GsAAEBCDwBAQg8AQEIPAEBCDwBAQg8AAGUEAAAAAAA=
atoms_occupancy: YPk8AGD5PAAgdTgAgLsAAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: APoAAIA4AQCgjAAAoIwAAKAJAQBgYQIAIDwDAMBXAQA=
atoms_aniso_label: ["Pb1", "Pb2", "As", "P", "O1", "O2", "O3", "Cl"]
atoms_aniso_u11: 4DcBALimAABoiAAAaIgAAAgkAQCo9wAAOIcEAChUAQA=
atoms_aniso_u22: 4DcBANjgAAAQcgAAEHIAAFjFAADoLwEACBcEAChUAQA=
atoms_aniso_u33: IIUAALgnAgDgkgAA4JIAAEBaAQDQ6QQA8BYDADhiAQA=
atoms_aniso_u12: 8JsAADBhAAAYPQAAGD0AALCLAAAohwAAWJ8DACiqAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAMN38/wAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAaNL8/wAAAAA=
qdat:
AAAAAAAAAAABAAAAAAIAEAACBAAEQAEQAAJICAQAAgkJBQBQIKAkEIQgwEDhioEooJEMGEFNKVUoRUzAANW5qwNcSTMVpOlmWDHZ3VptNsuxuY7puVNE+dYnaVi+b5eu+xZNNlXm23Q0n6k/t1/NY6f0sdfy1tmV0RD+6d==


formula: Pb5 As2.775 P.036 O12 Cl
compound: Pingtouling mine, Guangdong, China
formula_title: <missing>
a: 10.2396
b: 10.2396
c: 7.4405
alpha: 90
beta: 90
gamma: 120
cell_volume: 675.614
crystal_density: 7.238
atoms_sites: ["Pb1", "Pb2", "As", "P", "O1", "O2", "O3", "Cl"]
atoms_x: VVgUAHBODwBY+BgAWPgYAFAZFAAgiSQAkBMWAAAAAAA=
atoms_y: q7AoANA+AAAgeBcAIHgXAMAmHgAgsx0AkJsQAAAAAAA=
atoms_z: oGkAAEBCDwBAQg8AQEIPAEBCDwBAQg8AoEIEAAAAAAA=
atoms_occupancy: YPk8AGD5PAAgdTgAgLsAAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 4CgBAMBXAQDgqwAA4KsAAIA4AQBAkAIAILkDAAB3AQA=
atoms_aniso_label: ["Pb1", "Pb2", "As", "P", "O1", "O2", "O3", "Cl"]
atoms_aniso_u11: mE0BAMC8AABokgAAaJIAAEisAQA4swAAMGsFAHiLAQA=
atoms_aniso_u22: mE0BADjqAACgggAAoIIAABAXAQCArAAACP0EAHiLAQA=
atoms_aniso_u33: UNcAACB0AgBA4gAAQOIAABCPAQBo7AUAqEoDAJhcAQA=
atoms_aniso_u12: uKYAAOhsAABARwAAQEcAABAwAQBAEAAAkI4EANDFAAA=
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAiJT8/wAAAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACJf8/wAAAAA=
qdat:
AAAAAAAAAAABAAAAAAIAEAACBAAEQAEQAAJIBAQAAgkJBQBQIKAkEIQwoEDhioEooJEMGCFNKdUoY4zAANWpV4PaRS0LpPXlODHZrNptLky42Y3ZWXNk7d0j6Mj9a5e29RdNXzX13Vw2j52381utU3dcmd96zlnc6Jhe+L==


formula: Cu.55 Ga.19 Fe.13 In.08 Zn.08 S
compound: Capillitas mine, Argentina
pub_title: Ishiharaite, (Cu,Ga,Fe,In,Zn)S, a new mineral from the Capillitas mine, Northwestern Argentina
formula_title: <missing>
a: 5.368
b: 5.368
c: 5.368
alpha: 90
beta: 90
gamma: 90
cell_volume: 154.681
crystal_density: 4.377
atoms_sites: ["Cu", "Ga", "Fe", "In", "Zn", "S"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAABAQg8A
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAABAQg8A
atoms_z: AAAAAAAAAAAAAAAAAAAAAAAAAABAQg8A
atoms_occupancy: wJEhAMCYCwBA7wcAAOIEAADiBAAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAgAAAAAAAAAAAAAAAQAAAAAAAACAAEAAAAAAAAAAgAAAAAAgAQAAAAAAAEAAAAAIAAAAAAAAIAAAAEAgAAAAAIAAAAgEAAAAAQAAAICAAAAAgAABAAAAAAQAACBAAAAE==


formula: Ge Fe (O6 H6)
compound: Ongopolo mine, Namibia, Africa
pub_title: Die Kristallstruktur von Stottit: FeGe(OH)6
formula_title: <missing>
a: 7.55
b: 7.55
c: 7.47
alpha: 90
beta: 90
gamma: 90
cell_volume: 425.809
crystal_density: 3.596
atoms_sites: ["Ge", "Fe", "O-H1", "O-H2", "O-H3"]
atoms_x: gIQeAAAAAACA3g8AgPUgAICiGQA=
atoms_y: gIQeAAAAAABAWSAAgN4PAICiGQA=
atoms_z: gIQeAAAAAADgUCQA4FAkAMB6EAA=
atoms_occupancy: 0
atoms_u_iso: KFUAAChVAAAoVQAAKFUAAChVAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAACAAAAAAACgAAAAAwAAAAUAAABIAAAQAAAwAAEQABYAA0AAYAAUAD0AAAAyAFABcAaQGYDEBUARApAEA2QpAqhUDEAAbQgSzOkWDJOUkDIYSC4S0qHrAGqROuSRMpwyFzAtrLRwNoDxhScWzStUL==


formula: N H4 Cu4 S3
compound: Synthetic
pub_title: Ammonothermal crystal growth of sulfide materials
formula_title: NH4Cu4S3
a: 3.9101
b: 3.9101
c: 9.4758
alpha: 90
beta: 90
gamma: 90
cell_volume: 144.874
crystal_density: 4.223
atoms_sites: ["N", "H1", "H2", "Cu", "S1", "S2"]
atoms_x: gHvh//Cj2v8QU+j/AAAAAAAAAACAe+H/
atoms_y: gIQeAPCsFwAQXCUAgHvh/wAAAACAe+H/
atoms_z: AAAAAJBZAgBwpv3/mO4UABDyDACAhB4A
atoms_occupancy: AAk9AEBCDwBAQg8AAAk9AAAJPQAACT0A
atoms_u_iso: 4CgBAOCrAADgqwAAUFkBAMDBAABguAAA
atoms_aniso_label: ["N", "Cu", "S1", "S2"]
atoms_aniso_u11: IEgBADCIAQBAtQAA4MQAAA==
atoms_aniso_u22: IEgBAPDSAABAtQAA4MQAAA==
atoms_aniso_u33: oAkBAGCyAQAw2QAAYJ8AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAA==
qdat:
AAAAAAAAAAAgAAAAAAAAAAQAAABAAgAAAQCAABAEAACBQAAAAAICAECQAAwBBIAhAAIgEEAEAAIBMoBAIVCICYRGIIAiICgEUVAUCQgoQAVWIIMsSiSJpQIlMBlGIioDBAClQBpCDlKwEoEEqgyIlEBlgRGiVDGCKoTqkK==


formula: Ca Cu2 S2
compound: Synthetic
pub_title: Ammonothermal crystal growth of sulfide materials
formula_title: <missing>
a: 3.9400
b: 3.9400
c: 6.523
alpha: 90
beta: 90
gamma: 120
cell_volume: 87.694
crystal_density: 4.380
atoms_sites: ["Ca", "Cu", "S"]
atoms_x: AAAAAFVYFABVWBQA
atoms_y: AAAAAKuwKACrsCgA
atoms_z: AAAAAKj6FgDwjC0A
atoms_occupancy: 0
atoms_u_iso: gKIAANAzAQDAjwAA
atoms_aniso_label: ["Ca", "Cu", "S"]
atoms_aniso_u11: YJ8AAMA+AQBQkQAA
atoms_aniso_u22: YJ8AAMA+AQBQkQAA
atoms_aniso_u33: MKcAAIAfAQDAjwAA
atoms_aniso_u12: sE8AAGCfAADgRwAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAA
qdat:
AAAAAAAAAAAAAAAAgAAAAAAAAAAAAACAQACAAAAAAAAAIAAAQAAAAQAEAQAAAIQEQAAAAIASAAAAAAgAIQCIAAgIBAAAgEIAIEAAAwAFAAIEAAihQAQQGAAACARBQAhAkAABgaBACCGgCEYEMACCGAAAgFMAhigENAqYBF==


formula: Li Mn2 O4
compound: Synthetic
pub_title: Bond-length fluctuation in the orthorhombic 3x3x1 superstructure of LiMn2O4 Note: T = 320 K
formula_title: LiMn2O4
a: 8.25130
b: 8.25130
c: 8.25130
alpha: 90
beta: 90
gamma: 90
cell_volume: 561.781
crystal_density: 4.276
atoms_sites: ["Li1", "Mn1", "O1"]
atoms_x: IKEHAICEHgDQahAA
atoms_y: IKEHAICEHgDQahAA
atoms_z: IKEHAICEHgCgSw8A
atoms_occupancy: AAk9AAAJPQBIWBQA
atoms_u_iso: wMEAAGCfAABg0QAA
atoms_aniso_label: ["Li1", "Mn1", "O1"]
atoms_aniso_u11: wMEAAGCfAACwmgAA
atoms_aniso_u22: wMEAAGCfAACwmgAA
atoms_aniso_u33: wMEAAGCfAADAPgEA
atoms_aniso_u12: AAAAAGDr///Q/f//
atoms_aniso_u13: AAAAAGDr///Q7v//
atoms_aniso_u23: AAAAAGDr///Q7v//
qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAABAAAAAAQAAAAAAABAAAAIAAAAAAQAAAgAAAABAAAgAAAAIAAQAAAAgACAAAAgAEAAAEABAAACABAAAEACAAAgAQAAIAIAAEAQAAAAgAAgBAACAIAAgCAAIBAAEAgAAAgAEA==


formula: (Mg.5 Si.5) O2 H
compound: Synthetic
formula_title: <missing>
a: 4.733
b: 4.3250
c: 2.8420
alpha: 90
beta: 90
gamma: 90
cell_volume: 58.176
crystal_density: 3.380
atoms_sites: ["Mg", "Si", "O", "H"]
atoms_x: AAAAAAAAAACQMhUA4P0cAA==
atoms_y: AAAAAAAAAABwDg4AQJACAA==
atoms_z: AAAAAAAAAAAAAAAAAAAAAA==
atoms_occupancy: gIQeAICEHgAACT0AgIQeAA==
atoms_u_iso: cMYAAHDGAAAgFgEAABJ6AA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of dense hydrous magnesium silicates: The structure of phase H,
 MgSiH2O4, synthesized at 45 GPa and 1000 C

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAgwAAAEIEAAIAAAAAAAAEACCAAAACAACAJAAACCEQAIggAUIhCCAAABALIBAgAAhkEAAIAHQEYCKAgRGDiAgUAFkAQKARQYJiFAMBGAIQokCktAFEidAQZA4RKsJ==


formula: Pb5 As3 O9 Cl
compound: Synthetic
pub_title: Crystal chemistry of mimetite, Pb10(AsO4)6Cl1.48O0.26, and finnemanite, Pb10(AsO3)6Cl2
formula_title: <missing>
a: 10.2972
b: 10.2972
c: 7.0690
alpha: 90
beta: 90
gamma: 120
cell_volume: 649.123
crystal_density: 7.368
atoms_sites: ["Pb1", "Pb2", "As1", "O1", "O2", "Cl1"]
atoms_x: VVgUAEAjEABw/hgAwBUlAPCZFgAAAAAA
atoms_y: q7AoAIAyAgAAnBgAUGYcANAFEQAAAAAA
atoms_z: kKY8AEBCDwBAQg8AQEIPAIB3AwAAAAAA
atoms_occupancy: 0
atoms_u_iso: +MUAAPjFAACA7QAA+MUAAPjFAABoUAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAACAAAAAABAIAAEAQABACAhAAIQgBQACAIoBAggBIISAJQFCACQMsTDCJAhBhEFhqBmNqIwoI2MWriKTjgWjU8S6bFQOPdtaKvDOVqql5yXHnM69anHKfZ3h57l451uXbbd6MPy63i52Xr+aP6s7kxp+nz5sb==


formula: Pb5 As3 O12.13 Cl.74
compound: Synthetic
formula_title: <missing>
a: 10.2055
b: 10.2055
c: 7.4483
alpha: 90
beta: 90
gamma: 120
cell_volume: 671.825
crystal_density: 7.321
atoms_sites: ["Pb1", "Pb2", "As1", "O1", "O2", "O3a", "O3b", "O4", "Cl1"]
atoms_x: VVgUADA0DwDAxxgAQPITAFBoJACgLRQA8HoXAAAAAAAAAAAA
atoms_y: q7AoADAqAADgUxcAQBoeALCbHQDA6g4AEAYSAAAAAAAAAAAA
atoms_z: EHIAAEBCDwBAQg8AQEIPAJBiDQDQmAUA0A4DAEBCDwAAAAAA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AICEHgCAhB4AgIQeAEDvBwCAKi0A
atoms_u_iso: MAEBAAgVAQCA7QAAaFABAPB3AQCA7QAAkDwBALDuAQDgKAEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of mimetite, Pb10(AsO4)6Cl1.48O0.26, and finnemanite, Pb10(AsO3)6Cl2
 Note: T = 298 K

qdat:
AAAAAAAAAAABAAAAAAIAEAACBAAEQAEIAAJEBAQAAgSJAoBIIGASEEIQQEBRh0CUICmGCCCamUyKMqZwAKasZYDWJEmMsn1ZGgxU+y6tXqa8q2ayc1Lx2usL+Xo397b6/MaVruT42vUer5+253/xuXTdSPqqbGp9OCZZ3V==


formula: Pb5 As3 O12.13 Cl.74
compound: Synthetic
formula_title: <missing>
a: 10.2224
b: 10.2224
c: 7.4494
alpha: 90
beta: 90
gamma: 120
cell_volume: 674.152
crystal_density: 7.296
atoms_sites: ["Pb1", "Pb2", "As1", "O1", "O2", "O3a", "O3b", "O4", "Cl"]
atoms_x: VVgUAJA9DwAguBgAIAgUAPBeJADgMxQAgGMXAAAAAAAAAAAA
atoms_y: q7AoADBDAACQPxcAYB0eAJB/HQCA/Q4AMNcRAAAAAAAAAAAA
atoms_z: kEwAAEBCDwBAQg8AQEIPAJCUDQCgbgUAAFIDAEBCDwAAAAAA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AICEHgCAhB4AgIQeAEDvBwCAKi0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of mimetite, Pb10(AsO4)6Cl1.48O0.26, and finnemanite, Pb10(AsO3)6Cl2
 Note: T = 373 K

qdat:
AAAAAAAAAAABAAAAAAIAEAACBAAEQAEIAAJEBAQAAgiJAoBIIKAkEEQwwEDRhkCoYFGMCCEqqdUUIsTgAK1Y6YHWKJkNZPWzPBjZv008b2147cVo9atCvNcT9Lx/b632+Y8uX8vz2ao/Tytb2u/lsevcmPnZeVj9cEx6sr==


formula: Pb5 As3 O12.13 Cl.74
compound: Synthetic
formula_title: <missing>
a: 10.2323
b: 10.2323
c: 7.4533
alpha: 90
beta: 90
gamma: 120
cell_volume: 675.812
crystal_density: 7.278
atoms_sites: ["Pb1", "Pb2", "As1", "O1", "O2", "O3a", "O3b", "O4", "Cl1"]
atoms_x: VVgUALBADwAAtRgAsAkUAFBoJAAAaRQAYN0XAAAAAAAAAAAA
atoms_y: q7AoABBAAADgOhcAwA0eABBzHQBAKQ8AML4RAAAAAAAAAAAA
atoms_z: AEsAAEBCDwBAQg8AQEIPAGCDDQCghwUAQD8DAEBCDwAAAAAA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AICEHgCAhB4AgIQeAEDvBwCAKi0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of mimetite, Pb10(AsO4)6Cl1.48O0.26, and finnemanite, Pb10(AsO3)6Cl2
 Note: T = 423 K

qdat:
AAAAAAAAAAABAAAAAAIAEAACBAAEQAEIAAJECAQAAgiJBQBIIKAkEIQgwEDhioEoYFEMGEFVKVUYZUzgANWoqwOcSTMNpPlmWDDZ21p8vk95uc7pp2vE+dY35Vj7W9+3+RZMv1Xmu1Q+nl23s1vLY/P0sfPy9tnS4JD9eU==


formula: Pb5 As3 O12.13 Cl.74
compound: Synthetic
formula_title: <missing>
a: 10.2415
b: 10.2415
c: 7.4594
alpha: 90
beta: 90
gamma: 120
cell_volume: 677.582
crystal_density: 7.259
atoms_sites: ["Pb1", "Pb2", "As1", "O1", "O2", "O3a", "O3b", "O4", "Cl1"]
atoms_x: VVgUAKBLDwAQwxgAAAUUAOBpJADQPhQAUFIXAAAAAAAAAAAA
atoms_y: q7AoAFBGAABwPBcAEAkeAKB0HQBQHg8AcKsRAAAAAAAAAAAA
atoms_z: 4EcAAEBCDwBAQg8AQEIPALCXDQDwggUAMEoDAEBCDwAAAAAA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AICEHgCAhB4AgIQeAEDvBwCAKi0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of mimetite, Pb10(AsO4)6Cl1.48O0.26, and finnemanite, Pb10(AsO3)6Cl2
 Note: T = 473 K

qdat:
AAAAAAAAAAABAAAAAAIAEAACBAAEgAEQAASICAQABAkSBQBQIKAkEIQhQIChDoEooKMMEEFVUZYoRojAAVe51wOsSTUazetmWDGy/pr1Xp3R25axa1bF+7xnSfj2771v8x6dfrdN99g1PLt7JveNRefpYvWj5fO54SFs8Z==


formula: Mg2 Si O4
compound: Synthetic
formula_title: <missing>
a: 4.5232
b: 9.274
c: 5.5467
alpha: 90
beta: 90
gamma: 90
cell_volume: 232.674
crystal_density: 4.016
atoms_sites: ["Mg1", "Mg2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAANAWPACg8BkAMNguAHDcDQDgGRAA
atoms_y: AAAAAGC8EABA4gUAsHwFAPDlGgDAUwoA
atoms_z: AAAAAEBCDwBAQg8AQEIPAEBCDwAQbAEA
atoms_occupancy: 0
atoms_u_iso: YG0AADB1AABgbQAAMHUAAFBfAACQfgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Phase transitions and equation of state of forsterite to 90 GPa from single-crystal
 X-ray diffraction and molecular modeling
 Note: P = 45.3 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAiAAAAAABAAgAAAAFBAAAAAoSICACgMAARAAKBGJQQRCQgJCAgChwhMkEBliwwIUggAiKKuMMF5A5DbqEG4xyhWsR1HdKHGZfGslKp1c6MunN3EzJ3Nmdbr/Ns242aZm652jZuynGubb6pU/V==


formula: Mg2 Si O4
compound: Synthetic
formula_title: Mg2SiO4
a: 2.640
b: 8.596
c: 9.04
alpha: 90
beta: 90
gamma: 90
cell_volume: 205.149
crystal_density: 4.555
atoms_sites: ["Mg1", "Mg2", "Si1", "O1", "O2", "O3", "O4"]
atoms_x: gIQeAICEHgAAAAAAgIQeAICEHgCAhB4AgIQeAA==
atoms_y: IMQWAKBCNgCgTjQAYP87AGAZDgBAFysAQHEcAA==
atoms_z: wFwVAMD2JQAAAAAAgBMcAIDpIgBgihAAIAwLAA==
atoms_occupancy: 0
atoms_u_iso: oIwAAIC7AABAGQEAwFcBAIA+AABgZwEA4KsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Phase transitions and equation of state of forsterite to 90 GPa from single-crystal
 X-ray diffraction and molecular modeling
 Note: P = 58.2 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAAQIAAgAAAAACAAAAAAAEEgAAIECAQAIAwQAACBAARAQAAIAEAQCSgCKAAYCgChDAUAgAghCxjhhMQIbUAEjEARsyMAQIARy5pCQDsk8mTpIQYIhK1CCwYCYE2CEHJIU2mMCUAQcEKAMxaIYU==


formula: Mg2 Si O4
compound: Synthetic
formula_title: Mg2SiO4
a: 2.5910
b: 8.7260
c: 8.7940
alpha: 90
beta: 90
gamma: 90
cell_volume: 198.824
crystal_density: 4.700
atoms_sites: ["Mg1", "Mg2", "Si", "O1", "O2", "O3", "O4"]
atoms_x: gIQeAICEHgAAAAAAgIQeAICEHgCAhB4AgIQeAA==
atoms_y: QDEWAFAVNgAAOTUA0EgAABB8DwCABCsA4J8bAA==
atoms_z: 0JwVABBdKQAAAAAAYOQaACCCIQBw0RMAcA0KAA==
atoms_occupancy: 0
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Phase transitions and equation of state of forsterite to 90 GPa from single-crystal
 X-ray diffraction and molecular modeling
 Note: DFT Optimized
 Note: P = 58.2 GPa

qdat:
AAAAAAAAAAAAAAAAAAAAAAABgABAAAAAABAAAAAAAAQhAAACkEAAAMQMAAARAAACRAACAAAEooAJUAAAPAAgYQqCACACAXhQzgRJCGIISICRIlfIAggYgFcqkFIES2syKbFEAJwbKIA7gIsFaYyHgWCXIoCgEEJQAqZIg1==


formula: Fe1.946 O3
compound: Synthetic
pub_title: A refined monoclinic structure for a variety of "hydrohematite" Note: T = 38 C
formula_title: <missing>
a: 7.3951
b: 5.0117
c: 5.4417
alpha: 90
beta: 95.666
gamma: 90
cell_volume: 200.695
crystal_density: 5.185
atoms_sites: ["Fe", "O1", "O2"]
atoms_x: 0OcVANAgGQBAQg8A
atoms_y: 0Lz//7BcNABgKwsA
atoms_z: APgRAPCdJgAAAAAA
atoms_occupancy: IGM7AAAJPQAACT0A
atoms_u_iso: gD4AAGBtAABgbQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAIAAEAAACAAAAACAABAAAAgMAAUABAAQAgAAAAABMIAEAACFAASDAIYoAACSApBlIAAgQALgAU6AEbAAguAUBAIOZBBSgKAcTo4JUIVLVRKUAjQkECQxMO8msER4sKC/oAyQJF/QqCmIt5==


formula: (Fe2.017 Mg1.983) O5
compound: Synthetic
pub_title: Complete substitution of Fe2+ by Mg in Fe4O5: The crystal structure of the Mg2Fe2O5 end-member
formula_title: Fe2Mg2O5
a: 2.8889
b: 9.7282
c: 12.5523
alpha: 90
beta: 90
gamma: 90
cell_volume: 352.767
crystal_density: 4.534
atoms_sites: ["Fe1", "Mg1", "Fe2", "Mg2", "Fe3", "Mg3", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_y: AAAAAAAAAAAABBAAAAQQACBDHwAgQx8A0OQJALD9FQDg2AUA
atoms_z: AAAAAAAAAABQ/gYAUP4GAEBCDwBAQg8AQEIPAIBPIQD4TicA
atoms_occupancy: kIUcAHCDIACQ+SoAcA8SALCcCABQbDQAAAk9AAAJPQAACT0A
atoms_u_iso: wHYAAMB2AADgiAAA4IgAAKDwAACg8AAAsLMAABC9AAAgsgAA
atoms_aniso_label: ["Fe1", "Mg1", "Fe2", "Mg2", "Fe3", "Mg3", "O1", "O2", "O3"]
atoms_aniso_u11: 0J0AANCdAADQnQAA0J0AAMCoAADAqAAAMNkAAOCrAADA8wAA
atoms_aniso_u22: UEYAAFBGAAAwXAAAMFwAAJCXAACQlwAAMI4AAJB+AACgcwAA
atoms_aniso_u33: IIAAACCAAADwoAAA8KAAACCTAQAgkwEA0LYAADALAQAgsgAA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u23: oA8AAKAPAAAw/f//MP3//wAAAAAAAAAAAAAAAJAzAACwBAAA
qdat:
AAAAAAAAAAAAAAAACAAAAEAQAAAQAAAAAoAAABCCAIAhAIQgEJkIAAGAIAAggASAlUigAOQAGgIDSUQHACmKqI8qwKiCJVgGEkkyJAmFhGEmi8EEfLLMQpTAxKGRgBDDoBhSfIiI8EGgRIKACjjNTEoM4IogJBCqSgQBCI==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p0 Note: P = .0001 GPa
formula_title: <missing>
a: 4.7903
b: 4.7903
c: 15.72
alpha: 90
beta: 90
gamma: 120
cell_volume: 312.398
crystal_density: 3.647
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAMEcQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: wNoAAMDaAAAAfQAAYOoAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: oKUAAKClAADgqwAA
atoms_aniso_u22: oKUAAKClAADgKAEA
atoms_aniso_u33: cEMBAHBDAQDgKAEA
atoms_aniso_u12: 0FIAANBSAACgjAAA
atoms_aniso_u13: AAAAAAAAAADQ7v//
atoms_aniso_u23: AAAAAAAAAADA4P//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAACAAAgAACAAAAgAAAQAAAAQAwAAAAAAAQQAARAESCAAAAAEACAKAEACAIgAJAQgAAABIAEEgAAARABQQiAIAEAgIAAABACgIQCCQAQyAABUCSIAAAgQIEACQFCSBAIAGAAC==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p1 Note: P = 22.50 GPa
formula_title: <missing>
a: 4.6581
b: 4.6581
c: 14.213
alpha: 90
beta: 90
gamma: 120
cell_volume: 267.075
crystal_density: 4.266
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAkJsQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: IMUBACDFAQCghgEAYOQBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: QH0BAEB9AQBgZwEA
atoms_aniso_u22: QH0BAEB9AQDA1AEA
atoms_aniso_u33: wFECAMBRAgCArwIA
atoms_aniso_u12: oL4AAKC+AABg6gAA
atoms_aniso_u13: AAAAAAAAAADArv//
atoms_aniso_u23: AAAAAAAAAADAY///
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAIAAAAQgAAAAQAAAgAAAACAAAgEAAAAgQAAACAAB0AQAAAABAAAFUAEBCAAAQASAAABABAgACCAIQAAgA4AgAAIABKAACAAgBgSEQAEA0ACICEAUIAAEADQAiACBQCAA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p2 Note: P = 23.65 GPa
formula_title: <missing>
a: 4.6554
b: 4.6554
c: 14.149
alpha: 90
beta: 90
gamma: 120
cell_volume: 265.565
crystal_density: 4.290
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAAJoQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: QAABAEAAAQAgywAA4CgBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: 8OsAAPDrAACAuwAA
atoms_aniso_u22: 8OsAAPDrAAAAdwEA
atoms_aniso_u33: 4CgBAOAoAQCghgEA
atoms_aniso_u12: wHYAAMB2AACAuwAA
atoms_aniso_u13: AAAAAAAAAACA8///
atoms_aniso_u23: AAAAAAAAAADA4P//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAIAAAAIgAAAAQAAAgAAAABAAAQCAAAAQIAAABAAAlAIAAAAAgAACmACAhAAAQAKgAAAgAggABAgEQAAgA6AQAAEAAmAACAAQAoGCIACAqABIBCAWEAACABQASABAUCAA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p3 Note: P = 25.34 GPa
formula_title: <missing>
a: 4.6473
b: 4.6473
c: 14.075
alpha: 90
beta: 90
gamma: 120
cell_volume: 263.257
crystal_density: 4.328
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAEI8QAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: gLUBAIC1AQAgSAEAwNQBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: UHIBAFByAQBAGQEA
atoms_aniso_u22: UHIBAFByAQDgpQEA
atoms_aniso_u33: IEICACBCAgCg/QIA
atoms_aniso_u12: 8LkAAPC5AAAgywAA
atoms_aniso_u13: AAAAAAAAAABA1P//
atoms_aniso_u23: AAAAAAAAAABAov//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAEAAAACgAAAAIAAAQAAAAAgAAEAgAAAIEAAAAgAApgCAAAAAIAABRgBAQgAAEADIAAAQAIIAAQICIAAIAagIAABAAIgAAgAEASChEABAMQAkAJADhAABAAWAEgAgPAgA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p4 Note: P = 27.45 GPa
formula_title: <missing>
a: 4.6416
b: 4.6416
c: 13.967
alpha: 90
beta: 90
gamma: 120
cell_volume: 260.597
crystal_density: 4.372
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAkIIQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: cI4BAHCOAQCAOAEAQJYBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: kF8BAJBfAQCgCQEA
atoms_aniso_u22: kF8BAJBfAQBAlgEA
atoms_aniso_u33: MOwBADDsAQAAcQIA
atoms_aniso_u12: AK8AAACvAAAAyAAA
atoms_aniso_u13: AAAAAAAAAABw5f//
atoms_aniso_u23: AAAAAAAAAAAg0f//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAAAAACAAAAAwAAAAEAAAQAAAAAQAACAIAAAIEAAAAQAAUMAQAAAACAAAQIAgQQAACABRAAAIACEAAECBEAAEAKQEAAAgACMAAQACAIgQiAAgDIARAEQBIIAAIARACQAIDIQA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p5 Note: P = 30.48 GPa
formula_title: <missing>
a: 4.6301
b: 4.6301
c: 13.830
alpha: 90
beta: 90
gamma: 120
cell_volume: 256.764
crystal_density: 4.437
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAAIEQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: cCoBAHAqAQDA2gAAYGcBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: APoAAAD6AABg6gAA
atoms_aniso_u22: APoAAAD6AABAlgEA
atoms_aniso_u33: wIkBAMCJAQBg5AEA
atoms_aniso_u12: AH0AAAB9AAAgywAA
atoms_aniso_u13: AAAAAAAAAADgLgAA
atoms_aniso_u23: AAAAAAAAAADAXQAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAgAAAAUAAAACAAAIAAAAAIAAAQAgAAEBAAAAEAAJAgBAAAAAQAAEBgIEIAABAAUEAAEAAhAAAgIhAABAChBAAACAAggAEAAgCCDIgAEAQgEQAkAJBAABACEAiACAYiA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p6 Note: P = 31.19 GPa
formula_title: <missing>
a: 4.6278
b: 4.6278
c: 13.797
alpha: 90
beta: 90
gamma: 120
cell_volume: 255.897
crystal_density: 4.452
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAMJIQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: cBEBAHARAQBQwwAAgDgBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: UPUAAFD1AAAw2QAA
atoms_aniso_u22: UPUAAFD1AABgZwEA
atoms_aniso_u33: sEkBALBJAQDgpQEA
atoms_aniso_u12: 4HkAAOB5AAAgsgAA
atoms_aniso_u13: AAAAAAAAAACADAAA
atoms_aniso_u23: AAAAAAAAAABAHwAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAgAAAAUAAAACAAAEAAAAAEAAAQAQAAEBAAAAEAAJAYAgAAAAQAAGAwIEEAAAgAMCAACAARAAAQIRAABAChhAAACAAQwAEAAQBBDIgAEAYgCQAUAIggABABCASABAYiA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p7 Note: P = 33.56 GPa
formula_title: <missing>
a: 4.6193
b: 4.6193
c: 13.696
alpha: 90
beta: 90
gamma: 120
cell_volume: 253.091
crystal_density: 4.502
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAgKYQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: 4CgBAOAoAQCAuwAAwFcBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: gB8BAIAfAQCgCQEA
atoms_aniso_u22: gB8BAIAfAQBAGQEA
atoms_aniso_u33: EDoBABA6AQAA9AEA
atoms_aniso_u12: wI8AAMCPAACgjAAA
atoms_aniso_u13: AAAAAAAAAAAg6v//
atoms_aniso_u23: AAAAAAAAAAAg0f//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAIAAAAJAAAABAAAEAAAAACAAAEAEAACBAAAACAAEQFAEAAAAEAACgKECCAAAQADAQABAAEQAAEBIQAAQAoMQAAAgAEGABAAIAgJKIABAGEAkAEgCEEAAQAgwIgAQLEQ==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p8 Note: P = 36.20 GPa
formula_title: <missing>
a: 4.6100
b: 4.6100
c: 13.582
alpha: 90
beta: 90
gamma: 120
cell_volume: 249.975
crystal_density: 4.558
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAMJIQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: YDUBAGA1AQCgCQEAIMUBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: oCIBAKAiAQDgKAEA
atoms_aniso_u22: oCIBAKAiAQDgpQEA
atoms_aniso_u33: 4FoBAOBaAQCArwIA
atoms_aniso_u12: UJEAAFCRAAAgywAA
atoms_aniso_u13: AAAAAAAAAADQ1f//
atoms_aniso_u23: AAAAAAAAAADgsf//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAEAAAAEIAAAAgAACAAAAABAAABAAgABAQAAABAACIAkAgAAABAABIBSBBAAAEAAwCAAgAAoAABAMIAAEASCoAAAEABBQAgABAIBJiAAQBggRAAwAhggACAECBIAEBwU==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p9 Note: P = 37.58 GPa
formula_title: <missing>
a: 4.6024
b: 4.6024
c: 13.517
alpha: 90
beta: 90
gamma: 120
cell_volume: 247.959
crystal_density: 4.595
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAwJMQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: 4CgBAOAoAQBAGQEAgLUBAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: MAsBADALAQBg6gAA
atoms_aniso_u22: MAsBADALAQBg5AEA
atoms_aniso_u33: YGcBAGBnAQDgnwIA
atoms_aniso_u12: 0IQAANCEAABg6gAA
atoms_aniso_u13: AAAAAAAAAAAAzv//
atoms_aniso_u23: AAAAAAAAAABAov//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAACAAAAEEAAAAQAABAAAAAAgAAAgAIAAgQAAAAQABEARAIAAAAQAAkASgggAACAAYAQAQAAUAAAQDEAACAJAqAAACAAgUAIAAgEAMRAAEAIIEQAUAIUIAAgCBQkABAsF==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p10 Note: P = 40.80 GPa
formula_title: <missing>
a: 4.5927
b: 4.5927
c: 13.332
alpha: 90
beta: 90
gamma: 120
cell_volume: 243.535
crystal_density: 4.678
atoms_sites: ["Mn1", "Ca1", "C1", "O"]
atoms_x: AAAAAAAAAAAAAAAAsJ4QAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: EJ4BABCeAQAgSAEAQBMCAA==
atoms_aniso_label: ["Mn1", "Ca1", "O"]
atoms_aniso_u11: MD0BADA9AQAgSAEA
atoms_aniso_u22: MD0BADA9AQDgHAMA
atoms_aniso_u33: YGECAGBhAgAAcQIA
atoms_aniso_u12: 0J0AANCdAABAlgEA
atoms_aniso_u13: AAAAAAAAAACARP//
atoms_aniso_u23: AAAAAAAAAABgef7/
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAAAgAAACAQAAAIAAAgAAAAAIAAACAAQAQEAAAAEAAggAhAQAAACAAQgBSQQAAAgACAAgEAADAAABApAAAgCIDQAAAIAEBIEAAIBABlQABADBCIADABBIgAEAgFIgAQFA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p11 Note: P = 44.46 GPa
formula_title: <missing>
a: 2.936
b: 4.841
c: 5.568
alpha: 100.82
beta: 94.93
gamma: 90.18
cell_volume: 77.429
crystal_density: 4.905
atoms_sites: ["Mn1", "Ca1", "C1", "O1", "O2", "O3"]
atoms_x: IAYMACAGDABgmyIAwMwsAKABLACg/u3/
atoms_y: YMkSAGDJEgAA1DAAAOgDAMB5JQAgcQ8A
atoms_z: kHAsAJBwLABA/y4AoFoyAOBnNQCAohkA
atoms_occupancy: AJg6AABxAgAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: oAkBAKAJAQBgbQAAoIwAAMDaAABg6gAA
atoms_aniso_label: ["Mn1", "Ca1"]
atoms_aniso_u11: IMsAACDLAAA=
atoms_aniso_u22: QBkBAEAZAQA=
atoms_aniso_u33: IEgBACBIAQA=
atoms_aniso_u12: gD4AAIA+AAA=
atoms_aniso_u13: oA8AAKAPAAA=
atoms_aniso_u23: IE4AACBOAAA=
qdat:
AAAAAAAAAAAAAAAAAAAQAAgAAAAAAAABAAABAAEAAAYAgAABAEAIAABAAKAAAAgCgEgAAAECQAAZBIBAIBEBRAACQwQBACgFQAIgAkGBSEAEAEdEQgjIEoEAgtAZBAMYkEkhUCWAgXqgYhpYIqQBFYeEQBVoGBh6WoYzk1==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p11a Note: P = 46.79 GPa
formula_title: <missing>
a: 2.928
b: 4.816
c: 5.545
alpha: 101.71
beta: 94.99
gamma: 89.90
cell_volume: 76.264
crystal_density: 4.980
atoms_sites: ["Mn1", "Ca1", "C1", "O1", "O2", "O3"]
atoms_x: YCUMAGAlDABgGCMAoIoqAICzKwCgjev/
atoms_y: MLgSADC4EgCAGDAAIL8CAOBQJACAZw4A
atoms_z: wDYsAMA2LAAAYy4AoNEzAAC2NQCAnBoA
atoms_occupancy: AJg6AABxAgAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: gLsAAIC7AABAnAAAIEgBAEAfAABg6gAA
atoms_aniso_label: ["Mn1", "Ca1"]
atoms_aniso_u11: 4CgBAOAoAQA=
atoms_aniso_u22: IE4AACBOAAA=
atoms_aniso_u33: APoAAAD6AAA=
atoms_aniso_u12: YPD//2Dw//8=
atoms_aniso_u13: QJwAAECcAAA=
atoms_aniso_u23: 4C4AAOAuAAA=
qdat:
AAAAAAAAAAAAAAAAAAAIAAQAAAAAAAAAIAABAACAAAMAEAAAIBAAgAAgACgAAAEAEAKAAAAhAgAFwEgAiACCFgAARCkABADAJABCACIDEFQCAAY8kQESUaAAhGCgLkBCQwCoEYAOIQXFxBiSwTSJAUJloQgnkBhS12VSIY==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p12 Note: P = 44.01 GPa
formula_title: <missing>
a: 2.934
b: 4.839
c: 5.557
alpha: 101.87
beta: 95.29
gamma: 89.73
cell_volume: 76.872
crystal_density: 4.940
atoms_sites: ["Mn1", "Ca1", "C1", "O1", "O2", "O3"]
atoms_x: oMcLAKDHCwAg8yMAIEwqAGDiKwBAo+r/
atoms_y: YH4SAGB+EgCAEjEAQJACAAAcJQCgOA4A
atoms_z: AFYsAABWLADAwC4AYC80AODqNACAnBoA
atoms_occupancy: AJg6AABxAgAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: QJYBAECWAQAA9AEAwFcBAIA+AAAAdwEA
atoms_aniso_label: ["Mn1", "Ca1"]
atoms_aniso_u11: wNQBAMDUAQA=
atoms_aniso_u22: QJYBAECWAQA=
atoms_aniso_u33: IEgBACBIAQA=
atoms_aniso_u12: 4KsAAOCrAAA=
atoms_aniso_u13: IE4AACBOAAA=
atoms_aniso_u23: 4C4AAOAuAAA=
qdat:
AAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAQAABAACAAAIAQAAAIBABAAAQAIgAAAEAMAYAAAAiBAAJgIgBEAEIHAAAUCkAEAIgqAIEACgEQJQEAAa5EgKJzCAAoEHAWgBQhgCwWAAqgQ5KwGidAmUMAYLexBDpwQhrHwSoHY==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p13 Note: P = 41.55 GPa
formula_title: <missing>
a: 2.940
b: 4.856
c: 5.584
alpha: 101.99
beta: 95.58
gamma: 89.65
cell_volume: 77.604
crystal_density: 4.894
atoms_sites: ["Mn1", "Ca1", "C1", "O1", "O2", "O3"]
atoms_x: 4OYLAODmCwDgwSYAgLkqAKB+LABgbuv/
atoms_y: QK0SAECtEgDAojMAAO4CAKCoJQBAxQ4A
atoms_z: EEssABBLLABg3CwAwKIzAGCsNABgThoA
atoms_occupancy: AJg6AABxAgAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: IEICACBCAgDAVwEAwNQBAMBdAABAGQEA
atoms_aniso_label: ["Mn1", "Ca1"]
atoms_aniso_u11: wM4CAMDOAgA=
atoms_aniso_u22: AHECAABxAgA=
atoms_aniso_u33: gDgBAIA4AQA=
atoms_aniso_u12: oIYBAKCGAQA=
atoms_aniso_u13: YPD//2Dw//8=
atoms_aniso_u23: gMH//4DB//8=
qdat:
AAAAAAAAAAAAAAAAAAAIAAgAAAAAAAAAQAABAAEAAAIAQAAAQCACAAAQARAAAAEAIAwAAABCCAATAhACEAQQGAAAQDIAEASCMAQEADAYgSgIAAwsJA4nKEACQM0A5EBiHAGgoABJAnSVgZDUCYooBQM9iEcjBCCsdiQocY==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run1-p14 Note: P = 35.67 GPa
formula_title: <missing>
a: 2.9539
b: 4.843
c: 5.588
alpha: 101.78
beta: 95.09
gamma: 90.45
cell_volume: 77.921
crystal_density: 4.874
atoms_sites: ["Mn1", "Ca1", "C1", "O1", "O2", "O3"]
atoms_x: YCUMAGAlDADAAiQAAIEpAAD4KgBg5ez/
atoms_y: 4LwSAOC8EgCAjzEAwFECAGCPJABAPBAA
atoms_z: 4FIsAOBSLACAmy8AIJMzAEDbNABAfRoA
atoms_occupancy: AJg6AABxAgAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: gDICAIAyAgDA1AEAoIYBAIA+AAAgywAA
atoms_aniso_label: ["Mn1", "Ca1"]
atoms_aniso_u11: QJACAECQAgA=
atoms_aniso_u22: YOQBAGDkAQA=
atoms_aniso_u33: AHcBAAB3AQA=
atoms_aniso_u12: IEgBACBIAQA=
atoms_aniso_u13: oBX//6AV//8=
atoms_aniso_u23: IFT//yBU//8=
qdat:
AAAAAAAAAAAAAAAAAAAQAAQAAAAAAAAAQAACAAEAAAoAQAAAQCACAABAAGAAAAIAMBIAAAEQCAAWRCAEIAEQxAACIJIAEAYCUAEIAQQoQUBAAGMohDA4jgACFJSB1AgUHAshUgDQhRcMFosKKEKgMS5WRDaqQMmTPhRkIh==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p0 Note: P = .0001 GPa
formula_title: <missing>
a: 4.7799
b: 4.7799
c: 15.694
alpha: 90
beta: 90
gamma: 120
cell_volume: 310.529
crystal_density: 3.669
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAwGEQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: QOcAAEDnAADgqwAAAPoAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: YLgAAGC4AAAAfQAA
atoms_aniso_u22: YLgAAGC4AACgjAAA
atoms_aniso_u33: cEMBAHBDAQBg5AEA
atoms_aniso_u12: MFwAADBcAADARAAA
atoms_aniso_u13: AAAAAAAAAAAA5///
atoms_aniso_u23: AAAAAAAAAAAg0f//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAABAAAgAABAAAAQAAAIAAAAQAoAAAAAAAIQAAIgEJBAAAAACACADACABAEQAEgIQAAAAkACCQAAAEgAkIQgCACAQGAAAAQBIEEAgkAEYgAAlAoVAAAECCBAAkBQkgQBABgAA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p1 Note: P = .22 GPa
formula_title: <missing>
a: 4.7788
b: 4.7788
c: 15.685
alpha: 90
beta: 90
gamma: 120
cell_volume: 310.208
crystal_density: 3.673
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAkGkQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: cK0AAHCtAABwYgAAgLsAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: kJcAAJCXAAAAlgAA
atoms_aniso_u22: kJcAAJCXAADgqwAA
atoms_aniso_u33: wNoAAMDaAAAA+gAA
atoms_aniso_u12: AEsAAABLAADQUgAA
atoms_aniso_u13: AAAAAAAAAABg8P//
atoms_aniso_u23: AAAAAAAAAADA4P//
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAABAAAgAABAAAAQAAAIAAAAQAYAAAAAAAIIAAEgEJBAAAAACABADACABAEQAEgIQAAAAkACCQAAAEQAkEQgCABAQGAAAAQBICEAgUACMgAAlAYVAAAECCBAAkBQkgQBABgAA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p2 Note: P = .79 GPa
formula_title: <missing>
a: 4.7753
b: 4.7753
c: 15.6360
alpha: 90
beta: 90
gamma: 120
cell_volume: 308.786
crystal_density: 3.690
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAMGAQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: sLMAALCzAABgnwAAgLsAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: UJEAAFCRAABAgwAA
atoms_aniso_u22: UJEAAFCRAADgqwAA
atoms_aniso_u33: cPgAAHD4AACgCQEA
atoms_aniso_u12: 4EcAAOBHAACAVwAA
atoms_aniso_u13: AAAAAAAAAAAgAwAA
atoms_aniso_u23: AAAAAAAAAABABgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAABAAAQAABAAAAQAAAIAAAAIAMAAAAAAAIIAACQCFAgAAAABAAgBgCAAgEIACQEIAAAASABBEAAAEQASEIgBAAgEDAAAAIAUCEAgSACGQAASgUKgAAECBAgAUAYSgIAgAwAA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p3 Note: P = 1.62 GPa
formula_title: <missing>
a: 4.7714
b: 4.7714
c: 15.578
alpha: 90
beta: 90
gamma: 120
cell_volume: 307.138
crystal_density: 3.709
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAEF0QAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: ILIAACCyAADQhAAAQLUAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: UJEAAFCRAACQfgAA
atoms_aniso_u22: UJEAAFCRAAAgywAA
atoms_aniso_u33: MPIAADDyAABg6gAA
atoms_aniso_u12: 4EcAAOBHAAAgZwAA
atoms_aniso_u13: AAAAAAAAAABgCQAA
atoms_aniso_u23: AAAAAAAAAADAEgAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAgAAIAABAAAAIAAAEAAAAIAGAAAAAAAIIAABIBCggAAAABAAQAgBAAQCIAAwCIAAAAJABAiAAACIAKBEQBAAgCBAAAAIAMAiAQRACDIAAJgGEgAACAgggAKAUJQEAQAIAA==


formula: (Mn.96 Ca.04) C O3
compound: Sardegna, Italy
pub_title: The MnCO3-II high-pressure polymorph of rhodocrosite Note: Sample run2-p4 Note: P = 2.12 GPa
formula_title: <missing>
a: 4.7654
b: 4.7654
c: 15.531
alpha: 90
beta: 90
gamma: 120
cell_volume: 305.442
crystal_density: 3.730
atoms_sites: ["Mn1", "Ca1", "C1", "O1"]
atoms_x: AAAAAAAAAAAAAAAAwGEQAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAA==
atoms_z: AAAAAAAAAABAQg8AQEIPAA==
atoms_occupancy: AJg6AABxAgAACT0AAAk9AA==
atoms_u_iso: 8LkAAPC5AAAQiwAAsLMAAA==
atoms_aniso_label: ["Mn1", "Ca1", "O1"]
atoms_aniso_u11: cJQAAHCUAADwhwAA
atoms_aniso_u22: cJQAAHCUAAAgywAA
atoms_aniso_u33: gAYBAIAGAQDA2gAA
atoms_aniso_u12: cEkAAHBJAACwaAAA
atoms_aniso_u13: AAAAAAAAAACQAQAA
atoms_aniso_u23: AAAAAAAAAACQAQAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAACAAAAAAAAgAAEAAAgAAAIAAAEAAAAEACAAAAAAAEEAAAoAQwQAAAAAQAIAQBAAQCEAAYCEAAAAIgAgRAAABIADAiIAgAQBAwAAACAGARAIJAAhIAAIoDCQAAAgIQQAEgGEkBAEAEAA==


